  
data_1-La 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'As2 Fe4 H76 K La Na2 O104 W18' 
_chemical_formula_weight          5647.14 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'La'  'La'  -0.2871   2.4523 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.650(10) 
_cell_length_b                    13.180(10) 
_cell_length_c                    15.709(12) 
_cell_angle_alpha                 79.285(14) 
_cell_angle_beta                  89.130(15) 
_cell_angle_gamma                 65.290(12) 
_cell_volume                      2332(3) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     7882 
_cell_measurement_theta_min       1.78 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description         virgate  
_exptl_crystal_colour             'light yellow'
_exptl_crystal_size_max           0.24 
_exptl_crystal_size_mid           0.08 
_exptl_crystal_size_min           0.06 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     4.021 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2508 
_exptl_absorpt_coefficient_mu     24.026 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0687 
_exptl_absorpt_correction_T_max   0.3266 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             11198 
_diffrn_reflns_av_R_equivalents   0.0506 
_diffrn_reflns_av_sigmaI/netI     0.1042 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -18 
_diffrn_reflns_limit_l_max        16 
_diffrn_reflns_theta_min          1.78 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              7882 
_reflns_number_gt                 5194 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. The K+ and La3+ cations 
 are disordered with the site occupancy of 0.5, which are determined
 according to the mass percentages of K+ and La3+ cations from inductively
 coupled plasma atomic emission spectrometry and their magnitude of 
 anisotropic displacement parameters. The ISOR instruction is used for 
 O1W, O2, O3, O8, O10, O13, O18, O25, O28, O32, O33, O1, O6, O27, O29,
 O30, O15, O9, O17, O19, O24 and O5. The DFIX instruction is used for 
 Na1 and O24W. O13W is disordered over two positions (O13W and O13A)
 and O21W is disordered over two positions (O21W and O21A). The O6W, 
 O7W, O8W, O9W, O10W, O11W, O13W, O13A, O14W, O15W, O17W, O20W, O21W, 
 O21A, O23W and O24W are refined isostropicallly. 582 parameters and
 133 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1358P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    noedet 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          7882 
_refine_ls_number_parameters      582 
_refine_ls_number_restraints      133 
_refine_ls_R_factor_all           0.1072 
_refine_ls_R_factor_gt            0.0738 
_refine_ls_wR_factor_ref          0.2301 
_refine_ls_wR_factor_gt           0.2009 
_refine_ls_goodness_of_fit_ref    1.039 
_refine_ls_restrained_S_all       1.034 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Na1 Na 1.1892(12) -0.2889(11) 0.3036(11) 0.060(5) Uani 1 1 d D . . 
K1 K 0.5061(15) 0.7357(16) -0.1064(14) 0.069(6) Uani 0.50 1 d P . . 
W1 W 0.79496(8) 0.62789(9) 0.03493(8) 0.0230(3) Uani 1 1 d . . . 
W2 W 0.74293(9) 0.60685(9) 0.25045(9) 0.0258(3) Uani 1 1 d . . . 
W3 W 1.05720(9) 0.46352(9) 0.31618(8) 0.0245(3) Uani 1 1 d . . . 
W4 W 1.15858(9) 0.18254(9) 0.33223(9) 0.0258(3) Uani 1 1 d . . . 
W5 W 1.02772(9) 0.06625(9) 0.19112(9) 0.0277(3) Uani 1 1 d . . . 
W6 W 0.80414(9) 0.23894(9) 0.04672(9) 0.0257(3) Uani 1 1 d . . . 
W7 W 0.62300(9) 0.49917(9) 0.12332(9) 0.0252(3) Uani 1 1 d . . . 
W8 W 0.76225(9) 0.21341(9) 0.25952(9) 0.0262(3) Uani 1 1 d . . . 
W9 W 0.89444(9) 0.33315(9) 0.40150(9) 0.0263(3) Uani 1 1 d . . . 
La1 La 0.6223(3) 0.0668(3) 0.4685(3) 0.0340(9) Uani 0.50 1 d P . . 
As1 As 0.9514(2) 0.3598(2) 0.1586(2) 0.0225(7) Uani 1 1 d . . . 
Fe1 Fe 0.9067(3) 0.4123(3) -0.1025(3) 0.0237(9) Uani 1 1 d . . . 
Fe2 Fe 1.2745(3) 0.1116(3) 0.1362(3) 0.0294(10) Uani 1 1 d . . . 
O1W O 0.7454(15) 0.4364(16) -0.1585(14) 0.029(5) Uani 1 1 d U . . 
O2W O 0.9918(16) 0.2814(15) -0.1757(13) 0.031(5) Uani 1 1 d . . . 
O3W O 1.3339(19) -0.0436(15) 0.2268(16) 0.041(6) Uani 1 1 d . . . 
O4W O 1.4455(16) 0.0898(17) 0.1488(13) 0.033(5) Uani 1 1 d . . . 
O5W O 1.329(2) 0.008(2) 0.0421(14) 0.046(6) Uani 1 1 d . . . 
O7W O 0.449(3) 0.257(3) 0.412(3) 0.029(9) Uiso 0.50 1 d P B . 
O8W O 0.748(5) 0.149(5) 0.518(4) 0.080(18) Uiso 0.50 1 d P . . 
O9W O 0.832(5) -0.054(5) 0.429(4) 0.079(18) Uiso 0.50 1 d P B . 
O10W O 0.453(5) 0.042(5) 0.527(4) 0.069(16) Uiso 0.50 1 d P . . 
O11W O 0.531(5) 0.035(5) 0.341(4) 0.079(18) Uiso 0.50 1 d P B . 
O12W O 0.662(5) -0.146(5) 0.460(4) 0.083(18) Uiso 0.50 1 d P . . 
O13A O 1.016(5) -0.036(4) 0.442(4) 0.061(15) Uiso 0.50 1 d P . . 
O13W O 1.112(7) -0.076(7) 0.429(5) 0.11(3) Uiso 0.50 1 d P . . 
O14W O 0.785(6) -0.096(6) 0.255(5) 0.10(2) Uiso 0.50 1 d P . . 
O15W O 0.569(4) 0.438(4) 0.392(3) 0.125(14) Uiso 1 1 d . . . 
O16W O 1.1057(19) 0.0889(17) -0.0572(15) 0.043(6) Uani 1 1 d . . . 
O17W O 0.697(3) 0.580(3) 0.501(2) 0.102(11) Uiso 1 1 d . . . 
O18W O 0.625(2) 0.244(2) -0.192(2) 0.090(12) Uani 1 1 d . . . 
O19W O 0.6404(18) 0.664(2) -0.240(2) 0.071(9) Uani 1 1 d . . . 
O20W O 1.395(5) -0.361(5) 0.411(4) 0.074(17) Uiso 0.50 1 d P . . 
O21W O 0.569(6) -0.099(6) 0.089(5) 0.10(2) Uiso 0.50 1 d P . . 
O21A O 0.656(5) -0.085(5) 0.132(4) 0.081(18) Uiso 0.50 1 d P . . 
O22W O 1.135(2) 0.309(2) 0.5617(19) 0.070(10) Uani 1 1 d . . . 
O1 O 0.9361(15) 0.6105(15) 0.0636(13) 0.025(4) Uani 1 1 d U . . 
O2 O 0.7456(16) 0.7560(16) -0.0433(14) 0.033(5) Uani 1 1 d U . . 
O3 O 0.8350(15) 0.5257(15) -0.0327(13) 0.028(5) Uani 1 1 d U . . 
O4 O 0.6378(15) 0.6159(15) 0.0429(13) 0.029(5) Uani 1 1 d . . . 
O5 O 0.8168(15) 0.4847(14) 0.1503(12) 0.020(4) Uani 1 1 d U . . 
O6 O 0.7373(15) 0.6971(14) 0.1396(12) 0.024(4) Uani 1 1 d U . . 
O7 O 0.6715(16) 0.7087(16) 0.3097(15) 0.036(5) Uani 1 1 d . . . 
O8 O 0.6137(14) 0.5848(15) 0.2154(11) 0.019(4) Uani 1 1 d U . . 
O9 O 0.7740(15) 0.4661(14) 0.3417(12) 0.020(4) Uani 1 1 d U . . 
O10 O 0.8982(15) 0.5791(13) 0.2757(13) 0.022(4) Uani 1 1 d U . . 
O11 O 1.1141(18) 0.5408(16) 0.3588(15) 0.041(6) Uani 1 1 d . . . 
O12 O 0.9904(15) 0.3379(15) 0.2755(12) 0.024(4) Uani 1 1 d . . . 
O13 O 0.9737(15) 0.4244(16) 0.4162(13) 0.028(4) Uani 1 1 d U . . 
O14 O 1.1023(14) 0.4769(13) 0.2042(12) 0.020(4) Uani 1 1 d . . . 
O15 O 1.1767(15) 0.3140(15) 0.3576(13) 0.025(4) Uani 1 1 d U . . 
O16 O 1.2725(15) 0.0719(18) 0.3990(14) 0.036(5) Uani 1 1 d . . . 
O17 O 1.0453(13) 0.2050(13) 0.4222(11) 0.013(4) Uani 1 1 d U . . 
O18 O 1.2260(15) 0.1975(15) 0.2274(13) 0.025(4) Uani 1 1 d U . . 
O19 O 1.0863(14) 0.0988(13) 0.2946(11) 0.015(4) Uani 1 1 d U . . 
O20 O 1.1035(17) -0.0789(15) 0.2065(14) 0.033(5) Uani 1 1 d . . . 
O21 O 0.8996(16) 0.0721(14) 0.2644(13) 0.029(5) Uani 1 1 d . . . 
O22 O 1.1212(15) 0.1148(16) 0.1253(13) 0.028(5) Uani 1 1 d . . . 
O23 O 0.8930(15) 0.2541(16) 0.1713(12) 0.025(4) Uani 1 1 d . . . 
O24 O 0.9275(14) 0.0893(13) 0.0894(11) 0.018(4) Uani 1 1 d U . . 
O25 O 0.7388(19) 0.2114(17) -0.0370(15) 0.042(5) Uani 1 1 d U . . 
O26 O 0.8985(15) 0.2904(17) -0.0129(12) 0.027(4) Uani 1 1 d . . . 
O27 O 0.7230(15) 0.1987(15) 0.1470(12) 0.025(4) Uani 1 1 d U . . 
O28 O 0.6939(14) 0.3893(14) 0.0533(12) 0.019(4) Uani 1 1 d U . . 
O29 O 0.4796(16) 0.5321(16) 0.1059(14) 0.033(5) Uani 1 1 d U . . 
O30 O 0.6632(15) 0.3756(15) 0.2196(12) 0.023(4) Uani 1 1 d U . . 
O31 O 0.6722(15) 0.1660(17) 0.3209(14) 0.035(5) Uani 1 1 d . B . 
O32 O 0.8341(15) 0.2465(14) 0.3548(12) 0.023(4) Uani 1 1 d U . . 
O33 O 0.8397(16) 0.3241(15) 0.5004(14) 0.031(5) Uani 1 1 d U . . 
O23W O 0.508(9) 0.142(8) 0.644(7) 0.14(4) Uiso 0.50 1 d P A 2 
O6W O 0.541(4) 0.165(4) 0.611(3) 0.037(11) Uiso 0.50 1 d P B 1 
O24W O 1.025(2) -0.216(4) 0.335(4) 0.18(2) Uiso 1 1 d D . . 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Na1 O24W 1.993(10) . ? 
Na1 O20 2.67(2) . ? 
Na1 O11 2.78(2) 1_545 ? 
Na1 O20W 2.83(6) . ? 
K1 O4W 2.59(3) 2_765 ? 
K1 O4 2.70(3) . ? 
K1 O27 2.70(2) 2_665 ? 
K1 O19W 2.73(4) . ? 
K1 O2 3.33(2) . ? 
K1 W1 3.877(17) . ? 
K1 W6 3.912(18) 2_665 ? 
K1 W8 3.938(18) 2_665 ? 
K1 W7 4.107(18) 2_665 ? 
K1 W7 4.129(18) . ? 
W1 O1 1.757(17) . ? 
W1 O2 1.77(2) . ? 
W1 O3 1.773(19) . ? 
W1 O6 2.008(18) . ? 
W1 O4 2.059(19) . ? 
W1 O5 2.287(18) . ? 
W2 O7 1.705(19) . ? 
W2 O10 1.876(16) . ? 
W2 O8 1.883(16) . ? 
W2 O6 1.901(19) . ? 
W2 O9 2.017(17) . ? 
W2 O5 2.362(17) . ? 
W3 O11 1.699(19) . ? 
W3 O14 1.842(18) . ? 
W3 O15 1.912(18) . ? 
W3 O10 1.971(16) . ? 
W3 O13 1.99(2) . ? 
W3 O12 2.334(18) . ? 
W4 O16 1.74(2) . ? 
W4 O18 1.859(19) . ? 
W4 O19 1.872(16) . ? 
W4 O15 1.951(17) . ? 
W4 O17 1.969(17) . ? 
W4 O12 2.292(17) . ? 
W5 O20 1.714(18) . ? 
W5 O22 1.797(18) . ? 
W5 O24 1.952(16) . ? 
W5 O21 1.96(2) . ? 
W5 O19 1.985(16) . ? 
W5 O23 2.309(19) . ? 
W6 O25 1.73(2) . ? 
W6 O26 1.779(18) . ? 
W6 O28 1.909(16) . ? 
W6 O24 1.935(16) . ? 
W6 O27 1.978(19) . ? 
W6 O23 2.352(17) . ? 
W6 K1 3.912(18) 2_665 ? 
W7 O29 1.693(18) . ? 
W7 O4 1.87(2) . ? 
W7 O28 1.894(17) . ? 
W7 O30 1.901(19) . ? 
W7 O8 1.967(18) . ? 
W7 O5 2.416(17) . ? 
W7 K1 4.107(18) 2_665 ? 
W8 O31 1.72(2) . ? 
W8 O27 1.908(18) . ? 
W8 O21 1.933(18) . ? 
W8 O30 1.954(18) . ? 
W8 O32 1.967(18) . ? 
W8 O23 2.311(18) . ? 
W8 K1 3.938(18) 2_665 ? 
W9 O33 1.70(2) . ? 
W9 O9 1.864(16) . ? 
W9 O32 1.867(17) . ? 
W9 O13 1.904(18) . ? 
W9 O17 1.929(15) . ? 
W9 O12 2.31(2) . ? 
La1 O10W 2.01(6) 2_656 ? 
La1 O10W 2.44(6) . ? 
La1 O16 2.47(2) 2_756 ? 
La1 O8W 2.47(6) . ? 
La1 O11W 2.51(6) . ? 
La1 O7W 2.55(4) . ? 
La1 O9W 2.60(6) . ? 
La1 O31 2.65(2) . ? 
La1 O12W 2.66(6) . ? 
La1 O6W 2.76(5) . ? 
La1 La1 4.179(8) 2_656 ? 
As1 O5 1.792(17) . ? 
As1 O23 1.811(18) . ? 
As1 O12 1.846(18) . ? 
Fe1 O14 1.923(17) 2_765 ? 
Fe1 O3 1.925(19) . ? 
Fe1 O26 1.97(2) . ? 
Fe1 O1 1.971(17) 2_765 ? 
Fe1 O1W 2.109(17) . ? 
Fe1 O2W 2.15(2) . ? 
Fe2 O18 1.926(19) . ? 
Fe2 O22 1.932(17) . ? 
Fe2 O2 1.98(2) 2_765 ? 
Fe2 O4W 2.066(19) . ? 
Fe2 O5W 2.11(2) . ? 
Fe2 O3W 2.11(2) . ? 
O4W K1 2.59(3) 2_765 ? 
O8W O13W 1.76(10) 2_756 ? 
O10W O12W 1.57(7) 2_656 ? 
O10W O10W 1.60(11) 2_656 ? 
O10W La1 2.01(6) 2_656 ? 
O12W O10W 1.57(7) 2_656 ? 
O13A O13W 1.13(8) . ? 
O13W O8W 1.76(10) 2_756 ? 
O21W O21A 1.39(8) . ? 
O1 Fe1 1.971(17) 2_765 ? 
O2 Fe2 1.98(2) 2_765 ? 
O11 Na1 2.78(2) 1_565 ? 
O14 Fe1 1.923(17) 2_765 ? 
O16 La1 2.47(2) 2_756 ? 
O27 K1 2.70(2) 2_665 ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O24W Na1 O20 75.3(17) . . ? 
O24W Na1 O11 71.9(17) . 1_545 ? 
O20 Na1 O11 137.8(7) . 1_545 ? 
O24W Na1 O20W 128(2) . . ? 
O20 Na1 O20W 118.0(13) . . ? 
O11 Na1 O20W 103.1(13) 1_545 . ? 
O4W K1 O4 104.7(9) 2_765 . ? 
O4W K1 O27 109.0(8) 2_765 2_665 ? 
O4 K1 O27 130.3(9) . 2_665 ? 
O4W K1 O19W 83.2(9) 2_765 . ? 
O4 K1 O19W 107.0(9) . . ? 
O27 K1 O19W 112.2(10) 2_665 . ? 
O4W K1 O2 53.3(6) 2_765 . ? 
O4 K1 O2 55.6(6) . . ? 
O27 K1 O2 158.1(9) 2_665 . ? 
O19W K1 O2 80.7(8) . . ? 
O4W K1 W1 80.0(6) 2_765 . ? 
O4 K1 W1 30.3(5) . . ? 
O27 K1 W1 159.2(9) 2_665 . ? 
O19W K1 W1 87.0(7) . . ? 
O2 K1 W1 27.0(4) . . ? 
O4W K1 W6 123.1(8) 2_765 2_665 ? 
O4 K1 W6 102.5(7) . 2_665 ? 
O27 K1 W6 27.9(5) 2_665 2_665 ? 
O19W K1 W6 133.2(8) . 2_665 ? 
O2 K1 W6 145.9(8) . 2_665 ? 
W1 K1 W6 131.7(6) . 2_665 ? 
O4W K1 W8 107.8(7) 2_765 2_665 ? 
O4 K1 W8 146.1(7) . 2_665 ? 
O27 K1 W8 25.8(4) 2_665 2_665 ? 
O19W K1 W8 86.5(8) . 2_665 ? 
O2 K1 W8 158.1(7) . 2_665 ? 
W1 K1 W8 169.1(6) . 2_665 ? 
W6 K1 W8 50.6(2) 2_665 2_665 ? 
O4W K1 W7 160.5(8) 2_765 2_665 ? 
O4 K1 W7 94.5(6) . 2_665 ? 
O27 K1 W7 58.9(5) 2_665 2_665 ? 
O19W K1 W7 87.7(8) . 2_665 ? 
O2 K1 W7 141.9(6) . 2_665 ? 
W1 K1 W7 116.9(4) . 2_665 ? 
W6 K1 W7 54.1(2) 2_665 2_665 ? 
W8 K1 W7 54.2(2) 2_665 2_665 ? 
O4W K1 W7 124.8(7) 2_765 . ? 
O4 K1 W7 21.0(5) . . ? 
O27 K1 W7 112.1(7) 2_665 . ? 
O19W K1 W7 112.3(8) . . ? 
O2 K1 W7 76.4(5) . . ? 
W1 K1 W7 50.4(2) . . ? 
W6 K1 W7 85.2(4) 2_665 . ? 
W8 K1 W7 125.1(4) 2_665 . ? 
W7 K1 W7 74.7(3) 2_665 . ? 
O1 W1 O2 100.7(9) . . ? 
O1 W1 O3 97.6(8) . . ? 
O2 W1 O3 101.1(9) . . ? 
O1 W1 O6 89.6(8) . . ? 
O2 W1 O6 97.7(8) . . ? 
O3 W1 O6 158.3(8) . . ? 
O1 W1 O4 160.6(8) . . ? 
O2 W1 O4 96.8(8) . . ? 
O3 W1 O4 87.0(8) . . ? 
O6 W1 O4 79.9(7) . . ? 
O1 W1 O5 88.3(8) . . ? 
O2 W1 O5 166.0(8) . . ? 
O3 W1 O5 88.2(8) . . ? 
O6 W1 O5 71.5(7) . . ? 
O4 W1 O5 73.0(7) . . ? 
O1 W1 K1 157.9(7) . . ? 
O2 W1 K1 59.0(6) . . ? 
O3 W1 K1 79.4(7) . . ? 
O6 W1 K1 101.3(6) . . ? 
O4 W1 K1 41.5(6) . . ? 
O5 W1 K1 113.4(5) . . ? 
O7 W2 O10 100.8(8) . . ? 
O7 W2 O8 97.8(8) . . ? 
O10 W2 O8 160.2(7) . . ? 
O7 W2 O6 101.7(9) . . ? 
O10 W2 O6 92.0(8) . . ? 
O8 W2 O6 90.9(7) . . ? 
O7 W2 O9 99.5(9) . . ? 
O10 W2 O9 86.3(7) . . ? 
O8 W2 O9 83.9(7) . . ? 
O6 W2 O9 158.7(7) . . ? 
O7 W2 O5 170.5(8) . . ? 
O10 W2 O5 86.3(7) . . ? 
O8 W2 O5 76.0(7) . . ? 
O6 W2 O5 71.6(7) . . ? 
O9 W2 O5 87.2(7) . . ? 
O11 W3 O14 101.4(10) . . ? 
O11 W3 O15 99.4(8) . . ? 
O14 W3 O15 95.8(8) . . ? 
O11 W3 O10 101.7(8) . . ? 
O14 W3 O10 90.3(8) . . ? 
O15 W3 O10 156.4(7) . . ? 
O11 W3 O13 100.2(10) . . ? 
O14 W3 O13 158.1(7) . . ? 
O15 W3 O13 84.4(8) . . ? 
O10 W3 O13 81.6(8) . . ? 
O11 W3 O12 171.9(8) . . ? 
O14 W3 O12 84.2(7) . . ? 
O15 W3 O12 74.0(6) . . ? 
O10 W3 O12 84.0(6) . . ? 
O13 W3 O12 74.7(7) . . ? 
O16 W4 O18 102.9(9) . . ? 
O16 W4 O19 99.2(8) . . ? 
O18 W4 O19 92.7(8) . . ? 
O16 W4 O15 100.7(9) . . ? 
O18 W4 O15 89.9(8) . . ? 
O19 W4 O15 158.8(7) . . ? 
O16 W4 O17 94.7(8) . . ? 
O18 W4 O17 162.4(7) . . ? 
O19 W4 O17 84.3(7) . . ? 
O15 W4 O17 86.9(7) . . ? 
O16 W4 O12 166.2(8) . . ? 
O18 W4 O12 90.1(7) . . ? 
O19 W4 O12 84.6(7) . . ? 
O15 W4 O12 74.3(7) . . ? 
O17 W4 O12 72.4(7) . . ? 
O20 W5 O22 102.0(9) . . ? 
O20 W5 O24 98.5(8) . . ? 
O22 W5 O24 91.6(8) . . ? 
O20 W5 O21 98.5(9) . . ? 
O22 W5 O21 159.1(8) . . ? 
O24 W5 O21 89.2(7) . . ? 
O20 W5 O19 101.4(8) . . ? 
O22 W5 O19 89.9(8) . . ? 
O24 W5 O19 159.3(6) . . ? 
O21 W5 O19 82.2(7) . . ? 
O20 W5 O23 168.5(8) . . ? 
O22 W5 O23 87.7(8) . . ? 
O24 W5 O23 74.9(6) . . ? 
O21 W5 O23 72.4(7) . . ? 
O19 W5 O23 84.6(6) . . ? 
O25 W6 O26 99.9(10) . . ? 
O25 W6 O28 101.2(9) . . ? 
O26 W6 O28 92.3(8) . . ? 
O25 W6 O24 100.5(8) . . ? 
O26 W6 O24 93.8(8) . . ? 
O28 W6 O24 156.1(7) . . ? 
O25 W6 O27 101.2(9) . . ? 
O26 W6 O27 158.7(8) . . ? 
O28 W6 O27 81.8(7) . . ? 
O24 W6 O27 84.2(7) . . ? 
O25 W6 O23 172.4(8) . . ? 
O26 W6 O23 85.9(7) . . ? 
O28 W6 O23 83.2(7) . . ? 
O24 W6 O23 74.2(7) . . ? 
O27 W6 O23 73.1(7) . . ? 
O25 W6 K1 70.3(9) . 2_665 ? 
O26 W6 K1 152.0(6) . 2_665 ? 
O28 W6 K1 65.3(6) . 2_665 ? 
O24 W6 K1 113.5(6) . 2_665 ? 
O27 W6 K1 39.7(6) . 2_665 ? 
O23 W6 K1 106.6(5) . 2_665 ? 
O29 W7 O4 101.0(9) . . ? 
O29 W7 O28 102.3(8) . . ? 
O4 W7 O28 93.3(7) . . ? 
O29 W7 O30 99.9(9) . . ? 
O4 W7 O30 158.5(8) . . ? 
O28 W7 O30 87.2(8) . . ? 
O29 W7 O8 99.5(8) . . ? 
O4 W7 O8 89.1(7) . . ? 
O28 W7 O8 157.2(7) . . ? 
O30 W7 O8 82.4(7) . . ? 
O29 W7 O5 170.5(8) . . ? 
O4 W7 O5 73.1(7) . . ? 
O28 W7 O5 85.7(7) . . ? 
O30 W7 O5 85.4(7) . . ? 
O8 W7 O5 73.3(6) . . ? 
O29 W7 K1 56.0(7) . 2_665 ? 
O4 W7 K1 134.0(6) . 2_665 ? 
O28 W7 K1 60.2(6) . 2_665 ? 
O30 W7 K1 63.9(6) . 2_665 ? 
O8 W7 K1 130.3(6) . 2_665 ? 
O5 W7 K1 133.5(5) . 2_665 ? 
O29 W7 K1 73.0(8) . . ? 
O4 W7 K1 31.1(6) . . ? 
O28 W7 K1 86.3(6) . . ? 
O30 W7 K1 169.2(6) . . ? 
O8 W7 K1 106.6(6) . . ? 
O5 W7 K1 102.8(5) . . ? 
K1 W7 K1 105.3(3) 2_665 . ? 
O31 W8 O27 100.6(9) . . ? 
O31 W8 O21 100.9(9) . . ? 
O27 W8 O21 87.3(8) . . ? 
O31 W8 O30 103.0(8) . . ? 
O27 W8 O30 84.9(7) . . ? 
O21 W8 O30 155.8(8) . . ? 
O31 W8 O32 97.1(8) . . ? 
O27 W8 O32 162.3(8) . . ? 
O21 W8 O32 89.7(8) . . ? 
O30 W8 O32 90.8(7) . . ? 
O31 W8 O23 172.4(8) . . ? 
O27 W8 O23 75.3(7) . . ? 
O21 W8 O23 72.8(7) . . ? 
O30 W8 O23 83.2(7) . . ? 
O32 W8 O23 87.2(7) . . ? 
O31 W8 K1 72.1(7) . 2_665 ? 
O27 W8 K1 38.0(6) . 2_665 ? 
O21 W8 K1 116.7(6) . 2_665 ? 
O30 W8 K1 68.2(6) . 2_665 ? 
O32 W8 K1 152.5(6) . 2_665 ? 
O23 W8 K1 106.7(5) . 2_665 ? 
O33 W9 O9 99.9(9) . . ? 
O33 W9 O32 97.8(8) . . ? 
O9 W9 O32 89.8(7) . . ? 
O33 W9 O13 99.2(8) . . ? 
O9 W9 O13 87.2(8) . . ? 
O32 W9 O13 163.0(8) . . ? 
O33 W9 O17 101.9(8) . . ? 
O9 W9 O17 158.0(8) . . ? 
O32 W9 O17 90.0(7) . . ? 
O13 W9 O17 86.6(7) . . ? 
O33 W9 O12 173.2(7) . . ? 
O9 W9 O12 85.4(7) . . ? 
O32 W9 O12 86.3(7) . . ? 
O13 W9 O12 76.8(7) . . ? 
O17 W9 O12 72.6(6) . . ? 
O10W La1 O10W 41(3) 2_656 . ? 
O10W La1 O16 80.4(17) 2_656 2_756 ? 
O10W La1 O16 84.1(14) . 2_756 ? 
O10W La1 O8W 157(2) 2_656 . ? 
O10W La1 O8W 133(2) . . ? 
O16 La1 O8W 77.1(15) 2_756 . ? 
O10W La1 O11W 54(2) 2_656 . ? 
O10W La1 O11W 76.6(19) . . ? 
O16 La1 O11W 128.5(15) 2_756 . ? 
O8W La1 O11W 147(2) . . ? 
O10W La1 O7W 100.9(17) 2_656 . ? 
O10W La1 O7W 75.1(16) . . ? 
O16 La1 O7W 144.0(10) 2_756 . ? 
O8W La1 O7W 95.9(16) . . ? 
O11W La1 O7W 75.0(16) . . ? 
O10W La1 O9W 102(2) 2_656 . ? 
O10W La1 O9W 139.8(19) . . ? 
O16 La1 O9W 72.7(15) 2_756 . ? 
O8W La1 O9W 74(2) . . ? 
O11W La1 O9W 92(2) . . ? 
O7W La1 O9W 139.8(17) . . ? 
O10W La1 O31 122.6(17) 2_656 . ? 
O10W La1 O31 136.9(14) . . ? 
O16 La1 O31 138.2(6) 2_756 . ? 
O8W La1 O31 77.3(16) . . ? 
O11W La1 O31 69.3(15) . . ? 
O7W La1 O31 71.1(10) . . ? 
O9W La1 O31 68.7(15) . . ? 
O10W La1 O12W 36.0(19) 2_656 . ? 
O10W La1 O12W 74.8(19) . . ? 
O16 La1 O12W 67.2(15) 2_756 . ? 
O8W La1 O12W 132.2(19) . . ? 
O11W La1 O12W 61.8(19) . . ? 
O7W La1 O12W 131.6(16) . . ? 
O9W La1 O12W 66.1(19) . . ? 
O31 La1 O12W 109.4(15) . . ? 
O10W La1 O6W 102.6(19) 2_656 . ? 
O10W La1 O6W 65.4(17) . . ? 
O16 La1 O6W 71.4(11) 2_756 . ? 
O8W La1 O6W 67.8(18) . . ? 
O11W La1 O6W 135.3(17) . . ? 
O7W La1 O6W 73.3(13) . . ? 
O9W La1 O6W 131.8(17) . . ? 
O31 La1 O6W 126.3(11) . . ? 
O12W La1 O6W 124.3(18) . . ? 
O10W La1 La1 22.4(15) 2_656 2_656 ? 
O10W La1 La1 18.3(13) . 2_656 ? 
O16 La1 La1 81.9(5) 2_756 2_656 ? 
O8W La1 La1 147.4(16) . 2_656 ? 
O11W La1 La1 65.4(15) . 2_656 ? 
O7W La1 La1 86.6(9) . 2_656 ? 
O9W La1 La1 123.1(14) . 2_656 ? 
O31 La1 La1 133.3(4) . 2_656 ? 
O12W La1 La1 57.1(14) . 2_656 ? 
O6W La1 La1 82.0(10) . 2_656 ? 
O5 As1 O23 98.6(8) . . ? 
O5 As1 O12 98.5(8) . . ? 
O23 As1 O12 95.1(9) . . ? 
O14 Fe1 O3 93.4(8) 2_765 . ? 
O14 Fe1 O26 168.9(7) 2_765 . ? 
O3 Fe1 O26 92.6(8) . . ? 
O14 Fe1 O1 93.2(8) 2_765 2_765 ? 
O3 Fe1 O1 91.4(8) . 2_765 ? 
O26 Fe1 O1 96.0(8) . 2_765 ? 
O14 Fe1 O1W 82.1(7) 2_765 . ? 
O3 Fe1 O1W 93.3(8) . . ? 
O26 Fe1 O1W 88.3(7) . . ? 
O1 Fe1 O1W 173.5(9) 2_765 . ? 
O14 Fe1 O2W 88.5(7) 2_765 . ? 
O3 Fe1 O2W 177.6(8) . . ? 
O26 Fe1 O2W 85.8(8) . . ? 
O1 Fe1 O2W 86.9(7) 2_765 . ? 
O1W Fe1 O2W 88.5(7) . . ? 
O18 Fe2 O22 90.0(8) . . ? 
O18 Fe2 O2 95.4(8) . 2_765 ? 
O22 Fe2 O2 99.4(8) . 2_765 ? 
O18 Fe2 O4W 93.7(8) . . ? 
O22 Fe2 O4W 174.0(8) . . ? 
O2 Fe2 O4W 84.9(7) 2_765 . ? 
O18 Fe2 O5W 176.4(8) . . ? 
O22 Fe2 O5W 89.3(9) . . ? 
O2 Fe2 O5W 88.2(9) 2_765 . ? 
O4W Fe2 O5W 86.7(9) . . ? 
O18 Fe2 O3W 91.4(8) . . ? 
O22 Fe2 O3W 91.2(8) . . ? 
O2 Fe2 O3W 167.4(8) 2_765 . ? 
O4W Fe2 O3W 84.0(8) . . ? 
O5W Fe2 O3W 85.1(9) . . ? 
Fe2 O4W K1 119.5(9) . 2_765 ? 
O13W O8W La1 127(4) 2_756 . ? 
O12W O10W O10W 156(6) 2_656 2_656 ? 
O12W O10W La1 95(3) 2_656 2_656 ? 
O10W O10W La1 84(4) 2_656 2_656 ? 
O12W O10W La1 122(4) 2_656 . ? 
O10W O10W La1 55(3) 2_656 . ? 
La1 O10W La1 139(3) 2_656 . ? 
O10W O12W La1 49(3) 2_656 . ? 
O13A O13W O8W 142(8) . 2_756 ? 
W1 O1 Fe1 176.8(12) . 2_765 ? 
W1 O2 Fe2 167.9(11) . 2_765 ? 
W1 O2 K1 94.0(8) . . ? 
Fe2 O2 K1 95.3(7) 2_765 . ? 
W1 O3 Fe1 169.5(11) . . ? 
W7 O4 W1 120.4(9) . . ? 
W7 O4 K1 128.0(9) . . ? 
W1 O4 K1 108.2(9) . . ? 
As1 O5 W1 114.9(9) . . ? 
As1 O5 W2 128.8(9) . . ? 
W1 O5 W2 94.8(6) . . ? 
As1 O5 W7 126.9(8) . . ? 
W1 O5 W7 93.0(6) . . ? 
W2 O5 W7 89.2(6) . . ? 
W2 O6 W1 122.1(9) . . ? 
W2 O8 W7 121.2(9) . . ? 
W9 O9 W2 142.3(10) . . ? 
W2 O10 W3 146.3(9) . . ? 
W3 O11 Na1 139.4(12) . 1_565 ? 
As1 O12 W4 116.9(9) . . ? 
As1 O12 W9 135.5(9) . . ? 
W4 O12 W9 94.6(7) . . ? 
As1 O12 W3 116.3(9) . . ? 
W4 O12 W3 92.2(6) . . ? 
W9 O12 W3 91.2(6) . . ? 
W9 O13 W3 116.9(10) . . ? 
W3 O14 Fe1 142.3(9) . 2_765 ? 
W3 O15 W4 119.3(9) . . ? 
W4 O16 La1 158.9(11) . 2_756 ? 
W9 O17 W4 120.3(8) . . ? 
W4 O18 Fe2 135.8(10) . . ? 
W4 O19 W5 144.6(10) . . ? 
W5 O20 Na1 153.1(13) . . ? 
W8 O21 W5 120.6(9) . . ? 
W5 O22 Fe2 138.2(11) . . ? 
As1 O23 W5 116.3(8) . . ? 
As1 O23 W8 135.3(9) . . ? 
W5 O23 W8 94.0(7) . . ? 
As1 O23 W6 117.3(10) . . ? 
W5 O23 W6 91.9(6) . . ? 
W8 O23 W6 92.0(6) . . ? 
W6 O24 W5 119.0(8) . . ? 
W6 O26 Fe1 145.3(10) . . ? 
W8 O27 W6 119.3(9) . . ? 
W8 O27 K1 116.2(9) . 2_665 ? 
W6 O27 K1 112.4(9) . 2_665 ? 
W7 O28 W6 147.7(10) . . ? 
W7 O30 W8 144.0(10) . . ? 
W8 O31 La1 151.7(10) . . ? 
W9 O32 W8 152.9(10) . . ? 
  
_diffrn_measured_fraction_theta_max    0.961 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.961 
_refine_diff_density_max    3.940 
_refine_diff_density_min   -5.195 
_refine_diff_density_rms    0.687 
  
#===END

  
data_2-Pr 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'As2 Fe4 H76 K Na2 O104 Pr W18' 
_chemical_formula_weight          5649.14 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Pr'  'Pr'  -0.2180   2.8214 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.7027(13) 
_cell_length_b                    13.2756(14) 
_cell_length_c                    15.6850(17) 
_cell_angle_alpha                 78.960(2) 
_cell_angle_beta                  89.022(2) 
_cell_angle_gamma                 65.272(2) 
_cell_volume                      2352.2(4) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8104 
_cell_measurement_theta_min       1.72 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        virgate  
_exptl_crystal_colour             'light yellow' 
_exptl_crystal_size_max           0.55 
_exptl_crystal_size_mid           0.13 
_exptl_crystal_size_min           0.10 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.988 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2510 
_exptl_absorpt_coefficient_mu     23.885 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0267 
_exptl_absorpt_correction_T_max   0.1986 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             11716 
_diffrn_reflns_av_R_equivalents   0.0359 
_diffrn_reflns_av_sigmaI/netI     0.0730 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -18 
_diffrn_reflns_limit_l_max        18 
_diffrn_reflns_theta_min          1.72 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8104 
_reflns_number_gt                 6837 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. The K+ and Pr3+ cations 
 are disordered with the site occupancy of 0.5, which are determined 
 according to the mass percentages of K+ and Pr3+ cations from inductively
 coupled plasma atomic emission spectrometry and their magnitude of 
 anisotropic displacement parameters. The ISOR instruction is used for 
 O12, O16, O17, O21 and Na1. The DFIX instruction is used for
 Na1 and O24W. O13W is disordered over two positions (O13W and O13A) and 
 O21W is disordered over two positions (O21W and O21A). The O6W, O7W, 
 O8W, O9W, O10W, O11W, O13W, O13A, O14W, O15W, O17W, O20W, O21W, O21A, 
 O23W and O24W are refined isostropicallly. 582 parameters and 31 
 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0726P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    notdet 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          8104 
_refine_ls_number_parameters      582 
_refine_ls_number_restraints      31 
_refine_ls_R_factor_all           0.0524 
_refine_ls_R_factor_gt            0.0443 
_refine_ls_wR_factor_ref          0.1281 
_refine_ls_wR_factor_gt           0.1228 
_refine_ls_goodness_of_fit_ref    1.025 
_refine_ls_restrained_S_all       1.024 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Na1 Na 1.1906(6) -0.2917(5) 0.3045(5) 0.0417(16) Uani 1 1 d DU . . 
K1 K 0.5048(9) 0.7383(9) -0.1057(8) 0.073(3) Uani 0.50 1 d P . . 
W1 W 0.79500(4) 0.62744(4) 0.03493(4) 0.01573(14) Uani 1 1 d . . . 
W2 W 0.74326(4) 0.60607(4) 0.25095(4) 0.01869(15) Uani 1 1 d . . . 
W3 W 1.05785(4) 0.46247(4) 0.31651(4) 0.01758(15) Uani 1 1 d . . . 
W4 W 1.15914(4) 0.18172(4) 0.33313(4) 0.01885(15) Uani 1 1 d . . . 
W5 W 1.02780(5) 0.06656(4) 0.19183(4) 0.02089(15) Uani 1 1 d . . . 
W6 W 0.80395(4) 0.23977(4) 0.04674(4) 0.01844(15) Uani 1 1 d . . . 
W7 W 0.62313(4) 0.49912(4) 0.12383(4) 0.01797(15) Uani 1 1 d . . . 
W8 W 0.76263(5) 0.21340(4) 0.26035(4) 0.01903(15) Uani 1 1 d . . . 
W9 W 0.89511(5) 0.33247(4) 0.40223(4) 0.01912(15) Uani 1 1 d . . . 
Pr1 Pr 0.62369(13) 0.06685(13) 0.46831(11) 0.0255(4) Uani 0.50 1 d P . . 
As1 As 0.95184(11) 0.35980(10) 0.15865(9) 0.0137(3) Uani 1 1 d . . . 
Fe1 Fe 0.90693(15) 0.41203(15) -0.10223(13) 0.0173(4) Uani 1 1 d . . . 
Fe2 Fe 1.27480(16) 0.11209(15) 0.13668(14) 0.0209(4) Uani 1 1 d . . . 
O1W O 0.7427(8) 0.4400(8) -0.1585(7) 0.029(2) Uani 1 1 d . . . 
O2W O 0.9921(9) 0.2825(8) -0.1752(7) 0.031(2) Uani 1 1 d . . . 
O3W O 1.3329(9) -0.0415(8) 0.2258(7) 0.033(3) Uani 1 1 d . . . 
O4W O 1.4449(8) 0.0886(9) 0.1540(7) 0.031(2) Uani 1 1 d . . . 
O5W O 1.3257(11) 0.0087(10) 0.0446(8) 0.048(3) Uani 1 1 d . . . 
O7W O 0.4563(15) 0.2607(14) 0.4101(12) 0.020(4) Uiso 0.50 1 d P B . 
O8W O 0.746(2) 0.149(2) 0.513(2) 0.060(7) Uiso 0.50 1 d P B . 
O9W O 0.834(2) -0.048(2) 0.4298(17) 0.046(6) Uiso 0.50 1 d P B . 
O10W O 0.453(3) 0.041(3) 0.524(2) 0.073(9) Uiso 0.50 1 d P . . 
O11W O 0.530(3) 0.046(3) 0.333(2) 0.071(9) Uiso 0.50 1 d P B . 
O12W O 0.662(3) -0.139(3) 0.465(2) 0.075(9) Uiso 0.50 1 d P . . 
O13A O 1.027(3) -0.037(3) 0.439(2) 0.077(9) Uiso 0.50 1 d P . . 
O13W O 1.100(3) -0.078(3) 0.426(2) 0.069(9) Uiso 0.50 1 d P . . 
O14W O 0.791(4) -0.091(4) 0.245(3) 0.113(13) Uiso 0.50 1 d P . . 
O15W O 0.5602(18) 0.4390(17) 0.3952(14) 0.105(6) Uiso 1 1 d . . . 
O16W O 1.1067(9) 0.0893(8) -0.0578(7) 0.033(3) Uani 1 1 d . . . 
O17W O 0.6937(18) 0.5843(17) 0.5039(15) 0.108(6) Uiso 1 1 d . . . 
O18W O 0.6269(12) 0.2453(12) -0.1961(12) 0.080(5) Uani 1 1 d . . . 
O19W O 0.6387(11) 0.6631(10) -0.2403(10) 0.056(4) Uani 1 1 d . . . 
O20W O 1.399(3) -0.359(2) 0.409(2) 0.069(8) Uiso 0.50 1 d P . . 
O21W O 0.566(3) -0.092(2) 0.085(2) 0.062(7) Uiso 0.50 1 d P . . 
O21A O 0.646(3) -0.086(3) 0.138(2) 0.090(11) Uiso 0.50 1 d P . . 
O22W O 1.1368(9) 0.3073(10) 0.5606(7) 0.040(3) Uani 1 1 d . . . 
O1 O 0.9377(8) 0.6081(8) 0.0664(7) 0.031(3) Uani 1 1 d . . . 
O2 O 0.7421(8) 0.7561(8) -0.0437(7) 0.026(2) Uani 1 1 d . . . 
O3 O 0.8347(8) 0.5244(8) -0.0321(7) 0.024(2) Uani 1 1 d . . . 
O4 O 0.6401(8) 0.6142(7) 0.0446(6) 0.019(2) Uani 1 1 d . . . 
O5 O 0.8166(7) 0.4819(7) 0.1513(6) 0.0164(19) Uani 1 1 d . . . 
O6 O 0.7370(7) 0.6965(7) 0.1409(7) 0.021(2) Uani 1 1 d . . . 
O7 O 0.6731(8) 0.7069(8) 0.3102(7) 0.031(2) Uani 1 1 d . . . 
O8 O 0.6106(7) 0.5873(7) 0.2124(6) 0.020(2) Uani 1 1 d . . . 
O9 O 0.7770(8) 0.4689(8) 0.3352(7) 0.024(2) Uani 1 1 d . . . 
O10 O 0.9018(8) 0.5770(7) 0.2773(7) 0.025(2) Uani 1 1 d . . . 
O11 O 1.1129(8) 0.5374(9) 0.3659(7) 0.032(3) Uani 1 1 d . . . 
O12 O 0.9913(7) 0.3390(7) 0.2749(6) 0.019(2) Uani 1 1 d U . . 
O13 O 0.9727(8) 0.4230(8) 0.4150(6) 0.022(2) Uani 1 1 d . . . 
O14 O 1.1018(7) 0.4782(7) 0.2065(6) 0.017(2) Uani 1 1 d . . . 
O15 O 1.1760(8) 0.3120(7) 0.3575(6) 0.020(2) Uani 1 1 d . . . 
O16 O 1.2722(8) 0.0739(9) 0.4002(7) 0.033(3) Uani 1 1 d U . . 
O17 O 1.0430(8) 0.2057(7) 0.4231(6) 0.021(2) Uani 1 1 d U . . 
O18 O 1.2262(7) 0.1945(7) 0.2302(7) 0.021(2) Uani 1 1 d . . . 
O19 O 1.0869(7) 0.1003(7) 0.2893(7) 0.023(2) Uani 1 1 d . . . 
O20 O 1.1019(9) -0.0783(8) 0.2101(7) 0.031(3) Uani 1 1 d . . . 
O21 O 0.8961(8) 0.0748(7) 0.2642(6) 0.020(2) Uani 1 1 d U . . 
O22 O 1.1217(8) 0.1166(8) 0.1241(6) 0.023(2) Uani 1 1 d . . . 
O23 O 0.8936(7) 0.2559(7) 0.1697(6) 0.0159(19) Uani 1 1 d . . . 
O24 O 0.9274(8) 0.0910(7) 0.0891(7) 0.027(2) Uani 1 1 d . . . 
O25 O 0.7346(9) 0.2086(8) -0.0293(6) 0.026(2) Uani 1 1 d . . . 
O26 O 0.8982(8) 0.2928(7) -0.0157(6) 0.023(2) Uani 1 1 d . . . 
O27 O 0.7243(8) 0.1976(8) 0.1475(7) 0.026(2) Uani 1 1 d . . . 
O28 O 0.6947(8) 0.3898(7) 0.0534(7) 0.024(2) Uani 1 1 d . . . 
O29 O 0.4786(8) 0.5315(8) 0.1077(7) 0.028(2) Uani 1 1 d . . . 
O30 O 0.6686(8) 0.3707(7) 0.2206(7) 0.022(2) Uani 1 1 d . . . 
O31 O 0.6714(8) 0.1663(8) 0.3228(6) 0.027(2) Uani 1 1 d . B . 
O32 O 0.8331(8) 0.2497(8) 0.3459(6) 0.025(2) Uani 1 1 d . . . 
O33 O 0.8401(8) 0.3234(9) 0.5017(7) 0.030(2) Uani 1 1 d . . . 
O23W O 0.526(2) 0.144(2) 0.632(2) 0.055(7) Uiso 0.50 1 d P A 2 
O6W O 0.546(2) 0.173(2) 0.5960(18) 0.039(6) Uiso 0.50 1 d P B 1 
O24W O 1.0291(15) -0.216(3) 0.337(2) 0.198(13) Uiso 1 1 d D . . 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Na1 O24W 1.976(10) . ? 
Na1 O20 2.696(12) . ? 
Na1 O11 2.838(12) 1_545 ? 
Na1 O20W 2.85(3) . ? 
K1 O4W 2.611(15) 2_765 ? 
K1 O27 2.720(13) 2_665 ? 
K1 O4 2.740(14) . ? 
K1 O19W 2.758(18) . ? 
K1 O2 3.299(14) . ? 
K1 W1 3.889(10) . ? 
K1 W6 3.917(10) 2_665 ? 
K1 W8 3.961(11) 2_665 ? 
K1 W7 4.137(11) . ? 
W1 O2 1.775(10) . ? 
W1 O3 1.785(9) . ? 
W1 O1 1.786(10) . ? 
W1 O6 2.030(9) . ? 
W1 O4 2.048(9) . ? 
W1 O5 2.316(9) . ? 
W2 O7 1.703(10) . ? 
W2 O6 1.887(10) . ? 
W2 O9 1.921(9) . ? 
W2 O10 1.921(9) . ? 
W2 O8 1.926(9) . ? 
W2 O5 2.383(9) . ? 
W3 O11 1.725(10) . ? 
W3 O14 1.806(9) . ? 
W3 O15 1.920(9) . ? 
W3 O10 1.945(9) . ? 
W3 O13 1.984(9) . ? 
W3 O12 2.327(9) . ? 
W4 O16 1.725(11) . ? 
W4 O18 1.824(10) . ? 
W4 O19 1.902(9) . ? 
W4 O15 1.937(8) . ? 
W4 O17 1.994(9) . ? 
W4 O12 2.313(9) . ? 
W5 O20 1.717(9) . ? 
W5 O22 1.829(9) . ? 
W5 O19 1.920(10) . ? 
W5 O24 1.963(10) . ? 
W5 O21 1.981(9) . ? 
W5 O23 2.334(8) . ? 
W6 O25 1.702(10) . ? 
W6 O26 1.813(9) . ? 
W6 O28 1.914(8) . ? 
W6 O24 1.935(9) . ? 
W6 O27 1.978(10) . ? 
W6 O23 2.346(9) . ? 
W6 K1 3.917(10) 2_665 ? 
W7 O29 1.712(9) . ? 
W7 O4 1.861(9) . ? 
W7 O28 1.906(9) . ? 
W7 O30 1.939(9) . ? 
W7 O8 1.945(10) . ? 
W7 O5 2.409(9) . ? 
W8 O31 1.740(9) . ? 
W8 O32 1.867(10) . ? 
W8 O21 1.901(9) . ? 
W8 O30 1.901(9) . ? 
W8 O27 1.916(11) . ? 
W8 O23 2.346(9) . ? 
W8 K1 3.961(11) 2_665 ? 
W9 O33 1.702(10) . ? 
W9 O13 1.884(9) . ? 
W9 O17 1.906(9) . ? 
W9 O9 1.920(10) . ? 
W9 O32 1.930(10) . ? 
W9 O12 2.329(9) . ? 
Pr1 O10W 2.03(3) 2_656 ? 
Pr1 O8W 2.41(3) . ? 
Pr1 O10W 2.45(3) . ? 
Pr1 O16 2.458(11) 2_756 ? 
Pr1 O7W 2.562(17) . ? 
Pr1 O11W 2.57(3) . ? 
Pr1 O12W 2.59(3) . ? 
Pr1 O9W 2.59(2) . ? 
Pr1 O31 2.605(9) . ? 
Pr1 O6W 2.61(2) . ? 
As1 O5 1.788(8) . ? 
As1 O23 1.799(8) . ? 
As1 O12 1.837(10) . ? 
Fe1 O26 1.918(9) . ? 
Fe1 O3 1.930(9) . ? 
Fe1 O14 1.941(9) 2_765 ? 
Fe1 O1 1.954(10) 2_765 ? 
Fe1 O1W 2.134(10) . ? 
Fe1 O2W 2.144(10) . ? 
Fe2 O22 1.933(9) . ? 
Fe2 O18 1.937(10) . ? 
Fe2 O2 1.988(10) 2_765 ? 
Fe2 O4W 2.064(10) . ? 
Fe2 O3W 2.084(10) . ? 
Fe2 O5W 2.091(11) . ? 
O4W K1 2.611(15) 2_765 ? 
O10W O10W 1.53(6) 2_656 ? 
O10W O12W 1.54(4) 2_656 ? 
O10W Pr1 2.03(3) 2_656 ? 
O12W O10W 1.54(4) 2_656 ? 
O13A O13W 0.90(4) . ? 
O21W O21A 1.37(4) . ? 
O1 Fe1 1.954(10) 2_765 ? 
O2 Fe2 1.988(10) 2_765 ? 
O11 Na1 2.838(12) 1_565 ? 
O14 Fe1 1.941(9) 2_765 ? 
O16 Pr1 2.458(11) 2_756 ? 
O27 K1 2.720(13) 2_665 ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O24W Na1 O20 73.2(10) . . ? 
O24W Na1 O11 72.4(10) . 1_545 ? 
O20 Na1 O11 137.8(4) . 1_545 ? 
O24W Na1 O20W 127.5(13) . . ? 
O20 Na1 O20W 115.7(7) . . ? 
O11 Na1 O20W 104.5(7) 1_545 . ? 
O4W K1 O27 109.4(5) 2_765 2_665 ? 
O4W K1 O4 106.1(5) 2_765 . ? 
O27 K1 O4 130.8(5) 2_665 . ? 
O4W K1 O19W 82.5(4) 2_765 . ? 
O27 K1 O19W 111.4(6) 2_665 . ? 
O4 K1 O19W 106.0(5) . . ? 
O4W K1 O2 54.0(3) 2_765 . ? 
O27 K1 O2 159.0(5) 2_665 . ? 
O4 K1 O2 55.4(3) . . ? 
O19W K1 O2 81.2(4) . . ? 
O4W K1 W1 80.8(3) 2_765 . ? 
O27 K1 W1 159.8(5) 2_665 . ? 
O4 K1 W1 30.1(2) . . ? 
O19W K1 W1 86.8(4) . . ? 
O2 K1 W1 27.04(19) . . ? 
O4W K1 W6 124.6(4) 2_765 2_665 ? 
O27 K1 W6 27.9(2) 2_665 2_665 ? 
O4 K1 W6 103.0(4) . 2_665 ? 
O19W K1 W6 131.8(5) . 2_665 ? 
O2 K1 W6 146.7(4) . 2_665 ? 
W1 K1 W6 132.1(3) . 2_665 ? 
O4W K1 W8 107.4(4) 2_765 2_665 ? 
O27 K1 W8 25.7(3) 2_665 2_665 ? 
O4 K1 W8 145.7(4) . 2_665 ? 
O19W K1 W8 85.6(4) . 2_665 ? 
O2 K1 W8 158.4(4) . 2_665 ? 
W1 K1 W8 167.9(3) . 2_665 ? 
W6 K1 W8 50.44(13) 2_665 2_665 ? 
O4W K1 W7 126.4(4) 2_765 . ? 
O27 K1 W7 112.2(4) 2_665 . ? 
O4 K1 W7 21.0(2) . . ? 
O19W K1 W7 111.1(4) . . ? 
O2 K1 W7 76.4(3) . . ? 
W1 K1 W7 50.36(13) . . ? 
W6 K1 W7 85.3(2) 2_665 . ? 
W8 K1 W7 124.6(3) 2_665 . ? 
O2 W1 O3 101.9(5) . . ? 
O2 W1 O1 103.1(4) . . ? 
O3 W1 O1 98.2(4) . . ? 
O2 W1 O6 97.2(4) . . ? 
O3 W1 O6 157.6(4) . . ? 
O1 W1 O6 88.8(4) . . ? 
O2 W1 O4 96.2(4) . . ? 
O3 W1 O4 86.7(4) . . ? 
O1 W1 O4 158.6(4) . . ? 
O6 W1 O4 79.5(3) . . ? 
O2 W1 O5 165.0(3) . . ? 
O3 W1 O5 87.0(4) . . ? 
O1 W1 O5 87.4(4) . . ? 
O6 W1 O5 72.0(3) . . ? 
O4 W1 O5 72.0(3) . . ? 
O2 W1 K1 57.6(3) . . ? 
O3 W1 K1 80.1(4) . . ? 
O1 W1 K1 159.2(4) . . ? 
O6 W1 K1 100.7(3) . . ? 
O4 W1 K1 42.2(3) . . ? 
O5 W1 K1 113.1(3) . . ? 
O7 W2 O6 101.2(4) . . ? 
O7 W2 O9 101.8(5) . . ? 
O6 W2 O9 156.9(4) . . ? 
O7 W2 O10 100.4(4) . . ? 
O6 W2 O10 92.4(4) . . ? 
O9 W2 O10 85.1(4) . . ? 
O7 W2 O8 98.1(4) . . ? 
O6 W2 O8 89.4(4) . . ? 
O9 W2 O8 85.7(4) . . ? 
O10 W2 O8 160.7(4) . . ? 
O7 W2 O5 171.0(4) . . ? 
O6 W2 O5 72.8(3) . . ? 
O9 W2 O5 84.2(4) . . ? 
O10 W2 O5 86.7(4) . . ? 
O8 W2 O5 75.5(3) . . ? 
O11 W3 O14 104.1(5) . . ? 
O11 W3 O15 99.5(4) . . ? 
O14 W3 O15 96.3(4) . . ? 
O11 W3 O10 101.2(4) . . ? 
O14 W3 O10 90.3(4) . . ? 
O15 W3 O10 156.0(4) . . ? 
O11 W3 O13 97.8(5) . . ? 
O14 W3 O13 157.7(4) . . ? 
O15 W3 O13 84.5(4) . . ? 
O10 W3 O13 80.8(4) . . ? 
O11 W3 O12 169.4(4) . . ? 
O14 W3 O12 84.7(4) . . ? 
O15 W3 O12 73.3(3) . . ? 
O10 W3 O12 84.4(3) . . ? 
O13 W3 O12 74.1(4) . . ? 
O16 W4 O18 102.4(4) . . ? 
O16 W4 O19 101.5(4) . . ? 
O18 W4 O19 89.7(4) . . ? 
O16 W4 O15 100.3(5) . . ? 
O18 W4 O15 90.5(4) . . ? 
O19 W4 O15 157.6(4) . . ? 
O16 W4 O17 95.5(4) . . ? 
O18 W4 O17 162.1(4) . . ? 
O19 W4 O17 86.3(4) . . ? 
O15 W4 O17 86.7(4) . . ? 
O16 W4 O12 166.0(4) . . ? 
O18 W4 O12 90.3(3) . . ? 
O19 W4 O12 84.2(3) . . ? 
O15 W4 O12 73.4(3) . . ? 
O17 W4 O12 71.9(3) . . ? 
O20 W5 O22 103.6(4) . . ? 
O20 W5 O19 101.4(5) . . ? 
O22 W5 O19 88.0(4) . . ? 
O20 W5 O24 99.5(5) . . ? 
O22 W5 O24 91.1(4) . . ? 
O19 W5 O24 158.7(4) . . ? 
O20 W5 O21 98.0(4) . . ? 
O22 W5 O21 158.1(4) . . ? 
O19 W5 O21 84.7(4) . . ? 
O24 W5 O21 88.3(4) . . ? 
O20 W5 O23 168.3(4) . . ? 
O22 W5 O23 86.6(4) . . ? 
O19 W5 O23 84.3(3) . . ? 
O24 W5 O23 74.4(3) . . ? 
O21 W5 O23 72.2(3) . . ? 
O25 W6 O26 103.8(5) . . ? 
O25 W6 O28 101.6(4) . . ? 
O26 W6 O28 91.8(4) . . ? 
O25 W6 O24 99.5(4) . . ? 
O26 W6 O24 94.0(4) . . ? 
O28 W6 O24 156.1(5) . . ? 
O25 W6 O27 96.5(4) . . ? 
O26 W6 O27 159.6(4) . . ? 
O28 W6 O27 82.6(4) . . ? 
O24 W6 O27 84.0(4) . . ? 
O25 W6 O23 169.2(4) . . ? 
O26 W6 O23 85.8(4) . . ? 
O28 W6 O23 82.7(4) . . ? 
O24 W6 O23 74.6(4) . . ? 
O27 W6 O23 74.1(3) . . ? 
O25 W6 K1 65.9(4) . 2_665 ? 
O26 W6 K1 151.6(3) . 2_665 ? 
O28 W6 K1 66.3(3) . 2_665 ? 
O24 W6 K1 113.4(3) . 2_665 ? 
O27 W6 K1 40.1(3) . 2_665 ? 
O23 W6 K1 107.7(3) . 2_665 ? 
O29 W7 O4 102.6(4) . . ? 
O29 W7 O28 102.8(4) . . ? 
O4 W7 O28 93.2(4) . . ? 
O29 W7 O30 100.5(4) . . ? 
O4 W7 O30 156.5(4) . . ? 
O28 W7 O30 85.7(4) . . ? 
O29 W7 O8 98.1(4) . . ? 
O4 W7 O8 87.3(4) . . ? 
O28 W7 O8 158.4(4) . . ? 
O30 W7 O8 85.3(4) . . ? 
O29 W7 O5 171.3(4) . . ? 
O4 W7 O5 72.8(3) . . ? 
O28 W7 O5 85.0(3) . . ? 
O30 W7 O5 83.7(3) . . ? 
O8 W7 O5 74.5(3) . . ? 
O29 W7 K1 73.6(4) . . ? 
O4 W7 K1 31.9(3) . . ? 
O28 W7 K1 86.9(4) . . ? 
O30 W7 K1 169.3(3) . . ? 
O8 W7 K1 104.3(3) . . ? 
O5 W7 K1 103.4(3) . . ? 
O31 W8 O32 100.2(4) . . ? 
O31 W8 O21 101.0(4) . . ? 
O32 W8 O21 91.0(4) . . ? 
O31 W8 O30 103.5(4) . . ? 
O32 W8 O30 88.7(4) . . ? 
O21 W8 O30 155.1(4) . . ? 
O31 W8 O27 100.6(4) . . ? 
O32 W8 O27 159.2(4) . . ? 
O21 W8 O27 86.1(4) . . ? 
O30 W8 O27 85.5(4) . . ? 
O31 W8 O23 172.9(4) . . ? 
O32 W8 O23 84.3(4) . . ? 
O21 W8 O23 73.3(3) . . ? 
O30 W8 O23 81.9(3) . . ? 
O27 W8 O23 75.1(3) . . ? 
O31 W8 K1 71.9(4) . 2_665 ? 
O32 W8 K1 153.3(3) . 2_665 ? 
O21 W8 K1 115.4(3) . 2_665 ? 
O30 W8 K1 69.3(3) . 2_665 ? 
O27 W8 K1 38.0(3) . 2_665 ? 
O23 W8 K1 106.4(3) . 2_665 ? 
O33 W9 O13 99.8(4) . . ? 
O33 W9 O17 101.9(4) . . ? 
O13 W9 O17 87.3(4) . . ? 
O33 W9 O9 102.8(4) . . ? 
O13 W9 O9 85.5(4) . . ? 
O17 W9 O9 155.1(4) . . ? 
O33 W9 O32 101.5(4) . . ? 
O13 W9 O32 158.6(4) . . ? 
O17 W9 O32 90.7(4) . . ? 
O9 W9 O32 87.5(4) . . ? 
O33 W9 O12 173.2(4) . . ? 
O13 W9 O12 75.9(4) . . ? 
O17 W9 O12 73.0(3) . . ? 
O9 W9 O12 82.1(4) . . ? 
O32 W9 O12 83.2(4) . . ? 
O10W Pr1 O8W 157.8(12) 2_656 . ? 
O10W Pr1 O10W 38.6(14) 2_656 . ? 
O8W Pr1 O10W 135.2(10) . . ? 
O10W Pr1 O16 78.8(10) 2_656 2_756 ? 
O8W Pr1 O16 79.3(7) . 2_756 ? 
O10W Pr1 O16 84.6(8) . 2_756 ? 
O10W Pr1 O7W 103.1(9) 2_656 . ? 
O8W Pr1 O7W 93.0(8) . . ? 
O10W Pr1 O7W 77.1(8) . . ? 
O16 Pr1 O7W 145.2(5) 2_756 . ? 
O10W Pr1 O11W 58.4(12) 2_656 . ? 
O8W Pr1 O11W 142.4(10) . . ? 
O10W Pr1 O11W 77.2(10) . . ? 
O16 Pr1 O11W 130.4(7) 2_756 . ? 
O7W Pr1 O11W 74.0(8) . . ? 
O10W Pr1 O12W 36.5(10) 2_656 . ? 
O8W Pr1 O12W 132.3(10) . . ? 
O10W Pr1 O12W 73.5(10) . . ? 
O16 Pr1 O12W 64.8(8) 2_756 . ? 
O7W Pr1 O12W 134.3(8) . . ? 
O11W Pr1 O12W 65.9(10) . . ? 
O10W Pr1 O9W 104.7(10) 2_656 . ? 
O8W Pr1 O9W 71.7(8) . . ? 
O10W Pr1 O9W 141.1(9) . . ? 
O16 Pr1 O9W 72.6(6) 2_756 . ? 
O7W Pr1 O9W 137.2(7) . . ? 
O11W Pr1 O9W 93.8(9) . . ? 
O12W Pr1 O9W 68.4(9) . . ? 
O10W Pr1 O31 124.3(10) 2_656 . ? 
O8W Pr1 O31 75.6(7) . . ? 
O10W Pr1 O31 135.7(8) . . ? 
O16 Pr1 O31 138.6(3) 2_756 . ? 
O7W Pr1 O31 69.0(5) . . ? 
O11W Pr1 O31 66.8(7) . . ? 
O12W Pr1 O31 111.4(8) . . ? 
O9W Pr1 O31 68.5(6) . . ? 
O10W Pr1 O6W 104.7(10) 2_656 . ? 
O8W Pr1 O6W 66.3(9) . . ? 
O10W Pr1 O6W 69.3(9) . . ? 
O16 Pr1 O6W 75.7(6) 2_756 . ? 
O7W Pr1 O6W 70.2(7) . . ? 
O11W Pr1 O6W 135.1(9) . . ? 
O12W Pr1 O6W 127.3(9) . . ? 
O9W Pr1 O6W 131.0(8) . . ? 
O31 Pr1 O6W 121.3(6) . . ? 
O5 As1 O23 97.4(4) . . ? 
O5 As1 O12 98.1(4) . . ? 
O23 As1 O12 96.7(4) . . ? 
O26 Fe1 O3 93.1(4) . . ? 
O26 Fe1 O14 167.4(4) . 2_765 ? 
O3 Fe1 O14 94.4(4) . 2_765 ? 
O26 Fe1 O1 98.0(4) . 2_765 ? 
O3 Fe1 O1 91.9(4) . 2_765 ? 
O14 Fe1 O1 91.9(4) 2_765 2_765 ? 
O26 Fe1 O1W 88.2(4) . . ? 
O3 Fe1 O1W 92.0(4) . . ? 
O14 Fe1 O1W 81.4(4) 2_765 . ? 
O1 Fe1 O1W 172.4(4) 2_765 . ? 
O26 Fe1 O2W 85.3(4) . . ? 
O3 Fe1 O2W 177.5(4) . . ? 
O14 Fe1 O2W 87.6(4) 2_765 . ? 
O1 Fe1 O2W 86.5(4) 2_765 . ? 
O1W Fe1 O2W 89.8(4) . . ? 
O22 Fe2 O18 90.0(4) . . ? 
O22 Fe2 O2 99.8(4) . 2_765 ? 
O18 Fe2 O2 96.7(4) . 2_765 ? 
O22 Fe2 O4W 173.8(4) . . ? 
O18 Fe2 O4W 92.7(4) . . ? 
O2 Fe2 O4W 85.5(4) 2_765 . ? 
O22 Fe2 O3W 91.6(4) . . ? 
O18 Fe2 O3W 90.7(4) . . ? 
O2 Fe2 O3W 166.4(4) 2_765 . ? 
O4W Fe2 O3W 82.8(4) . . ? 
O22 Fe2 O5W 87.7(5) . . ? 
O18 Fe2 O5W 173.9(4) . . ? 
O2 Fe2 O5W 89.3(4) 2_765 . ? 
O4W Fe2 O5W 89.0(5) . . ? 
O3W Fe2 O5W 83.8(5) . . ? 
Fe2 O4W K1 118.7(5) . 2_765 ? 
O10W O10W O12W 158(4) 2_656 2_656 ? 
O10W O10W Pr1 85(2) 2_656 2_656 ? 
O12W O10W Pr1 91.7(18) 2_656 2_656 ? 
O10W O10W Pr1 56(2) 2_656 . ? 
O12W O10W Pr1 124(2) 2_656 . ? 
Pr1 O10W Pr1 141.4(14) 2_656 . ? 
O10W O12W Pr1 51.9(14) 2_656 . ? 
W1 O1 Fe1 179.2(7) . 2_765 ? 
W1 O2 Fe2 165.5(5) . 2_765 ? 
W1 O2 K1 95.3(4) . . ? 
Fe2 O2 K1 96.3(4) 2_765 . ? 
W1 O3 Fe1 169.0(6) . . ? 
W7 O4 W1 122.1(5) . . ? 
W7 O4 K1 127.0(5) . . ? 
W1 O4 K1 107.7(4) . . ? 
As1 O5 W1 114.0(4) . . ? 
As1 O5 W2 129.0(4) . . ? 
W1 O5 W2 93.4(3) . . ? 
As1 O5 W7 128.6(4) . . ? 
W1 O5 W7 92.8(3) . . ? 
W2 O5 W7 89.2(3) . . ? 
W2 O6 W1 121.7(4) . . ? 
W2 O8 W7 120.7(4) . . ? 
W9 O9 W2 146.6(5) . . ? 
W2 O10 W3 146.1(5) . . ? 
W3 O11 Na1 134.5(6) . 1_565 ? 
As1 O12 W4 116.9(4) . . ? 
As1 O12 W3 117.5(4) . . ? 
W4 O12 W3 92.5(3) . . ? 
As1 O12 W9 134.9(5) . . ? 
W4 O12 W9 94.0(3) . . ? 
W3 O12 W9 91.2(3) . . ? 
W9 O13 W3 118.6(5) . . ? 
W3 O14 Fe1 144.0(5) . 2_765 ? 
W3 O15 W4 120.8(5) . . ? 
W4 O16 Pr1 159.2(6) . 2_756 ? 
W9 O17 W4 120.9(5) . . ? 
W4 O18 Fe2 137.7(5) . . ? 
W4 O19 W5 149.4(6) . . ? 
W5 O20 Na1 156.3(6) . . ? 
W8 O21 W5 121.6(4) . . ? 
W5 O22 Fe2 137.1(6) . . ? 
As1 O23 W5 116.7(4) . . ? 
As1 O23 W6 119.1(4) . . ? 
W5 O23 W6 91.8(3) . . ? 
As1 O23 W8 134.8(4) . . ? 
W5 O23 W8 92.8(3) . . ? 
W6 O23 W8 91.4(3) . . ? 
W6 O24 W5 119.2(5) . . ? 
W6 O26 Fe1 146.2(5) . . ? 
W8 O27 W6 119.1(4) . . ? 
W8 O27 K1 116.3(5) . 2_665 ? 
W6 O27 K1 112.0(5) . 2_665 ? 
W7 O28 W6 147.9(6) . . ? 
W8 O30 W7 146.3(5) . . ? 
W8 O31 Pr1 151.6(5) . . ? 
W8 O32 W9 160.0(6) . . ? 
  
_diffrn_measured_fraction_theta_max    0.978 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.978 
_refine_diff_density_max    2.972 
_refine_diff_density_min   -2.459 
_refine_diff_density_rms    0.447 
  


#===END

  
data_3-Nd 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'As2 Fe4 H76 K Na2 Nd O104 W18' 
_chemical_formula_weight          5652.29 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Nd'  'Nd'  -0.1943   3.0179 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.7021(14) 
_cell_length_b                    13.2675(14) 
_cell_length_c                    15.6418(17) 
_cell_angle_alpha                 78.908(2) 
_cell_angle_beta                  88.859(2) 
_cell_angle_gamma                 65.171(2) 
_cell_volume                      2342.2(4) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     7942 
_cell_measurement_theta_min       1.73 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        virgate  
_exptl_crystal_colour             'light yellow' 
_exptl_crystal_size_max           0.53 
_exptl_crystal_size_mid           0.17 
_exptl_crystal_size_min           0.08 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     4.007 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2510 
_exptl_absorpt_coefficient_mu     24.021 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0276 
_exptl_absorpt_correction_T_max   0.2495 
_exptl_absorpt_process_details    SADABS
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             11222 
_diffrn_reflns_av_R_equivalents   0.0349 
_diffrn_reflns_av_sigmaI/netI     0.0715 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -18 
_diffrn_reflns_limit_l_max        13 
_diffrn_reflns_theta_min          1.73 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              7942 
_reflns_number_gt                 6385 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. The K+ and Nd3+ cations 
 are disordered with the site occupancy of 0.5, which are determined 
 according to the mass percentages of K+ and Nd3+ cations from inductively 
 coupled plasma atomic emission spectrometry and their magnitude of
 anisotropic displacement parameters. The ISOR instruction is used for
 O3, O12, O24, O5, O18, O15, O4, O17, O25, O31, O22W, O30 and O23. The 
 DFIX instruction is used for Na1 and O24W. O13W is disordered over two
 positions (O13W and O13A) and O21W is disordered over two positions 
 (O21W and O21A). The O6W, O7W, O8W, O9W, O10W, O11W, O13W, O13A, O14W, 
 O15W, O17W, O20W, O21W, O21A, O23W and O24W are refined isostropicallly. 
 577 parameters and 79 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1114P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    notdet 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          7942 
_refine_ls_number_parameters      577 
_refine_ls_number_restraints      79 
_refine_ls_R_factor_all           0.0737 
_refine_ls_R_factor_gt            0.0599 
_refine_ls_wR_factor_ref          0.1738 
_refine_ls_wR_factor_gt           0.1658 
_refine_ls_goodness_of_fit_ref    1.067 
_refine_ls_restrained_S_all       1.063 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Na1 Na 1.1901(8) -0.2917(7) 0.3046(6) 0.042(2) Uani 1 1 d D . . 
K1 K 0.5059(11) 0.7391(13) -0.1059(11) 0.074(4) Uani 0.50 1 d P . . 
W1 W 0.79468(6) 0.62776(6) 0.03501(5) 0.0167(2) Uani 1 1 d . . . 
W2 W 0.74298(6) 0.60604(6) 0.25143(6) 0.0201(2) Uani 1 1 d . . . 
W3 W 1.05785(6) 0.46186(6) 0.31715(5) 0.0183(2) Uani 1 1 d . . . 
W4 W 1.15937(6) 0.18087(6) 0.33359(6) 0.0203(2) Uani 1 1 d . . . 
W5 W 1.02803(6) 0.06620(6) 0.19189(6) 0.0215(2) Uani 1 1 d . . . 
W6 W 0.80402(6) 0.23974(6) 0.04675(6) 0.0195(2) Uani 1 1 d . . . 
W7 W 0.62286(6) 0.49937(6) 0.12422(6) 0.0185(2) Uani 1 1 d . . . 
W8 W 0.76273(6) 0.21288(6) 0.26082(6) 0.0197(2) Uani 1 1 d . . . 
W9 W 0.89510(6) 0.33186(6) 0.40296(6) 0.0195(2) Uani 1 1 d . . . 
Nd1 Nd 0.62381(17) 0.06657(17) 0.46797(16) 0.0240(5) Uani 0.50 1 d P . . 
As1 As 0.95153(14) 0.35956(14) 0.15934(13) 0.0157(4) Uani 1 1 d . . . 
Fe1 Fe 0.9069(2) 0.4126(2) -0.10263(19) 0.0183(6) Uani 1 1 d . . . 
Fe2 Fe 1.2759(2) 0.1112(2) 0.1368(2) 0.0210(6) Uani 1 1 d . . . 
O1W O 0.7434(12) 0.4397(12) -0.1621(11) 0.034(4) Uani 1 1 d . . . 
O2W O 0.9931(12) 0.2820(11) -0.1753(11) 0.035(4) Uani 1 1 d . . . 
O3W O 1.3344(12) -0.0435(11) 0.2252(12) 0.037(4) Uani 1 1 d . . . 
O4W O 1.4458(11) 0.0869(12) 0.1544(11) 0.037(4) Uani 1 1 d . . . 
O5W O 1.3276(14) 0.0079(14) 0.0458(12) 0.045(4) Uani 1 1 d . . . 
O7W O 0.459(2) 0.260(2) 0.4123(18) 0.021(6) Uiso 0.50 1 d P B . 
O8W O 0.744(3) 0.149(3) 0.514(2) 0.051(9) Uiso 0.50 1 d P B . 
O9W O 0.830(3) -0.049(2) 0.430(2) 0.034(7) Uiso 0.50 1 d P B . 
O10W O 0.453(3) 0.042(3) 0.526(3) 0.051(9) Uiso 0.50 1 d P . . 
O11W O 0.529(3) 0.047(3) 0.333(3) 0.065(11) Uiso 0.50 1 d P B . 
O12W O 0.664(4) -0.139(4) 0.467(3) 0.078(13) Uiso 0.50 1 d P . . 
O13W O 1.058(3) -0.055(3) 0.436(3) 0.142(12) Uiso 1 1 d . . . 
O14W O 0.797(5) -0.090(5) 0.251(4) 0.111(18) Uiso 0.50 1 d P . . 
O15W O 0.571(3) 0.435(2) 0.395(2) 0.113(9) Uiso 1 1 d . . . 
O16W O 1.1082(13) 0.0886(12) -0.0568(11) 0.038(4) Uani 1 1 d . . . 
O17W O 0.695(2) 0.578(2) 0.506(2) 0.110(9) Uiso 1 1 d . . . 
O18W O 0.6261(16) 0.2460(15) -0.1956(16) 0.072(7) Uani 1 1 d . . . 
O19W O 0.6377(14) 0.6655(14) -0.2428(15) 0.062(6) Uani 1 1 d . . . 
O20W O 1.400(5) -0.362(5) 0.418(5) 0.125 Uiso 0.50 1 d P . . 
O21W O 0.561(4) -0.095(4) 0.078(3) 0.077(12) Uiso 0.50 1 d P . . 
O21A O 0.649(5) -0.075(5) 0.145(4) 0.108(18) Uiso 0.50 1 d P . . 
O22W O 1.1361(13) 0.3058(13) 0.5630(11) 0.039(4) Uani 1 1 d U . . 
O1 O 0.9363(10) 0.6090(10) 0.0663(8) 0.016(3) Uani 1 1 d . . . 
O2 O 0.7416(11) 0.7563(10) -0.0419(11) 0.034(4) Uani 1 1 d . . . 
O3 O 0.8352(11) 0.5253(10) -0.0302(9) 0.023(3) Uani 1 1 d U . . 
O4 O 0.6399(10) 0.6141(10) 0.0425(9) 0.020(3) Uani 1 1 d U . . 
O5 O 0.8155(9) 0.4833(9) 0.1513(8) 0.013(2) Uani 1 1 d U . . 
O6 O 0.7366(10) 0.6969(10) 0.1427(10) 0.023(3) Uani 1 1 d . . . 
O7 O 0.6745(11) 0.7077(11) 0.3105(10) 0.029(3) Uani 1 1 d . . . 
O8 O 0.6104(10) 0.5861(10) 0.2145(10) 0.024(3) Uani 1 1 d . . . 
O9 O 0.7756(11) 0.4682(11) 0.3389(10) 0.030(4) Uani 1 1 d . . . 
O10 O 0.9010(10) 0.5772(10) 0.2758(10) 0.023(3) Uani 1 1 d . . . 
O11 O 1.1134(12) 0.5378(10) 0.3633(11) 0.034(4) Uani 1 1 d . . . 
O12 O 0.9903(10) 0.3390(10) 0.2739(10) 0.024(3) Uani 1 1 d U . . 
O13 O 0.9734(10) 0.4215(10) 0.4169(8) 0.019(3) Uani 1 1 d . . . 
O14 O 1.1016(11) 0.4764(10) 0.2063(9) 0.020(3) Uani 1 1 d . . . 
O15 O 1.1761(11) 0.3120(10) 0.3596(10) 0.027(3) Uani 1 1 d U . . 
O16 O 1.2706(11) 0.0702(11) 0.4005(11) 0.033(4) Uani 1 1 d . . . 
O17 O 1.0435(10) 0.2044(10) 0.4253(8) 0.018(3) Uani 1 1 d U . . 
O18 O 1.2271(10) 0.1943(10) 0.2274(9) 0.020(3) Uani 1 1 d U . . 
O19 O 1.0878(10) 0.0996(10) 0.2898(10) 0.023(3) Uani 1 1 d . . . 
O20 O 1.1014(12) -0.0790(10) 0.2113(11) 0.036(4) Uani 1 1 d . . . 
O21 O 0.8960(11) 0.0726(11) 0.2680(9) 0.024(3) Uani 1 1 d . . . 
O22 O 1.1223(11) 0.1146(11) 0.1236(9) 0.025(3) Uani 1 1 d . . . 
O23 O 0.8932(9) 0.2540(9) 0.1704(9) 0.016(3) Uani 1 1 d U . . 
O24 O 0.9296(10) 0.0878(10) 0.0903(9) 0.021(3) Uani 1 1 d U . . 
O25 O 0.7359(10) 0.2091(10) -0.0323(9) 0.021(3) Uani 1 1 d U . . 
O26 O 0.8981(11) 0.2920(10) -0.0151(10) 0.027(3) Uani 1 1 d . . . 
O27 O 0.7241(10) 0.1971(10) 0.1464(9) 0.023(3) Uani 1 1 d . . . 
O28 O 0.6942(10) 0.3902(10) 0.0549(9) 0.017(3) Uani 1 1 d . . . 
O29 O 0.4793(11) 0.5335(10) 0.1062(9) 0.022(3) Uani 1 1 d . . . 
O30 O 0.6660(10) 0.3724(10) 0.2214(9) 0.022(3) Uani 1 1 d U . . 
O31 O 0.6725(11) 0.1655(11) 0.3239(9) 0.026(3) Uani 1 1 d U B . 
O32 O 0.8350(10) 0.2461(10) 0.3477(9) 0.021(3) Uani 1 1 d . . . 
O33 O 0.8401(12) 0.3221(12) 0.5029(10) 0.035(4) Uani 1 1 d . . . 
O23W O 0.527(3) 0.143(3) 0.638(3) 0.042(8) Uiso 0.50 1 d P A 2 
O6W O 0.544(3) 0.175(3) 0.592(3) 0.051(9) Uiso 0.50 1 d P B 1 
O24W O 1.0305(19) -0.220(3) 0.345(3) 0.178(16) Uiso 1 1 d D . . 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Na1 O24W 1.993(10) . ? 
Na1 O20 2.678(15) . ? 
Na1 O11 2.815(15) 1_545 ? 
Na1 O20W 2.92(6) . ? 
Na1 O33 3.000(19) 2_756 ? 
K1 O4W 2.60(2) 2_765 ? 
K1 O4 2.710(19) . ? 
K1 O27 2.729(17) 2_665 ? 
K1 O19W 2.76(3) . ? 
K1 O2 3.286(18) . ? 
K1 W1 3.875(13) . ? 
K1 W6 3.932(13) 2_665 ? 
K1 W8 3.979(13) 2_665 ? 
K1 Fe2 4.007(14) 2_765 ? 
K1 W7 4.138(15) . ? 
W1 O3 1.754(13) . ? 
W1 O2 1.757(14) . ? 
W1 O1 1.775(11) . ? 
W1 O4 2.048(12) . ? 
W1 O6 2.050(13) . ? 
W1 O5 2.304(12) . ? 
W2 O7 1.700(15) . ? 
W2 O6 1.867(14) . ? 
W2 O10 1.910(11) . ? 
W2 O8 1.927(12) . ? 
W2 O9 1.953(13) . ? 
W2 O5 2.370(12) . ? 
W3 O11 1.712(13) . ? 
W3 O14 1.810(13) . ? 
W3 O15 1.916(12) . ? 
W3 O10 1.960(12) . ? 
W3 O13 1.992(13) . ? 
W3 O12 2.339(12) . ? 
W4 O16 1.724(13) . ? 
W4 O18 1.869(13) . ? 
W4 O19 1.894(13) . ? 
W4 O15 1.956(12) . ? 
W4 O17 2.006(13) . ? 
W4 O12 2.329(12) . ? 
W5 O20 1.718(12) . ? 
W5 O22 1.822(13) . ? 
W5 O19 1.926(14) . ? 
W5 O24 1.943(12) . ? 
W5 O21 2.018(13) . ? 
W5 O23 2.318(11) . ? 
W6 O25 1.724(13) . ? 
W6 O26 1.798(14) . ? 
W6 O28 1.923(12) . ? 
W6 O27 1.965(14) . ? 
W6 O24 1.971(12) . ? 
W6 O23 2.338(12) . ? 
W6 K1 3.932(13) 2_665 ? 
W7 O29 1.700(12) . ? 
W7 O4 1.874(12) . ? 
W7 O28 1.886(12) . ? 
W7 O30 1.929(12) . ? 
W7 O8 1.951(14) . ? 
W7 O5 2.404(11) . ? 
W8 O31 1.733(13) . ? 
W8 O32 1.871(13) . ? 
W8 O21 1.904(13) . ? 
W8 O30 1.927(11) . ? 
W8 O27 1.937(14) . ? 
W8 O23 2.327(12) . ? 
W8 K1 3.979(13) 2_665 ? 
W9 O33 1.703(16) . ? 
W9 O13 1.885(12) . ? 
W9 O9 1.907(12) . ? 
W9 O17 1.912(12) . ? 
W9 O32 1.939(13) . ? 
W9 O12 2.339(15) . ? 
Nd1 O10W 2.04(3) 2_656 ? 
Nd1 O8W 2.41(3) . ? 
Nd1 O16 2.440(15) 2_756 ? 
Nd1 O10W 2.46(3) . ? 
Nd1 O7W 2.53(2) . ? 
Nd1 O9W 2.55(3) . ? 
Nd1 O12W 2.56(4) . ? 
Nd1 O11W 2.57(4) . ? 
Nd1 O6W 2.58(4) . ? 
Nd1 O31 2.584(14) . ? 
As1 O5 1.801(11) . ? 
As1 O12 1.806(15) . ? 
As1 O23 1.820(11) . ? 
Fe1 O26 1.937(14) . ? 
Fe1 O14 1.940(13) 2_765 ? 
Fe1 O3 1.953(14) . ? 
Fe1 O1 1.968(12) 2_765 ? 
Fe1 O2W 2.147(15) . ? 
Fe1 O1W 2.152(13) . ? 
Fe2 O18 1.897(14) . ? 
Fe2 O22 1.947(12) . ? 
Fe2 O2 2.005(14) 2_765 ? 
Fe2 O4W 2.059(13) . ? 
Fe2 O5W 2.070(17) . ? 
Fe2 O3W 2.085(14) . ? 
Fe2 K1 4.007(14) 2_765 ? 
O4W K1 2.60(2) 2_765 ? 
O10W O12W 1.52(5) 2_656 ? 
O10W O10W 1.60(7) 2_656 ? 
O10W Nd1 2.04(3) 2_656 ? 
O12W O10W 1.52(5) 2_656 ? 
O21W O21A 1.68(7) . ? 
O1 Fe1 1.968(12) 2_765 ? 
O2 Fe2 2.005(14) 2_765 ? 
O11 Na1 2.814(15) 1_565 ? 
O14 Fe1 1.940(13) 2_765 ? 
O16 Nd1 2.440(15) 2_756 ? 
O27 K1 2.729(17) 2_665 ? 
O33 Na1 3.000(19) 2_756 ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O24W Na1 O20 75.6(12) . . ? 
O24W Na1 O11 71.6(12) . 1_545 ? 
O20 Na1 O11 137.6(5) . 1_545 ? 
O24W Na1 O20W 122.6(19) . . ? 
O20 Na1 O20W 116.7(13) . . ? 
O11 Na1 O20W 103.5(13) 1_545 . ? 
O24W Na1 O33 61.5(13) . 2_756 ? 
O20 Na1 O33 117.2(6) . 2_756 ? 
O11 Na1 O33 68.2(5) 1_545 2_756 ? 
O20W Na1 O33 64.0(14) . 2_756 ? 
O4W K1 O4 106.9(6) 2_765 . ? 
O4W K1 O27 109.3(6) 2_765 2_665 ? 
O4 K1 O27 130.3(7) . 2_665 ? 
O4W K1 O19W 82.8(7) 2_765 . ? 
O4 K1 O19W 106.4(7) . . ? 
O27 K1 O19W 110.9(8) 2_665 . ? 
O4W K1 O2 54.7(4) 2_765 . ? 
O4 K1 O2 55.3(4) . . ? 
O27 K1 O2 158.9(7) 2_665 . ? 
O19W K1 O2 82.4(6) . . ? 
O4W K1 W1 81.4(4) 2_765 . ? 
O4 K1 W1 30.1(3) . . ? 
O27 K1 W1 159.2(7) 2_665 . ? 
O19W K1 W1 87.7(5) . . ? 
O2 K1 W1 26.8(3) . . ? 
O4W K1 W6 124.3(6) 2_765 2_665 ? 
O4 K1 W6 103.0(5) . 2_665 ? 
O27 K1 W6 27.4(3) 2_665 2_665 ? 
O19W K1 W6 131.0(6) . 2_665 ? 
O2 K1 W6 146.3(6) . 2_665 ? 
W1 K1 W6 132.0(4) . 2_665 ? 
O4W K1 W8 107.3(5) 2_765 2_665 ? 
O4 K1 W8 145.1(5) . 2_665 ? 
O27 K1 W8 25.9(4) 2_665 2_665 ? 
O19W K1 W8 85.0(6) . 2_665 ? 
O2 K1 W8 159.2(6) . 2_665 ? 
W1 K1 W8 167.8(5) . 2_665 ? 
W6 K1 W8 50.15(15) 2_665 2_665 ? 
O4W K1 Fe2 27.0(3) 2_765 2_765 ? 
O4 K1 Fe2 85.0(4) . 2_765 ? 
O27 K1 Fe2 136.2(5) 2_665 2_765 ? 
O19W K1 Fe2 73.6(5) . 2_765 ? 
O2 K1 Fe2 29.9(3) . 2_765 ? 
W1 K1 Fe2 56.49(18) . 2_765 ? 
W6 K1 Fe2 147.8(5) 2_665 2_765 ? 
W8 K1 Fe2 129.8(4) 2_665 2_765 ? 
O4W K1 W7 126.8(6) 2_765 . ? 
O4 K1 W7 20.9(3) . . ? 
O27 K1 W7 111.5(5) 2_665 . ? 
O19W K1 W7 111.9(6) . . ? 
O2 K1 W7 76.1(4) . . ? 
W1 K1 W7 50.40(17) . . ? 
W6 K1 W7 85.1(3) 2_665 . ? 
W8 K1 W7 124.2(3) 2_665 . ? 
Fe2 K1 W7 105.9(3) 2_765 . ? 
O3 W1 O2 103.2(7) . . ? 
O3 W1 O1 97.9(6) . . ? 
O2 W1 O1 102.9(6) . . ? 
O3 W1 O4 86.1(6) . . ? 
O2 W1 O4 95.7(5) . . ? 
O1 W1 O4 159.4(5) . . ? 
O3 W1 O6 157.2(6) . . ? 
O2 W1 O6 96.7(6) . . ? 
O1 W1 O6 88.4(5) . . ? 
O4 W1 O6 80.8(5) . . ? 
O3 W1 O5 86.7(5) . . ? 
O2 W1 O5 164.2(5) . . ? 
O1 W1 O5 87.7(5) . . ? 
O4 W1 O5 72.4(4) . . ? 
O6 W1 O5 71.6(5) . . ? 
O3 W1 K1 80.7(5) . . ? 
O2 W1 K1 57.6(5) . . ? 
O1 W1 K1 158.9(5) . . ? 
O4 W1 K1 41.6(4) . . ? 
O6 W1 K1 101.1(4) . . ? 
O5 W1 K1 113.2(4) . . ? 
O7 W2 O6 100.1(6) . . ? 
O7 W2 O10 100.2(6) . . ? 
O6 W2 O10 91.6(6) . . ? 
O7 W2 O8 98.8(6) . . ? 
O6 W2 O8 90.6(6) . . ? 
O10 W2 O8 160.3(5) . . ? 
O7 W2 O9 101.2(7) . . ? 
O6 W2 O9 158.6(6) . . ? 
O10 W2 O9 85.9(5) . . ? 
O8 W2 O9 85.0(5) . . ? 
O7 W2 O5 170.9(5) . . ? 
O6 W2 O5 73.1(5) . . ? 
O10 W2 O5 86.3(5) . . ? 
O8 W2 O5 75.6(5) . . ? 
O9 W2 O5 85.5(6) . . ? 
O11 W3 O14 103.0(7) . . ? 
O11 W3 O15 99.4(6) . . ? 
O14 W3 O15 96.6(6) . . ? 
O11 W3 O10 101.5(5) . . ? 
O14 W3 O10 89.5(6) . . ? 
O15 W3 O10 156.3(5) . . ? 
O11 W3 O13 99.3(7) . . ? 
O14 W3 O13 157.3(5) . . ? 
O15 W3 O13 83.8(6) . . ? 
O10 W3 O13 82.0(5) . . ? 
O11 W3 O12 171.5(6) . . ? 
O14 W3 O12 83.6(5) . . ? 
O15 W3 O12 74.3(5) . . ? 
O10 W3 O12 83.7(5) . . ? 
O13 W3 O12 74.6(5) . . ? 
O16 W4 O18 103.1(6) . . ? 
O16 W4 O19 99.8(6) . . ? 
O18 W4 O19 89.3(6) . . ? 
O16 W4 O15 101.6(6) . . ? 
O18 W4 O15 91.3(6) . . ? 
O19 W4 O15 157.9(5) . . ? 
O16 W4 O17 94.6(6) . . ? 
O18 W4 O17 162.2(5) . . ? 
O19 W4 O17 86.7(6) . . ? 
O15 W4 O17 86.1(6) . . ? 
O16 W4 O12 166.6(6) . . ? 
O18 W4 O12 89.6(5) . . ? 
O19 W4 O12 84.0(5) . . ? 
O15 W4 O12 73.9(5) . . ? 
O17 W4 O12 72.7(5) . . ? 
O20 W5 O22 103.7(7) . . ? 
O20 W5 O19 101.0(6) . . ? 
O22 W5 O19 88.3(6) . . ? 
O20 W5 O24 98.8(6) . . ? 
O22 W5 O24 91.2(6) . . ? 
O19 W5 O24 159.8(5) . . ? 
O20 W5 O21 96.6(6) . . ? 
O22 W5 O21 159.3(5) . . ? 
O19 W5 O21 84.2(5) . . ? 
O24 W5 O21 89.3(5) . . ? 
O20 W5 O23 167.4(5) . . ? 
O22 W5 O23 87.6(5) . . ? 
O19 W5 O23 84.7(5) . . ? 
O24 W5 O23 75.1(4) . . ? 
O21 W5 O23 72.5(5) . . ? 
O25 W6 O26 102.6(6) . . ? 
O25 W6 O28 102.2(5) . . ? 
O26 W6 O28 92.3(5) . . ? 
O25 W6 O27 97.3(6) . . ? 
O26 W6 O27 160.0(6) . . ? 
O28 W6 O27 82.3(5) . . ? 
O25 W6 O24 99.6(5) . . ? 
O26 W6 O24 94.0(5) . . ? 
O28 W6 O24 155.4(6) . . ? 
O27 W6 O24 83.8(5) . . ? 
O25 W6 O23 169.7(5) . . ? 
O26 W6 O23 86.1(6) . . ? 
O28 W6 O23 82.6(5) . . ? 
O27 W6 O23 74.2(5) . . ? 
O24 W6 O23 74.1(4) . . ? 
O25 W6 K1 66.9(5) . 2_665 ? 
O26 W6 K1 151.9(4) . 2_665 ? 
O28 W6 K1 66.4(4) . 2_665 ? 
O27 W6 K1 39.8(4) . 2_665 ? 
O24 W6 K1 113.1(4) . 2_665 ? 
O23 W6 K1 107.7(4) . 2_665 ? 
O29 W7 O4 101.2(6) . . ? 
O29 W7 O28 102.6(6) . . ? 
O4 W7 O28 92.7(5) . . ? 
O29 W7 O30 101.1(6) . . ? 
O4 W7 O30 157.4(5) . . ? 
O28 W7 O30 85.9(6) . . ? 
O29 W7 O8 98.5(6) . . ? 
O4 W7 O8 89.1(6) . . ? 
O28 W7 O8 158.0(5) . . ? 
O30 W7 O8 84.1(6) . . ? 
O29 W7 O5 170.6(5) . . ? 
O4 W7 O5 72.9(5) . . ? 
O28 W7 O5 85.2(4) . . ? 
O30 W7 O5 84.5(4) . . ? 
O8 W7 O5 74.4(4) . . ? 
O29 W7 K1 72.6(5) . . ? 
O4 W7 K1 31.0(4) . . ? 
O28 W7 K1 87.3(5) . . ? 
O30 W7 K1 169.5(4) . . ? 
O8 W7 K1 104.9(5) . . ? 
O5 W7 K1 102.9(3) . . ? 
O31 W8 O32 99.5(6) . . ? 
O31 W8 O21 99.6(6) . . ? 
O32 W8 O21 89.2(5) . . ? 
O31 W8 O30 103.1(6) . . ? 
O32 W8 O30 89.8(5) . . ? 
O21 W8 O30 157.1(5) . . ? 
O31 W8 O27 100.9(6) . . ? 
O32 W8 O27 159.6(5) . . ? 
O21 W8 O27 87.4(6) . . ? 
O30 W8 O27 85.7(5) . . ? 
O31 W8 O23 172.5(5) . . ? 
O32 W8 O23 84.8(5) . . ? 
O21 W8 O23 74.3(5) . . ? 
O30 W8 O23 82.9(5) . . ? 
O27 W8 O23 75.0(5) . . ? 
O31 W8 K1 72.1(5) . 2_665 ? 
O32 W8 K1 154.2(4) . 2_665 ? 
O21 W8 K1 116.0(5) . 2_665 ? 
O30 W8 K1 69.3(4) . 2_665 ? 
O27 W8 K1 38.1(4) . 2_665 ? 
O23 W8 K1 106.5(4) . 2_665 ? 
O33 W9 O13 99.5(6) . . ? 
O33 W9 O9 101.6(7) . . ? 
O13 W9 O9 86.2(5) . . ? 
O33 W9 O17 101.0(6) . . ? 
O13 W9 O17 86.8(5) . . ? 
O9 W9 O17 157.2(6) . . ? 
O33 W9 O32 101.0(6) . . ? 
O13 W9 O32 159.5(6) . . ? 
O9 W9 O32 88.9(5) . . ? 
O17 W9 O32 90.2(5) . . ? 
O33 W9 O12 173.7(5) . . ? 
O13 W9 O12 76.5(5) . . ? 
O9 W9 O12 83.2(6) . . ? 
O17 W9 O12 74.1(5) . . ? 
O32 W9 O12 83.2(5) . . ? 
O10W Nd1 O8W 158.5(13) 2_656 . ? 
O10W Nd1 O16 81.0(11) 2_656 2_756 ? 
O8W Nd1 O16 77.7(9) . 2_756 ? 
O10W Nd1 O10W 40.2(17) 2_656 . ? 
O8W Nd1 O10W 133.4(13) . . ? 
O16 Nd1 O10W 85.0(9) 2_756 . ? 
O10W Nd1 O7W 103.6(11) 2_656 . ? 
O8W Nd1 O7W 91.9(10) . . ? 
O16 Nd1 O7W 144.0(7) 2_756 . ? 
O10W Nd1 O7W 77.4(10) . . ? 
O10W Nd1 O9W 103.5(11) 2_656 . ? 
O8W Nd1 O9W 73.0(11) . . ? 
O16 Nd1 O9W 72.3(8) 2_756 . ? 
O10W Nd1 O9W 140.9(10) . . ? 
O7W Nd1 O9W 137.7(9) . . ? 
O10W Nd1 O12W 36.4(13) 2_656 . ? 
O8W Nd1 O12W 132.0(13) . . ? 
O16 Nd1 O12W 65.3(11) 2_756 . ? 
O10W Nd1 O12W 74.1(13) . . ? 
O7W Nd1 O12W 135.9(11) . . ? 
O9W Nd1 O12W 67.6(12) . . ? 
O10W Nd1 O11W 57.4(14) 2_656 . ? 
O8W Nd1 O11W 143.0(13) . . ? 
O16 Nd1 O11W 132.2(10) 2_756 . ? 
O10W Nd1 O11W 77.9(13) . . ? 
O7W Nd1 O11W 74.4(11) . . ? 
O9W Nd1 O11W 94.0(11) . . ? 
O12W Nd1 O11W 67.2(14) . . ? 
O10W Nd1 O6W 106.0(13) 2_656 . ? 
O8W Nd1 O6W 65.8(12) . . ? 
O16 Nd1 O6W 76.1(9) 2_756 . ? 
O10W Nd1 O6W 68.1(12) . . ? 
O7W Nd1 O6W 68.2(10) . . ? 
O9W Nd1 O6W 132.2(11) . . ? 
O12W Nd1 O6W 127.5(14) . . ? 
O11W Nd1 O6W 133.6(12) . . ? 
O10W Nd1 O31 123.5(11) 2_656 . ? 
O8W Nd1 O31 75.7(10) . . ? 
O16 Nd1 O31 137.5(4) 2_756 . ? 
O10W Nd1 O31 136.8(9) . . ? 
O7W Nd1 O31 69.4(7) . . ? 
O9W Nd1 O31 68.6(7) . . ? 
O12W Nd1 O31 112.2(11) . . ? 
O11W Nd1 O31 67.3(10) . . ? 
O6W Nd1 O31 120.3(9) . . ? 
O5 As1 O12 98.4(6) . . ? 
O5 As1 O23 97.9(5) . . ? 
O12 As1 O23 96.9(6) . . ? 
O26 Fe1 O14 167.9(6) . 2_765 ? 
O26 Fe1 O3 92.7(6) . . ? 
O14 Fe1 O3 94.3(5) 2_765 . ? 
O26 Fe1 O1 97.7(5) . 2_765 ? 
O14 Fe1 O1 92.0(5) 2_765 2_765 ? 
O3 Fe1 O1 91.5(5) . 2_765 ? 
O26 Fe1 O2W 85.0(6) . . ? 
O14 Fe1 O2W 88.4(6) 2_765 . ? 
O3 Fe1 O2W 176.4(6) . . ? 
O1 Fe1 O2W 86.1(5) 2_765 . ? 
O26 Fe1 O1W 88.8(6) . . ? 
O14 Fe1 O1W 81.0(6) 2_765 . ? 
O3 Fe1 O1W 93.9(6) . . ? 
O1 Fe1 O1W 171.4(6) 2_765 . ? 
O2W Fe1 O1W 88.8(6) . . ? 
O18 Fe2 O22 90.5(6) . . ? 
O18 Fe2 O2 96.2(6) . 2_765 ? 
O22 Fe2 O2 99.6(5) . 2_765 ? 
O18 Fe2 O4W 92.8(6) . . ? 
O22 Fe2 O4W 173.2(6) . . ? 
O2 Fe2 O4W 86.0(6) 2_765 . ? 
O18 Fe2 O5W 174.6(6) . . ? 
O22 Fe2 O5W 87.4(6) . . ? 
O2 Fe2 O5W 89.1(7) 2_765 . ? 
O4W Fe2 O5W 88.7(7) . . ? 
O18 Fe2 O3W 92.1(6) . . ? 
O22 Fe2 O3W 91.3(6) . . ? 
O2 Fe2 O3W 166.2(6) 2_765 . ? 
O4W Fe2 O3W 82.6(6) . . ? 
O5W Fe2 O3W 82.9(7) . . ? 
O18 Fe2 K1 81.9(4) . 2_765 ? 
O22 Fe2 K1 151.7(4) . 2_765 ? 
O2 Fe2 K1 54.7(4) 2_765 2_765 ? 
O4W Fe2 K1 35.0(4) . 2_765 ? 
O5W Fe2 K1 102.3(5) . 2_765 ? 
O3W Fe2 K1 116.0(4) . 2_765 ? 
Fe2 O4W K1 118.0(6) . 2_765 ? 
O12W O10W O10W 152(4) 2_656 2_656 ? 
O12W O10W Nd1 91(2) 2_656 2_656 ? 
O10W O10W Nd1 84(2) 2_656 2_656 ? 
O12W O10W Nd1 124(2) 2_656 . ? 
O10W O10W Nd1 56(2) 2_656 . ? 
Nd1 O10W Nd1 139.8(17) 2_656 . ? 
O10W O12W Nd1 52.8(18) 2_656 . ? 
W1 O1 Fe1 179.2(8) . 2_765 ? 
W1 O2 Fe2 165.3(8) . 2_765 ? 
W1 O2 K1 95.6(5) . . ? 
Fe2 O2 K1 95.4(6) 2_765 . ? 
W1 O3 Fe1 169.8(8) . . ? 
W7 O4 W1 121.3(6) . . ? 
W7 O4 K1 128.1(6) . . ? 
W1 O4 K1 108.2(6) . . ? 
As1 O5 W1 114.2(6) . . ? 
As1 O5 W2 128.5(6) . . ? 
W1 O5 W2 93.9(4) . . ? 
As1 O5 W7 128.1(6) . . ? 
W1 O5 W7 93.2(4) . . ? 
W2 O5 W7 89.6(4) . . ? 
W2 O6 W1 121.3(6) . . ? 
W2 O8 W7 120.3(6) . . ? 
W9 O9 W2 144.9(7) . . ? 
W2 O10 W3 146.0(7) . . ? 
W3 O11 Na1 137.0(9) . 1_565 ? 
As1 O12 W4 117.4(7) . . ? 
As1 O12 W9 135.3(6) . . ? 
W4 O12 W9 93.2(5) . . ? 
As1 O12 W3 118.1(6) . . ? 
W4 O12 W3 91.8(4) . . ? 
W9 O12 W3 90.5(5) . . ? 
W9 O13 W3 118.0(7) . . ? 
W3 O14 Fe1 143.1(7) . 2_765 ? 
W3 O15 W4 119.9(6) . . ? 
W4 O16 Nd1 159.8(8) . 2_756 ? 
W9 O17 W4 119.9(6) . . ? 
W4 O18 Fe2 137.1(7) . . ? 
W4 O19 W5 149.5(8) . . ? 
W5 O20 Na1 157.2(10) . . ? 
W8 O21 W5 119.3(6) . . ? 
W5 O22 Fe2 136.9(8) . . ? 
As1 O23 W5 116.4(5) . . ? 
As1 O23 W8 134.2(6) . . ? 
W5 O23 W8 93.6(4) . . ? 
As1 O23 W6 118.6(6) . . ? 
W5 O23 W6 92.4(4) . . ? 
W8 O23 W6 91.9(4) . . ? 
W5 O24 W6 118.3(6) . . ? 
W6 O26 Fe1 146.0(7) . . ? 
W8 O27 W6 118.5(6) . . ? 
W8 O27 K1 116.0(7) . 2_665 ? 
W6 O27 K1 112.8(6) . 2_665 ? 
W7 O28 W6 148.9(8) . . ? 
W8 O30 W7 145.0(8) . . ? 
W8 O31 Nd1 152.4(7) . . ? 
W8 O32 W9 158.0(7) . . ? 
W9 O33 Na1 164.2(7) . 2_756 ? 
  
_diffrn_measured_fraction_theta_max    0.963 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.963 
_refine_diff_density_max    3.960 
_refine_diff_density_min   -3.374 
_refine_diff_density_rms    0.580 
  


#===END

  
data_4-Sm 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'As2 Fe4 H76 K Na2 O104 Sm W18' 
_chemical_formula_weight          5658.58 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Sm'  'Sm'  -0.1638   3.4418 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Na'  'Na'   0.0362   0.0249 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'K'  'K'   0.2009   0.2494 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.671(5) 
_cell_length_b                    13.247(5) 
_cell_length_c                    15.610(6) 
_cell_angle_alpha                 78.699(6) 
_cell_angle_beta                  88.927(6) 
_cell_angle_gamma                 65.208(6) 
_cell_volume                      2326.6(16) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8031  
_cell_measurement_theta_min       1.73 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        virgate  
_exptl_crystal_colour             'light yellow' 
_exptl_crystal_size_max           0.36 
_exptl_crystal_size_mid           0.14 
_exptl_crystal_size_min           0.05 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     4.039 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2513 
_exptl_absorpt_coefficient_mu     24.255 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0416 
_exptl_absorpt_correction_T_max   0.3768 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             11716 
_diffrn_reflns_av_R_equivalents   0.0403 
_diffrn_reflns_av_sigmaI/netI     0.0746 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -14 
_diffrn_reflns_limit_l_max        18 
_diffrn_reflns_theta_min          1.73 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8031 
_reflns_number_gt                 6869 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. The K+ and Sm3+ cations 
 are disordered with the site occupancy of 0.5, which are determined 
 according to the mass percentages of K+ and Sm3+ cations from inductively
 coupled plasma atomic emission spectrometry and their magnitude of 
 anisotropic displacement parameters. The ISOR instruction is used for
 O23. The DFIX instruction is used for Na1 and O24W. O13W is disordered 
 over two positions (O13W and O13A) and O21W is disordered over two 
 positions (O21W and O21A). The O6W, O7W, O8W, O9W, O10W, O11W, O13W,
 O13A, O14W, O15W, O17W, O20W, O21W, O21A, O23W and O24W are refined
 isostropicallly. 582 parameters and 7 restraints are used in 
 the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0686P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    notdet 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          8031 
_refine_ls_number_parameters      582 
_refine_ls_number_restraints      7 
_refine_ls_R_factor_all           0.0530 
_refine_ls_R_factor_gt            0.0458 
_refine_ls_wR_factor_ref          0.1242 
_refine_ls_wR_factor_gt           0.1196 
_refine_ls_goodness_of_fit_ref    1.020 
_refine_ls_restrained_S_all       1.021 
_refine_ls_shift/su_max           0.003 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
Na1 Na 1.1920(7) -0.2935(5) 0.3056(4) 0.0497(18) Uani 1 1 d D . . 
K1 K 0.5049(9) 0.7386(9) -0.1067(7) 0.070(3) Uani 0.50 1 d P . . 
W1 W 0.79476(4) 0.62775(4) 0.03467(3) 0.01644(14) Uani 1 1 d . . . 
W2 W 0.74315(4) 0.60617(4) 0.25107(3) 0.01917(14) Uani 1 1 d . . . 
W3 W 1.05820(4) 0.46190(4) 0.31704(3) 0.01803(14) Uani 1 1 d . . . 
W4 W 1.15952(4) 0.18042(4) 0.33446(3) 0.01873(14) Uani 1 1 d . . . 
W5 W 1.02792(4) 0.06567(4) 0.19284(4) 0.02102(15) Uani 1 1 d . . . 
W6 W 0.80365(4) 0.23960(4) 0.04736(3) 0.01909(14) Uani 1 1 d . . . 
W7 W 0.62254(4) 0.49955(4) 0.12402(3) 0.01797(14) Uani 1 1 d . . . 
W8 W 0.76248(4) 0.21293(4) 0.26126(3) 0.01921(14) Uani 1 1 d . . . 
W9 W 0.89508(4) 0.33206(4) 0.40295(3) 0.01925(14) Uani 1 1 d . . . 
Sm1 Sm 0.62528(12) 0.06569(11) 0.46814(9) 0.0212(3) Uani 0.50 1 d P . . 
As1 As 0.95204(11) 0.35934(10) 0.15922(8) 0.0151(3) Uani 1 1 d . . . 
Fe1 Fe 0.90695(15) 0.41226(14) -0.10239(11) 0.0176(4) Uani 1 1 d . . . 
Fe2 Fe 1.27513(16) 0.11163(15) 0.13749(12) 0.0192(4) Uani 1 1 d . . . 
O1W O 0.7422(8) 0.4403(8) -0.1594(6) 0.027(2) Uani 1 1 d . . . 
O2W O 0.9925(9) 0.2838(8) -0.1762(6) 0.032(2) Uani 1 1 d . . . 
O3W O 1.3348(9) -0.0435(8) 0.2253(6) 0.031(2) Uani 1 1 d . . . 
O4W O 1.4482(8) 0.0867(9) 0.1529(7) 0.037(3) Uani 1 1 d . . . 
O5W O 1.3265(11) 0.0078(10) 0.0449(8) 0.048(3) Uani 1 1 d . . . 
O7W O 0.4621(15) 0.2585(14) 0.4114(11) 0.019(4) Uiso 0.50 1 d P B . 
O8W O 0.738(2) 0.154(2) 0.5128(15) 0.048(6) Uiso 0.50 1 d P B . 
O9W O 0.8281(19) -0.0482(17) 0.4316(13) 0.036(5) Uiso 0.50 1 d P B . 
O10W O 0.460(3) 0.034(2) 0.5229(18) 0.061(7) Uiso 0.50 1 d P . . 
O11W O 0.532(2) 0.042(2) 0.3379(17) 0.061(7) Uiso 0.50 1 d P B . 
O12W O 0.663(3) -0.137(3) 0.467(2) 0.074(8) Uiso 0.50 1 d P . . 
O13A O 1.030(3) -0.037(3) 0.439(2) 0.069(8) Uiso 0.50 1 d P . . 
O13W O 1.100(3) -0.077(3) 0.430(2) 0.076(9) Uiso 0.50 1 d P . . 
O14W O 0.789(4) -0.086(3) 0.241(2) 0.102(12) Uiso 0.50 1 d P . . 
O15W O 0.5654(19) 0.4383(18) 0.3912(14) 0.113(7) Uiso 1 1 d . . . 
O16W O 1.1067(10) 0.0887(9) -0.0582(7) 0.039(3) Uani 1 1 d . . . 
O17W O 0.6906(17) 0.5834(16) 0.5055(12) 0.097(6) Uiso 1 1 d . . . 
O18W O 0.6285(11) 0.2425(10) -0.1939(10) 0.063(4) Uani 1 1 d . . . 
O19W O 0.6363(11) 0.6648(9) -0.2398(7) 0.049(3) Uani 1 1 d . . . 
O20W O 1.397(2) -0.356(2) 0.4110(17) 0.058(7) Uiso 0.50 1 d P . . 
O21W O 0.566(3) -0.096(3) 0.086(2) 0.073(8) Uiso 0.50 1 d P . . 
O21A O 0.648(3) -0.083(2) 0.1314(19) 0.070(8) Uiso 0.50 1 d P . . 
O22W O 1.1382(10) 0.3037(10) 0.5618(6) 0.038(3) Uani 1 1 d . . . 
O1 O 0.9360(8) 0.6098(8) 0.0662(6) 0.026(2) Uani 1 1 d . . . 
O2 O 0.7413(8) 0.7569(7) -0.0425(6) 0.023(2) Uani 1 1 d . . . 
O3 O 0.8348(8) 0.5247(8) -0.0321(6) 0.022(2) Uani 1 1 d . . . 
O4 O 0.6391(7) 0.6155(7) 0.0427(6) 0.0194(19) Uani 1 1 d . . . 
O5 O 0.8149(7) 0.4825(7) 0.1522(6) 0.0180(18) Uani 1 1 d . . . 
O6 O 0.7362(8) 0.6981(7) 0.1408(6) 0.023(2) Uani 1 1 d . . . 
O7 O 0.6724(9) 0.7083(8) 0.3109(6) 0.029(2) Uani 1 1 d . . . 
O8 O 0.6107(7) 0.5873(7) 0.2119(6) 0.0199(19) Uani 1 1 d . . . 
O9 O 0.7760(8) 0.4686(7) 0.3341(6) 0.022(2) Uani 1 1 d . . . 
O10 O 0.9010(7) 0.5786(7) 0.2770(6) 0.0191(19) Uani 1 1 d . . . 
O11 O 1.1127(9) 0.5398(8) 0.3632(6) 0.031(2) Uani 1 1 d . . . 
O12 O 0.9907(7) 0.3393(7) 0.2734(5) 0.0159(18) Uani 1 1 d . . . 
O13 O 0.9716(8) 0.4227(8) 0.4158(6) 0.024(2) Uani 1 1 d . . . 
O14 O 1.1018(7) 0.4759(7) 0.2057(6) 0.0197(19) Uani 1 1 d . . . 
O15 O 1.1762(8) 0.3100(7) 0.3588(6) 0.0206(19) Uani 1 1 d . . . 
O16 O 1.2730(8) 0.0711(8) 0.4035(6) 0.029(2) Uani 1 1 d . . . 
O17 O 1.0438(7) 0.2056(7) 0.4238(5) 0.0193(19) Uani 1 1 d . . . 
O18 O 1.2278(7) 0.1931(7) 0.2315(6) 0.022(2) Uani 1 1 d . . . 
O19 O 1.0866(8) 0.0985(7) 0.2918(6) 0.024(2) Uani 1 1 d . . . 
O20 O 1.0993(8) -0.0802(8) 0.2131(7) 0.030(2) Uani 1 1 d . . . 
O21 O 0.8963(8) 0.0731(7) 0.2659(6) 0.0212(19) Uani 1 1 d . . . 
O22 O 1.1231(8) 0.1161(8) 0.1242(7) 0.029(2) Uani 1 1 d . . . 
O23 O 0.8929(7) 0.2547(6) 0.1706(5) 0.0147(17) Uani 1 1 d U . . 
O24 O 0.9278(8) 0.0903(7) 0.0912(6) 0.024(2) Uani 1 1 d . . . 
O25 O 0.7344(9) 0.2087(8) -0.0298(6) 0.029(2) Uani 1 1 d . . . 
O26 O 0.8987(8) 0.2920(7) -0.0152(6) 0.027(2) Uani 1 1 d . . . 
O27 O 0.7254(8) 0.1966(8) 0.1492(6) 0.025(2) Uani 1 1 d . . . 
O28 O 0.6934(8) 0.3904(7) 0.0552(6) 0.022(2) Uani 1 1 d . . . 
O29 O 0.4784(8) 0.5337(8) 0.1053(6) 0.029(2) Uani 1 1 d . . . 
O30 O 0.6680(8) 0.3713(7) 0.2213(6) 0.022(2) Uani 1 1 d . . . 
O31 O 0.6722(8) 0.1662(8) 0.3246(6) 0.026(2) Uani 1 1 d . B . 
O32 O 0.8337(8) 0.2484(7) 0.3504(6) 0.022(2) Uani 1 1 d . . . 
O33 O 0.8381(8) 0.3230(8) 0.5031(6) 0.027(2) Uani 1 1 d . . . 
O23W O 0.526(2) 0.140(2) 0.6351(16) 0.044(6) Uiso 0.50 1 d P A 2 
O6W O 0.548(2) 0.1723(19) 0.5972(15) 0.039(5) Uiso 0.50 1 d P B 1 
O24W O 1.0301(12) -0.2163(17) 0.3355(15) 0.127(7) Uiso 1 1 d D . . 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
Na1 O24W 1.965(10) . ? 
Na1 O20 2.670(11) . ? 
Na1 O11 2.783(12) 1_545 ? 
Na1 O20W 2.82(3) . ? 
Na1 O33 2.973(12) 2_756 ? 
K1 O4W 2.591(14) 2_765 ? 
K1 O4 2.705(13) . ? 
K1 O19W 2.710(16) . ? 
K1 O27 2.728(13) 2_665 ? 
K1 O2 3.294(13) . ? 
K1 W1 3.876(10) . ? 
K1 W6 3.905(10) 2_665 ? 
K1 W8 3.949(10) 2_665 ? 
K1 W7 4.122(9) . ? 
W1 O2 1.757(8) . ? 
W1 O1 1.769(9) . ? 
W1 O3 1.778(9) . ? 
W1 O6 2.036(9) . ? 
W1 O4 2.045(8) . ? 
W1 O5 2.314(9) . ? 
W2 O7 1.718(9) . ? 
W2 O6 1.883(9) . ? 
W2 O9 1.906(8) . ? 
W2 O10 1.912(8) . ? 
W2 O8 1.925(9) . ? 
W2 O5 2.363(8) . ? 
W3 O11 1.723(10) . ? 
W3 O14 1.812(8) . ? 
W3 O15 1.926(8) . ? 
W3 O10 1.958(8) . ? 
W3 O13 1.988(9) . ? 
W3 O12 2.335(8) . ? 
W4 O16 1.740(9) . ? 
W4 O18 1.823(9) . ? 
W4 O19 1.903(9) . ? 
W4 O15 1.923(8) . ? 
W4 O17 1.975(8) . ? 
W4 O12 2.330(8) . ? 
W5 O20 1.720(9) . ? 
W5 O22 1.843(10) . ? 
W5 O19 1.925(10) . ? 
W5 O24 1.938(9) . ? 
W5 O21 1.981(9) . ? 
W5 O23 2.326(8) . ? 
W6 O25 1.709(9) . ? 
W6 O26 1.810(9) . ? 
W6 O28 1.925(8) . ? 
W6 O24 1.938(8) . ? 
W6 O27 1.973(9) . ? 
W6 O23 2.332(8) . ? 
W6 K1 3.905(10) 2_665 ? 
W7 O29 1.703(9) . ? 
W7 O4 1.874(8) . ? 
W7 O28 1.880(9) . ? 
W7 O30 1.931(8) . ? 
W7 O8 1.931(9) . ? 
W7 O5 2.393(8) . ? 
W8 O31 1.727(8) . ? 
W8 O27 1.895(10) . ? 
W8 O21 1.905(9) . ? 
W8 O30 1.905(8) . ? 
W8 O32 1.906(9) . ? 
W8 O23 2.327(8) . ? 
W8 K1 3.949(10) 2_665 ? 
W9 O33 1.713(9) . ? 
W9 O13 1.871(9) . ? 
W9 O32 1.899(9) . ? 
W9 O17 1.904(8) . ? 
W9 O9 1.927(9) . ? 
W9 O12 2.345(8) . ? 
Sm1 O10W 2.00(3) 2_656 ? 
Sm1 O16 2.381(10) 2_756 ? 
Sm1 O8W 2.38(2) . ? 
Sm1 O10W 2.42(3) . ? 
Sm1 O9W 2.50(2) . ? 
Sm1 O11W 2.50(3) . ? 
Sm1 O7W 2.517(17) . ? 
Sm1 O12W 2.53(3) . ? 
Sm1 O31 2.567(8) . ? 
Sm1 O6W 2.63(2) . ? 
As1 O12 1.796(8) . ? 
As1 O5 1.803(8) . ? 
As1 O23 1.812(8) . ? 
Fe1 O26 1.920(9) . ? 
Fe1 O3 1.929(9) . ? 
Fe1 O14 1.934(8) 2_765 ? 
Fe1 O1 1.963(9) 2_765 ? 
Fe1 O2W 2.139(9) . ? 
Fe1 O1W 2.140(9) . ? 
Fe2 O22 1.916(9) . ? 
Fe2 O18 1.929(9) . ? 
Fe2 O2 1.992(8) 2_765 ? 
Fe2 O3W 2.075(9) . ? 
Fe2 O4W 2.087(10) . ? 
Fe2 O5W 2.096(11) . ? 
O4W K1 2.591(14) 2_765 ? 
O10W O10W 1.35(5) 2_656 ? 
O10W O12W 1.61(4) 2_656 ? 
O10W Sm1 2.00(3) 2_656 ? 
O12W O10W 1.61(4) 2_656 ? 
O13A O13W 0.85(4) . ? 
O21W O21A 1.35(4) . ? 
O1 Fe1 1.963(9) 2_765 ? 
O2 Fe2 1.992(8) 2_765 ? 
O11 Na1 2.783(12) 1_565 ? 
O14 Fe1 1.934(8) 2_765 ? 
O16 Sm1 2.381(10) 2_756 ? 
O27 K1 2.728(13) 2_665 ? 
O33 Na1 2.973(12) 2_756 ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O24W Na1 O20 71.0(7) . . ? 
O24W Na1 O11 72.7(7) . 1_545 ? 
O20 Na1 O11 135.8(4) . 1_545 ? 
O24W Na1 O20W 127.4(9) . . ? 
O20 Na1 O20W 115.5(6) . . ? 
O11 Na1 O20W 106.3(6) 1_545 . ? 
O24W Na1 O33 65.8(7) . 2_756 ? 
O20 Na1 O33 116.3(4) . 2_756 ? 
O11 Na1 O33 68.6(3) 1_545 2_756 ? 
O20W Na1 O33 65.6(6) . 2_756 ? 
O4W K1 O4 105.8(4) 2_765 . ? 
O4W K1 O19W 83.9(4) 2_765 . ? 
O4 K1 O19W 106.1(5) . . ? 
O4W K1 O27 108.8(4) 2_765 2_665 ? 
O4 K1 O27 131.1(4) . 2_665 ? 
O19W K1 O27 111.0(5) . 2_665 ? 
O4W K1 O2 54.3(3) 2_765 . ? 
O4 K1 O2 55.0(3) . . ? 
O19W K1 O2 82.1(4) . . ? 
O27 K1 O2 158.7(5) 2_665 . ? 
O4W K1 W1 81.0(3) 2_765 . ? 
O4 K1 W1 30.0(2) . . ? 
O19W K1 W1 87.1(4) . . ? 
O27 K1 W1 159.9(4) 2_665 . ? 
O2 K1 W1 26.83(16) . . ? 
O4W K1 W6 123.6(4) 2_765 2_665 ? 
O4 K1 W6 103.1(3) . 2_665 ? 
O19W K1 W6 131.6(4) . 2_665 ? 
O27 K1 W6 28.1(2) 2_665 2_665 ? 
O2 K1 W6 146.0(4) . 2_665 ? 
W1 K1 W6 132.0(3) . 2_665 ? 
O4W K1 W8 107.5(4) 2_765 2_665 ? 
O4 K1 W8 145.7(4) . 2_665 ? 
O19W K1 W8 85.5(4) . 2_665 ? 
O27 K1 W8 25.5(2) 2_665 2_665 ? 
O2 K1 W8 158.9(3) . 2_665 ? 
W1 K1 W8 168.0(3) . 2_665 ? 
W6 K1 W8 50.37(12) 2_665 2_665 ? 
O4W K1 W7 126.0(4) 2_765 . ? 
O4 K1 W7 21.17(19) . . ? 
O19W K1 W7 111.4(4) . . ? 
O27 K1 W7 112.2(3) 2_665 . ? 
O2 K1 W7 76.1(2) . . ? 
W1 K1 W7 50.43(12) . . ? 
W6 K1 W7 85.17(18) 2_665 . ? 
W8 K1 W7 124.5(2) 2_665 . ? 
O2 W1 O1 102.7(4) . . ? 
O2 W1 O3 102.9(4) . . ? 
O1 W1 O3 98.5(4) . . ? 
O2 W1 O6 95.9(4) . . ? 
O1 W1 O6 88.4(4) . . ? 
O3 W1 O6 157.9(4) . . ? 
O2 W1 O4 95.4(4) . . ? 
O1 W1 O4 159.5(4) . . ? 
O3 W1 O4 86.5(4) . . ? 
O6 W1 O4 80.2(4) . . ? 
O2 W1 O5 163.8(4) . . ? 
O1 W1 O5 88.0(3) . . ? 
O3 W1 O5 87.2(4) . . ? 
O6 W1 O5 72.1(3) . . ? 
O4 W1 O5 72.3(3) . . ? 
O2 W1 K1 57.8(3) . . ? 
O1 W1 K1 159.0(3) . . ? 
O3 W1 K1 80.1(3) . . ? 
O6 W1 K1 100.7(3) . . ? 
O4 W1 K1 41.4(3) . . ? 
O5 W1 K1 112.7(2) . . ? 
O7 W2 O6 100.6(4) . . ? 
O7 W2 O9 102.5(4) . . ? 
O6 W2 O9 156.8(4) . . ? 
O7 W2 O10 100.0(4) . . ? 
O6 W2 O10 92.0(4) . . ? 
O9 W2 O10 86.2(4) . . ? 
O7 W2 O8 98.5(4) . . ? 
O6 W2 O8 89.4(4) . . ? 
O9 W2 O8 85.1(4) . . ? 
O10 W2 O8 160.9(4) . . ? 
O7 W2 O5 170.9(4) . . ? 
O6 W2 O5 73.5(3) . . ? 
O9 W2 O5 83.3(3) . . ? 
O10 W2 O5 87.3(3) . . ? 
O8 W2 O5 74.8(3) . . ? 
O11 W3 O14 103.5(4) . . ? 
O11 W3 O15 101.0(4) . . ? 
O14 W3 O15 96.0(4) . . ? 
O11 W3 O10 100.1(4) . . ? 
O14 W3 O10 90.2(4) . . ? 
O15 W3 O10 156.0(3) . . ? 
O11 W3 O13 99.5(4) . . ? 
O14 W3 O13 156.5(4) . . ? 
O15 W3 O13 84.5(4) . . ? 
O10 W3 O13 80.7(4) . . ? 
O11 W3 O12 172.1(4) . . ? 
O14 W3 O12 83.0(3) . . ? 
O15 W3 O12 73.5(3) . . ? 
O10 W3 O12 84.4(3) . . ? 
O13 W3 O12 74.6(3) . . ? 
O16 W4 O18 102.6(4) . . ? 
O16 W4 O19 101.3(4) . . ? 
O18 W4 O19 90.5(4) . . ? 
O16 W4 O15 100.3(4) . . ? 
O18 W4 O15 90.5(4) . . ? 
O19 W4 O15 157.7(4) . . ? 
O16 W4 O17 95.2(4) . . ? 
O18 W4 O17 162.2(4) . . ? 
O19 W4 O17 86.1(4) . . ? 
O15 W4 O17 86.1(4) . . ? 
O16 W4 O12 166.2(4) . . ? 
O18 W4 O12 89.9(3) . . ? 
O19 W4 O12 84.1(3) . . ? 
O15 W4 O12 73.6(3) . . ? 
O17 W4 O12 72.3(3) . . ? 
O20 W5 O22 105.1(4) . . ? 
O20 W5 O19 101.2(4) . . ? 
O22 W5 O19 88.5(4) . . ? 
O20 W5 O24 99.3(4) . . ? 
O22 W5 O24 91.4(4) . . ? 
O19 W5 O24 158.7(4) . . ? 
O20 W5 O21 96.2(4) . . ? 
O22 W5 O21 158.5(4) . . ? 
O19 W5 O21 84.2(4) . . ? 
O24 W5 O21 88.1(4) . . ? 
O20 W5 O23 166.6(4) . . ? 
O22 W5 O23 87.0(4) . . ? 
O19 W5 O23 84.6(3) . . ? 
O24 W5 O23 74.1(3) . . ? 
O21 W5 O23 72.2(3) . . ? 
O25 W6 O26 103.5(4) . . ? 
O25 W6 O28 102.0(4) . . ? 
O26 W6 O28 92.4(4) . . ? 
O25 W6 O24 100.0(4) . . ? 
O26 W6 O24 93.8(4) . . ? 
O28 W6 O24 155.0(4) . . ? 
O25 W6 O27 97.3(4) . . ? 
O26 W6 O27 159.1(4) . . ? 
O28 W6 O27 82.3(4) . . ? 
O24 W6 O27 83.3(4) . . ? 
O25 W6 O23 169.3(4) . . ? 
O26 W6 O23 85.9(4) . . ? 
O28 W6 O23 82.4(3) . . ? 
O24 W6 O23 74.0(3) . . ? 
O27 W6 O23 73.4(3) . . ? 
O25 W6 K1 66.2(4) . 2_665 ? 
O26 W6 K1 152.0(3) . 2_665 ? 
O28 W6 K1 66.1(3) . 2_665 ? 
O24 W6 K1 113.3(3) . 2_665 ? 
O27 W6 K1 40.6(3) . 2_665 ? 
O23 W6 K1 107.6(3) . 2_665 ? 
O29 W7 O4 101.0(4) . . ? 
O29 W7 O28 102.3(4) . . ? 
O4 W7 O28 93.3(4) . . ? 
O29 W7 O30 101.9(4) . . ? 
O4 W7 O30 156.7(4) . . ? 
O28 W7 O30 85.4(4) . . ? 
O29 W7 O8 98.9(4) . . ? 
O4 W7 O8 87.6(4) . . ? 
O28 W7 O8 158.1(4) . . ? 
O30 W7 O8 85.2(4) . . ? 
O29 W7 O5 170.8(4) . . ? 
O4 W7 O5 73.3(3) . . ? 
O28 W7 O5 85.4(3) . . ? 
O30 W7 O5 83.5(3) . . ? 
O8 W7 O5 74.0(3) . . ? 
O29 W7 K1 72.3(3) . . ? 
O4 W7 K1 31.4(3) . . ? 
O28 W7 K1 87.2(3) . . ? 
O30 W7 K1 169.4(3) . . ? 
O8 W7 K1 104.3(3) . . ? 
O5 W7 K1 103.5(2) . . ? 
O31 W8 O27 101.2(4) . . ? 
O31 W8 O21 100.7(4) . . ? 
O27 W8 O21 85.8(4) . . ? 
O31 W8 O30 103.5(4) . . ? 
O27 W8 O30 86.1(4) . . ? 
O21 W8 O30 155.5(4) . . ? 
O31 W8 O32 98.7(4) . . ? 
O27 W8 O32 160.1(4) . . ? 
O21 W8 O32 90.9(4) . . ? 
O30 W8 O32 88.9(4) . . ? 
O31 W8 O23 173.0(4) . . ? 
O27 W8 O23 74.9(3) . . ? 
O21 W8 O23 73.4(3) . . ? 
O30 W8 O23 82.2(3) . . ? 
O32 W8 O23 85.4(3) . . ? 
O31 W8 K1 72.3(3) . 2_665 ? 
O27 W8 K1 38.3(3) . 2_665 ? 
O21 W8 K1 115.3(3) . 2_665 ? 
O30 W8 K1 69.6(3) . 2_665 ? 
O32 W8 K1 153.2(3) . 2_665 ? 
O23 W8 K1 106.4(2) . 2_665 ? 
O33 W9 O13 100.0(4) . . ? 
O33 W9 O32 99.6(4) . . ? 
O13 W9 O32 160.3(4) . . ? 
O33 W9 O17 102.5(4) . . ? 
O13 W9 O17 87.2(4) . . ? 
O32 W9 O17 90.7(4) . . ? 
O33 W9 O9 102.8(4) . . ? 
O13 W9 O9 85.8(4) . . ? 
O32 W9 O9 87.8(4) . . ? 
O17 W9 O9 154.6(3) . . ? 
O33 W9 O12 174.3(4) . . ? 
O13 W9 O12 76.4(3) . . ? 
O32 W9 O12 84.2(3) . . ? 
O17 W9 O12 73.1(3) . . ? 
O9 W9 O12 81.5(3) . . ? 
O10W Sm1 O16 80.6(9) 2_656 2_756 ? 
O10W Sm1 O8W 159.1(10) 2_656 . ? 
O16 Sm1 O8W 80.4(6) 2_756 . ? 
O10W Sm1 O10W 33.9(13) 2_656 . ? 
O16 Sm1 O10W 83.9(7) 2_756 . ? 
O8W Sm1 O10W 134.7(9) . . ? 
O10W Sm1 O9W 107.0(9) 2_656 . ? 
O16 Sm1 O9W 72.1(5) 2_756 . ? 
O8W Sm1 O9W 74.9(8) . . ? 
O10W Sm1 O9W 138.3(8) . . ? 
O10W Sm1 O11W 56.9(10) 2_656 . ? 
O16 Sm1 O11W 129.5(7) 2_756 . ? 
O8W Sm1 O11W 143.9(8) . . ? 
O10W Sm1 O11W 75.3(9) . . ? 
O9W Sm1 O11W 94.0(8) . . ? 
O10W Sm1 O7W 101.0(9) 2_656 . ? 
O16 Sm1 O7W 144.8(4) 2_756 . ? 
O8W Sm1 O7W 89.8(7) . . ? 
O10W Sm1 O7W 79.4(8) . . ? 
O9W Sm1 O7W 137.7(6) . . ? 
O11W Sm1 O7W 75.5(7) . . ? 
O10W Sm1 O12W 39.6(10) 2_656 . ? 
O16 Sm1 O12W 64.5(7) 2_756 . ? 
O8W Sm1 O12W 134.6(9) . . ? 
O10W Sm1 O12W 71.4(10) . . ? 
O9W Sm1 O12W 67.7(9) . . ? 
O11W Sm1 O12W 65.3(9) . . ? 
O7W Sm1 O12W 135.5(8) . . ? 
O10W Sm1 O31 125.3(8) 2_656 . ? 
O16 Sm1 O31 138.5(3) 2_756 . ? 
O8W Sm1 O31 75.3(6) . . ? 
O10W Sm1 O31 136.4(7) . . ? 
O9W Sm1 O31 69.4(5) . . ? 
O11W Sm1 O31 68.7(6) . . ? 
O7W Sm1 O31 68.5(4) . . ? 
O12W Sm1 O31 112.5(7) . . ? 
O10W Sm1 O6W 102.5(9) 2_656 . ? 
O16 Sm1 O6W 75.5(6) 2_756 . ? 
O8W Sm1 O6W 64.3(8) . . ? 
O10W Sm1 O6W 70.7(8) . . ? 
O9W Sm1 O6W 131.1(7) . . ? 
O11W Sm1 O6W 134.9(8) . . ? 
O7W Sm1 O6W 69.8(6) . . ? 
O12W Sm1 O6W 126.7(8) . . ? 
O31 Sm1 O6W 120.7(6) . . ? 
O12 As1 O5 97.7(4) . . ? 
O12 As1 O23 97.1(4) . . ? 
O5 As1 O23 97.0(4) . . ? 
O26 Fe1 O3 93.2(4) . . ? 
O26 Fe1 O14 168.3(4) . 2_765 ? 
O3 Fe1 O14 93.5(4) . 2_765 ? 
O26 Fe1 O1 97.6(4) . 2_765 ? 
O3 Fe1 O1 92.2(4) . 2_765 ? 
O14 Fe1 O1 91.8(4) 2_765 2_765 ? 
O26 Fe1 O2W 85.6(4) . . ? 
O3 Fe1 O2W 177.7(4) . . ? 
O14 Fe1 O2W 88.0(4) 2_765 . ? 
O1 Fe1 O2W 85.9(4) 2_765 . ? 
O26 Fe1 O1W 88.3(4) . . ? 
O3 Fe1 O1W 92.4(4) . . ? 
O14 Fe1 O1W 81.8(4) 2_765 . ? 
O1 Fe1 O1W 172.3(4) 2_765 . ? 
O2W Fe1 O1W 89.7(4) . . ? 
O22 Fe2 O18 90.8(4) . . ? 
O22 Fe2 O2 99.5(4) . 2_765 ? 
O18 Fe2 O2 97.5(4) . 2_765 ? 
O22 Fe2 O3W 92.0(4) . . ? 
O18 Fe2 O3W 91.4(4) . . ? 
O2 Fe2 O3W 165.3(4) 2_765 . ? 
O22 Fe2 O4W 173.4(4) . . ? 
O18 Fe2 O4W 93.3(4) . . ? 
O2 Fe2 O4W 85.1(4) 2_765 . ? 
O3W Fe2 O4W 82.7(4) . . ? 
O22 Fe2 O5W 87.4(5) . . ? 
O18 Fe2 O5W 173.8(4) . . ? 
O2 Fe2 O5W 88.6(4) 2_765 . ? 
O3W Fe2 O5W 82.7(4) . . ? 
O4W Fe2 O5W 88.0(5) . . ? 
Fe2 O4W K1 118.0(5) . 2_765 ? 
O10W O10W O12W 154(4) 2_656 2_656 ? 
O10W O10W Sm1 90(2) 2_656 2_656 ? 
O12W O10W Sm1 87.9(16) 2_656 2_656 ? 
O10W O10W Sm1 56(2) 2_656 . ? 
O12W O10W Sm1 122.1(17) 2_656 . ? 
Sm1 O10W Sm1 146.1(13) 2_656 . ? 
O10W O12W Sm1 52.5(13) 2_656 . ? 
W1 O1 Fe1 179.1(6) . 2_765 ? 
W1 O2 Fe2 164.8(5) . 2_765 ? 
W1 O2 K1 95.4(4) . . ? 
Fe2 O2 K1 95.8(4) 2_765 . ? 
W1 O3 Fe1 169.2(5) . . ? 
W7 O4 W1 121.1(4) . . ? 
W7 O4 K1 127.4(4) . . ? 
W1 O4 K1 108.5(4) . . ? 
As1 O5 W1 113.1(4) . . ? 
As1 O5 W2 128.9(4) . . ? 
W1 O5 W2 93.5(3) . . ? 
As1 O5 W7 128.6(4) . . ? 
W1 O5 W7 93.0(3) . . ? 
W2 O5 W7 89.9(3) . . ? 
W2 O6 W1 120.8(4) . . ? 
W2 O8 W7 121.2(4) . . ? 
W2 O9 W9 146.1(5) . . ? 
W2 O10 W3 145.1(4) . . ? 
W3 O11 Na1 137.4(5) . 1_565 ? 
As1 O12 W4 117.5(4) . . ? 
As1 O12 W3 118.6(4) . . ? 
W4 O12 W3 91.8(3) . . ? 
As1 O12 W9 135.2(4) . . ? 
W4 O12 W9 92.8(3) . . ? 
W3 O12 W9 90.3(3) . . ? 
W9 O13 W3 118.5(5) . . ? 
W3 O14 Fe1 142.4(5) . 2_765 ? 
W4 O15 W3 121.0(5) . . ? 
W4 O16 Sm1 159.9(5) . 2_756 ? 
W9 O17 W4 121.6(4) . . ? 
W4 O18 Fe2 137.6(5) . . ? 
W4 O19 W5 148.3(5) . . ? 
W5 O20 Na1 158.2(6) . . ? 
W8 O21 W5 121.0(4) . . ? 
W5 O22 Fe2 136.8(6) . . ? 
As1 O23 W5 116.2(4) . . ? 
As1 O23 W8 134.6(4) . . ? 
W5 O23 W8 93.3(3) . . ? 
As1 O23 W6 118.9(4) . . ? 
W5 O23 W6 92.1(3) . . ? 
W8 O23 W6 91.7(3) . . ? 
W6 O24 W5 119.8(5) . . ? 
W6 O26 Fe1 145.8(5) . . ? 
W8 O27 W6 119.5(5) . . ? 
W8 O27 K1 116.1(5) . 2_665 ? 
W6 O27 K1 111.3(4) . 2_665 ? 
W7 O28 W6 148.9(5) . . ? 
W8 O30 W7 146.0(5) . . ? 
W8 O31 Sm1 152.3(5) . . ? 
W9 O32 W8 157.7(5) . . ? 
W9 O33 Na1 163.6(5) . 2_756 ? 
  
_diffrn_measured_fraction_theta_max    0.980 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.980 
_refine_diff_density_max    3.005 
_refine_diff_density_min   -2.694 
_refine_diff_density_rms    0.435 
  


#===END

  
data_5-La 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'As2 C8 Fe4 H106 La2 N2 O116 W18' 
_chemical_formula_weight          6047.31 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'La'  'La'  -0.2871   2.4523 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6669(13) 
_cell_length_b                    13.5788(13) 
_cell_length_c                    16.3488(17) 
_cell_angle_alpha                 107.303(2) 
_cell_angle_beta                  99.720(2) 
_cell_angle_gamma                 96.736(2) 
_cell_volume                      2604.0(5) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8975 
_cell_measurement_theta_min       1.72
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky  
_exptl_crystal_colour             'Light yellow' 
_exptl_crystal_size_max           0.48 
_exptl_crystal_size_mid           0.25 
_exptl_crystal_size_min           0.16 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.856 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2712 
_exptl_absorpt_coefficient_mu     21.889 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0338 
_exptl_absorpt_correction_T_max   0.1275 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             13131 
_diffrn_reflns_av_R_equivalents   0.0413 
_diffrn_reflns_av_sigmaI/netI     0.0734 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        8 
_diffrn_reflns_limit_l_min        -18 
_diffrn_reflns_limit_l_max        19 
_diffrn_reflns_theta_min          1.72 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8975 
_reflns_number_gt                 7806 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral. 
 However, its structure is pseudo-centrosymmetric, i.e. most of the 
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are
 rather common. An attempt to refine the structure in P¨C1 shows the 
 disorder around the chiral centre of L-thr (because we impose 
 inversion on a chiral entity), as a result, C1, C2, N1, O35 and 
 O36 atoms on L-thr are disordered over two positions. In addition, 
 some coordination water molecules on La3+ cations are disordered over
 two positions. The ISOR instruction is used for O5, O6 and O12. 
 The SADI instruction is used for C2' C1' C2 C1, O34 C1' O34 C1, O35' 
 C1' O35 C1, N1' C2' N1 C2, C3 C2' C3 C2, O36 C3 O36' C3, N1' C2' N1 C2.
 The EADP instruction is used for C2 and C2', N1 and N1', O36 and O36'. 
 The O7W, O7M, O8W, O10W, O10M, O11W, O11M, O12W, O12M, O13W, O14W, O15W,
 O16W, O16M, O18W, O18M, O22W, O35, O35', O36, O36', C1, C1', C2, C2', 
 N1 and N1' are refined isostropicallly. 656 parameters and 24
 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0458P)²+90.6685P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00013(3) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8975 
_refine_ls_number_parameters      656 
_refine_ls_number_restraints      24 
_refine_ls_R_factor_all           0.0563 
_refine_ls_R_factor_gt            0.0483 
_refine_ls_wR_factor_ref          0.1238 
_refine_ls_wR_factor_gt           0.1196 
_refine_ls_goodness_of_fit_ref    1.005 
_refine_ls_restrained_S_all       1.004 
_refine_ls_shift/su_max           0.003 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21390(5) 0.31251(5) 0.59641(4) 0.01528(16) Uani 1 1 d . . . 
W2 W 0.46806(5) 0.44225(5) 0.68197(4) 0.01462(16) Uani 1 1 d . . . 
W3 W 0.24718(5) 0.57503(5) 0.75650(4) 0.01451(15) Uani 1 1 d . . . 
W4 W 0.35739(5) 0.61359(4) 0.97184(4) 0.01156(15) Uani 1 1 d . . . 
W5 W 0.09591(5) 0.48747(5) 0.87935(4) 0.01365(15) Uani 1 1 d . . . 
W6 W 0.15194(5) 0.25793(5) 0.94385(4) 0.01505(16) Uani 1 1 d . . . 
W7 W 0.24894(5) 0.09157(5) 0.79072(4) 0.01605(16) Uani 1 1 d . . . 
W8 W 0.41480(5) 0.18502(5) 0.65472(4) 0.01700(16) Uani 1 1 d . . . 
W9 W 0.04523(5) 0.21530(5) 0.73193(4) 0.01427(15) Uani 1 1 d . . . 
La1 La 0.11705(9) 0.23244(9) 0.32727(7) 0.0333(3) Uani 1 1 d . . . 
As1 As 0.34053(11) 0.36009(11) 0.83625(10) 0.0101(3) Uani 1 1 d . . . 
Fe1 Fe 0.38168(16) 0.43051(16) 1.09895(14) 0.0133(4) Uani 1 1 d . . . 
O1W O 0.2406(8) 0.4520(9) 1.1540(8) 0.025(3) Uani 1 1 d . . . 
O2W O 0.4112(10) 0.3178(9) 1.1622(8) 0.031(3) Uani 1 1 d . . . 
O3W O 0.5530(12) 0.0482(10) 0.9289(10) 0.046(4) Uani 1 1 d . . . 
O4W O 0.6891(10) 0.1180(11) 0.8248(11) 0.047(4) Uani 1 1 d . . . 
O5W O 0.2614(16) 0.1386(15) 0.3793(16) 0.094(8) Uani 1 1 d . . . 
O6W O 0.2836(14) 0.3752(14) 0.4062(10) 0.066(5) Uani 1 1 d . . . 
O7W O -0.062(3) 0.182(2) 0.216(2) 0.089(9) Uiso 0.70 1 d P . . 
O7M O -0.078(4) 0.215(4) 0.330(4) 0.051(13) Uiso 0.30 1 d P . . 
O8W O 0.077(2) 0.045(2) 0.210(2) 0.132(10) Uiso 1 1 d . . . 
O9W O 0.2474(19) 0.2230(17) 0.2256(12) 0.089(7) Uani 1 1 d . . . 
O10W O 0.094(3) 0.359(3) 0.239(2) 0.099(10) Uiso 0.70 1 d P . . 
O10M O 0.045(4) 0.301(4) 0.198(3) 0.034(10) Uiso 0.30 1 d P . . 
O11W O 0.046(2) 0.078(2) 0.3738(19) 0.060(7) Uiso 0.60 1 d P . . 
O11M O -0.012(3) 0.112(3) 0.378(2) 0.036(8) Uiso 0.40 1 d P . . 
O12W O 0.048(3) 0.406(3) 0.381(2) 0.088(10) Uiso 0.60 1 d P . . 
O12M O -0.018(3) 0.348(3) 0.388(2) 0.044(9) Uiso 0.40 1 d P . . 
O13W O 0.111(2) -0.207(2) 0.9409(17) 0.106(8) Uiso 1 1 d . . . 
O14W O 0.197(4) 0.012(4) 1.065(3) 0.091(13) Uiso 0.50 1 d P . . 
O15W O 0.071(4) 0.531(4) 0.502(3) 0.102(15) Uiso 0.50 1 d P . . 
O16W O 0.303(3) -0.064(3) 0.361(3) 0.089(11) Uiso 0.60 1 d P . . 
O16M O 0.318(4) -0.121(4) 0.419(3) 0.077(14) Uiso 0.40 1 d P . . 
O17W O 0.3788(17) 0.1313(12) 1.0379(10) 0.068(6) Uani 1 1 d . . . 
O18W O 0.367(2) -0.120(2) 0.8982(17) 0.062(7) Uiso 0.70 1 d P . . 
O18M O 0.310(4) -0.123(4) 0.918(3) 0.038(11) Uiso 0.30 1 d P . . 
O19W O -0.1637(10) 0.2909(11) 0.8704(10) 0.045(4) Uani 1 1 d . . . 
O20W O 0.7405(17) 0.3492(14) 0.7304(13) 0.083(7) Uani 1 1 d . . . 
O21W O -0.0951(17) 0.3970(15) 0.6334(13) 0.079(6) Uani 1 1 d . . . 
O22W O 0.1176(16) 0.0062(16) 0.5060(13) 0.076(5) Uiso 1 1 d . . . 
O23W O 0.1362(19) -0.2008(18) 0.5099(13) 0.092(7) Uani 1 1 d . . . 
O1 O 0.1351(8) 0.2915(8) 0.4929(7) 0.018(2) Uani 1 1 d . . . 
O2 O 0.2882(9) 0.1977(8) 0.5694(7) 0.019(2) Uani 1 1 d . . . 
O3 O 0.1862(8) 0.4407(8) 0.6678(7) 0.019(2) Uani 1 1 d . . . 
O4 O 0.3424(8) 0.3322(7) 0.7209(6) 0.012(2) Uani 1 1 d . . . 
O5 O 0.1150(8) 0.2368(8) 0.6427(6) 0.014(2) Uani 1 1 d U . . 
O6 O 0.3402(8) 0.3960(8) 0.5841(6) 0.018(2) Uani 1 1 d U . . 
O7 O 0.5548(9) 0.5122(10) 0.6392(8) 0.028(3) Uani 1 1 d . . . 
O8 O 0.4980(8) 0.3022(8) 0.6371(7) 0.017(2) Uani 1 1 d . . . 
O9 O 0.5444(9) 0.4618(8) 0.7897(7) 0.019(2) Uani 1 1 d . . . 
O10 O 0.3841(9) 0.5485(8) 0.7303(7) 0.022(2) Uani 1 1 d . . . 
O11 O 0.2228(9) 0.6633(9) 0.7010(8) 0.024(3) Uani 1 1 d . . . 
O12 O 0.1112(8) 0.5598(8) 0.7941(7) 0.018(2) Uani 1 1 d U . . 
O13 O 0.2736(8) 0.4728(8) 0.8523(7) 0.016(2) Uani 1 1 d . . . 
O14 O 0.3154(8) 0.6672(7) 0.8692(7) 0.015(2) Uani 1 1 d . . . 
O15 O 0.4809(8) 0.5902(8) 0.9375(7) 0.020(2) Uani 1 1 d . . . 
O16 O 0.3558(9) 0.5292(8) 1.0368(7) 0.020(2) Uani 1 1 d . . . 
O17 O 0.3940(9) 0.7401(8) 1.0514(7) 0.019(2) Uani 1 1 d . . . 
O18 O 0.1929(8) 0.5990(8) 0.9637(7) 0.016(2) Uani 1 1 d . . . 
O19 O -0.0274(9) 0.5184(8) 0.8990(8) 0.023(3) Uani 1 1 d . . . 
O20 O 0.0476(9) 0.3623(8) 0.7763(7) 0.020(2) Uani 1 1 d . . . 
O21 O 0.1217(8) 0.3949(8) 0.9443(6) 0.016(2) Uani 1 1 d . . . 
O22 O 0.2235(8) 0.2616(7) 0.8206(7) 0.013(2) Uani 1 1 d . . . 
O23 O 0.2884(8) 0.3144(8) 1.0032(7) 0.018(2) Uani 1 1 d . . . 
O24 O 0.0871(9) 0.2402(8) 1.0237(7) 0.022(2) Uani 1 1 d . . . 
O25 O 0.0232(9) 0.2105(8) 0.8433(8) 0.021(2) Uani 1 1 d . . . 
O26 O 0.1822(8) 0.1209(8) 0.8932(7) 0.018(2) Uani 1 1 d . . . 
O27 O 0.2366(9) -0.0442(8) 0.7679(7) 0.022(2) Uani 1 1 d . . . 
O28 O 0.1025(8) 0.0885(8) 0.7199(7) 0.020(2) Uani 1 1 d . . . 
O29 O 0.3849(9) 0.1417(8) 0.8614(7) 0.023(3) Uani 1 1 d . . . 
O30 O 0.3055(9) 0.1077(8) 0.6941(7) 0.018(2) Uani 1 1 d . . . 
O31 O 0.4567(10) 0.0819(9) 0.5835(8) 0.031(3) Uani 1 1 d . . . 
O32 O 0.5062(9) 0.2068(9) 0.7596(7) 0.023(2) Uani 1 1 d . . . 
O33 O -0.0849(9) 0.1675(9) 0.6712(8) 0.024(3) Uani 1 1 d . . . 
O34 O 0.4832(10) -0.0050(9) 0.7473(9) 0.034(3) Uani 1 1 d D . . 
Fe2 Fe 0.53368(18) 0.13618(16) 0.84558(15) 0.0174(5) Uani 1 1 d . . . 
O35 O 0.615(2) -0.043(2) 0.685(2) 0.054(8) Uiso 0.50 1 d PD A 1 
O36 O 0.501(3) -0.273(3) 0.668(2) 0.081(8) Uiso 0.50 1 d PD B 1 
H36 H 0.5235 -0.3288 0.6553 0.122 Uiso 0.50 1 d PR B 1 
N1 N 0.325(2) -0.155(3) 0.628(2) 0.044(6) Uiso 0.50 1 d PD A 1 
H1A H 0.2888 -0.2077 0.5811 0.053 Uiso 0.50 1 d PR A 1 
H1B H 0.3171 -0.1712 0.6764 0.053 Uiso 0.50 1 d PR A 1 
H1C H 0.2996 -0.0969 0.6294 0.053 Uiso 0.50 1 d PR A 1 
C1 C 0.521(3) -0.058(3) 0.695(2) 0.038(9) Uiso 0.50 1 d PD A 1 
C2 C 0.444(3) -0.144(2) 0.617(2) 0.036(7) Uiso 0.50 1 d PD A 1 
H2 H 0.4458 -0.1245 0.5639 0.043 Uiso 0.50 1 calc PR A 1 
C3 C 0.460(2) -0.2574(18) 0.5974(15) 0.057(7) Uani 1 1 d D . . 
C4 C 0.385(3) -0.344(2) 0.537(2) 0.089(10) Uani 1 1 d . B . 
H4A H 0.3565 -0.3281 0.4851 0.133 Uiso 1 1 d R . . 
H4B H 0.4210 -0.4034 0.5213 0.133 Uiso 1 1 d R . . 
H4C H 0.3267 -0.3603 0.5640 0.133 Uiso 1 1 d R . . 
O35' O 0.546(3) -0.130(3) 0.773(2) 0.068(10) Uiso 0.50 1 d PD A 2 
O36' O 0.516(3) -0.212(3) 0.555(3) 0.081(8) Uiso 0.50 1 d PD B 2 
H36' H 0.5008 -0.1567 0.5510 0.122 Uiso 0.50 1 d PR B 2 
N1' N 0.345(3) -0.113(3) 0.599(2) 0.044(6) Uiso 0.50 1 d PD A 2 
H1'A H 0.2952 -0.1560 0.5537 0.066 Uiso 0.50 1 d PR A 2 
H1'B H 0.3139 -0.0655 0.6324 0.066 Uiso 0.50 1 d PR A 2 
H1'C H 0.3954 -0.0799 0.5792 0.066 Uiso 0.50 1 d PR A 2 
C1' C 0.484(3) -0.093(2) 0.729(2) 0.028(8) Uiso 0.50 1 d PD A 2 
C2' C 0.403(3) -0.176(3) 0.651(2) 0.036(7) Uiso 0.50 1 d PD A 2 
H2' H 0.3485 -0.2120 0.6737 0.043 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.737(10) . ? 
W1 O2 1.894(10) . ? 
W1 O3 1.894(11) . ? 
W1 O5 1.917(10) . ? 
W1 O6 1.925(11) . ? 
W1 O4 2.306(10) . ? 
W2 O7 1.734(11) . ? 
W2 O9 1.787(11) . ? 
W2 O8 1.932(10) . ? 
W2 O10 1.949(11) . ? 
W2 O6 1.967(10) . ? 
W2 O4 2.349(10) . ? 
W3 O11 1.731(11) . ? 
W3 O14 1.882(10) . ? 
W3 O10 1.905(11) . ? 
W3 O12 1.934(11) . ? 
W3 O3 1.935(11) . ? 
W3 O13 2.391(11) . ? 
W4 O17 1.772(11) . ? 
W4 O16 1.779(10) . ? 
W4 O15 1.781(10) . ? 
W4 O14 2.037(10) . ? 
W4 O18 2.047(10) . ? 
W4 O13 2.280(10) . ? 
W5 O19 1.721(10) . ? 
W5 O18 1.859(10) . ? 
W5 O21 1.894(10) . ? 
W5 O20 1.951(11) . ? 
W5 O12 1.951(10) . ? 
W5 O13 2.385(10) . ? 
W6 O24 1.715(11) . ? 
W6 O23 1.789(10) . ? 
W6 O26 1.911(10) . ? 
W6 O21 1.941(10) . ? 
W6 O25 1.999(11) . ? 
W6 O22 2.356(10) . ? 
W7 O27 1.751(10) . ? 
W7 O29 1.830(11) . ? 
W7 O30 1.900(11) . ? 
W7 O26 1.961(10) . ? 
W7 O28 2.002(10) . ? 
W7 O22 2.287(9) . ? 
W8 O31 1.735(11) . ? 
W8 O32 1.820(11) . ? 
W8 O8 1.925(11) . ? 
W8 O30 1.947(11) . ? 
W8 O2 1.999(11) . ? 
W8 O4 2.342(9) . ? 
W9 O33 1.714(10) . ? 
W9 O5 1.904(10) . ? 
W9 O20 1.905(11) . ? 
W9 O25 1.907(11) . ? 
W9 O28 1.915(10) . ? 
W9 O22 2.370(10) . ? 
La1 O7M 2.46(5) . ? 
La1 O5W 2.521(18) . ? 
La1 O9W 2.52(2) . ? 
La1 O7W 2.54(3) . ? 
La1 O1 2.547(10) . ? 
La1 O6W 2.551(15) . ? 
La1 O11W 2.55(3) . ? 
La1 O10W 2.56(3) . ? 
La1 O12W 2.57(4) . ? 
La1 O12M 2.58(4) . ? 
La1 O11M 2.58(3) . ? 
La1 O8W 2.62(3) . ? 
As1 O22 1.804(10) . ? 
As1 O13 1.809(10) . ? 
As1 O4 1.816(10) . ? 
Fe1 O16 1.933(10) . ? 
Fe1 O23 1.950(10) . ? 
Fe1 O15 1.956(10) 2_667 ? 
Fe1 O9 1.962(11) 2_667 ? 
Fe1 O2W 2.121(12) . ? 
Fe1 O1W 2.144(11) . ? 
O3W Fe2 2.066(14) . ? 
O4W Fe2 2.083(14) . ? 
O7M O12M 1.77(6) . ? 
O10W O10M 0.94(5) . ? 
O11W O11M 0.91(4) . ? 
O12W O12M 1.13(4) . ? 
O16W O16M 1.40(6) . ? 
O18W O18M 0.83(5) . ? 
O9 Fe1 1.962(11) 2_667 ? 
O15 Fe1 1.956(10) 2_667 ? 
O17 Fe2 1.983(11) 2_667 ? 
O29 Fe2 1.952(11) . ? 
O32 Fe2 1.932(11) . ? 
O34 C1' 1.15(3) . ? 
O34 C1 1.15(3) . ? 
O34 Fe2 2.049(12) . ? 
Fe2 O17 1.983(11) 2_667 ? 
O35 C1 1.22(3) . ? 
O36 C3 1.27(3) . ? 
N1 C2 1.54(3) . ? 
C1 C2 1.54(4) . ? 
C2 C3 1.53(3) . ? 
C3 O36' 1.29(3) . ? 
C3 C4 1.41(4) . ? 
C3 C2' 1.53(3) . ? 
O35' C1' 1.23(3) . ? 
N1' C2' 1.54(3) . ? 
C1' C2' 1.55(4) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O2 99.2(5) . . ? 
O1 W1 O3 105.1(5) . . ? 
O2 W1 O3 155.2(4) . . ? 
O1 W1 O5 100.0(5) . . ? 
O2 W1 O5 90.4(4) . . ? 
O3 W1 O5 90.0(4) . . ? 
O1 W1 O6 97.2(5) . . ? 
O2 W1 O6 86.8(5) . . ? 
O3 W1 O6 85.6(4) . . ? 
O5 W1 O6 162.8(4) . . ? 
O1 W1 O4 169.9(4) . . ? 
O2 W1 O4 73.2(4) . . ? 
O3 W1 O4 82.1(4) . . ? 
O5 W1 O4 86.8(4) . . ? 
O6 W1 O4 76.1(4) . . ? 
O7 W2 O9 103.3(5) . . ? 
O7 W2 O8 101.8(5) . . ? 
O9 W2 O8 92.7(4) . . ? 
O7 W2 O10 100.4(5) . . ? 
O9 W2 O10 90.3(5) . . ? 
O8 W2 O10 156.3(4) . . ? 
O7 W2 O6 99.6(5) . . ? 
O9 W2 O6 156.9(5) . . ? 
O8 W2 O6 85.8(4) . . ? 
O10 W2 O6 82.3(5) . . ? 
O7 W2 O4 172.4(5) . . ? 
O9 W2 O4 83.1(4) . . ? 
O8 W2 O4 73.6(4) . . ? 
O10 W2 O4 83.4(4) . . ? 
O6 W2 O4 74.3(4) . . ? 
O11 W3 O14 100.7(5) . . ? 
O11 W3 O10 99.4(5) . . ? 
O14 W3 O10 91.3(5) . . ? 
O11 W3 O12 99.4(5) . . ? 
O14 W3 O12 90.2(5) . . ? 
O10 W3 O12 160.6(4) . . ? 
O11 W3 O3 103.1(5) . . ? 
O14 W3 O3 156.2(4) . . ? 
O10 W3 O3 86.0(4) . . ? 
O12 W3 O3 84.9(5) . . ? 
O11 W3 O13 170.9(5) . . ? 
O14 W3 O13 72.2(4) . . ? 
O10 W3 O13 86.7(4) . . ? 
O12 W3 O13 75.3(4) . . ? 
O3 W3 O13 84.0(4) . . ? 
O17 W4 O16 103.0(5) . . ? 
O17 W4 O15 103.6(5) . . ? 
O16 W4 O15 97.8(5) . . ? 
O17 W4 O14 94.6(4) . . ? 
O16 W4 O14 159.2(5) . . ? 
O15 W4 O14 88.7(5) . . ? 
O17 W4 O18 96.9(4) . . ? 
O16 W4 O18 86.2(5) . . ? 
O15 W4 O18 157.6(5) . . ? 
O14 W4 O18 80.6(4) . . ? 
O17 W4 O13 163.6(4) . . ? 
O16 W4 O13 88.4(5) . . ? 
O15 W4 O13 86.2(4) . . ? 
O14 W4 O13 72.2(4) . . ? 
O18 W4 O13 71.8(4) . . ? 
O19 W5 O18 101.6(5) . . ? 
O19 W5 O21 102.3(5) . . ? 
O18 W5 O21 92.8(4) . . ? 
O19 W5 O20 100.6(5) . . ? 
O18 W5 O20 157.4(4) . . ? 
O21 W5 O20 86.4(4) . . ? 
O19 W5 O12 98.0(5) . . ? 
O18 W5 O12 88.5(5) . . ? 
O21 W5 O12 159.0(4) . . ? 
O20 W5 O12 84.5(4) . . ? 
O19 W5 O13 170.8(4) . . ? 
O18 W5 O13 72.5(4) . . ? 
O21 W5 O13 85.2(4) . . ? 
O20 W5 O13 84.9(4) . . ? 
O12 W5 O13 75.2(4) . . ? 
O24 W6 O23 103.0(5) . . ? 
O24 W6 O26 101.4(5) . . ? 
O23 W6 O26 95.4(5) . . ? 
O24 W6 O21 100.3(5) . . ? 
O23 W6 O21 90.8(5) . . ? 
O26 W6 O21 155.4(4) . . ? 
O24 W6 O25 98.3(5) . . ? 
O23 W6 O25 158.4(5) . . ? 
O26 W6 O25 83.7(4) . . ? 
O21 W6 O25 81.9(4) . . ? 
O24 W6 O22 172.0(4) . . ? 
O23 W6 O22 84.0(4) . . ? 
O26 W6 O22 73.6(4) . . ? 
O21 W6 O22 83.5(4) . . ? 
O25 W6 O22 75.0(4) . . ? 
O27 W7 O29 103.0(5) . . ? 
O27 W7 O30 100.5(5) . . ? 
O29 W7 O30 89.7(5) . . ? 
O27 W7 O26 97.5(5) . . ? 
O29 W7 O26 91.0(5) . . ? 
O30 W7 O26 161.4(4) . . ? 
O27 W7 O28 96.4(5) . . ? 
O29 W7 O28 160.6(5) . . ? 
O30 W7 O28 86.3(5) . . ? 
O26 W7 O28 86.9(5) . . ? 
O27 W7 O22 166.8(4) . . ? 
O29 W7 O22 87.7(4) . . ? 
O30 W7 O22 87.0(4) . . ? 
O26 W7 O22 74.4(4) . . ? 
O28 W7 O22 73.1(4) . . ? 
O31 W8 O32 103.4(5) . . ? 
O31 W8 O8 100.3(5) . . ? 
O32 W8 O8 91.5(5) . . ? 
O31 W8 O30 100.2(5) . . ? 
O32 W8 O30 87.8(5) . . ? 
O8 W8 O30 159.1(4) . . ? 
O31 W8 O2 97.5(5) . . ? 
O32 W8 O2 158.7(5) . . ? 
O8 W8 O2 88.4(4) . . ? 
O30 W8 O2 84.8(4) . . ? 
O31 W8 O4 166.7(5) . . ? 
O32 W8 O4 88.9(4) . . ? 
O8 W8 O4 73.9(4) . . ? 
O30 W8 O4 85.2(4) . . ? 
O2 W8 O4 70.7(4) . . ? 
O33 W9 O5 99.3(5) . . ? 
O33 W9 O20 103.1(5) . . ? 
O5 W9 O20 89.3(4) . . ? 
O33 W9 O25 99.6(5) . . ? 
O5 W9 O25 161.1(4) . . ? 
O20 W9 O25 86.7(5) . . ? 
O33 W9 O28 101.3(5) . . ? 
O5 W9 O28 89.1(5) . . ? 
O20 W9 O28 155.5(4) . . ? 
O25 W9 O28 86.9(5) . . ? 
O33 W9 O22 172.7(4) . . ? 
O5 W9 O22 84.8(4) . . ? 
O20 W9 O22 82.8(4) . . ? 
O25 W9 O22 76.3(4) . . ? 
O28 W9 O22 72.7(4) . . ? 
O7M La1 O5W 131.3(13) . . ? 
O7M La1 O9W 142.5(13) . . ? 
O5W La1 O9W 74.3(8) . . ? 
O7M La1 O7W 42.8(14) . . ? 
O5W La1 O7W 136.5(9) . . ? 
O9W La1 O7W 99.8(9) . . ? 
O7M La1 O1 81.8(13) . . ? 
O5W La1 O1 76.3(6) . . ? 
O9W La1 O1 135.4(5) . . ? 
O7W La1 O1 124.5(8) . . ? 
O7M La1 O6W 134.5(13) . . ? 
O5W La1 O6W 74.8(6) . . ? 
O9W La1 O6W 72.0(6) . . ? 
O7W La1 O6W 145.6(8) . . ? 
O1 La1 O6W 68.4(4) . . ? 
O7M La1 O11W 66.4(14) . . ? 
O5W La1 O11W 65.3(9) . . ? 
O9W La1 O11W 123.7(9) . . ? 
O7W La1 O11W 85.3(10) . . ? 
O1 La1 O11W 70.2(7) . . ? 
O6W La1 O11W 127.6(8) . . ? 
O7M La1 O10W 89.6(14) . . ? 
O5W La1 O10W 138.8(10) . . ? 
O9W La1 O10W 67.6(10) . . ? 
O7W La1 O10W 67.2(11) . . ? 
O1 La1 O10W 122.0(9) . . ? 
O6W La1 O10W 79.0(9) . . ? 
O11W La1 O10W 152.2(11) . . ? 
O7M La1 O12W 64.8(15) . . ? 
O5W La1 O12W 139.2(10) . . ? 
O9W La1 O12W 117.0(10) . . ? 
O7W La1 O12W 82.6(11) . . ? 
O1 La1 O12W 69.2(9) . . ? 
O6W La1 O12W 72.7(10) . . ? 
O11W La1 O12W 119.2(11) . . ? 
O10W La1 O12W 55.6(12) . . ? 
O7M La1 O12M 41.0(15) . . ? 
O5W La1 O12M 139.8(10) . . ? 
O9W La1 O12M 139.6(10) . . ? 
O7W La1 O12M 70.3(11) . . ? 
O1 La1 O12M 63.7(8) . . ? 
O6W La1 O12M 94.0(10) . . ? 
O11W La1 O12M 95.2(11) . . ? 
O10W La1 O12M 72.6(11) . . ? 
O12W La1 O12M 25.5(10) . . ? 
O7M La1 O11M 46.6(15) . . ? 
O5W La1 O11M 84.7(9) . . ? 
O9W La1 O11M 140.7(9) . . ? 
O7W La1 O11M 73.3(10) . . ? 
O1 La1 O11M 66.9(8) . . ? 
O6W La1 O11M 134.0(8) . . ? 
O11W La1 O11M 20.4(8) . . ? 
O10W La1 O11M 135.5(11) . . ? 
O12W La1 O11M 100.6(12) . . ? 
O12M La1 O11M 75.7(11) . . ? 
O7M La1 O8W 89.0(14) . . ? 
O5W La1 O8W 74.8(8) . . ? 
O9W La1 O8W 70.2(8) . . ? 
O7W La1 O8W 63.0(10) . . ? 
O1 La1 O8W 131.6(7) . . ? 
O6W La1 O8W 136.5(8) . . ? 
O11W La1 O8W 62.7(9) . . ? 
O10W La1 O8W 105.2(11) . . ? 
O12W La1 O8W 145.5(11) . . ? 
O12M La1 O8W 129.1(11) . . ? 
O11M La1 O8W 72.4(10) . . ? 
O22 As1 O13 98.4(4) . . ? 
O22 As1 O4 96.3(4) . . ? 
O13 As1 O4 99.1(5) . . ? 
O16 Fe1 O23 92.3(5) . . ? 
O16 Fe1 O15 93.2(5) . 2_667 ? 
O23 Fe1 O15 97.0(5) . 2_667 ? 
O16 Fe1 O9 94.7(5) . 2_667 ? 
O23 Fe1 O9 167.9(5) . 2_667 ? 
O15 Fe1 O9 92.4(5) 2_667 2_667 ? 
O16 Fe1 O2W 177.6(5) . . ? 
O23 Fe1 O2W 86.0(5) . . ? 
O15 Fe1 O2W 85.3(5) 2_667 . ? 
O9 Fe1 O2W 87.2(5) 2_667 . ? 
O16 Fe1 O1W 92.4(5) . . ? 
O23 Fe1 O1W 87.0(4) . . ? 
O15 Fe1 O1W 173.0(5) 2_667 . ? 
O9 Fe1 O1W 82.9(4) 2_667 . ? 
O2W Fe1 O1W 89.3(5) . . ? 
O12M O7M La1 73(2) . . ? 
O10M O10W La1 84(4) . . ? 
O10W O10M La1 75(4) . . ? 
O11M O11W La1 81(3) . . ? 
O11W O11M La1 78(3) . . ? 
O12M O12W La1 78(3) . . ? 
O12W O12M O7M 135(4) . . ? 
O12W O12M La1 77(3) . . ? 
O7M O12M La1 66(2) . . ? 
W1 O1 La1 148.8(5) . . ? 
W1 O2 W8 121.8(5) . . ? 
W1 O3 W3 146.7(6) . . ? 
As1 O4 W1 134.6(5) . . ? 
As1 O4 W8 116.8(5) . . ? 
W1 O4 W8 94.1(3) . . ? 
As1 O4 W2 118.2(5) . . ? 
W1 O4 W2 91.4(3) . . ? 
W8 O4 W2 91.4(3) . . ? 
W9 O5 W1 154.5(6) . . ? 
W1 O6 W2 117.8(5) . . ? 
W8 O8 W2 121.0(5) . . ? 
W2 O9 Fe1 143.5(6) . 2_667 ? 
W3 O10 W2 146.1(6) . . ? 
W3 O12 W5 119.9(5) . . ? 
As1 O13 W4 114.9(5) . . ? 
As1 O13 W5 128.7(5) . . ? 
W4 O13 W5 93.9(4) . . ? 
As1 O13 W3 126.8(5) . . ? 
W4 O13 W3 94.1(4) . . ? 
W5 O13 W3 89.5(3) . . ? 
W3 O14 W4 121.4(5) . . ? 
W4 O15 Fe1 178.1(6) . 2_667 ? 
W4 O16 Fe1 167.9(7) . . ? 
W4 O17 Fe2 164.3(6) . 2_667 ? 
W5 O18 W4 121.5(5) . . ? 
W9 O20 W5 144.8(6) . . ? 
W5 O21 W6 147.5(6) . . ? 
As1 O22 W7 117.5(5) . . ? 
As1 O22 W6 118.2(5) . . ? 
W7 O22 W6 92.3(4) . . ? 
As1 O22 W9 134.8(5) . . ? 
W7 O22 W9 93.7(3) . . ? 
W6 O22 W9 90.2(3) . . ? 
W6 O23 Fe1 145.7(6) . . ? 
W9 O25 W6 118.0(5) . . ? 
W6 O26 W7 119.7(5) . . ? 
W9 O28 W7 120.3(5) . . ? 
W7 O29 Fe2 135.4(6) . . ? 
W7 O30 W8 146.8(6) . . ? 
W8 O32 Fe2 138.6(6) . . ? 
C1' O34 C1 50(2) . . ? 
C1' O34 Fe2 144.1(19) . . ? 
C1 O34 Fe2 136(2) . . ? 
O32 Fe2 O29 88.4(5) . . ? 
O32 Fe2 O17 98.6(5) . 2_667 ? 
O29 Fe2 O17 97.0(5) . 2_667 ? 
O32 Fe2 O34 89.3(5) . . ? 
O29 Fe2 O34 91.0(5) . . ? 
O17 Fe2 O34 168.8(5) 2_667 . ? 
O32 Fe2 O3W 174.5(5) . . ? 
O29 Fe2 O3W 89.7(6) . . ? 
O17 Fe2 O3W 86.8(5) 2_667 . ? 
O34 Fe2 O3W 85.5(6) . . ? 
O32 Fe2 O4W 93.4(6) . . ? 
O29 Fe2 O4W 175.7(5) . . ? 
O17 Fe2 O4W 86.6(5) 2_667 . ? 
O34 Fe2 O4W 85.0(5) . . ? 
O3W Fe2 O4W 88.2(6) . . ? 
O34 C1 O35 127(3) . . ? 
O34 C1 C2 118(3) . . ? 
O35 C1 C2 114(3) . . ? 
C3 C2 N1 100(2) . . ? 
C3 C2 C1 119(3) . . ? 
N1 C2 C1 112(3) . . ? 
O36 C3 O36' 124(4) . . ? 
O36 C3 C4 114(3) . . ? 
O36' C3 C4 109(3) . . ? 
O36 C3 C2 110(3) . . ? 
O36' C3 C2 70(2) . . ? 
C4 C3 C2 125(3) . . ? 
O36 C3 C2' 88(3) . . ? 
O36' C3 C2' 108(3) . . ? 
C4 C3 C2' 112(3) . . ? 
C2 C3 C2' 38(2) . . ? 
O34 C1' O35' 123(3) . . ? 
O34 C1' C2' 123(3) . . ? 
O35' C1' C2' 114(3) . . ? 
C3 C2' N1' 114(3) . . ? 
C3 C2' C1' 111(2) . . ? 
N1' C2' C1' 105(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.979 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.979 
_refine_diff_density_max    2.138 
_refine_diff_density_min   -3.669 
_refine_diff_density_rms    0.395 
  


#===END

  
data_6-Pr 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Fe4 N2 O116 Pr2 W18' 
_chemical_formula_weight          6051.31 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Pr'  'Pr'  -0.2180   2.8214 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6523(18) 
_cell_length_b                    13.5456(19) 
_cell_length_c                    16.272(2) 
_cell_angle_alpha                 107.169(2) 
_cell_angle_beta                  99.786(2) 
_cell_angle_gamma                 96.861(2) 
_cell_volume                      2582.7(6) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8830 
_cell_measurement_theta_min       1.72 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky 
_exptl_crystal_colour             'Light yellow'  
_exptl_crystal_size_max           0.50 
_exptl_crystal_size_mid           0.27 
_exptl_crystal_size_min           0.19 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.891 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2716 
_exptl_absorpt_coefficient_mu     22.185 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0319 
_exptl_absorpt_correction_T_max   0.1016 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12556 
_diffrn_reflns_av_R_equivalents   0.0416 
_diffrn_reflns_av_sigmaI/netI     0.0780 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -9 
_diffrn_reflns_limit_k_max        16 
_diffrn_reflns_limit_l_min        -19 
_diffrn_reflns_limit_l_max        19 
_diffrn_reflns_theta_min          1.72 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8830 
_reflns_number_gt                 7412 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral. 
 However, its structure is pseudo-centrosymmetric, i.e. most of the 
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are 
 rather common. An attempt to refine the structure in P¨C1 shows 
 the disorder around the chiral centre of L-thr (because we impose 
 inversion on a chiral entity), as a result, C1, C2 N1, O35 and O36 
 atoms on L-thr are disordered over two positions. In addition, 
 some coordination water molecules on Pr3+ cations are disordered
 over two positions. The ISOR instruction is used for O2, O3, O13, 
 O18, O10, O16, O33, O21, O23, O24 and O29. The DELU instruction is
 used for Pr1 and O5W. The SADI instruction is used for C2' C1' C2 C1,
 O34 C1' O34 C1, O35' C1' O35 C1, N1' C2' N1 C2, C3 C2' C3 C2, O36 C3 
 O36' C3, N1' C2' N1 C2. The EADP instruction is used for C2 and C2',
 N1 and N1', O36 and O36'. The O7W, O7M, O8W, O10W, O10M, O11W, O11M,
 O12W, O12M, O13W, O14W, O15W, O16W, O16M, O18W, O18M, O22W, O35, O35', 
 O36, O36', C1, C1', C2, C2', N1 and N1' are refined isostropicallly.
 656 parameters and 79 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1064P)²+33.6685P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00008(5) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8830 
_refine_ls_number_parameters      656 
_refine_ls_number_restraints      79 
_refine_ls_R_factor_all           0.0699 
_refine_ls_R_factor_gt            0.0586 
_refine_ls_wR_factor_ref          0.1682 
_refine_ls_wR_factor_gt           0.1604 
_refine_ls_goodness_of_fit_ref    1.023 
_refine_ls_restrained_S_all       1.020 
_refine_ls_shift/su_max           0.000 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21320(5) 0.31213(5) 0.59528(5) 0.0168(2) Uani 1 1 d . . . 
W2 W 0.46761(5) 0.44219(5) 0.68106(5) 0.0162(2) Uani 1 1 d . . . 
W3 W 0.24636(5) 0.57493(5) 0.75560(5) 0.01576(19) Uani 1 1 d . . . 
W4 W 0.35704(5) 0.61368(5) 0.97155(4) 0.01239(19) Uani 1 1 d . . . 
W5 W 0.09513(5) 0.48714(5) 0.87897(5) 0.01467(19) Uani 1 1 d . . . 
W6 W 0.15141(5) 0.25745(5) 0.94404(5) 0.0166(2) Uani 1 1 d . . . 
W7 W 0.24829(5) 0.09088(5) 0.79049(5) 0.0174(2) Uani 1 1 d . . . 
W8 W 0.41432(6) 0.18456(5) 0.65395(5) 0.0183(2) Uani 1 1 d . . . 
W9 W 0.04433(5) 0.21453(5) 0.73136(5) 0.01562(19) Uani 1 1 d . . . 
Pr1 Pr 0.11676(10) 0.23350(10) 0.32757(9) 0.0377(3) Uani 1 1 d U . . 
As1 As 0.33986(13) 0.36009(12) 0.83593(11) 0.0104(3) Uani 1 1 d . . . 
Fe1 Fe 0.38208(18) 0.42990(18) 1.09937(17) 0.0150(5) Uani 1 1 d . . . 
O1W O 0.2403(10) 0.4523(10) 1.1518(10) 0.031(3) Uani 1 1 d . . . 
O2W O 0.4100(12) 0.3161(11) 1.1620(10) 0.036(4) Uani 1 1 d . . . 
O3W O 0.5534(13) 0.0485(11) 0.9293(11) 0.043(4) Uani 1 1 d . . . 
O4W O 0.6883(11) 0.1188(13) 0.8250(11) 0.041(4) Uani 1 1 d . . . 
O5W O 0.255(2) 0.1388(19) 0.3808(19) 0.111(11) Uani 1 1 d U . . 
O6W O 0.280(2) 0.3791(18) 0.4067(15) 0.094(9) Uani 1 1 d . . . 
O7W O -0.060(3) 0.183(3) 0.216(3) 0.092(11) Uiso 0.70 1 d P . . 
O7M O -0.065(3) 0.220(3) 0.332(3) 0.023(9) Uiso 0.30 1 d P . . 
O8W O 0.068(3) 0.054(3) 0.207(3) 0.167(15) Uiso 1 1 d . . . 
O9W O 0.245(2) 0.223(3) 0.2261(18) 0.133(13) Uani 1 1 d . . . 
O10W O 0.087(3) 0.343(3) 0.238(3) 0.094(11) Uiso 0.70 1 d P . . 
O10M O 0.023(7) 0.283(6) 0.201(6) 0.08(2) Uiso 0.30 1 d P . . 
O11W O 0.048(4) 0.081(3) 0.379(3) 0.086(12) Uiso 0.60 1 d P . . 
O11M O -0.008(4) 0.112(3) 0.375(3) 0.045(10) Uiso 0.40 1 d P . . 
O12W O 0.054(3) 0.413(3) 0.380(3) 0.086(12) Uiso 0.60 1 d P . . 
O12M O -0.018(4) 0.347(4) 0.380(4) 0.071(14) Uiso 0.40 1 d P . . 
O13W O 0.116(2) -0.196(2) 0.945(2) 0.108(9) Uiso 1 1 d . . . 
O14W O 0.204(5) 0.021(5) 1.067(4) 0.112(19) Uiso 0.50 1 d P . . 
O15W O 0.071(5) 0.519(5) 0.501(4) 0.112(19) Uiso 0.50 1 d P . . 
O16W O 0.302(3) -0.052(3) 0.355(3) 0.077(10) Uiso 0.60 1 d P . . 
O16M O 0.318(5) -0.131(5) 0.412(5) 0.092(18) Uiso 0.40 1 d P . . 
O17W O 0.3757(18) 0.1332(14) 1.0379(14) 0.072(6) Uani 1 1 d . . . 
O18W O 0.365(3) -0.119(2) 0.898(2) 0.064(8) Uiso 0.70 1 d P . . 
O18M O 0.307(6) -0.112(5) 0.918(5) 0.058(16) Uiso 0.30 1 d P . . 
O19W O -0.1654(11) 0.2892(12) 0.8700(10) 0.038(4) Uani 1 1 d . . . 
O20W O 0.7401(17) 0.3506(16) 0.7288(13) 0.074(7) Uani 1 1 d . . . 
O21W O -0.0958(18) 0.3975(17) 0.6339(14) 0.069(6) Uani 1 1 d U . . 
O22W O 0.1183(18) 0.0079(17) 0.5079(15) 0.070(6) Uiso 1 1 d . . . 
O23W O 0.139(2) -0.203(2) 0.5110(16) 0.090(7) Uani 1 1 d . . . 
O1 O 0.1349(11) 0.2908(10) 0.4919(9) 0.026(3) Uani 1 1 d . . . 
O2 O 0.2887(9) 0.1971(9) 0.5682(8) 0.018(3) Uani 1 1 d U . . 
O3 O 0.1829(9) 0.4398(9) 0.6655(8) 0.014(2) Uani 1 1 d U . . 
O4 O 0.3404(9) 0.3318(8) 0.7205(7) 0.010(2) Uani 1 1 d . . . 
O5 O 0.1175(9) 0.2388(9) 0.6440(8) 0.020(3) Uani 1 1 d . . . 
O6 O 0.3404(10) 0.3933(11) 0.5845(8) 0.025(3) Uani 1 1 d . . . 
O7 O 0.5536(12) 0.5117(11) 0.6386(11) 0.037(4) Uani 1 1 d . . . 
O8 O 0.4952(10) 0.3025(9) 0.6327(9) 0.022(3) Uani 1 1 d . . . 
O9 O 0.5454(10) 0.4618(9) 0.7918(8) 0.017(3) Uani 1 1 d . . . 
O10 O 0.3843(9) 0.5481(9) 0.7326(8) 0.015(2) Uani 1 1 d U . . 
O11 O 0.2219(10) 0.6639(10) 0.7003(8) 0.021(3) Uani 1 1 d . . . 
O12 O 0.1110(10) 0.5598(9) 0.7937(9) 0.025(3) Uani 1 1 d . . . 
O13 O 0.2722(9) 0.4727(8) 0.8501(7) 0.013(2) Uani 1 1 d U . . 
O14 O 0.3145(10) 0.6681(9) 0.8684(8) 0.020(3) Uani 1 1 d . . . 
O15 O 0.4808(10) 0.5910(9) 0.9386(9) 0.025(3) Uani 1 1 d . . . 
O16 O 0.3559(10) 0.5280(10) 1.0349(8) 0.021(3) Uani 1 1 d U . . 
O17 O 0.3935(9) 0.7394(9) 1.0510(8) 0.020(3) Uani 1 1 d . . . 
O18 O 0.1921(9) 0.6000(10) 0.9643(8) 0.019(3) Uani 1 1 d U . . 
O19 O -0.0290(10) 0.5187(10) 0.8980(9) 0.027(3) Uani 1 1 d . . . 
O20 O 0.0473(9) 0.3645(9) 0.7763(8) 0.017(3) Uani 1 1 d . . . 
O21 O 0.1207(9) 0.3948(8) 0.9427(8) 0.013(2) Uani 1 1 d U . . 
O22 O 0.2231(9) 0.2610(9) 0.8211(8) 0.015(2) Uani 1 1 d . . . 
O23 O 0.2899(9) 0.3134(9) 1.0062(8) 0.014(2) Uani 1 1 d U . . 
O24 O 0.0867(10) 0.2358(10) 1.0215(9) 0.025(3) Uani 1 1 d U . . 
O25 O 0.0241(9) 0.2111(9) 0.8450(10) 0.027(3) Uani 1 1 d . . . 
O26 O 0.1822(10) 0.1212(9) 0.8934(8) 0.022(3) Uani 1 1 d . . . 
O27 O 0.2343(12) -0.0434(10) 0.7675(10) 0.033(3) Uani 1 1 d . . . 
O28 O 0.1023(10) 0.0879(9) 0.7202(9) 0.021(3) Uani 1 1 d . . . 
O29 O 0.3826(9) 0.1417(8) 0.8600(8) 0.013(2) Uani 1 1 d U . . 
O30 O 0.3045(10) 0.1095(10) 0.6940(10) 0.027(3) Uani 1 1 d . . . 
O31 O 0.4538(12) 0.0808(11) 0.5807(9) 0.031(3) Uani 1 1 d . . . 
O32 O 0.5061(10) 0.2068(10) 0.7600(10) 0.027(3) Uani 1 1 d . . . 
O33 O -0.0878(10) 0.1677(9) 0.6713(8) 0.019(3) Uani 1 1 d U . . 
O34 O 0.4815(11) -0.0066(10) 0.7468(9) 0.030(3) Uani 1 1 d D . . 
Fe2 Fe 0.53340(19) 0.13604(19) 0.84586(17) 0.0176(5) Uani 1 1 d . . . 
O35 O 0.615(3) -0.035(3) 0.681(2) 0.049(8) Uiso 0.50 1 d PD . 1 
O36 O 0.500(4) -0.279(3) 0.664(3) 0.075(9) Uiso 0.50 1 d PD A 1 
H36 H 0.5230 -0.3340 0.6515 0.113 Uiso 0.50 1 d PR A 1 
N1 N 0.329(3) -0.146(3) 0.629(3) 0.048(8) Uiso 0.50 1 d PD A 1 
H1A H 0.2924 -0.1980 0.5818 0.057 Uiso 0.50 1 d PR A 1 
H1B H 0.3207 -0.1616 0.6771 0.057 Uiso 0.50 1 d PR A 1 
H1C H 0.3032 -0.0873 0.6302 0.057 Uiso 0.50 1 d PR A 1 
C1 C 0.520(3) -0.054(3) 0.688(3) 0.035(10) Uiso 0.50 1 d PD A 1 
C2 C 0.443(3) -0.144(2) 0.612(3) 0.028(6) Uiso 0.50 1 d PD A 1 
H2 H 0.4427 -0.1276 0.5570 0.033 Uiso 0.50 1 calc PR A 1 
C3 C 0.464(3) -0.258(2) 0.5972(17) 0.057(7) Uani 1 1 d D . . 
C4 C 0.389(3) -0.345(2) 0.538(2) 0.092(13) Uani 1 1 d . A . 
H4A H 0.3602 -0.3294 0.4861 0.138 Uiso 1 1 d R . . 
H4B H 0.4247 -0.4047 0.5223 0.138 Uiso 1 1 d R . . 
H4C H 0.3304 -0.3616 0.5650 0.138 Uiso 1 1 d R . . 
O35' O 0.553(5) -0.131(5) 0.778(4) 0.13(2) Uiso 0.50 1 d PD A 2 
O36' O 0.518(4) -0.223(3) 0.552(3) 0.075(9) Uiso 0.50 1 d PD A 2 
H36' H 0.5036 -0.1674 0.5474 0.113 Uiso 0.50 1 d PR A 2 
N1' N 0.345(3) -0.116(3) 0.600(3) 0.048(8) Uiso 0.50 1 d PD A 2 
H1'A H 0.2950 -0.1599 0.5546 0.072 Uiso 0.50 1 d PR A 2 
H1'B H 0.3137 -0.0694 0.6333 0.072 Uiso 0.50 1 d PR A 2 
H1'C H 0.3953 -0.0838 0.5801 0.072 Uiso 0.50 1 d PR A 2 
C1' C 0.487(3) -0.098(3) 0.731(3) 0.039(11) Uiso 0.50 1 d PD A 2 
C2' C 0.403(3) -0.178(3) 0.652(2) 0.028(6) Uiso 0.50 1 d PD A 2 
H2' H 0.3497 -0.2152 0.6743 0.033 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.724(14) . ? 
W1 O3 1.894(11) . ? 
W1 O5 1.894(12) . ? 
W1 O6 1.901(13) . ? 
W1 O2 1.905(11) . ? 
W1 O4 2.297(11) . ? 
W2 O7 1.715(13) . ? 
W2 O9 1.828(12) . ? 
W2 O8 1.922(11) . ? 
W2 O6 1.942(12) . ? 
W2 O10 1.955(11) . ? 
W2 O4 2.362(10) . ? 
W3 O11 1.730(13) . ? 
W3 O14 1.881(12) . ? 
W3 O10 1.901(11) . ? 
W3 O12 1.927(13) . ? 
W3 O3 1.952(11) . ? 
W3 O13 2.364(12) . ? 
W4 O17 1.758(11) . ? 
W4 O16 1.766(13) . ? 
W4 O15 1.771(12) . ? 
W4 O14 2.041(12) . ? 
W4 O18 2.053(11) . ? 
W4 O13 2.295(11) . ? 
W5 O19 1.730(12) . ? 
W5 O18 1.868(12) . ? 
W5 O21 1.869(11) . ? 
W5 O20 1.923(12) . ? 
W5 O12 1.947(13) . ? 
W5 O13 2.385(11) . ? 
W6 O24 1.690(13) . ? 
W6 O23 1.816(11) . ? 
W6 O26 1.903(12) . ? 
W6 O21 1.951(11) . ? 
W6 O25 1.966(14) . ? 
W6 O22 2.343(11) . ? 
W7 O27 1.725(13) . ? 
W7 O29 1.802(11) . ? 
W7 O30 1.899(14) . ? 
W7 O26 1.955(13) . ? 
W7 O28 1.989(12) . ? 
W7 O22 2.283(11) . ? 
W8 O31 1.740(13) . ? 
W8 O32 1.828(14) . ? 
W8 O30 1.937(13) . ? 
W8 O8 1.942(12) . ? 
W8 O2 1.987(12) . ? 
W8 O4 2.354(11) . ? 
W9 O33 1.726(12) . ? 
W9 O5 1.906(12) . ? 
W9 O28 1.917(12) . ? 
W9 O25 1.922(15) . ? 
W9 O20 1.938(12) . ? 
W9 O22 2.375(11) . ? 
Pr1 O7M 2.29(4) . ? 
Pr1 O10W 2.39(4) . ? 
Pr1 O5W 2.48(2) . ? 
Pr1 O9W 2.49(2) . ? 
Pr1 O10M 2.51(8) . ? 
Pr1 O7W 2.51(4) . ? 
Pr1 O1 2.516(14) . ? 
Pr1 O12M 2.52(5) . ? 
Pr1 O11M 2.52(4) . ? 
Pr1 O6W 2.539(18) . ? 
Pr1 O11W 2.56(4) . ? 
Pr1 O8W 2.56(4) . ? 
As1 O4 1.804(11) . ? 
As1 O22 1.804(11) . ? 
As1 O13 1.812(10) . ? 
Fe1 O23 1.922(12) . ? 
Fe1 O9 1.929(12) 2_667 ? 
Fe1 O16 1.946(13) . ? 
Fe1 O15 1.962(13) 2_667 ? 
Fe1 O2W 2.115(14) . ? 
Fe1 O1W 2.130(13) . ? 
O3W Fe2 2.054(15) . ? 
O4W Fe2 2.074(14) . ? 
O7W O10M 1.71(9) . ? 
O7W O7M 1.82(6) . ? 
O7M O12M 1.65(7) . ? 
O10W O10M 1.03(8) . ? 
O11W O11M 0.87(5) . ? 
O12W O12M 1.20(6) . ? 
O15W O15W 1.81(12) 2_566 ? 
O16W O16M 1.61(7) . ? 
O16W O35 1.77(5) 2_656 ? 
O18W O18M 0.86(6) . ? 
O9 Fe1 1.929(12) 2_667 ? 
O15 Fe1 1.962(13) 2_667 ? 
O17 Fe2 1.987(12) 2_667 ? 
O29 Fe2 1.968(11) . ? 
O32 Fe2 1.923(14) . ? 
O34 C1 1.20(3) . ? 
O34 C1' 1.20(3) . ? 
O34 Fe2 2.064(13) . ? 
Fe2 O17 1.987(12) 2_667 ? 
O35 C1 1.23(4) . ? 
O35 O16W 1.77(5) 2_656 ? 
O36 C3 1.23(4) . ? 
N1 C2 1.51(4) . ? 
C1 C2 1.54(4) . ? 
C2 C3 1.56(4) . ? 
C3 O36' 1.25(4) . ? 
C3 C4 1.41(4) . ? 
C3 C2' 1.56(4) . ? 
O35' C1' 1.24(4) . ? 
N1' C2' 1.52(4) . ? 
C1' C2' 1.54(4) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O3 104.4(5) . . ? 
O1 W1 O5 101.4(6) . . ? 
O3 W1 O5 88.8(5) . . ? 
O1 W1 O6 98.3(6) . . ? 
O3 W1 O6 86.9(5) . . ? 
O5 W1 O6 160.3(5) . . ? 
O1 W1 O2 99.1(6) . . ? 
O3 W1 O2 156.1(5) . . ? 
O5 W1 O2 90.8(5) . . ? 
O6 W1 O2 85.5(5) . . ? 
O1 W1 O4 170.2(5) . . ? 
O3 W1 O4 82.8(4) . . ? 
O5 W1 O4 85.1(5) . . ? 
O6 W1 O4 75.3(5) . . ? 
O2 W1 O4 73.3(5) . . ? 
O7 W2 O9 103.6(7) . . ? 
O7 W2 O8 101.1(6) . . ? 
O9 W2 O8 94.4(6) . . ? 
O7 W2 O6 100.7(7) . . ? 
O9 W2 O6 155.6(5) . . ? 
O8 W2 O6 83.3(6) . . ? 
O7 W2 O10 101.4(6) . . ? 
O9 W2 O10 88.8(5) . . ? 
O8 W2 O10 155.9(5) . . ? 
O6 W2 O10 83.9(5) . . ? 
O7 W2 O4 172.5(6) . . ? 
O9 W2 O4 82.9(4) . . ? 
O8 W2 O4 74.4(4) . . ? 
O6 W2 O4 73.1(5) . . ? 
O10 W2 O4 82.3(4) . . ? 
O11 W3 O14 100.0(6) . . ? 
O11 W3 O10 100.9(5) . . ? 
O14 W3 O10 90.3(5) . . ? 
O11 W3 O12 99.3(5) . . ? 
O14 W3 O12 89.9(6) . . ? 
O10 W3 O12 159.4(5) . . ? 
O11 W3 O3 102.9(6) . . ? 
O14 W3 O3 157.0(5) . . ? 
O10 W3 O3 87.2(5) . . ? 
O12 W3 O3 84.6(5) . . ? 
O11 W3 O13 170.9(5) . . ? 
O14 W3 O13 73.0(4) . . ? 
O10 W3 O13 85.2(4) . . ? 
O12 W3 O13 75.2(5) . . ? 
O3 W3 O13 84.0(4) . . ? 
O17 W4 O16 103.7(6) . . ? 
O17 W4 O15 103.2(6) . . ? 
O16 W4 O15 96.8(6) . . ? 
O17 W4 O14 94.5(5) . . ? 
O16 W4 O14 158.8(5) . . ? 
O15 W4 O14 89.4(6) . . ? 
O17 W4 O18 96.3(5) . . ? 
O16 W4 O18 86.5(5) . . ? 
O15 W4 O18 158.7(5) . . ? 
O14 W4 O18 80.6(5) . . ? 
O17 W4 O13 163.3(5) . . ? 
O16 W4 O13 88.2(5) . . ? 
O15 W4 O13 86.7(5) . . ? 
O14 W4 O13 71.9(4) . . ? 
O18 W4 O13 72.3(4) . . ? 
O19 W5 O18 101.2(6) . . ? 
O19 W5 O21 103.0(6) . . ? 
O18 W5 O21 93.3(5) . . ? 
O19 W5 O20 100.5(6) . . ? 
O18 W5 O20 157.7(5) . . ? 
O21 W5 O20 86.6(5) . . ? 
O19 W5 O12 97.6(6) . . ? 
O18 W5 O12 88.3(6) . . ? 
O21 W5 O12 158.6(5) . . ? 
O20 W5 O12 84.0(5) . . ? 
O19 W5 O13 170.2(5) . . ? 
O18 W5 O13 73.3(4) . . ? 
O21 W5 O13 85.6(4) . . ? 
O20 W5 O13 84.4(4) . . ? 
O12 W5 O13 74.4(5) . . ? 
O24 W6 O23 102.7(6) . . ? 
O24 W6 O26 100.1(6) . . ? 
O23 W6 O26 94.7(5) . . ? 
O24 W6 O21 102.3(5) . . ? 
O23 W6 O21 92.0(5) . . ? 
O26 W6 O21 154.5(5) . . ? 
O24 W6 O25 97.5(6) . . ? 
O23 W6 O25 159.7(5) . . ? 
O26 W6 O25 84.1(5) . . ? 
O21 W6 O25 81.1(5) . . ? 
O24 W6 O22 170.5(5) . . ? 
O23 W6 O22 84.8(5) . . ? 
O26 W6 O22 73.2(5) . . ? 
O21 W6 O22 83.1(4) . . ? 
O25 W6 O22 75.4(5) . . ? 
O27 W7 O29 104.3(6) . . ? 
O27 W7 O30 101.6(6) . . ? 
O29 W7 O30 89.2(6) . . ? 
O27 W7 O26 97.8(6) . . ? 
O29 W7 O26 91.0(5) . . ? 
O30 W7 O26 160.0(5) . . ? 
O27 W7 O28 95.8(6) . . ? 
O29 W7 O28 159.9(5) . . ? 
O30 W7 O28 86.3(6) . . ? 
O26 W7 O28 86.7(5) . . ? 
O27 W7 O22 166.1(6) . . ? 
O29 W7 O22 87.0(5) . . ? 
O30 W7 O22 86.4(5) . . ? 
O26 W7 O22 73.7(5) . . ? 
O28 W7 O22 73.2(4) . . ? 
O31 W8 O32 104.8(6) . . ? 
O31 W8 O30 101.0(6) . . ? 
O32 W8 O30 87.8(6) . . ? 
O31 W8 O8 100.0(6) . . ? 
O32 W8 O8 93.2(6) . . ? 
O30 W8 O8 158.0(5) . . ? 
O31 W8 O2 96.1(6) . . ? 
O32 W8 O2 158.8(5) . . ? 
O30 W8 O2 84.7(5) . . ? 
O8 W8 O2 86.5(5) . . ? 
O31 W8 O4 165.7(5) . . ? 
O32 W8 O4 88.8(5) . . ? 
O30 W8 O4 83.8(4) . . ? 
O8 W8 O4 74.3(4) . . ? 
O2 W8 O4 70.7(4) . . ? 
O33 W9 O5 101.4(5) . . ? 
O33 W9 O28 102.3(5) . . ? 
O5 W9 O28 89.4(5) . . ? 
O33 W9 O25 99.8(5) . . ? 
O5 W9 O25 158.8(5) . . ? 
O28 W9 O25 86.8(5) . . ? 
O33 W9 O20 102.4(5) . . ? 
O5 W9 O20 88.3(5) . . ? 
O28 W9 O20 155.1(5) . . ? 
O25 W9 O20 86.4(5) . . ? 
O33 W9 O22 172.8(5) . . ? 
O5 W9 O22 83.6(5) . . ? 
O28 W9 O22 72.3(5) . . ? 
O25 W9 O22 75.4(4) . . ? 
O20 W9 O22 82.8(4) . . ? 
O7M Pr1 O10W 87.8(14) . . ? 
O7M Pr1 O5W 130.0(13) . . ? 
O10W Pr1 O5W 141.4(12) . . ? 
O7M Pr1 O9W 142.8(13) . . ? 
O10W Pr1 O9W 67.4(13) . . ? 
O5W Pr1 O9W 75.7(13) . . ? 
O7M Pr1 O10M 73(2) . . ? 
O10W Pr1 O10M 24.2(18) . . ? 
O5W Pr1 O10M 147(2) . . ? 
O9W Pr1 O10M 74(2) . . ? 
O7M Pr1 O7W 44.2(14) . . ? 
O10W Pr1 O7W 63.5(13) . . ? 
O5W Pr1 O7W 135.8(10) . . ? 
O9W Pr1 O7W 98.8(11) . . ? 
O10M Pr1 O7W 40(2) . . ? 
O7M Pr1 O1 81.1(12) . . ? 
O10W Pr1 O1 125.3(10) . . ? 
O5W Pr1 O1 75.3(8) . . ? 
O9W Pr1 O1 135.7(7) . . ? 
O10M Pr1 O1 136.9(19) . . ? 
O7W Pr1 O1 125.3(9) . . ? 
O7M Pr1 O12M 39.8(16) . . ? 
O10W Pr1 O12M 71.2(16) . . ? 
O5W Pr1 O12M 141.3(15) . . ? 
O9W Pr1 O12M 137.7(16) . . ? 
O10M Pr1 O12M 72(2) . . ? 
O7W Pr1 O12M 69.0(16) . . ? 
O1 Pr1 O12M 66.4(13) . . ? 
O7M Pr1 O11M 47.9(15) . . ? 
O10W Pr1 O11M 134.0(14) . . ? 
O5W Pr1 O11M 82.3(13) . . ? 
O9W Pr1 O11M 139.2(13) . . ? 
O10M Pr1 O11M 113(2) . . ? 
O7W Pr1 O11M 74.0(13) . . ? 
O1 Pr1 O11M 67.4(10) . . ? 
O12M Pr1 O11M 78.2(16) . . ? 
O7M Pr1 O6W 132.4(12) . . ? 
O10W Pr1 O6W 81.7(12) . . ? 
O5W Pr1 O6W 77.0(9) . . ? 
O9W Pr1 O6W 73.0(9) . . ? 
O10M Pr1 O6W 106(2) . . ? 
O7W Pr1 O6W 144.3(11) . . ? 
O1 Pr1 O6W 68.3(6) . . ? 
O12M Pr1 O6W 93.4(15) . . ? 
O11M Pr1 O6W 134.5(11) . . ? 
O7M Pr1 O11W 67.5(15) . . ? 
O10W Pr1 O11W 150.5(15) . . ? 
O5W Pr1 O11W 63.0(13) . . ? 
O9W Pr1 O11W 124.0(14) . . ? 
O10M Pr1 O11W 127(2) . . ? 
O7W Pr1 O11W 87.2(13) . . ? 
O1 Pr1 O11W 68.4(10) . . ? 
O12M Pr1 O11W 96.5(16) . . ? 
O11M Pr1 O11W 19.7(11) . . ? 
O6W Pr1 O11W 126.6(12) . . ? 
O7M Pr1 O8W 87.6(14) . . ? 
O10W Pr1 O8W 99.0(14) . . ? 
O5W Pr1 O8W 78.2(11) . . ? 
O9W Pr1 O8W 70.5(12) . . ? 
O10M Pr1 O8W 80(2) . . ? 
O7W Pr1 O8W 59.2(13) . . ? 
O1 Pr1 O8W 133.4(10) . . ? 
O12M Pr1 O8W 125.1(16) . . ? 
O11M Pr1 O8W 71.6(14) . . ? 
O6W Pr1 O8W 139.8(11) . . ? 
O11W Pr1 O8W 65.5(14) . . ? 
O4 As1 O22 96.2(5) . . ? 
O4 As1 O13 98.2(5) . . ? 
O22 As1 O13 98.5(5) . . ? 
O23 Fe1 O9 167.7(5) . 2_667 ? 
O23 Fe1 O16 92.8(5) . . ? 
O9 Fe1 O16 94.2(5) 2_667 . ? 
O23 Fe1 O15 96.7(5) . 2_667 ? 
O9 Fe1 O15 93.0(5) 2_667 2_667 ? 
O16 Fe1 O15 92.4(6) . 2_667 ? 
O23 Fe1 O2W 84.3(5) . . ? 
O9 Fe1 O2W 89.0(5) 2_667 . ? 
O16 Fe1 O2W 176.5(6) . . ? 
O15 Fe1 O2W 86.0(6) 2_667 . ? 
O23 Fe1 O1W 86.3(5) . . ? 
O9 Fe1 O1W 83.4(5) 2_667 . ? 
O16 Fe1 O1W 91.5(6) . . ? 
O15 Fe1 O1W 174.9(6) 2_667 . ? 
O2W Fe1 O1W 90.3(6) . . ? 
O10M O7W O7M 107(4) . . ? 
O10M O7W Pr1 70(3) . . ? 
O7M O7W Pr1 61.6(17) . . ? 
O12M O7M O7W 110(3) . . ? 
O12M O7M Pr1 77(2) . . ? 
O7W O7M Pr1 74.3(18) . . ? 
O10M O10W Pr1 84(5) . . ? 
O10W O10M O7W 138(8) . . ? 
O10W O10M Pr1 71(5) . . ? 
O7W O10M Pr1 70(3) . . ? 
O11M O11W Pr1 78(4) . . ? 
O11W O11M Pr1 83(4) . . ? 
O12M O12W Pr1 73(3) . . ? 
O12W O12M O7M 139(5) . . ? 
O12W O12M Pr1 80(3) . . ? 
O7M O12M Pr1 63(2) . . ? 
O16M O16W O35 138(4) . 2_656 ? 
W1 O1 Pr1 149.1(7) . . ? 
W1 O2 W8 121.8(6) . . ? 
W1 O3 W3 144.9(6) . . ? 
As1 O4 W1 135.5(6) . . ? 
As1 O4 W8 116.9(5) . . ? 
W1 O4 W8 94.0(4) . . ? 
As1 O4 W2 117.8(5) . . ? 
W1 O4 W2 91.2(4) . . ? 
W8 O4 W2 90.7(4) . . ? 
W1 O5 W9 157.2(7) . . ? 
W1 O6 W2 120.0(7) . . ? 
W2 O8 W8 120.5(6) . . ? 
W2 O9 Fe1 142.2(6) . 2_667 ? 
W3 O10 W2 146.2(6) . . ? 
W3 O12 W5 120.2(7) . . ? 
As1 O13 W4 113.8(5) . . ? 
As1 O13 W3 127.8(6) . . ? 
W4 O13 W3 94.2(4) . . ? 
As1 O13 W5 128.4(6) . . ? 
W4 O13 W5 93.4(4) . . ? 
W3 O13 W5 90.0(4) . . ? 
W3 O14 W4 120.9(6) . . ? 
W4 O15 Fe1 178.0(8) . 2_667 ? 
W4 O16 Fe1 168.8(8) . . ? 
W4 O17 Fe2 164.4(7) . 2_667 ? 
W5 O18 W4 120.6(6) . . ? 
W5 O20 W9 144.1(7) . . ? 
W5 O21 W6 148.7(7) . . ? 
As1 O22 W7 117.7(5) . . ? 
As1 O22 W6 118.6(6) . . ? 
W7 O22 W6 92.7(4) . . ? 
As1 O22 W9 134.1(6) . . ? 
W7 O22 W9 93.6(4) . . ? 
W6 O22 W9 90.3(4) . . ? 
W6 O23 Fe1 145.5(6) . . ? 
W9 O25 W6 118.6(6) . . ? 
W6 O26 W7 120.4(7) . . ? 
W9 O28 W7 120.7(6) . . ? 
W7 O29 Fe2 136.2(7) . . ? 
W7 O30 W8 147.7(9) . . ? 
W8 O32 Fe2 138.4(7) . . ? 
C1 O34 C1' 57(3) . . ? 
C1 O34 Fe2 133(2) . . ? 
C1' O34 Fe2 141(2) . . ? 
O32 Fe2 O29 87.5(5) . . ? 
O32 Fe2 O17 98.2(6) . 2_667 ? 
O29 Fe2 O17 97.6(5) . 2_667 ? 
O32 Fe2 O3W 174.8(6) . . ? 
O29 Fe2 O3W 90.8(6) . . ? 
O17 Fe2 O3W 86.9(6) 2_667 . ? 
O32 Fe2 O34 89.6(6) . . ? 
O29 Fe2 O34 90.4(5) . . ? 
O17 Fe2 O34 169.1(5) 2_667 . ? 
O3W Fe2 O34 85.5(6) . . ? 
O32 Fe2 O4W 93.1(6) . . ? 
O29 Fe2 O4W 175.8(6) . . ? 
O17 Fe2 O4W 86.4(6) 2_667 . ? 
O3W Fe2 O4W 88.2(7) . . ? 
O34 Fe2 O4W 85.5(6) . . ? 
C1 O35 O16W 139(4) . 2_656 ? 
O34 C1 O35 126(4) . . ? 
O34 C1 C2 117(3) . . ? 
O35 C1 C2 117(3) . . ? 
N1 C2 C1 108(3) . . ? 
N1 C2 C3 105(3) . . ? 
C1 C2 C3 118(3) . . ? 
O36 C3 O36' 126(4) . . ? 
O36 C3 C4 109(3) . . ? 
O36' C3 C4 106(3) . . ? 
O36 C3 C2' 89(3) . . ? 
O36' C3 C2' 114(3) . . ? 
C4 C3 C2' 110(3) . . ? 
O36 C3 C2 116(3) . . ? 
O36' C3 C2 75(3) . . ? 
C4 C3 C2 122(3) . . ? 
C2' C3 C2 40(2) . . ? 
O34 C1' O35' 123(5) . . ? 
O34 C1' C2' 117(3) . . ? 
O35' C1' C2' 120(4) . . ? 
N1' C2' C1' 108(3) . . ? 
N1' C2' C3 113(3) . . ? 
C1' C2' C3 109(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.970 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.970 
_refine_diff_density_max    4.557 
_refine_diff_density_min   -4.440 
_refine_diff_density_rms    0.549 
  


#===END

  
data_7-Nd
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Fe4 N2 Nd2 O116 W18' 
_chemical_formula_weight          6057.79 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Nd'  'Nd'  -0.1943   3.0179 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6668(10) 
_cell_length_b                    13.5691(11) 
_cell_length_c                    16.3027(13) 
_cell_angle_alpha                 107.1270(10) 
_cell_angle_beta                  99.7630(10) 
_cell_angle_gamma                 96.8760(10) 
_cell_volume                      2595.8(4) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8997 
_cell_measurement_theta_min       1.72 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky 
_exptl_crystal_colour             'Light yellow'  
_exptl_crystal_size_max           0.44 
_exptl_crystal_size_mid           0.18 
_exptl_crystal_size_min           0.15 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.875 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2717 
_exptl_absorpt_coefficient_mu     22.134 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0367 
_exptl_absorpt_correction_T_max   0.1360 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             13219 
_diffrn_reflns_av_R_equivalents   0.0379 
_diffrn_reflns_av_sigmaI/netI     0.0704 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        12 
_diffrn_reflns_limit_l_min        -17 
_diffrn_reflns_limit_l_max        19 
_diffrn_reflns_theta_min          1.72 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8997 
_reflns_number_gt                 7903 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral.
 However, its structure is pseudo-centrosymmetric, i.e. most of the 
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are 
 rather common. An attempt to refine the structure in P¨C1 shows the 
 disorder around the chiral centre of L-thr (because we impose inversion 
 on a chiral entity), as a result, C1, C2, N1, O35 and O36 atoms on L-thr 
 are disordered over two positions. In addition, some coordination water 
 molecules on Nd3+ cations are disordered over two positions. The ISOR 
 instruction is used for O3, O11, O30, O16, O19, O12, O13, O14 and O9. 
 The DELU instruction is used for C3 and C4. The SADI instruction is used 
 for C2' C1' C2 C1, O34 C1' O34 C1, O35' C1' O35 C1, N1' C2' N1 C2, C3 C2' 
 C3 C2, O36 C3 O36' C3, N1' C2' N1 C2. The EADP instruction is used for 
 C2 and C2', N1 and N1', O36 and O36'. The O7W, O7M, O8W, O10W, O10M, 
 O11W, O11M, O12W, O12M, O13W, O14W, O15W, O16W, O16M, O18W, O18M, O22W,
 O35, O35', O36, O36', C1, C1', C2, C2', N1 and N1' are refined 
 isostropicallly. 655 parameters and 73 restraints are used in
 the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0574P)²+71.9268P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          8997 
_refine_ls_number_parameters      655 
_refine_ls_number_restraints      73 
_refine_ls_R_factor_all           0.0572 
_refine_ls_R_factor_gt            0.0502 
_refine_ls_wR_factor_ref          0.1273 
_refine_ls_wR_factor_gt           0.1235 
_refine_ls_goodness_of_fit_ref    1.027 
_refine_ls_restrained_S_all       1.024 
_refine_ls_shift/su_max           0.002 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21343(5) 0.31173(5) 0.59522(4) 0.01343(15) Uani 1 1 d . . . 
W2 W 0.46796(5) 0.44210(5) 0.68077(4) 0.01277(15) Uani 1 1 d . . . 
W3 W 0.24673(5) 0.57499(5) 0.75513(4) 0.01240(15) Uani 1 1 d . . . 
W4 W 0.35715(4) 0.61374(4) 0.97134(4) 0.00958(14) Uani 1 1 d . . . 
W5 W 0.09519(5) 0.48715(5) 0.87863(4) 0.01162(14) Uani 1 1 d . . . 
W6 W 0.15114(5) 0.25743(5) 0.94419(4) 0.01333(15) Uani 1 1 d . . . 
W7 W 0.24825(5) 0.09088(5) 0.79087(4) 0.01391(15) Uani 1 1 d . . . 
W8 W 0.41462(5) 0.18434(5) 0.65418(4) 0.01479(15) Uani 1 1 d . . . 
W9 W 0.04427(5) 0.21447(5) 0.73135(4) 0.01239(15) Uani 1 1 d . . . 
Nd1 Nd 0.11650(8) 0.23378(8) 0.32795(6) 0.0302(2) Uani 1 1 d . . . 
As1 As 0.34012(11) 0.35986(11) 0.83588(9) 0.0083(3) Uani 1 1 d . . . 
Fe1 Fe 0.38158(16) 0.43033(16) 1.09924(13) 0.0113(4) Uani 1 1 d . . . 
O1W O 0.2416(9) 0.4519(10) 1.1538(8) 0.028(3) Uani 1 1 d . . . 
O2W O 0.4115(10) 0.3157(9) 1.1627(7) 0.026(3) Uani 1 1 d . . . 
O3W O 0.5520(12) 0.0463(10) 0.9296(9) 0.038(3) Uani 1 1 d U . . 
O4W O 0.6874(11) 0.1182(11) 0.8248(10) 0.047(4) Uani 1 1 d . . . 
O5W O 0.2553(16) 0.1427(15) 0.3806(13) 0.078(6) Uani 1 1 d . . . 
O6W O 0.2790(14) 0.3774(15) 0.4056(10) 0.065(5) Uani 1 1 d . . . 
O7W O -0.055(3) 0.180(3) 0.215(2) 0.086(9) Uiso 0.70 1 d P . . 
O7M O -0.070(3) 0.219(3) 0.332(3) 0.033(10) Uiso 0.30 1 d P . . 
O8W O 0.082(2) 0.048(2) 0.2095(18) 0.117(9) Uiso 1 1 d . . . 
O9W O 0.2409(18) 0.2229(19) 0.2246(14) 0.091(7) Uani 1 1 d . . . 
O10W O 0.094(3) 0.353(3) 0.237(2) 0.079(8) Uiso 0.70 1 d P . . 
O10M O 0.042(5) 0.298(5) 0.203(4) 0.055(14) Uiso 0.30 1 d P . . 
O11W O 0.045(3) 0.084(3) 0.378(2) 0.071(9) Uiso 0.60 1 d P . . 
O11M O -0.013(3) 0.111(3) 0.373(2) 0.031(7) Uiso 0.40 1 d P . . 
O12W O 0.047(3) 0.405(3) 0.384(2) 0.081(10) Uiso 0.60 1 d P . . 
O12M O -0.018(3) 0.345(3) 0.386(3) 0.052(10) Uiso 0.40 1 d P . . 
O13W O 0.116(2) -0.201(2) 0.9454(16) 0.104(8) Uiso 1 1 d . . . 
O14W O 0.208(4) 0.013(4) 1.077(3) 0.090(13) Uiso 0.50 1 d P . . 
O15W O 0.068(4) 0.529(4) 0.505(3) 0.086(12) Uiso 0.50 1 d P . . 
O16W O 0.305(3) -0.061(3) 0.359(2) 0.075(9) Uiso 0.60 1 d P . . 
O16M O 0.322(5) -0.130(5) 0.413(4) 0.11(2) Uiso 0.40 1 d P . . 
O17W O 0.3775(17) 0.1306(13) 1.0417(10) 0.067(5) Uani 1 1 d . . . 
O18W O 0.365(2) -0.1165(19) 0.8991(16) 0.057(6) Uiso 0.70 1 d P . . 
O18M O 0.303(4) -0.122(4) 0.915(3) 0.035(10) Uiso 0.30 1 d P . . 
O19W O -0.1659(10) 0.2895(11) 0.8701(8) 0.036(3) Uani 1 1 d . . . 
O20W O 0.7432(16) 0.3519(17) 0.7305(13) 0.085(7) Uani 1 1 d . . . 
O21W O -0.0961(19) 0.3974(15) 0.6332(12) 0.080(6) Uani 1 1 d . . . 
O22W O 0.1187(18) 0.0047(17) 0.5094(14) 0.083(6) Uiso 1 1 d . . . 
O23W O 0.1370(17) -0.2002(16) 0.5083(11) 0.074(6) Uani 1 1 d . . . 
O1 O 0.1333(9) 0.2894(8) 0.4918(7) 0.018(2) Uani 1 1 d . . . 
O2 O 0.2898(8) 0.1964(8) 0.5698(6) 0.014(2) Uani 1 1 d . . . 
O3 O 0.1849(8) 0.4401(8) 0.6665(6) 0.015(2) Uani 1 1 d U . . 
O4 O 0.3421(8) 0.3320(8) 0.7202(6) 0.011(2) Uani 1 1 d . . . 
O5 O 0.1154(8) 0.2390(8) 0.6420(6) 0.013(2) Uani 1 1 d . . . 
O6 O 0.3396(9) 0.3934(9) 0.5817(6) 0.019(2) Uani 1 1 d . . . 
O7 O 0.5552(10) 0.5120(10) 0.6382(7) 0.029(3) Uani 1 1 d . . . 
O8 O 0.4958(9) 0.2996(9) 0.6348(7) 0.021(2) Uani 1 1 d . . . 
O9 O 0.5447(8) 0.4620(8) 0.7908(6) 0.014(2) Uani 1 1 d U . . 
O10 O 0.3839(9) 0.5497(8) 0.7302(7) 0.020(2) Uani 1 1 d . . . 
O11 O 0.2223(9) 0.6640(9) 0.6997(7) 0.020(2) Uani 1 1 d U . . 
O12 O 0.1121(8) 0.5603(8) 0.7937(6) 0.014(2) Uani 1 1 d U . . 
O13 O 0.2743(7) 0.4733(7) 0.8511(6) 0.0085(19) Uani 1 1 d U . . 
O14 O 0.3148(8) 0.6693(8) 0.8681(6) 0.012(2) Uani 1 1 d U . . 
O15 O 0.4820(9) 0.5913(8) 0.9381(7) 0.020(2) Uani 1 1 d . . . 
O16 O 0.3553(9) 0.5280(8) 1.0373(7) 0.017(2) Uani 1 1 d U . . 
O17 O 0.3935(8) 0.7405(8) 1.0506(6) 0.016(2) Uani 1 1 d . . . 
O18 O 0.1935(8) 0.6011(8) 0.9645(6) 0.013(2) Uani 1 1 d . . . 
O19 O -0.0271(8) 0.5193(9) 0.8978(7) 0.021(2) Uani 1 1 d U . . 
O20 O 0.0484(8) 0.3629(8) 0.7757(6) 0.014(2) Uani 1 1 d . . . 
O21 O 0.1216(8) 0.3937(8) 0.9443(6) 0.014(2) Uani 1 1 d . . . 
O22 O 0.2226(8) 0.2626(7) 0.8199(6) 0.009(2) Uani 1 1 d . . . 
O23 O 0.2888(8) 0.3154(7) 1.0037(7) 0.012(2) Uani 1 1 d . . . 
O24 O 0.0859(9) 0.2383(9) 1.0250(7) 0.022(2) Uani 1 1 d . . . 
O25 O 0.0216(8) 0.2117(8) 0.8436(7) 0.015(2) Uani 1 1 d . . . 
O26 O 0.1826(8) 0.1197(8) 0.8939(7) 0.017(2) Uani 1 1 d . . . 
O27 O 0.2358(10) -0.0445(9) 0.7677(8) 0.026(3) Uani 1 1 d . . . 
O28 O 0.1019(8) 0.0877(8) 0.7200(7) 0.015(2) Uani 1 1 d . . . 
O29 O 0.3858(9) 0.1419(8) 0.8621(7) 0.018(2) Uani 1 1 d . . . 
O30 O 0.3039(9) 0.1071(8) 0.6940(7) 0.019(2) Uani 1 1 d U . . 
O31 O 0.4536(10) 0.0795(9) 0.5811(7) 0.026(3) Uani 1 1 d . . . 
O32 O 0.5066(9) 0.2074(9) 0.7597(7) 0.021(2) Uani 1 1 d . . . 
O33 O -0.0883(8) 0.1688(9) 0.6712(7) 0.022(2) Uani 1 1 d . . . 
O34 O 0.4816(10) -0.0059(9) 0.7478(8) 0.029(3) Uani 1 1 d DU . . 
Fe2 Fe 0.53352(17) 0.13563(16) 0.84587(14) 0.0149(5) Uani 1 1 d . . . 
O35 O 0.616(2) -0.041(2) 0.681(2) 0.049(8) Uiso 0.50 1 d PD A 1 
O36 O 0.513(3) -0.273(3) 0.670(3) 0.085(9) Uiso 0.50 1 d PD B 1 
H36 H 0.5360 -0.3288 0.6571 0.128 Uiso 0.50 1 d PR B 1 
N1 N 0.327(3) -0.148(3) 0.631(2) 0.043(6) Uiso 0.50 1 d PD A 1 
H1A H 0.2902 -0.1997 0.5834 0.051 Uiso 0.50 1 d PR A 1 
H1B H 0.3185 -0.1633 0.6787 0.051 Uiso 0.50 1 d PR A 1 
H1C H 0.3010 -0.0890 0.6318 0.051 Uiso 0.50 1 d PR A 1 
C1 C 0.522(2) -0.059(3) 0.692(2) 0.027(8) Uiso 0.50 1 d PD A 1 
C2 C 0.448(3) -0.147(2) 0.617(2) 0.037(7) Uiso 0.50 1 d PD A 1 
H2 H 0.4506 -0.1295 0.5627 0.045 Uiso 0.50 1 calc PR A 1 
C3 C 0.457(2) -0.259(2) 0.5984(17) 0.056(6) Uani 1 1 d DU . . 
C4 C 0.381(3) -0.344(2) 0.5316(19) 0.080(9) Uani 1 1 d U B . 
H4A H 0.3528 -0.3278 0.4798 0.120 Uiso 1 1 d R . . 
H4B H 0.4173 -0.4031 0.5160 0.120 Uiso 1 1 d R . . 
H4C H 0.3230 -0.3600 0.5587 0.120 Uiso 1 1 d R . . 
O35' O 0.557(3) -0.131(3) 0.771(3) 0.083(12) Uiso 0.50 1 d PD A 2 
O36' O 0.514(3) -0.215(3) 0.552(3) 0.085(9) Uiso 0.50 1 d PD B 2 
H36' H 0.4987 -0.1590 0.5474 0.128 Uiso 0.50 1 d PR B 2 
N1' N 0.347(3) -0.115(3) 0.596(2) 0.043(6) Uiso 0.50 1 d PD A 2 
H1'A H 0.2965 -0.1584 0.5512 0.064 Uiso 0.50 1 d PR A 2 
H1'B H 0.3152 -0.0679 0.6299 0.064 Uiso 0.50 1 d PR A 2 
H1'C H 0.3967 -0.0823 0.5767 0.064 Uiso 0.50 1 d PR A 2 
C1' C 0.490(3) -0.097(2) 0.728(2) 0.037(9) Uiso 0.50 1 d PD A 2 
C2' C 0.406(3) -0.178(3) 0.653(2) 0.037(7) Uiso 0.50 1 d PD A 2 
H2' H 0.3526 -0.2115 0.6780 0.045 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.735(10) . ? 
W1 O5 1.889(10) . ? 
W1 O3 1.901(10) . ? 
W1 O6 1.916(11) . ? 
W1 O2 1.916(10) . ? 
W1 O4 2.306(9) . ? 
W2 O7 1.731(12) . ? 
W2 O9 1.815(10) . ? 
W2 O8 1.956(11) . ? 
W2 O10 1.971(11) . ? 
W2 O6 1.978(10) . ? 
W2 O4 2.351(10) . ? 
W3 O11 1.734(10) . ? 
W3 O14 1.892(10) . ? 
W3 O10 1.898(11) . ? 
W3 O12 1.924(10) . ? 
W3 O3 1.941(10) . ? 
W3 O13 2.382(9) . ? 
W4 O17 1.771(10) . ? 
W4 O15 1.788(11) . ? 
W4 O16 1.803(10) . ? 
W4 O18 2.040(10) . ? 
W4 O14 2.057(9) . ? 
W4 O13 2.280(9) . ? 
W5 O19 1.713(11) . ? 
W5 O18 1.891(10) . ? 
W5 O21 1.908(10) . ? 
W5 O20 1.941(10) . ? 
W5 O12 1.951(10) . ? 
W5 O13 2.405(9) . ? 
W6 O24 1.733(11) . ? 
W6 O23 1.802(9) . ? 
W6 O26 1.926(11) . ? 
W6 O21 1.930(10) . ? 
W6 O25 2.003(10) . ? 
W6 O22 2.371(9) . ? 
W7 O27 1.745(11) . ? 
W7 O29 1.848(10) . ? 
W7 O30 1.893(11) . ? 
W7 O26 1.958(11) . ? 
W7 O28 2.000(10) . ? 
W7 O22 2.311(9) . ? 
W8 O31 1.748(11) . ? 
W8 O32 1.824(11) . ? 
W8 O8 1.903(11) . ? 
W8 O30 1.960(11) . ? 
W8 O2 1.970(10) . ? 
W8 O4 2.350(10) . ? 
W9 O33 1.732(10) . ? 
W9 O25 1.909(11) . ? 
W9 O28 1.919(10) . ? 
W9 O20 1.920(10) . ? 
W9 O5 1.924(10) . ? 
W9 O22 2.366(9) . ? 
Nd1 O7M 2.36(4) . ? 
Nd1 O5W 2.447(16) . ? 
Nd1 O7W 2.48(3) . ? 
Nd1 O9W 2.48(2) . ? 
Nd1 O10W 2.50(3) . ? 
Nd1 O1 2.516(11) . ? 
Nd1 O6W 2.517(16) . ? 
Nd1 O12M 2.53(4) . ? 
Nd1 O10M 2.53(6) . ? 
Nd1 O11W 2.53(3) . ? 
Nd1 O11M 2.54(3) . ? 
Nd1 O12W 2.55(4) . ? 
As1 O22 1.795(9) . ? 
As1 O13 1.811(9) . ? 
As1 O4 1.816(9) . ? 
Fe1 O16 1.914(10) . ? 
Fe1 O23 1.936(10) . ? 
Fe1 O9 1.945(10) 2_667 ? 
Fe1 O15 1.954(12) 2_667 ? 
Fe1 O1W 2.128(12) . ? 
Fe1 O2W 2.142(12) . ? 
O3W Fe2 2.078(12) . ? 
O4W Fe2 2.065(14) . ? 
O7M O12M 1.66(6) . ? 
O10W O10M 0.90(6) . ? 
O11W O11M 0.86(4) . ? 
O12W O12M 1.10(5) . ? 
O15W O15W 1.76(9) 2_566 ? 
O16W O16M 1.48(7) . ? 
O18W O18M 0.86(5) . ? 
O9 Fe1 1.945(10) 2_667 ? 
O15 Fe1 1.954(11) 2_667 ? 
O17 Fe2 1.990(10) 2_667 ? 
O29 Fe2 1.942(11) . ? 
O32 Fe2 1.940(11) . ? 
O34 C1' 1.20(3) . ? 
O34 C1 1.21(3) . ? 
O34 Fe2 2.052(12) . ? 
Fe2 O17 1.990(10) 2_667 ? 
O35 C1 1.23(4) . ? 
O36 C3 1.34(3) . ? 
O36 H36 0.8207 . ? 
N1 C2 1.59(4) . ? 
N1 H1A 0.8892 . ? 
N1 H1B 0.8872 . ? 
N1 H1C 0.8902 . ? 
N1 H1'A 1.2487 . ? 
N1 H1'B 1.1115 . ? 
C1 C2 1.51(4) . ? 
C2 C3 1.49(4) . ? 
C2 H2 0.9800 . ? 
C2 H36' 1.3741 . ? 
C2 H1'C 1.3907 . ? 
C3 O36' 1.35(3) . ? 
C3 C4 1.44(4) . ? 
C3 C2' 1.49(4) . ? 
C4 H4A 0.9572 . ? 
C4 H4B 0.9612 . ? 
C4 H4C 0.9586 . ? 
O35' C1' 1.23(4) . ? 
O36' H36' 0.8196 . ? 
N1' C2' 1.59(4) . ? 
N1' H1A 1.2195 . ? 
N1' H1C 0.9115 . ? 
N1' H1'A 0.8888 . ? 
N1' H1'B 0.8909 . ? 
N1' H1'C 0.8882 . ? 
C1' C2' 1.52(4) . ? 
C2' H1B 1.2651 . ? 
C2' H2' 0.9800 . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O5 99.5(5) . . ? 
O1 W1 O3 105.0(4) . . ? 
O5 W1 O3 88.9(4) . . ? 
O1 W1 O6 97.7(5) . . ? 
O5 W1 O6 162.9(4) . . ? 
O3 W1 O6 86.6(5) . . ? 
O1 W1 O2 99.9(4) . . ? 
O5 W1 O2 91.2(4) . . ? 
O3 W1 O2 154.7(4) . . ? 
O6 W1 O2 86.0(5) . . ? 
O1 W1 O4 170.4(4) . . ? 
O5 W1 O4 86.8(4) . . ? 
O3 W1 O4 82.2(4) . . ? 
O6 W1 O4 76.2(4) . . ? 
O2 W1 O4 72.5(4) . . ? 
O7 W2 O9 103.4(5) . . ? 
O7 W2 O8 102.1(5) . . ? 
O9 W2 O8 93.4(4) . . ? 
O7 W2 O10 100.6(5) . . ? 
O9 W2 O10 89.6(5) . . ? 
O8 W2 O10 155.7(5) . . ? 
O7 W2 O6 100.1(5) . . ? 
O9 W2 O6 156.3(5) . . ? 
O8 W2 O6 84.2(5) . . ? 
O10 W2 O6 83.4(5) . . ? 
O7 W2 O4 172.6(4) . . ? 
O9 W2 O4 82.7(4) . . ? 
O8 W2 O4 73.2(4) . . ? 
O10 W2 O4 83.4(4) . . ? 
O6 W2 O4 74.0(4) . . ? 
O11 W3 O14 99.6(5) . . ? 
O11 W3 O10 99.6(5) . . ? 
O14 W3 O10 91.0(4) . . ? 
O11 W3 O12 99.5(5) . . ? 
O14 W3 O12 89.6(4) . . ? 
O10 W3 O12 160.5(4) . . ? 
O11 W3 O3 103.5(5) . . ? 
O14 W3 O3 156.8(4) . . ? 
O10 W3 O3 86.7(4) . . ? 
O12 W3 O3 85.1(4) . . ? 
O11 W3 O13 170.7(4) . . ? 
O14 W3 O13 72.9(4) . . ? 
O10 W3 O13 86.2(4) . . ? 
O12 W3 O13 75.4(4) . . ? 
O3 W3 O13 83.9(4) . . ? 
O17 W4 O15 103.1(5) . . ? 
O17 W4 O16 103.3(5) . . ? 
O15 W4 O16 97.6(5) . . ? 
O17 W4 O18 95.9(4) . . ? 
O15 W4 O18 159.0(4) . . ? 
O16 W4 O18 86.4(4) . . ? 
O17 W4 O14 93.8(4) . . ? 
O15 W4 O14 89.3(4) . . ? 
O16 W4 O14 159.5(4) . . ? 
O18 W4 O14 80.6(4) . . ? 
O17 W4 O13 163.4(4) . . ? 
O15 W4 O13 86.4(4) . . ? 
O16 W4 O13 88.7(4) . . ? 
O18 W4 O13 73.1(4) . . ? 
O14 W4 O13 72.5(4) . . ? 
O19 W5 O18 101.0(5) . . ? 
O19 W5 O21 103.2(5) . . ? 
O18 W5 O21 93.0(4) . . ? 
O19 W5 O20 101.5(5) . . ? 
O18 W5 O20 157.1(4) . . ? 
O21 W5 O20 86.5(4) . . ? 
O19 W5 O12 97.7(5) . . ? 
O18 W5 O12 87.9(4) . . ? 
O21 W5 O12 158.5(4) . . ? 
O20 W5 O12 84.5(4) . . ? 
O19 W5 O13 169.8(4) . . ? 
O18 W5 O13 72.7(4) . . ? 
O21 W5 O13 85.3(4) . . ? 
O20 W5 O13 84.4(4) . . ? 
O12 W5 O13 74.4(4) . . ? 
O24 W6 O23 103.3(5) . . ? 
O24 W6 O26 101.0(5) . . ? 
O23 W6 O26 95.2(4) . . ? 
O24 W6 O21 100.9(5) . . ? 
O23 W6 O21 90.2(4) . . ? 
O26 W6 O21 155.5(4) . . ? 
O24 W6 O25 98.4(5) . . ? 
O23 W6 O25 157.8(4) . . ? 
O26 W6 O25 84.9(4) . . ? 
O21 W6 O25 81.2(4) . . ? 
O24 W6 O22 171.9(4) . . ? 
O23 W6 O22 83.7(4) . . ? 
O26 W6 O22 74.1(4) . . ? 
O21 W6 O22 82.9(4) . . ? 
O25 W6 O22 75.0(4) . . ? 
O27 W7 O29 103.3(5) . . ? 
O27 W7 O30 100.2(5) . . ? 
O29 W7 O30 89.7(5) . . ? 
O27 W7 O26 97.7(5) . . ? 
O29 W7 O26 90.8(5) . . ? 
O30 W7 O26 161.5(4) . . ? 
O27 W7 O28 96.2(5) . . ? 
O29 W7 O28 160.4(4) . . ? 
O30 W7 O28 86.1(4) . . ? 
O26 W7 O28 87.3(4) . . ? 
O27 W7 O22 166.9(5) . . ? 
O29 W7 O22 87.7(4) . . ? 
O30 W7 O22 86.6(4) . . ? 
O26 W7 O22 74.9(4) . . ? 
O28 W7 O22 73.0(4) . . ? 
O31 W8 O32 104.8(5) . . ? 
O31 W8 O8 100.5(5) . . ? 
O32 W8 O8 91.9(5) . . ? 
O31 W8 O30 99.8(5) . . ? 
O32 W8 O30 88.3(5) . . ? 
O8 W8 O30 158.9(5) . . ? 
O31 W8 O2 96.3(5) . . ? 
O32 W8 O2 158.6(5) . . ? 
O8 W8 O2 87.8(4) . . ? 
O30 W8 O2 84.5(4) . . ? 
O31 W8 O4 165.8(4) . . ? 
O32 W8 O4 88.6(4) . . ? 
O8 W8 O4 74.1(4) . . ? 
O30 W8 O4 84.8(4) . . ? 
O2 W8 O4 70.7(4) . . ? 
O33 W9 O25 99.1(5) . . ? 
O33 W9 O28 102.7(5) . . ? 
O25 W9 O28 87.7(4) . . ? 
O33 W9 O20 102.3(5) . . ? 
O25 W9 O20 86.2(4) . . ? 
O28 W9 O20 154.9(4) . . ? 
O33 W9 O5 100.2(5) . . ? 
O25 W9 O5 160.6(4) . . ? 
O28 W9 O5 90.0(4) . . ? 
O20 W9 O5 87.9(4) . . ? 
O33 W9 O22 174.0(4) . . ? 
O25 W9 O22 76.8(4) . . ? 
O28 W9 O22 73.0(4) . . ? 
O20 W9 O22 81.9(4) . . ? 
O5 W9 O22 84.1(4) . . ? 
O7M Nd1 O5W 130.6(12) . . ? 
O7M Nd1 O7W 45.5(12) . . ? 
O5W Nd1 O7W 135.1(9) . . ? 
O7M Nd1 O9W 141.7(12) . . ? 
O5W Nd1 O9W 76.0(8) . . ? 
O7W Nd1 O9W 96.4(9) . . ? 
O7M Nd1 O10W 90.1(13) . . ? 
O5W Nd1 O10W 138.9(9) . . ? 
O7W Nd1 O10W 66.4(11) . . ? 
O9W Nd1 O10W 65.7(9) . . ? 
O7M Nd1 O1 80.8(10) . . ? 
O5W Nd1 O1 75.3(6) . . ? 
O7W Nd1 O1 126.3(8) . . ? 
O9W Nd1 O1 137.2(6) . . ? 
O10W Nd1 O1 124.5(8) . . ? 
O7M Nd1 O6W 133.0(12) . . ? 
O5W Nd1 O6W 76.1(7) . . ? 
O7W Nd1 O6W 145.0(8) . . ? 
O9W Nd1 O6W 73.6(7) . . ? 
O10W Nd1 O6W 79.1(9) . . ? 
O1 Nd1 O6W 69.1(4) . . ? 
O7M Nd1 O12M 39.7(14) . . ? 
O5W Nd1 O12M 139.2(11) . . ? 
O7W Nd1 O12M 72.0(12) . . ? 
O9W Nd1 O12M 139.5(11) . . ? 
O10W Nd1 O12M 74.3(12) . . ? 
O1 Nd1 O12M 64.2(9) . . ? 
O6W Nd1 O12M 93.7(11) . . ? 
O7M Nd1 O10M 78.3(17) . . ? 
O5W Nd1 O10M 144.4(14) . . ? 
O7W Nd1 O10M 46.5(16) . . ? 
O9W Nd1 O10M 68.9(14) . . ? 
O10W Nd1 O10M 20.7(13) . . ? 
O1 Nd1 O10M 137.0(13) . . ? 
O6W Nd1 O10M 99.5(15) . . ? 
O12M Nd1 O10M 75.9(16) . . ? 
O7M Nd1 O11W 66.1(13) . . ? 
O5W Nd1 O11W 64.9(10) . . ? 
O7W Nd1 O11W 86.1(11) . . ? 
O9W Nd1 O11W 124.7(10) . . ? 
O10W Nd1 O11W 152.1(11) . . ? 
O1 Nd1 O11W 68.0(8) . . ? 
O6W Nd1 O11W 127.5(8) . . ? 
O12M Nd1 O11W 93.8(13) . . ? 
O10M Nd1 O11W 132.6(16) . . ? 
O7M Nd1 O11M 46.6(13) . . ? 
O5W Nd1 O11M 84.2(9) . . ? 
O7W Nd1 O11M 72.8(10) . . ? 
O9W Nd1 O11M 138.8(10) . . ? 
O10W Nd1 O11M 135.1(11) . . ? 
O1 Nd1 O11M 67.9(8) . . ? 
O6W Nd1 O11M 135.9(8) . . ? 
O12M Nd1 O11M 76.1(13) . . ? 
O10M Nd1 O11M 118.4(16) . . ? 
O11W Nd1 O11M 19.6(9) . . ? 
O7M Nd1 O12W 63.4(13) . . ? 
O5W Nd1 O12W 138.3(9) . . ? 
O7W Nd1 O12W 84.6(11) . . ? 
O9W Nd1 O12W 118.4(10) . . ? 
O10W Nd1 O12W 58.7(11) . . ? 
O1 Nd1 O12W 68.6(8) . . ? 
O6W Nd1 O12W 72.1(10) . . ? 
O12M Nd1 O12W 25.0(10) . . ? 
O10M Nd1 O12W 68.4(16) . . ? 
O11W Nd1 O12W 116.8(12) . . ? 
O11M Nd1 O12W 100.4(12) . . ? 
O22 As1 O13 98.4(4) . . ? 
O22 As1 O4 96.1(4) . . ? 
O13 As1 O4 98.7(4) . . ? 
O16 Fe1 O23 91.9(4) . . ? 
O16 Fe1 O9 94.3(4) . 2_667 ? 
O23 Fe1 O9 168.5(5) . 2_667 ? 
O16 Fe1 O15 93.4(5) . 2_667 ? 
O23 Fe1 O15 96.4(4) . 2_667 ? 
O9 Fe1 O15 92.9(4) 2_667 2_667 ? 
O16 Fe1 O1W 92.0(5) . . ? 
O23 Fe1 O1W 87.2(5) . . ? 
O9 Fe1 O1W 83.0(4) 2_667 . ? 
O15 Fe1 O1W 173.4(5) 2_667 . ? 
O16 Fe1 O2W 177.2(5) . . ? 
O23 Fe1 O2W 86.0(4) . . ? 
O9 Fe1 O2W 88.1(4) 2_667 . ? 
O15 Fe1 O2W 85.0(5) 2_667 . ? 
O1W Fe1 O2W 89.7(5) . . ? 
O12M O7M Nd1 76(2) . . ? 
O10M O10W Nd1 81(4) . . ? 
O10W O10M Nd1 78(4) . . ? 
O11M O11W Nd1 81(3) . . ? 
O11W O11M Nd1 79(3) . . ? 
O12M O12W Nd1 76(3) . . ? 
O12W O12M O7M 138(4) . . ? 
O12W O12M Nd1 79(3) . . ? 
O7M O12M Nd1 65(2) . . ? 
W1 O1 Nd1 148.3(6) . . ? 
W1 O2 W8 122.5(5) . . ? 
W1 O3 W3 146.2(6) . . ? 
As1 O4 W1 134.6(5) . . ? 
As1 O4 W8 116.8(5) . . ? 
W1 O4 W8 94.1(3) . . ? 
As1 O4 W2 118.3(4) . . ? 
W1 O4 W2 91.5(3) . . ? 
W8 O4 W2 91.4(3) . . ? 
W1 O5 W9 156.1(6) . . ? 
W1 O6 W2 117.9(5) . . ? 
W8 O8 W2 121.3(6) . . ? 
W2 O9 Fe1 143.1(6) . 2_667 ? 
W3 O10 W2 145.4(6) . . ? 
W3 O12 W5 120.7(5) . . ? 
As1 O13 W4 115.0(4) . . ? 
As1 O13 W3 127.6(5) . . ? 
W4 O13 W3 94.5(3) . . ? 
As1 O13 W5 127.8(5) . . ? 
W4 O13 W5 93.5(3) . . ? 
W3 O13 W5 89.4(3) . . ? 
W3 O14 W4 120.1(5) . . ? 
W4 O15 Fe1 178.6(7) . 2_667 ? 
W4 O16 Fe1 167.6(7) . . ? 
W4 O17 Fe2 163.9(6) . 2_667 ? 
W5 O18 W4 120.5(5) . . ? 
W9 O20 W5 144.8(6) . . ? 
W5 O21 W6 147.7(5) . . ? 
As1 O22 W7 117.0(5) . . ? 
As1 O22 W9 135.9(5) . . ? 
W7 O22 W9 93.3(3) . . ? 
As1 O22 W6 118.2(4) . . ? 
W7 O22 W6 91.5(3) . . ? 
W9 O22 W6 90.1(3) . . ? 
W6 O23 Fe1 145.9(6) . . ? 
W9 O25 W6 117.9(5) . . ? 
W6 O26 W7 119.5(5) . . ? 
W9 O28 W7 120.5(5) . . ? 
W7 O29 Fe2 135.3(6) . . ? 
W7 O30 W8 146.7(6) . . ? 
W8 O32 Fe2 137.7(6) . . ? 
C1' O34 C1 48(2) . . ? 
C1' O34 Fe2 143.3(18) . . ? 
C1 O34 Fe2 134.6(17) . . ? 
O32 Fe2 O29 88.5(5) . . ? 
O32 Fe2 O17 98.3(5) . 2_667 ? 
O29 Fe2 O17 96.7(4) . 2_667 ? 
O32 Fe2 O34 89.8(5) . . ? 
O29 Fe2 O34 91.0(5) . . ? 
O17 Fe2 O34 168.9(5) 2_667 . ? 
O32 Fe2 O4W 92.9(6) . . ? 
O29 Fe2 O4W 176.1(5) . . ? 
O17 Fe2 O4W 86.6(5) 2_667 . ? 
O34 Fe2 O4W 85.4(5) . . ? 
O32 Fe2 O3W 174.5(5) . . ? 
O29 Fe2 O3W 89.6(5) . . ? 
O17 Fe2 O3W 87.0(5) 2_667 . ? 
O34 Fe2 O3W 85.1(5) . . ? 
O4W Fe2 O3W 88.7(6) . . ? 
C3 O36 H36 111.3 . . ? 
C2 N1 H1A 101.1 . . ? 
C2 N1 H1B 111.9 . . ? 
H1A N1 H1B 109.4 . . ? 
C2 N1 H1C 115.1 . . ? 
H1A N1 H1C 109.6 . . ? 
H1B N1 H1C 109.3 . . ? 
C2 N1 H1'A 88.4 . . ? 
H1A N1 H1'A 44.8 . . ? 
H1B N1 H1'A 151.6 . . ? 
H1C N1 H1'A 76.9 . . ? 
C2 N1 H1'B 100.9 . . ? 
H1A N1 H1'B 115.0 . . ? 
H1B N1 H1'B 117.1 . . ? 
H1C N1 H1'B 14.2 . . ? 
H1'A N1 H1'B 75.8 . . ? 
O34 C1 O35 127(3) . . ? 
O34 C1 C2 118(3) . . ? 
O35 C1 C2 114(3) . . ? 
C3 C2 C1 123(3) . . ? 
C3 C2 N1 102(2) . . ? 
C1 C2 N1 108(3) . . ? 
C3 C2 H2 107.5 . . ? 
C1 C2 H2 107.5 . . ? 
N1 C2 H2 107.5 . . ? 
C3 C2 H36' 81.0 . . ? 
C1 C2 H36' 105.3 . . ? 
N1 C2 H36' 136.8 . . ? 
H2 C2 H36' 35.1 . . ? 
C3 C2 H1'C 139.6 . . ? 
C1 C2 H1'C 96.4 . . ? 
N1 C2 H1'C 69.2 . . ? 
H2 C2 H1'C 46.0 . . ? 
H36' C2 H1'C 80.9 . . ? 
O36 C3 O36' 117(3) . . ? 
O36 C3 C4 121(3) . . ? 
O36' C3 C4 103(3) . . ? 
O36 C3 C2 110(3) . . ? 
O36' C3 C2 69(3) . . ? 
C4 C3 C2 124(3) . . ? 
O36 C3 C2' 91(3) . . ? 
O36' C3 C2' 108(3) . . ? 
C4 C3 C2' 115(3) . . ? 
C2 C3 C2' 39(2) . . ? 
C3 C4 H4A 114.4 . . ? 
C3 C4 H4B 108.6 . . ? 
H4A C4 H4B 109.5 . . ? 
C3 C4 H4C 105.3 . . ? 
H4A C4 H4C 109.3 . . ? 
H4B C4 H4C 109.6 . . ? 
C3 O36' H36' 116.3 . . ? 
C2' N1' H1A 69.7 . . ? 
C2' N1' H1C 98.9 . . ? 
H1A N1' H1C 84.7 . . ? 
C2' N1' H1'A 110.8 . . ? 
H1A N1' H1'A 46.1 . . ? 
H1C N1' H1'A 98.1 . . ? 
C2' N1' H1'B 109.7 . . ? 
H1A N1' H1'B 105.5 . . ? 
H1C N1' H1'B 21.1 . . ? 
H1'A N1' H1'B 109.5 . . ? 
C2' N1' H1'C 107.8 . . ? 
H1A N1' H1'C 143.2 . . ? 
H1C N1' H1'C 130.6 . . ? 
H1'A N1' H1'C 109.5 . . ? 
H1'B N1' H1'C 109.5 . . ? 
O34 C1' O35' 123(3) . . ? 
O34 C1' C2' 120(3) . . ? 
O35' C1' C2' 116(3) . . ? 
C3 C2' C1' 112(3) . . ? 
C3 C2' N1' 111(3) . . ? 
C1' C2' N1' 107(3) . . ? 
C3 C2' H1B 142.0 . . ? 
C1' C2' H1B 101.6 . . ? 
N1' C2' H1B 73.4 . . ? 
C3 C2' H2' 109.0 . . ? 
C1' C2' H2' 109.0 . . ? 
N1' C2' H2' 109.0 . . ? 
H1B C2' H2' 40.7 . . ? 
  
_diffrn_measured_fraction_theta_max    0.984 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.984 
_refine_diff_density_max    2.884 
_refine_diff_density_min   -3.923 
_refine_diff_density_rms    0.436 
  



#===END

  
data_8-Sm 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Fe4 N2 O116 Sm2 W18' 
_chemical_formula_weight          6070.19 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Sm'  'Sm'  -0.1638   3.4418 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6577(16) 
_cell_length_b                    13.5693(17) 
_cell_length_c                    16.278(2) 
_cell_angle_alpha                 107.165(2) 
_cell_angle_beta                  99.801(2) 
_cell_angle_gamma                 96.896(2) 
_cell_volume                      2588.9(6) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8797 
_cell_measurement_theta_min       1.72 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky 
_exptl_crystal_colour             'Light yellow'   
_exptl_crystal_size_max           0.49 
_exptl_crystal_size_mid           0.34 
_exptl_crystal_size_min           0.17 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.893 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2722 
_exptl_absorpt_coefficient_mu     22.325 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0323 
_exptl_absorpt_correction_T_max   0.1156 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12546 
_diffrn_reflns_av_R_equivalents   0.0453 
_diffrn_reflns_av_sigmaI/netI     0.0812 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        14 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        8 
_diffrn_reflns_limit_l_min        -17 
_diffrn_reflns_limit_l_max        19 
_diffrn_reflns_theta_min          1.72 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8797 
_reflns_number_gt                 7351 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains
 a chiral L-thr ligand, theoretically its structure should be chiral.
 However, its structure is pseudo-centrosymmetric, i.e. most of the
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are 
 rather common. An attempt to refine the structure in P¨C1 shows the 
 disorder around the chiral centre of L-thr (because we impose inversion 
 on a chiral entity), as a result, C1, C2, N1, O35 and O36 atoms on L-thr
 are disordered over two positions. In addition, some coordination water
 molecules on Sm3+ cations are disordered over two positions. The ISOR
 instruction is used for O2, O12, O18, O25, O26, O29, O30, O33, C4, O17,
 O14, O24, O5, O28, O34, O22, O23, O13, O34 and O21. The SADI instruction
 is used for C2' C1' C2 C1, O34 C1' O34 C1, O35' C1' O35 C1, N1' C2' N1 C2,
 C3 C2' C3 C2, O36 C3 O36' C3, N1' C2' N1 C2. The EADP instruction is 
 used for C2 and C2', N1 and N1', O36 and O36'. The O7W, O7M, O8W, O10W,
 O10M, O11W, O11M, O12W, O12M, O13W, O14W, O15W, O16W, O16M, O18W, O18M,
 O22W, O35, O35', O36, O36', C1, C1', C2, C2', N1 and N1' are refined 
 isostropicallly. 656 parameters and 120 restraints are used in
 the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1029P)²+26.2448P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00014(5) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8797 
_refine_ls_number_parameters      656 
_refine_ls_number_restraints      120 
_refine_ls_R_factor_all           0.0718 
_refine_ls_R_factor_gt            0.0602 
_refine_ls_wR_factor_ref          0.1656 
_refine_ls_wR_factor_gt           0.1578 
_refine_ls_goodness_of_fit_ref    1.023 
_refine_ls_restrained_S_all       1.017 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21283(6) 0.31260(6) 0.59461(5) 0.01469(19) Uani 1 1 d . . . 
W2 W 0.46759(6) 0.44286(6) 0.68088(5) 0.01381(19) Uani 1 1 d . . . 
W3 W 0.24631(6) 0.57531(5) 0.75518(5) 0.01363(19) Uani 1 1 d . . . 
W4 W 0.35711(5) 0.61363(5) 0.97146(4) 0.01034(19) Uani 1 1 d . . . 
W5 W 0.09502(5) 0.48709(5) 0.87851(5) 0.01285(19) Uani 1 1 d . . . 
W6 W 0.15115(5) 0.25732(6) 0.94344(5) 0.01452(19) Uani 1 1 d . . . 
W7 W 0.24745(6) 0.09065(5) 0.78965(5) 0.0153(2) Uani 1 1 d . . . 
W8 W 0.41378(6) 0.18494(6) 0.65341(5) 0.0162(2) Uani 1 1 d . . . 
W9 W 0.04371(5) 0.21454(5) 0.73066(5) 0.01357(19) Uani 1 1 d . . . 
Sm1 Sm 0.11694(10) 0.23522(10) 0.32857(8) 0.0387(3) Uani 1 1 d . . . 
As1 As 0.33960(13) 0.36010(13) 0.83527(11) 0.0085(3) Uani 1 1 d . . . 
Fe1 Fe 0.38140(19) 0.42979(19) 1.09917(16) 0.0127(5) Uani 1 1 d . . . 
O1W O 0.2424(10) 0.4524(11) 1.1547(9) 0.027(3) Uani 1 1 d . . . 
O2W O 0.4091(13) 0.3160(10) 1.1624(9) 0.032(3) Uani 1 1 d . . . 
O3W O 0.5521(13) 0.0484(12) 0.9287(11) 0.042(4) Uani 1 1 d . . . 
O4W O 0.6881(12) 0.1211(13) 0.8242(12) 0.045(4) Uani 1 1 d . . . 
O5W O 0.2541(18) 0.147(2) 0.3833(19) 0.093(8) Uani 1 1 d . . . 
O6W O 0.272(2) 0.379(2) 0.4064(13) 0.089(8) Uani 1 1 d . . . 
O7W O -0.054(3) 0.190(3) 0.217(2) 0.082(9) Uiso 0.70 1 d P . . 
O7M O -0.059(5) 0.221(5) 0.333(4) 0.061(17) Uiso 0.30 1 d P . . 
O8W O 0.082(3) 0.048(3) 0.216(2) 0.122(10) Uiso 1 1 d . . . 
O9W O 0.247(2) 0.221(3) 0.2270(17) 0.107(9) Uani 1 1 d . . . 
O10W O 0.087(4) 0.335(3) 0.234(3) 0.097(12) Uiso 0.70 1 d P . . 
O10M O 0.021(8) 0.291(8) 0.199(6) 0.09(3) Uiso 0.30 1 d P . . 
O11W O 0.031(6) 0.105(6) 0.386(5) 0.14(2) Uiso 0.60 1 d P . . 
O11M O -0.010(3) 0.126(3) 0.371(3) 0.033(9) Uiso 0.40 1 d P . . 
O12W O 0.054(3) 0.398(3) 0.375(2) 0.060(8) Uiso 0.60 1 d P . . 
O12M O -0.013(3) 0.342(3) 0.385(3) 0.046(10) Uiso 0.40 1 d P . . 
O13W O 0.117(2) -0.200(2) 0.9401(18) 0.097(8) Uiso 1 1 d . . . 
O14W O 0.218(4) 0.020(4) 1.080(3) 0.071(12) Uiso 0.50 1 d P . . 
O15W O 0.099(10) 0.537(9) 0.494(8) 0.22(4) Uiso 0.50 1 d P . . 
O16W O 0.298(3) -0.056(3) 0.357(3) 0.079(12) Uiso 0.60 1 d P . . 
O16M O 0.294(9) -0.064(9) 0.403(8) 0.16(4) Uiso 0.40 1 d P . . 
O17W O 0.3781(19) 0.1331(14) 1.0417(11) 0.066(6) Uani 1 1 d . . . 
O18W O 0.364(3) -0.121(2) 0.898(2) 0.057(8) Uiso 0.70 1 d P . . 
O18M O 0.315(5) -0.129(4) 0.911(4) 0.036(13) Uiso 0.30 1 d P . . 
O19W O -0.1664(12) 0.2879(14) 0.8702(11) 0.043(4) Uani 1 1 d . . . 
O20W O 0.7385(19) 0.346(2) 0.7290(14) 0.087(8) Uani 1 1 d . . . 
O21W O -0.095(2) 0.403(2) 0.6341(14) 0.088(8) Uani 1 1 d . . . 
O22W O 0.117(2) 0.004(2) 0.5122(17) 0.086(7) Uiso 1 1 d . . . 
O23W O 0.1309(19) -0.1986(19) 0.5136(13) 0.077(7) Uani 1 1 d . . . 
O1 O 0.1341(10) 0.2935(10) 0.4903(8) 0.019(3) Uani 1 1 d . . . 
O2 O 0.2860(10) 0.1966(10) 0.5678(8) 0.018(3) Uani 1 1 d U . . 
O3 O 0.1856(10) 0.4424(10) 0.6676(8) 0.019(3) Uani 1 1 d . . . 
O4 O 0.3412(9) 0.3347(9) 0.7212(8) 0.013(2) Uani 1 1 d . . . 
O5 O 0.1136(9) 0.2364(9) 0.6388(8) 0.016(3) Uani 1 1 d U . . 
O6 O 0.3397(10) 0.3961(10) 0.5831(8) 0.020(3) Uani 1 1 d . . . 
O7 O 0.5555(11) 0.5150(11) 0.6397(10) 0.029(3) Uani 1 1 d . . . 
O8 O 0.4971(9) 0.3022(10) 0.6348(8) 0.017(3) Uani 1 1 d . . . 
O9 O 0.5443(9) 0.4614(9) 0.7899(8) 0.014(2) Uani 1 1 d . . . 
O10 O 0.3830(10) 0.5496(10) 0.7305(9) 0.021(3) Uani 1 1 d . . . 
O11 O 0.2218(9) 0.6642(11) 0.6988(8) 0.020(3) Uani 1 1 d . . . 
O12 O 0.1108(10) 0.5594(9) 0.7925(8) 0.016(3) Uani 1 1 d U . . 
O13 O 0.2731(9) 0.4731(9) 0.8507(8) 0.012(2) Uani 1 1 d U . . 
O14 O 0.3151(9) 0.6698(9) 0.8692(8) 0.017(3) Uani 1 1 d U . . 
O15 O 0.4820(9) 0.5908(9) 0.9385(8) 0.017(3) Uani 1 1 d . . . 
O16 O 0.3550(11) 0.5296(10) 1.0377(8) 0.022(3) Uani 1 1 d . . . 
O17 O 0.3951(9) 0.7413(9) 1.0525(7) 0.013(2) Uani 1 1 d U . . 
O18 O 0.1921(9) 0.6004(9) 0.9644(8) 0.014(2) Uani 1 1 d U . . 
O19 O -0.0272(10) 0.5186(11) 0.9000(9) 0.022(3) Uani 1 1 d . . . 
O20 O 0.0473(9) 0.3606(10) 0.7748(9) 0.020(3) Uani 1 1 d . . . 
O21 O 0.1218(9) 0.3936(9) 0.9433(8) 0.015(3) Uani 1 1 d U . . 
O22 O 0.2224(9) 0.2609(9) 0.8195(7) 0.011(2) Uani 1 1 d U . . 
O23 O 0.2881(9) 0.3139(9) 1.0036(8) 0.014(2) Uani 1 1 d U . . 
O24 O 0.0870(11) 0.2388(12) 1.0255(10) 0.033(3) Uani 1 1 d U . . 
O25 O 0.0239(9) 0.2128(10) 0.8442(8) 0.019(3) Uani 1 1 d U . . 
O26 O 0.1831(10) 0.1219(9) 0.8938(8) 0.018(3) Uani 1 1 d U . . 
O27 O 0.2355(12) -0.0421(11) 0.7670(9) 0.027(3) Uani 1 1 d . . . 
O28 O 0.1003(9) 0.0871(9) 0.7175(8) 0.016(3) Uani 1 1 d U . . 
O29 O 0.3849(9) 0.1411(10) 0.8607(8) 0.018(3) Uani 1 1 d U . . 
O30 O 0.3025(10) 0.1051(10) 0.6905(9) 0.021(3) Uani 1 1 d U . . 
O31 O 0.4537(12) 0.0802(11) 0.5807(9) 0.032(3) Uani 1 1 d . . . 
O32 O 0.5056(10) 0.2071(11) 0.7590(8) 0.021(3) Uani 1 1 d . . . 
O33 O -0.0876(9) 0.1676(10) 0.6706(9) 0.020(3) Uani 1 1 d U . . 
O34 O 0.4816(11) -0.0063(10) 0.7470(9) 0.026(3) Uani 1 1 d DU . . 
Fe2 Fe 0.5327(2) 0.13593(19) 0.84481(17) 0.0161(5) Uani 1 1 d . . . 
O35 O 0.611(2) -0.038(3) 0.681(2) 0.041(8) Uiso 0.50 1 d PD A 1 
O36 O 0.520(3) -0.271(4) 0.668(3) 0.073(8) Uiso 0.50 1 d PD B 1 
H36 H 0.5426 -0.3259 0.6558 0.109 Uiso 0.50 1 d PR B 1 
N1 N 0.328(3) -0.136(3) 0.625(3) 0.042(8) Uiso 0.50 1 d PD A 1 
H1A H 0.2915 -0.1887 0.5776 0.051 Uiso 0.50 1 d PR A 1 
H1B H 0.3198 -0.1522 0.6729 0.051 Uiso 0.50 1 d PR A 1 
H1C H 0.3024 -0.0779 0.6259 0.051 Uiso 0.50 1 d PR A 1 
C1 C 0.523(3) -0.056(3) 0.693(2) 0.021(8) Uiso 0.50 1 d PD A 1 
C2 C 0.444(3) -0.143(2) 0.616(3) 0.032(7) Uiso 0.50 1 d PD A 1 
H2 H 0.4520 -0.1272 0.5625 0.038 Uiso 0.50 1 calc PR A 1 
C3 C 0.459(3) -0.255(2) 0.600(2) 0.067(9) Uani 1 1 d D . . 
C4 C 0.386(3) -0.347(3) 0.532(2) 0.072(9) Uani 1 1 d U B . 
H4A H 0.3578 -0.3307 0.4805 0.108 Uiso 1 1 d R . . 
H4B H 0.4223 -0.4061 0.5167 0.108 Uiso 1 1 d R . . 
H4C H 0.3281 -0.3630 0.5593 0.108 Uiso 1 1 d R . . 
O35' O 0.557(5) -0.119(6) 0.776(4) 0.13(2) Uiso 0.50 1 d PD A 2 
O36' O 0.519(3) -0.216(4) 0.553(3) 0.073(8) Uiso 0.50 1 d PD B 2 
H36' H 0.5042 -0.1600 0.5482 0.109 Uiso 0.50 1 d PR B 2 
N1' N 0.348(3) -0.111(3) 0.596(3) 0.042(8) Uiso 0.50 1 d PD A 2 
H1'A H 0.2977 -0.1546 0.5506 0.063 Uiso 0.50 1 d PR A 2 
H1'B H 0.3164 -0.0641 0.6294 0.063 Uiso 0.50 1 d PR A 2 
H1'C H 0.3979 -0.0785 0.5761 0.063 Uiso 0.50 1 d PR A 2 
C1' C 0.493(3) -0.094(2) 0.727(3) 0.028(9) Uiso 0.50 1 d PD A 2 
C2' C 0.406(3) -0.171(3) 0.650(2) 0.032(7) Uiso 0.50 1 d PD A 2 
H2' H 0.3515 -0.2037 0.6750 0.038 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.745(12) . ? 
W1 O5 1.897(12) . ? 
W1 O2 1.899(12) . ? 
W1 O3 1.919(13) . ? 
W1 O6 1.921(13) . ? 
W1 O4 2.314(11) . ? 
W2 O7 1.739(14) . ? 
W2 O9 1.802(11) . ? 
W2 O8 1.941(12) . ? 
W2 O6 1.959(13) . ? 
W2 O10 1.968(12) . ? 
W2 O4 2.347(11) . ? 
W3 O11 1.743(12) . ? 
W3 O10 1.891(11) . ? 
W3 O14 1.904(12) . ? 
W3 O3 1.911(13) . ? 
W3 O12 1.925(12) . ? 
W3 O13 2.380(11) . ? 
W4 O16 1.786(11) . ? 
W4 O15 1.787(12) . ? 
W4 O17 1.791(11) . ? 
W4 O14 2.044(12) . ? 
W4 O18 2.055(11) . ? 
W4 O13 2.285(12) . ? 
W5 O19 1.719(12) . ? 
W5 O18 1.877(12) . ? 
W5 O21 1.900(11) . ? 
W5 O12 1.954(12) . ? 
W5 O20 1.964(14) . ? 
W5 O13 2.392(11) . ? 
W6 O24 1.740(13) . ? 
W6 O23 1.792(12) . ? 
W6 O26 1.899(12) . ? 
W6 O21 1.929(12) . ? 
W6 O25 1.967(12) . ? 
W6 O22 2.356(11) . ? 
W7 O27 1.711(13) . ? 
W7 O29 1.842(12) . ? 
W7 O30 1.914(13) . ? 
W7 O26 1.961(13) . ? 
W7 O28 2.013(12) . ? 
W7 O22 2.289(11) . ? 
W8 O31 1.749(14) . ? 
W8 O32 1.824(12) . ? 
W8 O8 1.930(11) . ? 
W8 O30 1.957(12) . ? 
W8 O2 2.003(12) . ? 
W8 O4 2.380(11) . ? 
W9 O33 1.717(12) . ? 
W9 O20 1.890(13) . ? 
W9 O25 1.914(12) . ? 
W9 O28 1.918(12) . ? 
W9 O5 1.938(12) . ? 
W9 O22 2.368(11) . ? 
Sm1 O7M 2.23(6) . ? 
Sm1 O10W 2.35(4) . ? 
Sm1 O11M 2.38(4) . ? 
Sm1 O12W 2.39(3) . ? 
Sm1 O5W 2.42(2) . ? 
Sm1 O12M 2.44(4) . ? 
Sm1 O6W 2.45(2) . ? 
Sm1 O11W 2.46(7) . ? 
Sm1 O7W 2.46(3) . ? 
Sm1 O1 2.478(12) . ? 
Sm1 O9W 2.51(3) . ? 
Sm1 O8W 2.59(3) . ? 
As1 O4 1.790(11) . ? 
As1 O22 1.808(11) . ? 
As1 O13 1.810(11) . ? 
Fe1 O16 1.935(12) . ? 
Fe1 O23 1.942(12) . ? 
Fe1 O15 1.954(12) 2_667 ? 
Fe1 O9 1.959(12) 2_667 ? 
Fe1 O2W 2.124(13) . ? 
Fe1 O1W 2.125(13) . ? 
O3W Fe2 2.061(14) . ? 
O4W Fe2 2.074(15) . ? 
O7W O10M 1.70(10) . ? 
O7M O12M 1.60(8) . ? 
O7M O11M 1.73(8) . ? 
O10W O10M 0.94(9) . ? 
O11W O11M 0.66(7) . ? 
O12W O12M 1.13(5) . ? 
O16W O16M 0.81(11) . ? 
O18W O18M 0.69(5) . ? 
O9 Fe1 1.959(12) 2_667 ? 
O15 Fe1 1.954(12) 2_667 ? 
O17 Fe2 1.969(12) 2_667 ? 
O29 Fe2 1.938(12) . ? 
O32 Fe2 1.927(12) . ? 
O34 C1' 1.18(3) . ? 
O34 C1 1.18(3) . ? 
O34 Fe2 2.053(14) . ? 
Fe2 O17 1.969(12) 2_667 ? 
O35 C1 1.17(4) . ? 
O36 C3 1.33(4) . ? 
N1 C2 1.51(4) . ? 
C1 C2 1.54(4) . ? 
C2 C3 1.50(4) . ? 
C3 O36' 1.34(4) . ? 
C3 C4 1.47(5) . ? 
C3 C2' 1.50(4) . ? 
O35' C1' 1.17(4) . ? 
N1' C2' 1.52(4) . ? 
C1' C2' 1.54(4) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O5 99.9(5) . . ? 
O1 W1 O2 99.8(5) . . ? 
O5 W1 O2 89.6(5) . . ? 
O1 W1 O3 104.7(5) . . ? 
O5 W1 O3 90.4(5) . . ? 
O2 W1 O3 155.1(5) . . ? 
O1 W1 O6 96.9(6) . . ? 
O5 W1 O6 163.2(5) . . ? 
O2 W1 O6 87.3(5) . . ? 
O3 W1 O6 85.5(5) . . ? 
O1 W1 O4 170.5(5) . . ? 
O5 W1 O4 87.6(4) . . ? 
O2 W1 O4 74.2(4) . . ? 
O3 W1 O4 80.9(5) . . ? 
O6 W1 O4 75.7(4) . . ? 
O7 W2 O9 102.9(6) . . ? 
O7 W2 O8 102.2(6) . . ? 
O9 W2 O8 92.8(5) . . ? 
O7 W2 O6 100.6(6) . . ? 
O9 W2 O6 156.3(5) . . ? 
O8 W2 O6 85.3(5) . . ? 
O7 W2 O10 100.2(6) . . ? 
O9 W2 O10 90.1(5) . . ? 
O8 W2 O10 156.1(5) . . ? 
O6 W2 O10 82.6(5) . . ? 
O7 W2 O4 174.0(6) . . ? 
O9 W2 O4 82.4(5) . . ? 
O8 W2 O4 74.6(4) . . ? 
O6 W2 O4 74.2(5) . . ? 
O10 W2 O4 82.3(5) . . ? 
O11 W3 O10 99.7(6) . . ? 
O11 W3 O14 100.2(6) . . ? 
O10 W3 O14 91.0(6) . . ? 
O11 W3 O3 103.2(6) . . ? 
O10 W3 O3 86.5(5) . . ? 
O14 W3 O3 156.6(5) . . ? 
O11 W3 O12 99.6(5) . . ? 
O10 W3 O12 160.2(5) . . ? 
O14 W3 O12 90.2(5) . . ? 
O3 W3 O12 84.6(5) . . ? 
O11 W3 O13 171.2(5) . . ? 
O10 W3 O13 86.1(5) . . ? 
O14 W3 O13 72.9(4) . . ? 
O3 W3 O13 83.7(5) . . ? 
O12 W3 O13 75.4(4) . . ? 
O16 W4 O15 97.7(6) . . ? 
O16 W4 O17 102.3(6) . . ? 
O15 W4 O17 102.8(5) . . ? 
O16 W4 O14 160.0(5) . . ? 
O15 W4 O14 89.7(5) . . ? 
O17 W4 O14 94.0(5) . . ? 
O16 W4 O18 86.1(5) . . ? 
O15 W4 O18 159.0(5) . . ? 
O17 W4 O18 96.5(5) . . ? 
O14 W4 O18 80.7(5) . . ? 
O16 W4 O13 89.1(5) . . ? 
O15 W4 O13 86.7(5) . . ? 
O17 W4 O13 163.8(4) . . ? 
O14 W4 O13 72.7(4) . . ? 
O18 W4 O13 72.7(4) . . ? 
O19 W5 O18 100.2(6) . . ? 
O19 W5 O21 102.3(6) . . ? 
O18 W5 O21 93.1(5) . . ? 
O19 W5 O12 98.8(5) . . ? 
O18 W5 O12 88.6(5) . . ? 
O21 W5 O12 158.2(5) . . ? 
O19 W5 O20 101.9(6) . . ? 
O18 W5 O20 157.6(5) . . ? 
O21 W5 O20 85.7(5) . . ? 
O12 W5 O20 84.6(5) . . ? 
O19 W5 O13 170.5(5) . . ? 
O18 W5 O13 73.2(4) . . ? 
O21 W5 O13 85.1(4) . . ? 
O12 W5 O13 74.6(4) . . ? 
O20 W5 O13 84.4(4) . . ? 
O24 W6 O23 102.1(6) . . ? 
O24 W6 O26 101.4(6) . . ? 
O23 W6 O26 94.6(5) . . ? 
O24 W6 O21 101.0(6) . . ? 
O23 W6 O21 90.8(5) . . ? 
O26 W6 O21 155.3(5) . . ? 
O24 W6 O25 99.1(6) . . ? 
O23 W6 O25 158.3(5) . . ? 
O26 W6 O25 85.3(5) . . ? 
O21 W6 O25 81.0(5) . . ? 
O24 W6 O22 172.2(6) . . ? 
O23 W6 O22 84.3(5) . . ? 
O26 W6 O22 73.3(4) . . ? 
O21 W6 O22 83.3(4) . . ? 
O25 W6 O22 74.9(4) . . ? 
O27 W7 O29 102.9(6) . . ? 
O27 W7 O30 99.6(6) . . ? 
O29 W7 O30 90.3(5) . . ? 
O27 W7 O26 98.5(6) . . ? 
O29 W7 O26 90.3(5) . . ? 
O30 W7 O26 161.3(5) . . ? 
O27 W7 O28 96.3(6) . . ? 
O29 W7 O28 160.7(5) . . ? 
O30 W7 O28 85.4(5) . . ? 
O26 W7 O28 88.0(5) . . ? 
O27 W7 O22 167.0(6) . . ? 
O29 W7 O22 87.8(5) . . ? 
O30 W7 O22 87.5(5) . . ? 
O26 W7 O22 73.9(4) . . ? 
O28 W7 O22 73.3(4) . . ? 
O31 W8 O32 104.2(6) . . ? 
O31 W8 O8 100.6(6) . . ? 
O32 W8 O8 91.7(6) . . ? 
O31 W8 O30 98.8(6) . . ? 
O32 W8 O30 89.0(6) . . ? 
O8 W8 O30 159.8(5) . . ? 
O31 W8 O2 96.8(6) . . ? 
O32 W8 O2 158.6(5) . . ? 
O8 W8 O2 88.6(5) . . ? 
O30 W8 O2 83.6(5) . . ? 
O31 W8 O4 166.4(5) . . ? 
O32 W8 O4 88.6(5) . . ? 
O8 W8 O4 74.0(4) . . ? 
O30 W8 O4 85.9(5) . . ? 
O2 W8 O4 71.0(4) . . ? 
O33 W9 O20 102.9(6) . . ? 
O33 W9 O25 100.1(6) . . ? 
O20 W9 O25 85.7(5) . . ? 
O33 W9 O28 101.4(5) . . ? 
O20 W9 O28 155.7(5) . . ? 
O25 W9 O28 88.1(5) . . ? 
O33 W9 O5 99.4(5) . . ? 
O20 W9 O5 89.1(5) . . ? 
O25 W9 O5 160.5(5) . . ? 
O28 W9 O5 88.9(5) . . ? 
O33 W9 O22 172.9(5) . . ? 
O20 W9 O22 82.6(5) . . ? 
O25 W9 O22 75.5(4) . . ? 
O28 W9 O22 73.1(4) . . ? 
O5 W9 O22 85.2(4) . . ? 
O7M Sm1 O10W 88(2) . . ? 
O7M Sm1 O11M 44(2) . . ? 
O10W Sm1 O11M 130.0(15) . . ? 
O7M Sm1 O12W 64.9(19) . . ? 
O10W Sm1 O12W 58.8(13) . . ? 
O11M Sm1 O12W 100.4(13) . . ? 
O7M Sm1 O5W 130.0(18) . . ? 
O10W Sm1 O5W 140.6(12) . . ? 
O11M Sm1 O5W 86.4(12) . . ? 
O12W Sm1 O5W 138.8(10) . . ? 
O7M Sm1 O12M 40(2) . . ? 
O10W Sm1 O12M 75.5(14) . . ? 
O11M Sm1 O12M 73.6(14) . . ? 
O12W Sm1 O12M 27.1(11) . . ? 
O5W Sm1 O12M 138.1(13) . . ? 
O7M Sm1 O6W 131(2) . . ? 
O10W Sm1 O6W 83.3(13) . . ? 
O11M Sm1 O6W 135.6(11) . . ? 
O12W Sm1 O6W 69.9(11) . . ? 
O5W Sm1 O6W 77.0(9) . . ? 
O12M Sm1 O6W 92.0(13) . . ? 
O7M Sm1 O11W 59(2) . . ? 
O10W Sm1 O11W 145(2) . . ? 
O11M Sm1 O11W 15.5(16) . . ? 
O12W Sm1 O11W 111.6(18) . . ? 
O5W Sm1 O11W 70.9(18) . . ? 
O12M Sm1 O11W 85.8(19) . . ? 
O6W Sm1 O11W 127.7(17) . . ? 
O7M Sm1 O7W 45.3(19) . . ? 
O10W Sm1 O7W 60.0(14) . . ? 
O11M Sm1 O7W 72.9(13) . . ? 
O12W Sm1 O7W 81.5(11) . . ? 
O5W Sm1 O7W 138.2(10) . . ? 
O12M Sm1 O7W 70.3(13) . . ? 
O6W Sm1 O7W 141.9(10) . . ? 
O11W Sm1 O7W 85.7(18) . . ? 
O7M Sm1 O1 80.8(18) . . ? 
O10W Sm1 O1 127.4(11) . . ? 
O11M Sm1 O1 68.5(11) . . ? 
O12W Sm1 O1 70.2(8) . . ? 
O5W Sm1 O1 75.0(8) . . ? 
O12M Sm1 O1 63.6(10) . . ? 
O6W Sm1 O1 67.5(6) . . ? 
O11W Sm1 O1 65.0(17) . . ? 
O7W Sm1 O1 126.0(9) . . ? 
O7M Sm1 O9W 143.5(19) . . ? 
O10W Sm1 O9W 67.4(13) . . ? 
O11M Sm1 O9W 139.7(12) . . ? 
O12W Sm1 O9W 117.4(11) . . ? 
O5W Sm1 O9W 74.6(10) . . ? 
O12M Sm1 O9W 141.6(13) . . ? 
O6W Sm1 O9W 74.6(9) . . ? 
O11W Sm1 O9W 131.0(18) . . ? 
O7W Sm1 O9W 98.2(10) . . ? 
O1 Sm1 O9W 135.5(7) . . ? 
O7M Sm1 O8W 91(2) . . ? 
O10W Sm1 O8W 100.9(13) . . ? 
O11M Sm1 O8W 71.8(13) . . ? 
O12W Sm1 O8W 146.9(11) . . ? 
O5W Sm1 O8W 73.8(10) . . ? 
O12M Sm1 O8W 129.8(13) . . ? 
O6W Sm1 O8W 137.9(10) . . ? 
O11W Sm1 O8W 68.7(18) . . ? 
O7W Sm1 O8W 65.4(11) . . ? 
O1 Sm1 O8W 130.3(8) . . ? 
O9W Sm1 O8W 69.0(10) . . ? 
O4 As1 O22 96.7(5) . . ? 
O4 As1 O13 98.0(5) . . ? 
O22 As1 O13 98.8(5) . . ? 
O16 Fe1 O23 92.8(5) . . ? 
O16 Fe1 O15 93.2(5) . 2_667 ? 
O23 Fe1 O15 96.6(5) . 2_667 ? 
O16 Fe1 O9 93.6(5) . 2_667 ? 
O23 Fe1 O9 168.3(5) . 2_667 ? 
O15 Fe1 O9 92.8(5) 2_667 2_667 ? 
O16 Fe1 O2W 178.0(6) . . ? 
O23 Fe1 O2W 85.4(5) . . ? 
O15 Fe1 O2W 86.2(6) 2_667 . ? 
O9 Fe1 O2W 88.3(5) 2_667 . ? 
O16 Fe1 O1W 91.7(6) . . ? 
O23 Fe1 O1W 87.5(5) . . ? 
O15 Fe1 O1W 173.4(5) 2_667 . ? 
O9 Fe1 O1W 82.5(5) 2_667 . ? 
O2W Fe1 O1W 89.1(6) . . ? 
O10M O7W Sm1 75(4) . . ? 
O12M O7M O11M 120(5) . . ? 
O12M O7M Sm1 77(3) . . ? 
O11M O7M Sm1 73(3) . . ? 
O10M O10W Sm1 95(6) . . ? 
O10W O10M O7W 129(9) . . ? 
O10W O10M Sm1 64(6) . . ? 
O7W O10M Sm1 66(3) . . ? 
O11M O11W Sm1 75(8) . . ? 
O11W O11M O7M 152(9) . . ? 
O11W O11M Sm1 89(8) . . ? 
O7M O11M Sm1 63(3) . . ? 
O12M O12W Sm1 79(3) . . ? 
O12W O12M O7M 130(4) . . ? 
O12W O12M Sm1 74(3) . . ? 
O7M O12M Sm1 63(3) . . ? 
W1 O1 Sm1 148.4(6) . . ? 
W1 O2 W8 121.5(6) . . ? 
W3 O3 W1 146.9(7) . . ? 
As1 O4 W1 135.4(6) . . ? 
As1 O4 W2 119.3(6) . . ? 
W1 O4 W2 91.4(4) . . ? 
As1 O4 W8 116.2(5) . . ? 
W1 O4 W8 93.0(4) . . ? 
W2 O4 W8 90.7(4) . . ? 
W1 O5 W9 153.3(7) . . ? 
W1 O6 W2 118.5(6) . . ? 
W8 O8 W2 120.7(6) . . ? 
W2 O9 Fe1 142.4(6) . 2_667 ? 
W3 O10 W2 146.0(7) . . ? 
W3 O12 W5 120.2(6) . . ? 
As1 O13 W4 114.7(5) . . ? 
As1 O13 W3 127.4(6) . . ? 
W4 O13 W3 94.3(4) . . ? 
As1 O13 W5 128.2(6) . . ? 
W4 O13 W5 93.6(4) . . ? 
W3 O13 W5 89.6(4) . . ? 
W3 O14 W4 120.0(6) . . ? 
W4 O15 Fe1 177.9(7) . 2_667 ? 
W4 O16 Fe1 167.0(8) . . ? 
W4 O17 Fe2 164.6(7) . 2_667 ? 
W5 O18 W4 120.3(6) . . ? 
W9 O20 W5 145.3(7) . . ? 
W5 O21 W6 148.2(7) . . ? 
As1 O22 W7 117.7(5) . . ? 
As1 O22 W6 118.0(6) . . ? 
W7 O22 W6 92.3(4) . . ? 
As1 O22 W9 134.7(5) . . ? 
W7 O22 W9 93.7(4) . . ? 
W6 O22 W9 90.2(4) . . ? 
W6 O23 Fe1 145.8(7) . . ? 
W9 O25 W6 119.1(6) . . ? 
W6 O26 W7 120.5(6) . . ? 
W9 O28 W7 119.6(6) . . ? 
W7 O29 Fe2 135.7(7) . . ? 
W7 O30 W8 144.6(8) . . ? 
W8 O32 Fe2 138.2(8) . . ? 
C1' O34 C1 48(2) . . ? 
C1' O34 Fe2 143(2) . . ? 
C1 O34 Fe2 133.4(19) . . ? 
O32 Fe2 O29 88.6(5) . . ? 
O32 Fe2 O17 98.4(5) . 2_667 ? 
O29 Fe2 O17 97.0(5) . 2_667 ? 
O32 Fe2 O34 90.1(6) . . ? 
O29 Fe2 O34 90.9(5) . . ? 
O17 Fe2 O34 168.5(5) 2_667 . ? 
O32 Fe2 O3W 174.9(6) . . ? 
O29 Fe2 O3W 89.6(6) . . ? 
O17 Fe2 O3W 86.6(6) 2_667 . ? 
O34 Fe2 O3W 85.1(6) . . ? 
O32 Fe2 O4W 92.5(6) . . ? 
O29 Fe2 O4W 176.7(6) . . ? 
O17 Fe2 O4W 85.9(6) 2_667 . ? 
O34 Fe2 O4W 86.0(6) . . ? 
O3W Fe2 O4W 89.0(7) . . ? 
O35 C1 O34 129(4) . . ? 
O35 C1 C2 115(3) . . ? 
O34 C1 C2 115(3) . . ? 
C3 C2 N1 108(3) . . ? 
C3 C2 C1 120(3) . . ? 
N1 C2 C1 109(3) . . ? 
O36 C3 O36' 112(4) . . ? 
O36 C3 C4 118(3) . . ? 
O36' C3 C4 103(3) . . ? 
O36 C3 C2 113(3) . . ? 
O36' C3 C2 73(3) . . ? 
C4 C3 C2 125(3) . . ? 
O36 C3 C2' 98(3) . . ? 
O36' C3 C2' 109(3) . . ? 
C4 C3 C2' 117(3) . . ? 
C2 C3 C2' 36(2) . . ? 
O35' C1' O34 118(5) . . ? 
O35' C1' C2' 125(4) . . ? 
O34 C1' C2' 115(3) . . ? 
C3 C2' N1' 115(3) . . ? 
C3 C2' C1' 108(3) . . ? 
N1' C2' C1' 110(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.964 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.964 
_refine_diff_density_max    4.027 
_refine_diff_density_min   -4.951 
_refine_diff_density_rms    0.545 
  


#===END

  
data_9-Eu 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Eu2 Fe4 N2 O116 W18' 
_chemical_formula_weight          6073.41 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Eu'  'Eu'  -0.1578   3.6682 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6292(14) 
_cell_length_b                    13.5134(15) 
_cell_length_c                    16.1999(18) 
_cell_angle_alpha                 106.993(2) 
_cell_angle_beta                  99.753(2) 
_cell_angle_gamma                 97.011(2) 
_cell_volume                      2562.3(5) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8691 
_cell_measurement_theta_min       1.66 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky 
_exptl_crystal_colour             'Light yellow'  
_exptl_crystal_size_max           0.45 
_exptl_crystal_size_mid           0.26 
_exptl_crystal_size_min           0.21 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.936 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2724 
_exptl_absorpt_coefficient_mu     22.635 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0350 
_exptl_absorpt_correction_T_max   0.0874 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none
_diffrn_standards_number          none  
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12504 
_diffrn_reflns_av_R_equivalents   0.0372 
_diffrn_reflns_av_sigmaI/netI     0.0691 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -19 
_diffrn_reflns_limit_l_max        15 
_diffrn_reflns_theta_min          1.66 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8691 
_reflns_number_gt                 7817 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral.
 However, its structure is pseudo-centrosymmetric, i.e. most of the
 structure fits space group P¨C1, therefore, its structure was solved and
 refined in centrosymmetric space group P¨C1. Such phenomena are rather
 common. An attempt to refine the structure in P¨C1 shows the disorder
 around the chiral centre of L-thr (because we impose inversion on a chiral
 entity), as a result, C1, C2, N1, O35 and O36 atoms on L-thr are
 disordered over two positions. In addition, some coordination water
 molecules on Eu3+ cations are disordered over two positions. The ISOR
 instruction is used for O1, O20, O30, O11, O12, O5, O21W, O1W, N1, C4,
 O7, O26, O29, O30, O2, O16, O21, O27, O33, O25, O9, O24, W2, O10, O23, O4,
 O8, O18, O22, O16 and O6. The SADI instruction is used for C2' C1' C2 C1,
 O34 C1' O34 C1, O35' C1' O35 C1, N1' C2' N1 C2, C3 C2' C3 C2, O36 C3 O36'
 C3, N1' C2' N1 C2. The EADP instruction is used for C2 and C2', N1 and N1',
 O36 and O36'. The As1, O7W, O7M, O8W, O10W, O10M, O11W, O11M, O12W, O12M,
 O13W, O14W, O15W, O16W, O16M, O18W, O18M, O22W, O35, O35', O36, O36', C1,
 C1', C2, C2', N1 and N1' are refined isostropicallly. 651 parameters and
 186 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1286P)²+77.2216P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00042(7) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8691 
_refine_ls_number_parameters      651 
_refine_ls_number_restraints      186 
_refine_ls_R_factor_all           0.0739 
_refine_ls_R_factor_gt            0.0681 
_refine_ls_wR_factor_ref          0.1890 
_refine_ls_wR_factor_gt           0.1836 
_refine_ls_goodness_of_fit_ref    1.048 
_refine_ls_restrained_S_all       1.042 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21204(6) 0.31146(6) 0.59461(5) 0.0123(2) Uani 1 1 d . . . 
W2 W 0.46713(6) 0.44223(6) 0.68019(5) 0.0116(2) Uani 1 1 d U . . 
W3 W 0.24576(6) 0.57477(6) 0.75417(5) 0.0114(2) Uani 1 1 d . . . 
W4 W 0.35701(5) 0.61348(5) 0.97102(5) 0.0086(2) Uani 1 1 d . . . 
W5 W 0.09454(6) 0.48656(6) 0.87848(5) 0.0106(2) Uani 1 1 d . . . 
W6 W 0.15070(6) 0.25673(6) 0.94473(5) 0.0127(2) Uani 1 1 d . . . 
W7 W 0.24704(6) 0.08989(6) 0.79103(5) 0.0127(2) Uani 1 1 d . . . 
W8 W 0.41356(6) 0.18405(6) 0.65376(5) 0.0139(2) Uani 1 1 d . . . 
W9 W 0.04281(6) 0.21353(6) 0.73146(5) 0.0115(2) Uani 1 1 d . . . 
Eu1 Eu 0.11714(10) 0.23719(10) 0.32926(8) 0.0324(3) Uani 1 1 d . . . 
As1 As 0.33929(13) 0.35953(13) 0.83556(12) 0.0065(4) Uiso 1 1 d . . . 
Fe1 Fe 0.38125(19) 0.4298(2) 1.09995(17) 0.0101(5) Uani 1 1 d . . . 
O1W O 0.2403(11) 0.4503(12) 1.1550(10) 0.025(3) Uani 1 1 d U . . 
O2W O 0.4100(14) 0.3177(12) 1.1624(10) 0.029(4) Uani 1 1 d . . . 
O3W O 0.5527(15) 0.0491(12) 0.9324(12) 0.036(4) Uani 1 1 d . . . 
O4W O 0.6873(12) 0.1192(12) 0.8259(12) 0.036(4) Uani 1 1 d . . . 
O5W O 0.252(2) 0.143(2) 0.379(3) 0.123(15) Uani 1 1 d . . . 
O6W O 0.2758(18) 0.3795(18) 0.4098(15) 0.062(6) Uani 1 1 d . . . 
O7W O -0.051(4) 0.178(4) 0.218(3) 0.102(14) Uiso 0.70 1 d P . . 
O7M O -0.061(5) 0.218(5) 0.334(4) 0.042(14) Uiso 0.30 1 d P . . 
O8W O 0.073(5) 0.061(5) 0.211(4) 0.19(2) Uiso 1 1 d . . . 
O9W O 0.239(2) 0.226(3) 0.2288(17) 0.096(10) Uani 1 1 d . . . 
O10W O 0.084(4) 0.343(4) 0.236(4) 0.107(16) Uiso 0.70 1 d P . . 
O10M O 0.036(6) 0.295(6) 0.201(5) 0.055(18) Uiso 0.30 1 d P . . 
O11W O 0.049(5) 0.083(4) 0.365(4) 0.092(15) Uiso 0.60 1 d P . . 
O11M O -0.005(4) 0.116(3) 0.372(3) 0.035(10) Uiso 0.40 1 d P . . 
O12W O 0.048(5) 0.406(5) 0.379(4) 0.116(19) Uiso 0.60 1 d P . . 
O12M O -0.009(4) 0.342(4) 0.388(4) 0.054(13) Uiso 0.40 1 d P . . 
O13W O 0.113(3) -0.193(3) 0.943(3) 0.123(12) Uiso 1 1 d . . . 
O14W O 0.206(5) 0.021(5) 1.080(4) 0.093(17) Uiso 0.50 1 d P . . 
O15W O 0.068(6) 0.521(5) 0.506(5) 0.11(2) Uiso 0.50 1 d P . . 
O16W O 0.301(3) -0.054(3) 0.353(3) 0.062(10) Uiso 0.60 1 d P . . 
O16M O 0.325(6) -0.138(6) 0.417(5) 0.09(2) Uiso 0.40 1 d P . . 
O17W O 0.376(2) 0.1327(16) 1.0429(13) 0.068(8) Uani 1 1 d . . . 
O18W O 0.367(3) -0.122(2) 0.897(2) 0.052(7) Uiso 0.70 1 d P . . 
O18M O 0.305(5) -0.125(4) 0.913(4) 0.035(13) Uiso 0.30 1 d P . . 
O19W O -0.1652(13) 0.2890(15) 0.8703(13) 0.044(5) Uani 1 1 d . . . 
O20W O 0.7382(18) 0.347(2) 0.7249(15) 0.068(7) Uani 1 1 d . . . 
O21W O -0.0940(19) 0.3981(18) 0.6336(14) 0.060(6) Uani 1 1 d U . . 
O22W O 0.118(2) 0.004(2) 0.5100(18) 0.074(7) Uiso 1 1 d . . . 
O23W O 0.137(3) -0.202(2) 0.5090(16) 0.085(8) Uani 1 1 d . . . 
O1 O 0.1331(11) 0.2905(11) 0.4908(10) 0.023(3) Uani 1 1 d U . . 
O2 O 0.2872(11) 0.1962(11) 0.5681(9) 0.017(3) Uani 1 1 d U . . 
O3 O 0.1826(10) 0.4402(10) 0.6657(10) 0.018(3) Uani 1 1 d . . . 
O4 O 0.3415(10) 0.3314(10) 0.7193(9) 0.014(3) Uani 1 1 d U . . 
O5 O 0.1130(10) 0.2363(10) 0.6414(8) 0.011(3) Uani 1 1 d U . . 
O6 O 0.3393(11) 0.3957(10) 0.5833(9) 0.017(3) Uani 1 1 d U . . 
O7 O 0.5557(12) 0.5139(12) 0.6405(11) 0.028(3) Uani 1 1 d U . . 
O8 O 0.4965(10) 0.3017(10) 0.6338(9) 0.016(3) Uani 1 1 d U . . 
O9 O 0.5437(10) 0.4609(10) 0.7893(9) 0.016(3) Uani 1 1 d U . . 
O10 O 0.3844(10) 0.5464(10) 0.7271(9) 0.014(3) Uani 1 1 d U . . 
O11 O 0.2222(11) 0.6650(11) 0.6984(9) 0.019(3) Uani 1 1 d U . . 
O12 O 0.1104(10) 0.5599(9) 0.7922(8) 0.013(3) Uani 1 1 d U . . 
O13 O 0.2718(10) 0.4708(9) 0.8490(9) 0.013(3) Uani 1 1 d . . . 
O14 O 0.3150(10) 0.6683(9) 0.8684(9) 0.013(3) Uani 1 1 d . . . 
O15 O 0.4828(11) 0.5908(10) 0.9378(8) 0.014(3) Uani 1 1 d . . . 
O16 O 0.3552(10) 0.5287(10) 1.0372(9) 0.017(3) Uani 1 1 d U . . 
O17 O 0.3936(11) 0.7417(11) 1.0520(10) 0.021(3) Uani 1 1 d . . . 
O18 O 0.1904(10) 0.6000(10) 0.9628(8) 0.012(3) Uani 1 1 d U . . 
O19 O -0.0285(11) 0.5184(11) 0.8977(11) 0.024(3) Uani 1 1 d . . . 
O20 O 0.0457(11) 0.3606(11) 0.7743(9) 0.018(3) Uani 1 1 d U . . 
O21 O 0.1205(10) 0.3954(9) 0.9455(8) 0.011(3) Uani 1 1 d U . . 
O22 O 0.2220(9) 0.2609(9) 0.8217(8) 0.009(2) Uani 1 1 d U . . 
O23 O 0.2892(9) 0.3144(9) 1.0061(8) 0.010(2) Uani 1 1 d U . . 
O24 O 0.0867(11) 0.2397(11) 1.0268(10) 0.021(3) Uani 1 1 d U . . 
O25 O 0.0201(11) 0.2107(11) 0.8426(11) 0.023(3) Uani 1 1 d U . . 
O26 O 0.1814(10) 0.1195(10) 0.8954(8) 0.016(3) Uani 1 1 d U . . 
O27 O 0.2321(12) -0.0444(11) 0.7706(10) 0.022(3) Uani 1 1 d U . . 
O28 O 0.1003(11) 0.0860(10) 0.7205(9) 0.019(3) Uani 1 1 d . . . 
O29 O 0.3818(11) 0.1396(10) 0.8611(9) 0.017(3) Uani 1 1 d U . . 
O30 O 0.3028(10) 0.1048(10) 0.6922(8) 0.012(3) Uani 1 1 d U . . 
O31 O 0.4535(12) 0.0793(11) 0.5826(10) 0.023(3) Uani 1 1 d . . . 
O32 O 0.5067(11) 0.2062(11) 0.7614(9) 0.016(3) Uani 1 1 d . . . 
O33 O -0.0895(11) 0.1664(11) 0.6706(9) 0.018(3) Uani 1 1 d U . . 
O34 O 0.4836(13) -0.0064(12) 0.7465(11) 0.036(4) Uani 1 1 d D . . 
Fe2 Fe 0.5331(2) 0.1352(2) 0.84646(18) 0.0141(6) Uani 1 1 d . . . 
O35 O 0.613(3) -0.044(3) 0.677(2) 0.043(9) Uiso 0.50 1 d PD A 1 
O36 O 0.499(5) -0.274(4) 0.659(4) 0.081(11) Uiso 0.50 1 d PD B 1 
H36 H 0.5221 -0.3291 0.6465 0.121 Uiso 0.50 1 d PR B 1 
N1 N 0.328(3) -0.151(3) 0.625(3) 0.025(6) Uiso 0.50 1 d PD A 1 
H1A H 0.2917 -0.2034 0.5775 0.030 Uiso 0.50 1 d PR A 1 
H1B H 0.3200 -0.1670 0.6728 0.030 Uiso 0.50 1 d PR A 1 
H1C H 0.3025 -0.0927 0.6258 0.030 Uiso 0.50 1 d PR A 1 
C1 C 0.528(3) -0.055(3) 0.693(2) 0.023(9) Uiso 0.50 1 d PD A 1 
C2 C 0.446(3) -0.142(3) 0.612(3) 0.041(9) Uiso 0.50 1 d PD A 1 
H2 H 0.4485 -0.1223 0.5588 0.049 Uiso 0.50 1 calc PR A 1 
C3 C 0.462(3) -0.257(3) 0.593(3) 0.077(12) Uani 1 1 d D . . 
C4 C 0.380(4) -0.351(4) 0.530(3) 0.100(15) Uani 1 1 d U B . 
H4A H 0.3511 -0.3345 0.4779 0.150 Uiso 1 1 d R . . 
H4B H 0.4156 -0.4098 0.5141 0.150 Uiso 1 1 d R . . 
H4C H 0.3213 -0.3667 0.5568 0.150 Uiso 1 1 d R . . 
O35' O 0.549(4) -0.131(4) 0.775(3) 0.062(12) Uiso 0.50 1 d PD A 2 
O36' O 0.516(4) -0.223(4) 0.550(4) 0.081(11) Uiso 0.50 1 d PD B 2 
H36' H 0.5014 -0.1676 0.5459 0.121 Uiso 0.50 1 d PR B 2 
N1' N 0.347(3) -0.113(3) 0.602(3) 0.025(6) Uiso 0.50 1 d PD A 2 
H1'A H 0.2966 -0.1567 0.5571 0.038 Uiso 0.50 1 d PR A 2 
H1'B H 0.3154 -0.0662 0.6359 0.038 Uiso 0.50 1 d PR A 2 
H1'C H 0.3969 -0.0806 0.5826 0.038 Uiso 0.50 1 d PR A 2 
C1' C 0.489(3) -0.097(2) 0.736(2) 0.017(8) Uiso 0.50 1 d PD A 2 
C2' C 0.406(4) -0.178(3) 0.653(3) 0.041(9) Uiso 0.50 1 d PD A 2 
H2' H 0.3522 -0.2170 0.6736 0.049 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.728(14) . ? 
W1 O2 1.902(14) . ? 
W1 O3 1.904(14) . ? 
W1 O5 1.906(12) . ? 
W1 O6 1.921(13) . ? 
W1 O4 2.298(12) . ? 
W2 O7 1.716(14) . ? 
W2 O9 1.796(13) . ? 
W2 O10 1.912(13) . ? 
W2 O8 1.933(13) . ? 
W2 O6 1.945(13) . ? 
W2 O4 2.340(13) . ? 
W3 O11 1.742(13) . ? 
W3 O14 1.898(13) . ? 
W3 O12 1.920(13) . ? 
W3 O10 1.931(13) . ? 
W3 O3 1.932(14) . ? 
W3 O13 2.376(13) . ? 
W4 O16 1.783(13) . ? 
W4 O17 1.790(14) . ? 
W4 O15 1.794(13) . ? 
W4 O14 2.027(12) . ? 
W4 O18 2.068(12) . ? 
W4 O13 2.309(13) . ? 
W5 O19 1.716(13) . ? 
W5 O18 1.856(13) . ? 
W5 O21 1.888(12) . ? 
W5 O12 1.957(13) . ? 
W5 O20 1.958(14) . ? 
W5 O13 2.389(13) . ? 
W6 O24 1.724(15) . ? 
W6 O23 1.811(12) . ? 
W6 O26 1.909(14) . ? 
W6 O21 1.954(12) . ? 
W6 O25 2.017(15) . ? 
W6 O22 2.333(12) . ? 
W7 O27 1.727(14) . ? 
W7 O29 1.805(13) . ? 
W7 O30 1.908(13) . ? 
W7 O26 1.966(13) . ? 
W7 O28 1.992(13) . ? 
W7 O22 2.290(12) . ? 
W8 O31 1.733(13) . ? 
W8 O32 1.851(13) . ? 
W8 O8 1.933(13) . ? 
W8 O30 1.951(13) . ? 
W8 O2 1.986(14) . ? 
W8 O4 2.335(13) . ? 
W9 O33 1.728(13) . ? 
W9 O25 1.881(16) . ? 
W9 O20 1.898(14) . ? 
W9 O5 1.908(13) . ? 
W9 O28 1.923(14) . ? 
W9 O22 2.376(12) . ? 
Eu1 O7M 2.25(6) . ? 
Eu1 O10W 2.39(5) . ? 
Eu1 O12M 2.39(5) . ? 
Eu1 O5W 2.41(3) . ? 
Eu1 O9W 2.41(2) . ? 
Eu1 O7W 2.42(5) . ? 
Eu1 O11W 2.43(5) . ? 
Eu1 O11M 2.44(4) . ? 
Eu1 O1 2.469(15) . ? 
Eu1 O6W 2.474(19) . ? 
Eu1 O12W 2.50(6) . ? 
Eu1 O8W 2.51(6) . ? 
As1 O13 1.794(12) . ? 
As1 O22 1.804(12) . ? 
As1 O4 1.815(13) . ? 
Fe1 O23 1.916(12) . ? 
Fe1 O16 1.928(14) . ? 
Fe1 O15 1.942(14) 2_667 ? 
Fe1 O9 1.957(14) 2_667 ? 
Fe1 O2W 2.086(15) . ? 
Fe1 O1W 2.134(14) . ? 
O3W Fe2 2.063(16) . ? 
O4W Fe2 2.057(16) . ? 
O7M O12M 1.64(8) . ? 
O10W O10M 0.83(8) . ? 
O11W O11M 0.86(6) . ? 
O12W O12M 1.11(7) . ? 
O15W O15W 1.70(14) 2_566 ? 
O16W O16M 1.77(8) . ? 
O18W O18M 0.86(6) . ? 
O9 Fe1 1.957(14) 2_667 ? 
O15 Fe1 1.942(14) 2_667 ? 
O17 Fe2 1.960(14) 2_667 ? 
O29 Fe2 1.971(14) . ? 
O32 Fe2 1.905(13) . ? 
O34 C1' 1.19(3) . ? 
O34 C1 1.20(3) . ? 
O34 Fe2 2.056(15) . ? 
Fe2 O17 1.960(14) 2_667 ? 
O35 C1 1.14(4) . ? 
O36 C3 1.19(4) . ? 
N1 C2 1.53(4) . ? 
C1 C2 1.58(5) . ? 
C2 C3 1.54(5) . ? 
C3 O36' 1.20(4) . ? 
C3 C4 1.51(6) . ? 
C3 C2' 1.54(5) . ? 
O35' C1' 1.14(4) . ? 
N1' C2' 1.53(4) . ? 
C1' C2' 1.58(5) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O2 99.5(6) . . ? 
O1 W1 O3 104.5(6) . . ? 
O2 W1 O3 155.6(6) . . ? 
O1 W1 O5 100.0(6) . . ? 
O2 W1 O5 90.7(5) . . ? 
O3 W1 O5 89.3(5) . . ? 
O1 W1 O6 97.8(6) . . ? 
O2 W1 O6 86.7(6) . . ? 
O3 W1 O6 85.8(5) . . ? 
O5 W1 O6 162.2(5) . . ? 
O1 W1 O4 169.7(6) . . ? 
O2 W1 O4 72.8(5) . . ? 
O3 W1 O4 82.9(5) . . ? 
O5 W1 O4 87.2(5) . . ? 
O6 W1 O4 75.2(5) . . ? 
O7 W2 O9 102.0(7) . . ? 
O7 W2 O10 100.0(7) . . ? 
O9 W2 O10 90.7(6) . . ? 
O7 W2 O8 102.0(7) . . ? 
O9 W2 O8 93.1(6) . . ? 
O10 W2 O8 156.4(5) . . ? 
O7 W2 O6 101.7(7) . . ? 
O9 W2 O6 156.0(6) . . ? 
O10 W2 O6 81.9(5) . . ? 
O8 W2 O6 85.2(6) . . ? 
O7 W2 O4 173.9(6) . . ? 
O9 W2 O4 82.7(5) . . ? 
O10 W2 O4 83.6(5) . . ? 
O8 W2 O4 73.8(5) . . ? 
O6 W2 O4 73.8(5) . . ? 
O11 W3 O14 100.0(6) . . ? 
O11 W3 O12 99.5(6) . . ? 
O14 W3 O12 89.9(6) . . ? 
O11 W3 O10 99.7(6) . . ? 
O14 W3 O10 91.7(6) . . ? 
O12 W3 O10 160.2(5) . . ? 
O11 W3 O3 103.7(6) . . ? 
O14 W3 O3 156.2(5) . . ? 
O12 W3 O3 84.4(5) . . ? 
O10 W3 O3 86.1(5) . . ? 
O11 W3 O13 171.2(6) . . ? 
O14 W3 O13 73.0(5) . . ? 
O12 W3 O13 75.6(5) . . ? 
O10 W3 O13 86.0(5) . . ? 
O3 W3 O13 83.2(5) . . ? 
O16 W4 O17 102.7(6) . . ? 
O16 W4 O15 97.5(6) . . ? 
O17 W4 O15 103.4(6) . . ? 
O16 W4 O14 159.6(5) . . ? 
O17 W4 O14 94.2(6) . . ? 
O15 W4 O14 89.6(5) . . ? 
O16 W4 O18 86.7(5) . . ? 
O17 W4 O18 96.1(6) . . ? 
O15 W4 O18 158.6(5) . . ? 
O14 W4 O18 80.1(5) . . ? 
O16 W4 O13 88.8(5) . . ? 
O17 W4 O13 163.3(5) . . ? 
O15 W4 O13 86.8(5) . . ? 
O14 W4 O13 72.4(5) . . ? 
O18 W4 O13 72.3(5) . . ? 
O19 W5 O18 100.6(6) . . ? 
O19 W5 O21 102.6(7) . . ? 
O18 W5 O21 93.0(5) . . ? 
O19 W5 O12 97.5(7) . . ? 
O18 W5 O12 87.8(6) . . ? 
O21 W5 O12 159.4(5) . . ? 
O19 W5 O20 100.9(6) . . ? 
O18 W5 O20 158.0(6) . . ? 
O21 W5 O20 87.2(6) . . ? 
O12 W5 O20 84.5(5) . . ? 
O19 W5 O13 170.4(6) . . ? 
O18 W5 O13 74.0(5) . . ? 
O21 W5 O13 85.8(5) . . ? 
O12 W5 O13 74.6(5) . . ? 
O20 W5 O13 84.1(5) . . ? 
O24 W6 O23 101.8(6) . . ? 
O24 W6 O26 101.4(6) . . ? 
O23 W6 O26 95.1(5) . . ? 
O24 W6 O21 99.8(6) . . ? 
O23 W6 O21 90.7(5) . . ? 
O26 W6 O21 156.3(5) . . ? 
O24 W6 O25 99.2(6) . . ? 
O23 W6 O25 158.5(6) . . ? 
O26 W6 O25 85.0(6) . . ? 
O21 W6 O25 81.3(5) . . ? 
O24 W6 O22 172.8(6) . . ? 
O23 W6 O22 84.3(5) . . ? 
O26 W6 O22 74.0(5) . . ? 
O21 W6 O22 83.8(5) . . ? 
O25 W6 O22 75.0(5) . . ? 
O27 W7 O29 103.5(6) . . ? 
O27 W7 O30 101.4(6) . . ? 
O29 W7 O30 90.1(6) . . ? 
O27 W7 O26 96.1(6) . . ? 
O29 W7 O26 90.5(6) . . ? 
O30 W7 O26 161.9(5) . . ? 
O27 W7 O28 95.7(6) . . ? 
O29 W7 O28 160.9(6) . . ? 
O30 W7 O28 86.4(5) . . ? 
O26 W7 O28 87.1(6) . . ? 
O27 W7 O22 165.5(6) . . ? 
O29 W7 O22 87.5(5) . . ? 
O30 W7 O22 87.9(5) . . ? 
O26 W7 O22 74.0(5) . . ? 
O28 W7 O22 73.5(5) . . ? 
O31 W8 O32 103.6(6) . . ? 
O31 W8 O8 100.9(6) . . ? 
O32 W8 O8 92.4(6) . . ? 
O31 W8 O30 98.7(6) . . ? 
O32 W8 O30 88.3(6) . . ? 
O8 W8 O30 159.6(5) . . ? 
O31 W8 O2 97.3(6) . . ? 
O32 W8 O2 158.7(6) . . ? 
O8 W8 O2 87.8(5) . . ? 
O30 W8 O2 84.2(5) . . ? 
O31 W8 O4 166.7(6) . . ? 
O32 W8 O4 89.0(5) . . ? 
O8 W8 O4 73.9(5) . . ? 
O30 W8 O4 85.7(5) . . ? 
O2 W8 O4 70.6(5) . . ? 
O33 W9 O25 99.2(6) . . ? 
O33 W9 O20 102.3(6) . . ? 
O25 W9 O20 86.5(6) . . ? 
O33 W9 O5 99.7(6) . . ? 
O25 W9 O5 161.1(6) . . ? 
O20 W9 O5 88.3(6) . . ? 
O33 W9 O28 102.1(6) . . ? 
O25 W9 O28 87.5(6) . . ? 
O20 W9 O28 155.5(6) . . ? 
O5 W9 O28 89.7(6) . . ? 
O33 W9 O22 173.1(5) . . ? 
O25 W9 O22 76.4(5) . . ? 
O20 W9 O22 82.8(5) . . ? 
O5 W9 O22 85.0(5) . . ? 
O28 W9 O22 72.7(5) . . ? 
O7M Eu1 O10W 89(2) . . ? 
O7M Eu1 O12M 41(2) . . ? 
O10W Eu1 O12M 75.0(19) . . ? 
O7M Eu1 O5W 128.0(19) . . ? 
O10W Eu1 O5W 141.6(17) . . ? 
O12M Eu1 O5W 138.3(17) . . ? 
O7M Eu1 O9W 142.7(18) . . ? 
O10W Eu1 O9W 67.5(16) . . ? 
O12M Eu1 O9W 141.3(16) . . ? 
O5W Eu1 O9W 75.3(14) . . ? 
O7M Eu1 O7W 46(2) . . ? 
O10W Eu1 O7W 64.0(18) . . ? 
O12M Eu1 O7W 74.6(17) . . ? 
O5W Eu1 O7W 131.6(13) . . ? 
O9W Eu1 O7W 96.5(14) . . ? 
O7M Eu1 O11W 65(2) . . ? 
O10W Eu1 O11W 146.1(19) . . ? 
O12M Eu1 O11W 96.3(19) . . ? 
O5W Eu1 O11W 63.5(16) . . ? 
O9W Eu1 O11W 120.1(17) . . ? 
O7W Eu1 O11W 82.1(18) . . ? 
O7M Eu1 O11M 45.7(19) . . ? 
O10W Eu1 O11M 132.3(17) . . ? 
O12M Eu1 O11M 76.6(18) . . ? 
O5W Eu1 O11M 82.4(14) . . ? 
O9W Eu1 O11M 137.3(14) . . ? 
O7W Eu1 O11M 72.0(16) . . ? 
O11W Eu1 O11M 20.4(14) . . ? 
O7M Eu1 O1 80.1(17) . . ? 
O10W Eu1 O1 127.1(14) . . ? 
O12M Eu1 O1 62.9(13) . . ? 
O5W Eu1 O1 75.9(11) . . ? 
O9W Eu1 O1 137.1(8) . . ? 
O7W Eu1 O1 126.4(12) . . ? 
O11W Eu1 O1 72.3(13) . . ? 
O11M Eu1 O1 67.8(11) . . ? 
O7M Eu1 O6W 132.9(17) . . ? 
O10W Eu1 O6W 84.2(15) . . ? 
O12M Eu1 O6W 92.3(14) . . ? 
O5W Eu1 O6W 77.3(9) . . ? 
O9W Eu1 O6W 75.2(9) . . ? 
O7W Eu1 O6W 147.7(13) . . ? 
O11W Eu1 O6W 129.4(14) . . ? 
O11M Eu1 O6W 134.5(11) . . ? 
O1 Eu1 O6W 67.9(6) . . ? 
O7M Eu1 O12W 65(2) . . ? 
O10W Eu1 O12W 58(2) . . ? 
O12M Eu1 O12W 26.2(17) . . ? 
O5W Eu1 O12W 141.0(16) . . ? 
O9W Eu1 O12W 117.7(18) . . ? 
O7W Eu1 O12W 85.5(18) . . ? 
O11W Eu1 O12W 122(2) . . ? 
O11M Eu1 O12W 102.6(19) . . ? 
O1 Eu1 O12W 70.7(15) . . ? 
O6W Eu1 O12W 71.9(16) . . ? 
O7M Eu1 O8W 88(2) . . ? 
O10W Eu1 O8W 97.8(19) . . ? 
O12M Eu1 O8W 127.4(19) . . ? 
O5W Eu1 O8W 76.6(15) . . ? 
O9W Eu1 O8W 68.6(15) . . ? 
O7W Eu1 O8W 56.7(18) . . ? 
O11W Eu1 O8W 61.1(19) . . ? 
O11M Eu1 O8W 71.1(17) . . ? 
O1 Eu1 O8W 132.8(14) . . ? 
O6W Eu1 O8W 139.5(15) . . ? 
O12W Eu1 O8W 142(2) . . ? 
O13 As1 O22 98.0(5) . . ? 
O13 As1 O4 98.3(6) . . ? 
O22 As1 O4 97.1(6) . . ? 
O23 Fe1 O16 92.8(5) . . ? 
O23 Fe1 O15 96.5(5) . 2_667 ? 
O16 Fe1 O15 92.9(6) . 2_667 ? 
O23 Fe1 O9 168.3(6) . 2_667 ? 
O16 Fe1 O9 93.9(6) . 2_667 ? 
O15 Fe1 O9 92.6(5) 2_667 2_667 ? 
O23 Fe1 O2W 85.1(6) . . ? 
O16 Fe1 O2W 177.3(6) . . ? 
O15 Fe1 O2W 85.6(6) 2_667 . ? 
O9 Fe1 O2W 88.4(6) 2_667 . ? 
O23 Fe1 O1W 86.8(6) . . ? 
O16 Fe1 O1W 92.4(6) . . ? 
O15 Fe1 O1W 173.5(6) 2_667 . ? 
O9 Fe1 O1W 83.4(6) 2_667 . ? 
O2W Fe1 O1W 89.2(6) . . ? 
O12M O7M Eu1 74(3) . . ? 
O10M O10W Eu1 91(7) . . ? 
O10W O10M Eu1 70(7) . . ? 
O11M O11W Eu1 81(5) . . ? 
O11W O11M Eu1 79(5) . . ? 
O12M O12W Eu1 72(4) . . ? 
O12W O12M O7M 137(6) . . ? 
O12W O12M Eu1 82(5) . . ? 
O7M O12M Eu1 65(3) . . ? 
W1 O1 Eu1 148.6(8) . . ? 
W1 O2 W8 122.0(7) . . ? 
W1 O3 W3 145.3(7) . . ? 
As1 O4 W1 134.1(6) . . ? 
As1 O4 W8 116.8(6) . . ? 
W1 O4 W8 94.5(5) . . ? 
As1 O4 W2 118.1(6) . . ? 
W1 O4 W2 91.8(5) . . ? 
W8 O4 W2 91.8(4) . . ? 
W1 O5 W9 155.0(7) . . ? 
W1 O6 W2 118.9(7) . . ? 
W8 O8 W2 120.5(7) . . ? 
W2 O9 Fe1 142.4(8) . 2_667 ? 
W2 O10 W3 146.8(7) . . ? 
W3 O12 W5 120.0(6) . . ? 
As1 O13 W4 113.8(6) . . ? 
As1 O13 W3 128.3(7) . . ? 
W4 O13 W3 93.6(4) . . ? 
As1 O13 W5 128.9(6) . . ? 
W4 O13 W5 92.9(5) . . ? 
W3 O13 W5 89.6(4) . . ? 
W3 O14 W4 120.9(6) . . ? 
W4 O15 Fe1 178.0(8) . 2_667 ? 
W4 O16 Fe1 167.7(8) . . ? 
W4 O17 Fe2 164.0(8) . 2_667 ? 
W5 O18 W4 120.4(6) . . ? 
W9 O20 W5 144.1(8) . . ? 
W5 O21 W6 146.4(7) . . ? 
As1 O22 W7 117.3(6) . . ? 
As1 O22 W6 119.0(6) . . ? 
W7 O22 W6 92.6(4) . . ? 
As1 O22 W9 134.1(6) . . ? 
W7 O22 W9 93.3(4) . . ? 
W6 O22 W9 90.4(4) . . ? 
W6 O23 Fe1 145.8(7) . . ? 
W9 O25 W6 118.0(7) . . ? 
W6 O26 W7 119.3(6) . . ? 
W9 O28 W7 120.3(6) . . ? 
W7 O29 Fe2 136.2(8) . . ? 
W7 O30 W8 145.4(7) . . ? 
W8 O32 Fe2 138.2(8) . . ? 
C1' O34 C1 57(3) . . ? 
C1' O34 Fe2 138(2) . . ? 
C1 O34 Fe2 133(2) . . ? 
O32 Fe2 O17 97.7(6) . 2_667 ? 
O32 Fe2 O29 88.2(6) . . ? 
O17 Fe2 O29 98.1(6) 2_667 . ? 
O32 Fe2 O34 89.3(7) . . ? 
O17 Fe2 O34 168.4(6) 2_667 . ? 
O29 Fe2 O34 91.2(6) . . ? 
O32 Fe2 O4W 92.8(7) . . ? 
O17 Fe2 O4W 85.7(6) 2_667 . ? 
O29 Fe2 O4W 175.9(6) . . ? 
O34 Fe2 O4W 84.8(6) . . ? 
O32 Fe2 O3W 175.7(6) . . ? 
O17 Fe2 O3W 86.3(6) 2_667 . ? 
O29 Fe2 O3W 89.8(7) . . ? 
O34 Fe2 O3W 86.9(7) . . ? 
O4W Fe2 O3W 88.9(8) . . ? 
O35 C1 O34 135(4) . . ? 
O35 C1 C2 110(3) . . ? 
O34 C1 C2 113(3) . . ? 
N1 C2 C3 101(3) . . ? 
N1 C2 C1 113(4) . . ? 
C3 C2 C1 118(3) . . ? 
O36 C3 O36' 124(5) . . ? 
O36 C3 C4 112(4) . . ? 
O36' C3 C4 107(4) . . ? 
O36 C3 C2 111(5) . . ? 
O36' C3 C2 76(4) . . ? 
C4 C3 C2 124(4) . . ? 
O36 C3 C2' 85(4) . . ? 
O36' C3 C2' 116(4) . . ? 
C4 C3 C2' 112(4) . . ? 
C2 C3 C2' 41(3) . . ? 
O35' C1' O34 128(4) . . ? 
O35' C1' C2' 116(4) . . ? 
O34 C1' C2' 115(3) . . ? 
N1' C2' C3 112(3) . . ? 
N1' C2' C1' 107(3) . . ? 
C3 C2' C1' 113(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.964 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.964 
_refine_diff_density_max    4.385 
_refine_diff_density_min   -5.703 
_refine_diff_density_rms    0.679 
  



#===END

  
data_10-Gd 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Fe4 Gd2 N2 O116 W18' 
_chemical_formula_weight          6083.99 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Gd'  'Gd'  -0.1653   3.9035 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6230(7) 
_cell_length_b                    13.5118(8) 
_cell_length_c                    16.1922(9) 
_cell_angle_alpha                 106.7890(10) 
_cell_angle_beta                  99.7550(10) 
_cell_angle_gamma                 97.1520(10) 
_cell_volume                      2561.4(3) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8773 
_cell_measurement_theta_min       1.60 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky 
_exptl_crystal_colour             'Light yellow'  
_exptl_crystal_size_max           0.38 
_exptl_crystal_size_mid           0.19 
_exptl_crystal_size_min           0.11 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.944 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2726 
_exptl_absorpt_coefficient_mu     22.713 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0422 
_exptl_absorpt_correction_T_max   0.1890 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12855 
_diffrn_reflns_av_R_equivalents   0.0379 
_diffrn_reflns_av_sigmaI/netI     0.0710 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        16 
_diffrn_reflns_limit_l_min        -19 
_diffrn_reflns_limit_l_max        10 
_diffrn_reflns_theta_min          1.60 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8773 
_reflns_number_gt                 7550 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral. 
 However, its structure is pseudo-centrosymmetric, i.e. most of the 
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are rather
 common. An attempt to refine the structure in P¨C1 shows the disorder 
 around the chiral centre of L-thr (because we impose inversion on a 
 chiral entity), as a result, C1, C2, N1, O35 and O36 atoms on L-thr
 are disordered over two positions. In addition, some coordination water
 molecules on Gd3+ cations are disordered over two positions. The ISOR
 instruction is used for O1W, C3, C4, O8, O33, O12 and O18. The SADI 
 instruction is used for C2' C1' C2 C1, O34 C1' O34 C1, O35' C1' O35 C1,
 N1' C2' N1 C2, C3 C2' C3 C2, O36 C3 O36' C3, N1' C2' N1 C2. The EADP
 instruction is used for C2 and C2', N1 and N1', O36 and O36'. The O7W,
 O7M, O8W, O10W, O10M, O11W, O11M, O12W, O12M, O13W, O14W, O15W, O16W,
 O16M, O18W, O18M, O22W, O35, O35', O36, O36', C1, C1', C2, C2', N1
 and N1' are refined isostropicallly. 655 parameters and 37 restraints
 are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0733P)²+33.8955P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          8773 
_refine_ls_number_parameters      655 
_refine_ls_number_restraints      37 
_refine_ls_R_factor_all           0.0589 
_refine_ls_R_factor_gt            0.0507 
_refine_ls_wR_factor_ref          0.1341 
_refine_ls_wR_factor_gt           0.1292 
_refine_ls_goodness_of_fit_ref    1.024 
_refine_ls_restrained_S_all       1.023 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21123(5) 0.31113(5) 0.59440(4) 0.01625(16) Uani 1 1 d . . . 
W2 W 0.46663(5) 0.44217(5) 0.67972(4) 0.01529(15) Uani 1 1 d . . . 
W3 W 0.24537(5) 0.57455(5) 0.75380(4) 0.01538(15) Uani 1 1 d . . . 
W4 W 0.35697(4) 0.61330(4) 0.97079(4) 0.01231(15) Uani 1 1 d . . . 
W5 W 0.09438(5) 0.48602(4) 0.87850(4) 0.01441(15) Uani 1 1 d . . . 
W6 W 0.15057(5) 0.25636(5) 0.94523(4) 0.01586(16) Uani 1 1 d . . . 
W7 W 0.24663(5) 0.08955(4) 0.79151(4) 0.01667(16) Uani 1 1 d . . . 
W8 W 0.41299(5) 0.18404(5) 0.65363(4) 0.01772(16) Uani 1 1 d . . . 
W9 W 0.04225(5) 0.21286(4) 0.73177(4) 0.01536(15) Uani 1 1 d . . . 
Gd1 Gd 0.11752(8) 0.23879(8) 0.32949(6) 0.0375(2) Uani 1 1 d . . . 
As1 As 0.33915(11) 0.35924(11) 0.83542(9) 0.0101(3) Uani 1 1 d . . . 
Fe1 Fe 0.38139(16) 0.42965(16) 1.10056(14) 0.0149(4) Uani 1 1 d . . . 
O1W O 0.2403(9) 0.4528(9) 1.1559(8) 0.024(3) Uani 1 1 d U . . 
O2W O 0.4092(11) 0.3161(9) 1.1634(9) 0.037(3) Uani 1 1 d . . . 
O3W O 0.5540(12) 0.0498(10) 0.9336(9) 0.041(3) Uani 1 1 d . . . 
O4W O 0.6868(9) 0.1191(10) 0.8244(10) 0.041(4) Uani 1 1 d . . . 
O5W O 0.2510(18) 0.1448(16) 0.3814(17) 0.106(9) Uani 1 1 d . . . 
O6W O 0.2730(15) 0.3798(14) 0.4079(11) 0.073(6) Uani 1 1 d . . . 
O7W O -0.046(3) 0.181(3) 0.217(3) 0.118(12) Uiso 0.70 1 d P . . 
O7M O -0.055(4) 0.218(4) 0.341(4) 0.057(14) Uiso 0.30 1 d P . . 
O8W O 0.075(3) 0.057(3) 0.219(2) 0.161(12) Uiso 1 1 d . . . 
O9W O 0.2438(19) 0.226(2) 0.2308(13) 0.104(8) Uani 1 1 d . . . 
O10W O 0.084(3) 0.343(3) 0.235(3) 0.108(12) Uiso 0.70 1 d P . . 
O10M O 0.036(5) 0.295(4) 0.200(4) 0.050(13) Uiso 0.30 1 d P . . 
O11W O 0.042(4) 0.077(4) 0.374(3) 0.119(15) Uiso 0.60 1 d P . . 
O11M O -0.003(3) 0.117(3) 0.375(3) 0.052(10) Uiso 0.40 1 d P . . 
O12W O 0.053(3) 0.409(3) 0.382(2) 0.076(9) Uiso 0.60 1 d P . . 
O12M O -0.009(4) 0.349(3) 0.387(3) 0.063(11) Uiso 0.40 1 d P . . 
O13W O 0.115(3) -0.196(2) 0.939(2) 0.143(11) Uiso 1 1 d . . . 
O14W O 0.208(4) 0.024(3) 1.080(3) 0.087(12) Uiso 0.50 1 d P . . 
O15W O 0.067(7) 0.529(7) 0.504(6) 0.19(3) Uiso 0.50 1 d P . . 
O16W O 0.306(3) -0.052(3) 0.361(3) 0.088(10) Uiso 0.60 1 d P . . 
O16M O 0.321(5) -0.129(5) 0.421(4) 0.100(18) Uiso 0.40 1 d P . . 
O17W O 0.3766(17) 0.1319(12) 1.0415(10) 0.068(6) Uani 1 1 d . . . 
O18W O 0.365(2) -0.120(2) 0.8937(19) 0.072(7) Uiso 0.70 1 d P . . 
O18M O 0.301(5) -0.127(4) 0.917(4) 0.051(13) Uiso 0.30 1 d P . . 
O19W O -0.1653(10) 0.2882(11) 0.8705(10) 0.046(4) Uani 1 1 d . . . 
O20W O 0.7372(14) 0.3490(13) 0.7321(12) 0.069(5) Uani 1 1 d . . . 
O21W O -0.0964(15) 0.3952(14) 0.6329(11) 0.067(5) Uani 1 1 d . . . 
O22W O 0.1159(16) 0.0031(15) 0.5070(14) 0.076(5) Uiso 1 1 d . . . 
O23W O 0.1366(18) -0.2024(16) 0.5100(12) 0.080(6) Uani 1 1 d . . . 
O1 O 0.1322(9) 0.2910(8) 0.4893(7) 0.024(3) Uani 1 1 d . . . 
O2 O 0.2869(8) 0.1964(8) 0.5678(7) 0.018(2) Uani 1 1 d . . . 
O3 O 0.1827(8) 0.4404(7) 0.6649(7) 0.017(2) Uani 1 1 d . . . 
O4 O 0.3394(8) 0.3319(7) 0.7198(6) 0.012(2) Uani 1 1 d . . . 
O5 O 0.1134(8) 0.2367(8) 0.6424(7) 0.017(2) Uani 1 1 d . . . 
O6 O 0.3383(9) 0.3947(8) 0.5813(7) 0.021(2) Uani 1 1 d . . . 
O7 O 0.5533(10) 0.5130(9) 0.6388(9) 0.036(3) Uani 1 1 d . . . 
O8 O 0.4950(8) 0.3017(8) 0.6338(7) 0.018(2) Uani 1 1 d U . . 
O9 O 0.5442(8) 0.4615(8) 0.7900(7) 0.020(2) Uani 1 1 d . . . 
O10 O 0.3835(8) 0.5488(8) 0.7276(7) 0.015(2) Uani 1 1 d . . . 
O11 O 0.2209(10) 0.6637(9) 0.6984(8) 0.027(3) Uani 1 1 d . . . 
O12 O 0.1109(8) 0.5580(8) 0.7920(7) 0.018(2) Uani 1 1 d U . . 
O13 O 0.2720(8) 0.4715(7) 0.8505(7) 0.015(2) Uani 1 1 d . . . 
O14 O 0.3133(8) 0.6667(8) 0.8659(7) 0.020(2) Uani 1 1 d . . . 
O15 O 0.4814(8) 0.5909(8) 0.9371(7) 0.020(2) Uani 1 1 d . . . 
O16 O 0.3550(9) 0.5287(9) 1.0363(8) 0.025(3) Uani 1 1 d . . . 
O17 O 0.3933(9) 0.7396(8) 1.0502(7) 0.022(2) Uani 1 1 d . . . 
O18 O 0.1926(8) 0.5987(7) 0.9628(7) 0.017(2) Uani 1 1 d U . . 
O19 O -0.0288(8) 0.5182(8) 0.8984(8) 0.023(3) Uani 1 1 d . . . 
O20 O 0.0454(8) 0.3606(7) 0.7757(7) 0.017(2) Uani 1 1 d . . . 
O21 O 0.1207(8) 0.3942(8) 0.9439(7) 0.017(2) Uani 1 1 d . . . 
O22 O 0.2213(8) 0.2598(7) 0.8212(7) 0.015(2) Uani 1 1 d . . . 
O23 O 0.2900(8) 0.3135(8) 1.0063(7) 0.017(2) Uani 1 1 d . . . 
O24 O 0.0859(10) 0.2361(9) 1.0263(7) 0.026(3) Uani 1 1 d . . . 
O25 O 0.0205(8) 0.2091(8) 0.8426(8) 0.024(3) Uani 1 1 d . . . 
O26 O 0.1816(8) 0.1194(7) 0.8934(7) 0.015(2) Uani 1 1 d . . . 
O27 O 0.2325(10) -0.0469(8) 0.7702(8) 0.026(3) Uani 1 1 d . . . 
O28 O 0.0996(8) 0.0862(8) 0.7216(7) 0.017(2) Uani 1 1 d . . . 
O29 O 0.3815(9) 0.1401(8) 0.8619(7) 0.017(2) Uani 1 1 d . . . 
O30 O 0.3016(9) 0.1066(8) 0.6923(7) 0.020(2) Uani 1 1 d . . . 
O31 O 0.4533(9) 0.0810(9) 0.5825(8) 0.030(3) Uani 1 1 d . . . 
O32 O 0.5057(8) 0.2069(8) 0.7606(7) 0.021(2) Uani 1 1 d . . . 
O33 O -0.0890(9) 0.1663(8) 0.6726(7) 0.023(2) Uani 1 1 d U . . 
O34 O 0.4843(9) -0.0053(9) 0.7486(8) 0.031(3) Uani 1 1 d D . . 
Fe2 Fe 0.53297(17) 0.13557(16) 0.84659(15) 0.0179(5) Uani 1 1 d . . . 
O35 O 0.614(2) -0.0399(19) 0.6801(18) 0.037(6) Uiso 0.50 1 d PD A 1 
O36 O 0.508(4) -0.277(3) 0.660(3) 0.089(9) Uiso 0.50 1 d PD B 1 
H36 H 0.5314 -0.3325 0.6477 0.134 Uiso 0.50 1 d PR B 1 
N1 N 0.332(3) -0.141(3) 0.625(3) 0.044(6) Uiso 0.50 1 d PD A 1 
H1A H 0.2951 -0.1933 0.5774 0.052 Uiso 0.50 1 d PR A 1 
H1B H 0.3234 -0.1568 0.6727 0.052 Uiso 0.50 1 d PR A 1 
H1C H 0.3059 -0.0825 0.6257 0.052 Uiso 0.50 1 d PR A 1 
C1 C 0.523(2) -0.057(2) 0.6948(18) 0.015(6) Uiso 0.50 1 d PD A 1 
C2 C 0.452(3) -0.144(2) 0.615(2) 0.039(7) Uiso 0.50 1 d PD A 1 
H2 H 0.4602 -0.1257 0.5620 0.047 Uiso 0.50 1 calc PR A 1 
C3 C 0.462(2) -0.2579(18) 0.5970(17) 0.054(6) Uani 1 1 d DU . . 
C4 C 0.388(3) -0.346(2) 0.5354(19) 0.084(10) Uani 1 1 d U B . 
H4A H 0.3589 -0.3299 0.4836 0.125 Uiso 1 1 d R . . 
H4B H 0.4234 -0.4053 0.5198 0.125 Uiso 1 1 d R . . 
H4C H 0.3291 -0.3621 0.5624 0.125 Uiso 1 1 d R . . 
O35' O 0.567(4) -0.124(4) 0.766(3) 0.105(15) Uiso 0.50 1 d PD A 2 
O36' O 0.521(4) -0.219(3) 0.559(3) 0.089(9) Uiso 0.50 1 d PD B 2 
H36' H 0.5066 -0.1629 0.5544 0.134 Uiso 0.50 1 d PR B 2 
N1' N 0.345(3) -0.113(3) 0.598(2) 0.044(6) Uiso 0.50 1 d PD A 2 
H1'A H 0.2947 -0.1564 0.5524 0.065 Uiso 0.50 1 d PR A 2 
H1'B H 0.3134 -0.0659 0.6312 0.065 Uiso 0.50 1 d PR A 2 
H1'C H 0.3949 -0.0803 0.5779 0.065 Uiso 0.50 1 d PR A 2 
C1' C 0.491(3) -0.093(2) 0.730(2) 0.038(9) Uiso 0.50 1 d PD A 2 
C2' C 0.411(3) -0.174(3) 0.651(2) 0.039(7) Uiso 0.50 1 d PD A 2 
H2' H 0.3580 -0.2099 0.6747 0.047 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.747(11) . ? 
W1 O2 1.903(10) . ? 
W1 O3 1.905(10) . ? 
W1 O5 1.900(10) . ? 
W1 O6 1.922(11) . ? 
W1 O4 2.294(10) . ? 
W2 O7 1.704(12) . ? 
W2 O9 1.814(11) . ? 
W2 O8 1.930(10) . ? 
W2 O10 1.946(10) . ? 
W2 O6 1.962(11) . ? 
W2 O4 2.352(10) . ? 
W3 O11 1.725(11) . ? 
W3 O14 1.866(10) . ? 
W3 O10 1.912(9) . ? 
W3 O12 1.912(10) . ? 
W3 O3 1.932(10) . ? 
W3 O13 2.388(11) . ? 
W4 O16 1.771(12) . ? 
W4 O17 1.765(10) . ? 
W4 O15 1.780(11) . ? 
W4 O14 2.049(11) . ? 
W4 O18 2.038(10) . ? 
W4 O13 2.289(10) . ? 
W5 O19 1.723(10) . ? 
W5 O18 1.864(10) . ? 
W5 O21 1.874(10) . ? 
W5 O12 1.946(11) . ? 
W5 O20 1.946(10) . ? 
W5 O13 2.383(9) . ? 
W6 O24 1.727(11) . ? 
W6 O23 1.817(10) . ? 
W6 O26 1.918(9) . ? 
W6 O21 1.951(10) . ? 
W6 O25 2.016(12) . ? 
W6 O22 2.341(10) . ? 
W7 O27 1.754(10) . ? 
W7 O29 1.807(10) . ? 
W7 O30 1.915(12) . ? 
W7 O26 1.927(10) . ? 
W7 O28 1.991(10) . ? 
W7 O22 2.285(9) . ? 
W8 O31 1.724(11) . ? 
W8 O32 1.838(11) . ? 
W8 O8 1.924(10) . ? 
W8 O30 1.943(12) . ? 
W8 O2 1.986(11) . ? 
W8 O4 2.359(9) . ? 
W9 O33 1.706(10) . ? 
W9 O5 1.908(10) . ? 
W9 O25 1.875(12) . ? 
W9 O20 1.909(9) . ? 
W9 O28 1.915(10) . ? 
W9 O22 2.369(10) . ? 
Gd1 O7M 2.20(6) . ? 
Gd1 O9W 2.43(2) . ? 
Gd1 O5W 2.41(2) . ? 
Gd1 O7W 2.39(4) . ? 
Gd1 O1 2.445(11) . ? 
Gd1 O11W 2.62(5) . ? 
Gd1 O10W 2.37(4) . ? 
Gd1 O6W 2.433(15) . ? 
Gd1 O11M 2.46(4) . ? 
Gd1 O12W 2.50(3) . ? 
Gd1 O12M 2.43(4) . ? 
Gd1 O10M 2.54(5) . ? 
As1 O22 1.811(9) . ? 
As1 O4 1.802(9) . ? 
As1 O13 1.803(9) . ? 
Fe1 O16 1.945(12) . ? 
Fe1 O23 1.921(10) . ? 
Fe1 O15 1.957(11) 2_667 ? 
Fe1 O9 1.942(11) 2_667 ? 
Fe1 O2W 2.105(13) . ? 
Fe1 O1W 2.143(10) . ? 
O3W Fe2 2.072(13) . ? 
O4W Fe2 2.061(12) . ? 
O7W O7M 1.94(7) . ? 
O7M O12M 1.69(7) . ? 
O10W O10M 0.83(6) . ? 
O11W O11M 0.83(5) . ? 
O12W O12M 1.08(5) . ? 
O16W O16M 1.62(7) . ? 
O18W O18M 0.95(5) . ? 
O9 Fe1 1.942(10) 2_667 ? 
O15 Fe1 1.957(11) 2_667 ? 
O17 Fe2 1.989(10) 2_667 ? 
O29 Fe2 1.975(11) . ? 
O32 Fe2 1.919(12) . ? 
O34 C1' 1.16(3) . ? 
O34 C1 1.17(2) . ? 
O34 Fe2 2.037(11) . ? 
Fe2 O17 1.989(11) 2_667 ? 
O35 C1 1.21(3) . ? 
O36 C3 1.21(4) . ? 
N1 C2 1.56(3) . ? 
C1 C2 1.53(4) . ? 
C2 C3 1.50(3) . ? 
C3 O36' 1.22(4) . ? 
C3 C4 1.42(4) . ? 
C3 C2' 1.50(3) . ? 
O35' C1' 1.22(3) . ? 
N1' C2' 1.56(3) . ? 
C1' C2' 1.53(4) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O2 99.5(5) . . ? 
O1 W1 O3 104.2(5) . . ? 
O2 W1 O3 155.7(4) . . ? 
O1 W1 O5 101.1(5) . . ? 
O2 W1 O5 91.1(4) . . ? 
O3 W1 O5 89.6(4) . . ? 
O1 W1 O6 96.6(5) . . ? 
O2 W1 O6 86.2(4) . . ? 
O3 W1 O6 85.8(4) . . ? 
O5 W1 O6 162.2(5) . . ? 
O1 W1 O4 170.0(4) . . ? 
O2 W1 O4 73.4(4) . . ? 
O3 W1 O4 82.4(4) . . ? 
O5 W1 O4 86.3(4) . . ? 
O6 W1 O4 76.1(4) . . ? 
O7 W2 O9 102.7(6) . . ? 
O7 W2 O8 102.2(5) . . ? 
O9 W2 O8 93.3(4) . . ? 
O7 W2 O10 99.7(5) . . ? 
O9 W2 O10 90.3(4) . . ? 
O8 W2 O10 156.5(4) . . ? 
O7 W2 O6 100.7(6) . . ? 
O9 W2 O6 156.4(5) . . ? 
O8 W2 O6 84.7(4) . . ? 
O10 W2 O6 82.7(4) . . ? 
O7 W2 O4 173.6(5) . . ? 
O9 W2 O4 82.9(4) . . ? 
O8 W2 O4 74.0(4) . . ? 
O10 W2 O4 83.4(4) . . ? 
O6 W2 O4 74.0(4) . . ? 
O11 W3 O14 100.0(5) . . ? 
O11 W3 O10 99.6(5) . . ? 
O14 W3 O10 91.3(5) . . ? 
O11 W3 O12 99.7(5) . . ? 
O14 W3 O12 89.9(5) . . ? 
O10 W3 O12 160.1(4) . . ? 
O11 W3 O3 103.2(5) . . ? 
O14 W3 O3 156.7(4) . . ? 
O10 W3 O3 86.6(4) . . ? 
O12 W3 O3 84.5(4) . . ? 
O11 W3 O13 170.6(4) . . ? 
O14 W3 O13 72.6(4) . . ? 
O10 W3 O13 86.6(4) . . ? 
O12 W3 O13 74.9(4) . . ? 
O3 W3 O13 84.1(4) . . ? 
O16 W4 O17 103.0(5) . . ? 
O16 W4 O15 97.7(5) . . ? 
O17 W4 O15 103.5(5) . . ? 
O16 W4 O14 158.6(4) . . ? 
O17 W4 O14 94.9(5) . . ? 
O15 W4 O14 89.3(5) . . ? 
O16 W4 O18 86.3(5) . . ? 
O17 W4 O18 96.4(4) . . ? 
O15 W4 O18 158.2(4) . . ? 
O14 W4 O18 80.1(4) . . ? 
O16 W4 O13 88.3(5) . . ? 
O17 W4 O13 163.5(4) . . ? 
O15 W4 O13 86.6(4) . . ? 
O14 W4 O13 71.9(4) . . ? 
O18 W4 O13 72.0(4) . . ? 
O19 W5 O18 101.1(5) . . ? 
O19 W5 O21 103.1(5) . . ? 
O18 W5 O21 92.9(4) . . ? 
O19 W5 O12 98.1(5) . . ? 
O18 W5 O12 88.2(5) . . ? 
O21 W5 O12 158.2(4) . . ? 
O19 W5 O20 101.1(5) . . ? 
O18 W5 O20 157.3(4) . . ? 
O21 W5 O20 86.3(4) . . ? 
O12 W5 O20 84.4(4) . . ? 
O19 W5 O13 170.2(4) . . ? 
O18 W5 O13 72.7(4) . . ? 
O21 W5 O13 85.0(4) . . ? 
O12 W5 O13 74.5(4) . . ? 
O20 W5 O13 84.7(4) . . ? 
O24 W6 O23 102.5(5) . . ? 
O24 W6 O26 101.5(5) . . ? 
O23 W6 O26 95.0(4) . . ? 
O24 W6 O21 101.7(5) . . ? 
O23 W6 O21 91.2(4) . . ? 
O26 W6 O21 154.1(4) . . ? 
O24 W6 O25 99.0(5) . . ? 
O23 W6 O25 158.3(5) . . ? 
O26 W6 O25 83.8(4) . . ? 
O21 W6 O25 81.3(4) . . ? 
O24 W6 O22 171.3(4) . . ? 
O23 W6 O22 84.5(4) . . ? 
O26 W6 O22 72.5(4) . . ? 
O21 W6 O22 83.2(4) . . ? 
O25 W6 O22 74.4(4) . . ? 
O27 W7 O29 103.5(5) . . ? 
O27 W7 O30 101.5(5) . . ? 
O29 W7 O30 90.5(5) . . ? 
O27 W7 O26 97.2(5) . . ? 
O29 W7 O26 90.5(4) . . ? 
O30 W7 O26 160.5(4) . . ? 
O27 W7 O28 96.1(5) . . ? 
O29 W7 O28 160.4(4) . . ? 
O30 W7 O28 86.1(4) . . ? 
O26 W7 O28 86.4(4) . . ? 
O27 W7 O22 166.0(5) . . ? 
O29 W7 O22 87.4(4) . . ? 
O30 W7 O22 86.9(4) . . ? 
O26 W7 O22 73.7(4) . . ? 
O28 W7 O22 73.1(4) . . ? 
O31 W8 O32 104.0(5) . . ? 
O31 W8 O8 100.6(5) . . ? 
O32 W8 O8 92.1(5) . . ? 
O31 W8 O30 100.0(5) . . ? 
O32 W8 O30 88.8(5) . . ? 
O8 W8 O30 158.5(4) . . ? 
O31 W8 O2 97.1(5) . . ? 
O32 W8 O2 158.6(4) . . ? 
O8 W8 O2 87.5(4) . . ? 
O30 W8 O2 84.0(4) . . ? 
O31 W8 O4 166.4(5) . . ? 
O32 W8 O4 88.7(4) . . ? 
O8 W8 O4 74.0(4) . . ? 
O30 W8 O4 84.6(4) . . ? 
O2 W8 O4 70.5(4) . . ? 
O33 W9 O5 100.6(5) . . ? 
O33 W9 O25 98.9(5) . . ? 
O5 W9 O25 160.5(5) . . ? 
O33 W9 O20 102.4(5) . . ? 
O5 W9 O20 88.5(4) . . ? 
O25 W9 O20 86.4(5) . . ? 
O33 W9 O28 102.3(5) . . ? 
O5 W9 O28 90.0(4) . . ? 
O25 W9 O28 86.9(4) . . ? 
O20 W9 O28 155.1(4) . . ? 
O33 W9 O22 172.8(5) . . ? 
O5 W9 O22 84.4(4) . . ? 
O25 W9 O22 76.2(4) . . ? 
O20 W9 O22 82.7(4) . . ? 
O28 W9 O22 72.4(4) . . ? 
O7M Gd1 O9W 146.5(16) . . ? 
O7M Gd1 O5W 125.0(16) . . ? 
O9W Gd1 O5W 74.9(10) . . ? 
O7M Gd1 O7W 49.9(18) . . ? 
O9W Gd1 O7W 96.7(11) . . ? 
O5W Gd1 O7W 132.1(10) . . ? 
O7M Gd1 O1 77.2(15) . . ? 
O9W Gd1 O1 136.3(6) . . ? 
O5W Gd1 O1 75.4(7) . . ? 
O7W Gd1 O1 127.1(10) . . ? 
O7M Gd1 O11W 62.3(18) . . ? 
O9W Gd1 O11W 121.8(13) . . ? 
O5W Gd1 O11W 63.7(13) . . ? 
O7W Gd1 O11W 83.8(15) . . ? 
O1 Gd1 O11W 70.1(11) . . ? 
O7M Gd1 O10W 91.4(18) . . ? 
O9W Gd1 O10W 68.5(11) . . ? 
O5W Gd1 O10W 142.5(12) . . ? 
O7W Gd1 O10W 62.6(14) . . ? 
O1 Gd1 O10W 127.5(10) . . ? 
O11W Gd1 O10W 146.2(15) . . ? 
O7M Gd1 O6W 131.8(15) . . ? 
O9W Gd1 O6W 74.6(7) . . ? 
O5W Gd1 O6W 78.0(7) . . ? 
O7W Gd1 O6W 146.3(11) . . ? 
O1 Gd1 O6W 68.3(5) . . ? 
O11W Gd1 O6W 128.8(12) . . ? 
O10W Gd1 O6W 84.2(11) . . ? 
O7M Gd1 O11M 44.1(17) . . ? 
O9W Gd1 O11M 137.3(12) . . ? 
O5W Gd1 O11M 81.2(12) . . ? 
O7W Gd1 O11M 74.0(14) . . ? 
O1 Gd1 O11M 66.8(10) . . ? 
O11W Gd1 O11M 18.5(12) . . ? 
O10W Gd1 O11M 132.8(14) . . ? 
O6W Gd1 O11M 133.9(10) . . ? 
O7M Gd1 O12W 66.7(16) . . ? 
O9W Gd1 O12W 118.2(11) . . ? 
O5W Gd1 O12W 139.2(9) . . ? 
O7W Gd1 O12W 86.9(12) . . ? 
O1 Gd1 O12W 69.6(9) . . ? 
O11W Gd1 O12W 120.0(14) . . ? 
O10W Gd1 O12W 59.0(12) . . ? 
O6W Gd1 O12W 70.1(10) . . ? 
O11M Gd1 O12W 103.1(13) . . ? 
O7M Gd1 O12M 42.4(17) . . ? 
O9W Gd1 O12M 140.4(13) . . ? 
O5W Gd1 O12M 138.8(13) . . ? 
O7W Gd1 O12M 74.9(14) . . ? 
O1 Gd1 O12M 63.7(11) . . ? 
O11W Gd1 O12M 96.1(16) . . ? 
O10W Gd1 O12M 73.5(14) . . ? 
O6W Gd1 O12M 91.1(12) . . ? 
O11M Gd1 O12M 78.4(15) . . ? 
O12W Gd1 O12M 25.2(11) . . ? 
O7M Gd1 O10M 81.1(19) . . ? 
O9W Gd1 O10M 71.5(14) . . ? 
O5W Gd1 O10M 144.7(14) . . ? 
O7W Gd1 O10M 44.3(16) . . ? 
O1 Gd1 O10M 138.5(12) . . ? 
O11W Gd1 O10M 128.0(17) . . ? 
O10W Gd1 O10M 19.1(13) . . ? 
O6W Gd1 O10M 103.0(14) . . ? 
O11M Gd1 O10M 117.4(16) . . ? 
O12W Gd1 O10M 69.3(14) . . ? 
O12M Gd1 O10M 76.4(16) . . ? 
O22 As1 O4 96.5(5) . . ? 
O22 As1 O13 98.3(4) . . ? 
O4 As1 O13 98.6(5) . . ? 
O16 Fe1 O23 92.6(5) . . ? 
O16 Fe1 O15 92.9(5) . 2_667 ? 
O23 Fe1 O15 96.2(4) . 2_667 ? 
O16 Fe1 O9 94.0(5) . 2_667 ? 
O23 Fe1 O9 168.8(5) . 2_667 ? 
O15 Fe1 O9 92.6(4) 2_667 2_667 ? 
O16 Fe1 O2W 176.9(5) . . ? 
O23 Fe1 O2W 84.7(5) . . ? 
O15 Fe1 O2W 85.7(5) 2_667 . ? 
O9 Fe1 O2W 88.9(5) 2_667 . ? 
O16 Fe1 O1W 91.7(5) . . ? 
O23 Fe1 O1W 87.9(5) . . ? 
O15 Fe1 O1W 173.7(5) 2_667 . ? 
O9 Fe1 O1W 82.9(4) 2_667 . ? 
O2W Fe1 O1W 89.9(5) . . ? 
O7M O7W Gd1 60(2) . . ? 
O12M O7M O7W 108(4) . . ? 
O12M O7M Gd1 76(3) . . ? 
O7W O7M Gd1 70(2) . . ? 
O10M O10W Gd1 92(5) . . ? 
O10W O10M Gd1 69(5) . . ? 
O11M O11W Gd1 70(5) . . ? 
O11W O11M Gd1 92(5) . . ? 
O12M O12W Gd1 74(3) . . ? 
O12W O12M O7M 138(5) . . ? 
O12W O12M Gd1 81(3) . . ? 
O7M O12M Gd1 61(2) . . ? 
W1 O1 Gd1 148.6(6) . . ? 
W1 O2 W8 122.0(5) . . ? 
W1 O3 W3 145.8(6) . . ? 
As1 O4 W1 135.4(5) . . ? 
As1 O4 W2 118.0(5) . . ? 
W1 O4 W2 91.6(3) . . ? 
As1 O4 W8 116.4(5) . . ? 
W1 O4 W8 93.9(3) . . ? 
W2 O4 W8 90.9(3) . . ? 
W9 O5 W1 155.9(6) . . ? 
W1 O6 W2 118.1(6) . . ? 
W8 O8 W2 121.1(5) . . ? 
W2 O9 Fe1 142.3(6) . 2_667 ? 
W3 O10 W2 145.6(6) . . ? 
W3 O12 W5 121.0(5) . . ? 
As1 O13 W4 114.6(5) . . ? 
As1 O13 W3 127.2(5) . . ? 
W4 O13 W3 93.9(3) . . ? 
As1 O13 W5 128.9(5) . . ? 
W4 O13 W5 93.6(3) . . ? 
W3 O13 W5 89.5(3) . . ? 
W3 O14 W4 121.6(5) . . ? 
W4 O15 Fe1 178.3(7) . 2_667 ? 
W4 O16 Fe1 167.9(7) . . ? 
W4 O17 Fe2 164.2(7) . 2_667 ? 
W5 O18 W4 121.5(5) . . ? 
W9 O20 W5 144.8(6) . . ? 
W5 O21 W6 148.1(6) . . ? 
As1 O22 W7 117.4(5) . . ? 
As1 O22 W6 118.4(5) . . ? 
W7 O22 W6 92.7(4) . . ? 
As1 O22 W9 134.3(5) . . ? 
W7 O22 W9 93.7(3) . . ? 
W6 O22 W9 90.5(3) . . ? 
W6 O23 Fe1 145.0(6) . . ? 
W9 O25 W6 118.5(5) . . ? 
W6 O26 W7 121.1(5) . . ? 
W9 O28 W7 120.7(5) . . ? 
W7 O29 Fe2 135.6(6) . . ? 
W7 O30 W8 145.7(6) . . ? 
W8 O32 Fe2 138.1(6) . . ? 
C1' O34 C1 49(2) . . ? 
C1' O34 Fe2 143(2) . . ? 
C1 O34 Fe2 136.0(16) . . ? 
O32 Fe2 O29 88.1(4) . . ? 
O32 Fe2 O17 98.0(5) . 2_667 ? 
O29 Fe2 O17 97.6(4) . 2_667 ? 
O32 Fe2 O34 89.8(5) . . ? 
O29 Fe2 O34 91.5(4) . . ? 
O17 Fe2 O34 168.2(5) 2_667 . ? 
O32 Fe2 O3W 176.0(5) . . ? 
O29 Fe2 O3W 90.1(5) . . ? 
O17 Fe2 O3W 85.8(5) 2_667 . ? 
O34 Fe2 O3W 86.7(5) . . ? 
O32 Fe2 O4W 92.6(6) . . ? 
O29 Fe2 O4W 175.6(4) . . ? 
O17 Fe2 O4W 86.6(5) 2_667 . ? 
O34 Fe2 O4W 84.1(5) . . ? 
O3W Fe2 O4W 88.9(6) . . ? 
O34 C1 O35 129(3) . . ? 
O34 C1 C2 121(2) . . ? 
O35 C1 C2 108(2) . . ? 
C3 C2 C1 123(3) . . ? 
C3 C2 N1 105(2) . . ? 
C1 C2 N1 106(3) . . ? 
O36 C3 O36' 115(4) . . ? 
O36 C3 C4 113(3) . . ? 
O36' C3 C4 110(3) . . ? 
O36 C3 C2 114(3) . . ? 
O36' C3 C2 71(3) . . ? 
C4 C3 C2 127(3) . . ? 
O36 C3 C2' 94(3) . . ? 
O36' C3 C2' 109(3) . . ? 
C4 C3 C2' 116(3) . . ? 
C2 C3 C2' 38(2) . . ? 
O34 C1' O35' 123(4) . . ? 
O34 C1' C2' 120(3) . . ? 
O35' C1' C2' 117(3) . . ? 
C3 C2' N1' 116(3) . . ? 
C3 C2' C1' 114(3) . . ? 
N1' C2' C1' 109(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.973 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.973 
_refine_diff_density_max    2.473 
_refine_diff_density_min   -4.361 
_refine_diff_density_rms    0.450 
  
  

#===END

  
data_11-Tb 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Fe4 N2 O116 Tb2 W18' 
_chemical_formula_weight          6087.33 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Tb'  'Tb'  -0.1723   4.1537 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6063(13) 
_cell_length_b                    13.4464(14) 
_cell_length_c                    16.0241(17) 
_cell_angle_alpha                 106.473(2) 
_cell_angle_beta                  99.828(2) 
_cell_angle_gamma                 97.290(2) 
_cell_volume                      2522.0(5) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8575 
_cell_measurement_theta_min       1.75 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky 
_exptl_crystal_colour             'Light yellow'  
_exptl_crystal_size_max           0.48 
_exptl_crystal_size_mid           0.17 
_exptl_crystal_size_min           0.14 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     4.008 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2728 
_exptl_absorpt_coefficient_mu     23.155 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0318 
_exptl_absorpt_correction_T_max   0.1399 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12412 
_diffrn_reflns_av_R_equivalents   0.0358 
_diffrn_reflns_av_sigmaI/netI     0.0647 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        14 
_diffrn_reflns_limit_k_min        -11 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -19 
_diffrn_reflns_limit_l_max        18 
_diffrn_reflns_theta_min          1.75 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8575 
_reflns_number_gt                 7565 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral.
 However, its structure is pseudo-centrosymmetric, i.e. most of the 
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are 
 rather common. An attempt to refine the structure in P¨C1 shows the 
 disorder around the chiral centre of L-thr (because we impose inversion
 on a chiral entity), as a result, C1, C2, N1, O35 and O36 atoms on 
 L-thr are disordered over two positions. In addition, some coordination
 water molecules on Tb3+ cations are disordered over two positions. 
 The ISOR instruction is used for O3, O9W, O8, O13, O15, O22, O12, 
 O33, O24, O9, O17, O4, O23, O14 and O29. The SADI instruction is used
 for C2' C1' C2 C1, O34 C1' O34 C1, O35' C1' O35 C1, N1' C2' N1 C2, C3
 C2' C3 C2, O36 C3 O36' C3, N1' C2' N1 C2. The EADP instruction is used 
 for C2 and C2', N1 and N1', O36 and O36'. The O7W, O7M, O8W, O10W, O10M,
 O11W, O11M, O12W, O12M, O13W, O14W, O15W, O16W, O16M, O18W, O18M, O22W,
 O35, O35', O36, O36', C1, C1', C2, C2', N1 and N1' are refined 
 isostropicallly. 654 parameters and 96 restraints are used in
 the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0866P)²+80.9921P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00011(4) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8575 
_refine_ls_number_parameters      654 
_refine_ls_number_restraints      96 
_refine_ls_R_factor_all           0.0641 
_refine_ls_R_factor_gt            0.0569 
_refine_ls_wR_factor_ref          0.1507 
_refine_ls_wR_factor_gt           0.1459 
_refine_ls_goodness_of_fit_ref    1.039 
_refine_ls_restrained_S_all       1.034 
_refine_ls_shift/su_max           0.005 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.20811(6) 0.31038(5) 0.59245(4) 0.01527(18) Uani 1 1 d . . . 
W2 W 0.46392(5) 0.44173(5) 0.67700(4) 0.01335(18) Uani 1 1 d . . . 
W3 W 0.24311(5) 0.57409(5) 0.75215(4) 0.01348(18) Uani 1 1 d . . . 
W4 W 0.35683(5) 0.61309(5) 0.97037(4) 0.00918(17) Uani 1 1 d . . . 
W5 W 0.09390(5) 0.48496(5) 0.87902(4) 0.01144(17) Uani 1 1 d . . . 
W6 W 0.15143(5) 0.25519(5) 0.94704(4) 0.01334(18) Uani 1 1 d . . . 
W7 W 0.24633(5) 0.08820(5) 0.79185(4) 0.01378(18) Uani 1 1 d . . . 
W8 W 0.41039(6) 0.18333(5) 0.65141(4) 0.01508(18) Uani 1 1 d . . . 
W9 W 0.04143(5) 0.21118(5) 0.73221(4) 0.01350(18) Uani 1 1 d . . . 
Tb1 Tb 0.11668(10) 0.24331(11) 0.33018(8) 0.0454(3) Uani 1 1 d . . . 
As1 As 0.33835(12) 0.35848(12) 0.83522(10) 0.0076(3) Uani 1 1 d . . . 
Fe1 Fe 0.38292(18) 0.42937(17) 1.10214(15) 0.0107(5) Uani 1 1 d . . . 
O1W O 0.2430(11) 0.4532(11) 1.1563(9) 0.027(3) Uani 1 1 d . . . 
O2W O 0.4070(12) 0.3162(11) 1.1682(10) 0.032(3) Uani 1 1 d . . . 
O3W O 0.5533(15) 0.0507(12) 0.9345(12) 0.045(4) Uani 1 1 d . . . 
O4W O 0.6859(12) 0.1172(13) 0.8223(13) 0.049(5) Uani 1 1 d . . . 
O5W O 0.238(3) 0.143(2) 0.3785(18) 0.103(10) Uani 1 1 d . . . 
O6W O 0.279(2) 0.3744(18) 0.4038(13) 0.072(6) Uani 1 1 d . . . 
O7W O -0.041(4) 0.164(3) 0.223(3) 0.083(11) Uiso 0.60 1 d P . . 
O7M O -0.051(3) 0.208(3) 0.342(3) 0.036(9) Uiso 0.40 1 d P . . 
O8W O 0.058(3) 0.063(3) 0.221(3) 0.134(12) Uiso 1 1 d . . . 
O9W O 0.234(3) 0.220(3) 0.221(2) 0.114(10) Uani 1 1 d U . . 
O10W O 0.058(5) 0.313(4) 0.217(4) 0.101(16) Uiso 0.65 1 d P . . 
O10M O 0.011(9) 0.279(8) 0.205(7) 0.10(3) Uiso 0.35 1 d P . . 
O11W O -0.004(5) 0.098(4) 0.370(4) 0.111(16) Uiso 0.60 1 d P . . 
O11M O -0.067(12) 0.072(11) 0.448(10) 0.20(5) Uiso 0.40 1 d P . . 
O12W O 0.056(3) 0.415(3) 0.382(2) 0.062(9) Uiso 0.60 1 d P . . 
O12M O 0.000(14) 0.350(13) 0.374(11) 0.21(6) Uiso 0.40 1 d P . . 
O13W O -0.117(4) 0.183(4) 0.070(3) 0.178(18) Uiso 1 1 d . . . 
O14W O 0.795(4) -0.034(4) 0.916(3) 0.072(12) Uiso 0.50 1 d P . . 
O15W O 0.127(8) 0.528(8) 0.493(7) 0.17(3) Uiso 0.50 1 d P . . 
O16W O 0.311(4) -0.046(4) 0.361(3) 0.094(13) Uiso 0.60 1 d P . . 
O16M O 0.317(7) -0.122(6) 0.412(6) 0.11(2) Uiso 0.40 1 d P . . 
O17W O 0.385(2) 0.1358(16) 1.0437(14) 0.072(6) Uani 1 1 d . . . 
O18W O 0.359(4) -0.119(3) 0.891(3) 0.097(12) Uiso 0.70 1 d P . . 
O18M O 0.285(3) -0.133(3) 0.915(2) 0.010(7) Uiso 0.30 1 d P . . 
O19W O -0.1648(12) 0.2900(13) 0.8732(11) 0.040(4) Uani 1 1 d . . . 
O20W O 0.7335(18) 0.3445(18) 0.7316(14) 0.076(7) Uani 1 1 d . . . 
O21W O -0.0965(19) 0.3993(18) 0.6346(15) 0.069(6) Uani 1 1 d . . . 
O22W O 0.121(2) -0.002(2) 0.5149(17) 0.078(6) Uiso 1 1 d . . . 
O23W O 0.128(3) -0.210(2) 0.5100(18) 0.103(9) Uani 1 1 d . . . 
O1 O 0.1303(10) 0.2903(10) 0.4879(8) 0.023(3) Uani 1 1 d . . . 
O2 O 0.2854(11) 0.1948(9) 0.5652(8) 0.019(3) Uani 1 1 d . . . 
O3 O 0.1785(10) 0.4385(9) 0.6622(8) 0.019(3) Uani 1 1 d U . . 
O4 O 0.3374(9) 0.3317(8) 0.7195(7) 0.012(2) Uani 1 1 d U . . 
O5 O 0.1103(9) 0.2356(9) 0.6401(8) 0.018(3) Uani 1 1 d . . . 
O6 O 0.3350(10) 0.3922(9) 0.5792(7) 0.017(3) Uani 1 1 d . . . 
O7 O 0.5495(12) 0.5127(10) 0.6327(10) 0.030(3) Uani 1 1 d . . . 
O8 O 0.4926(9) 0.3017(9) 0.6310(8) 0.017(3) Uani 1 1 d U . . 
O9 O 0.5408(9) 0.4603(9) 0.7858(8) 0.016(2) Uani 1 1 d U . . 
O10 O 0.3802(9) 0.5490(9) 0.7257(8) 0.015(2) Uani 1 1 d . . . 
O11 O 0.2161(11) 0.6631(10) 0.6969(8) 0.024(3) Uani 1 1 d . . . 
O12 O 0.1057(9) 0.5570(9) 0.7921(8) 0.015(2) Uani 1 1 d U . . 
O13 O 0.2717(9) 0.4715(8) 0.8499(7) 0.009(2) Uani 1 1 d U . . 
O14 O 0.3125(9) 0.6665(9) 0.8647(8) 0.013(2) Uani 1 1 d U . . 
O15 O 0.4822(9) 0.5939(10) 0.9359(8) 0.019(3) Uani 1 1 d U . . 
O16 O 0.3576(10) 0.5267(9) 1.0369(8) 0.019(3) Uani 1 1 d . . . 
O17 O 0.3934(9) 0.7406(8) 1.0501(8) 0.015(2) Uani 1 1 d U . . 
O18 O 0.1928(9) 0.5988(9) 0.9639(7) 0.011(2) Uani 1 1 d . . . 
O19 O -0.0311(10) 0.5155(11) 0.8982(10) 0.028(3) Uani 1 1 d . . . 
O20 O 0.0458(10) 0.3602(9) 0.7765(8) 0.018(3) Uani 1 1 d . . . 
O21 O 0.1211(10) 0.3932(9) 0.9460(8) 0.017(3) Uani 1 1 d . . . 
O22 O 0.2210(10) 0.2602(9) 0.8209(8) 0.015(2) Uani 1 1 d U . . 
O23 O 0.2904(9) 0.3135(8) 1.0075(7) 0.011(2) Uani 1 1 d U . . 
O24 O 0.0877(11) 0.2348(10) 1.0277(8) 0.023(3) Uani 1 1 d U . . 
O25 O 0.0211(10) 0.2095(10) 0.8473(9) 0.023(3) Uani 1 1 d . . . 
O26 O 0.1822(10) 0.1174(9) 0.8948(8) 0.019(3) Uani 1 1 d . . . 
O27 O 0.2317(10) -0.0473(9) 0.7680(9) 0.022(3) Uani 1 1 d . . . 
O28 O 0.0981(10) 0.0825(9) 0.7206(8) 0.019(3) Uani 1 1 d . . . 
O29 O 0.3835(9) 0.1380(8) 0.8601(8) 0.012(2) Uani 1 1 d U . . 
O30 O 0.2989(9) 0.1066(9) 0.6916(8) 0.014(2) Uani 1 1 d . . . 
O31 O 0.4490(12) 0.0799(11) 0.5815(9) 0.029(3) Uani 1 1 d . . . 
O32 O 0.5040(10) 0.2061(9) 0.7591(8) 0.018(3) Uani 1 1 d . . . 
O33 O -0.0916(10) 0.1623(10) 0.6720(8) 0.021(3) Uani 1 1 d U . . 
O34 O 0.4850(11) -0.0067(9) 0.7507(9) 0.024(3) Uani 1 1 d D . . 
Fe2 Fe 0.53325(19) 0.13591(18) 0.84597(16) 0.0146(5) Uani 1 1 d . . . 
O35 O 0.623(3) -0.036(4) 0.684(3) 0.076(9) Uiso 0.50 1 d PD . 1 
O36 O 0.458(4) -0.249(4) 0.688(3) 0.085(10) Uiso 0.50 1 d PD A 1 
H36 H 0.4812 -0.3043 0.6757 0.127 Uiso 0.50 1 d PR A 1 
N1 N 0.331(3) -0.132(3) 0.617(3) 0.038(7) Uiso 0.50 1 d PD A 1 
H1A H 0.2941 -0.1838 0.5693 0.046 Uiso 0.50 1 d PR A 1 
H1B H 0.3224 -0.1473 0.6646 0.046 Uiso 0.50 1 d PR A 1 
H1C H 0.3049 -0.0730 0.6176 0.046 Uiso 0.50 1 d PR A 1 
C1 C 0.526(3) -0.057(3) 0.690(3) 0.034(7) Uiso 0.50 1 d PD A 1 
C2 C 0.453(3) -0.146(2) 0.616(3) 0.029(6) Uiso 0.50 1 d PD A 1 
H2 H 0.4673 -0.1335 0.5616 0.035 Uiso 0.50 1 calc PR A 1 
C3 C 0.460(3) -0.258(2) 0.6038(18) 0.056(7) Uani 1 1 d D . . 
C4 C 0.381(3) -0.342(2) 0.533(2) 0.072(10) Uani 1 1 d . A . 
H4A H 0.3519 -0.3261 0.4809 0.108 Uiso 1 1 d R . . 
H4B H 0.4164 -0.4015 0.5171 0.108 Uiso 1 1 d R . . 
H4C H 0.3221 -0.3584 0.5598 0.108 Uiso 1 1 d R . . 
O35' O 0.580(3) -0.119(4) 0.761(3) 0.076(9) Uiso 0.50 1 d PD A 2 
O36' O 0.524(4) -0.218(4) 0.559(3) 0.085(10) Uiso 0.50 1 d PD A 2 
H36' H 0.5095 -0.1619 0.5547 0.127 Uiso 0.50 1 d PR A 2 
N1' N 0.351(3) -0.111(3) 0.598(3) 0.038(7) Uiso 0.50 1 d PD A 2 
H1'A H 0.3012 -0.1547 0.5532 0.057 Uiso 0.50 1 d PR A 2 
H1'B H 0.3199 -0.0641 0.6320 0.057 Uiso 0.50 1 d PR A 2 
H1'C H 0.4015 -0.0786 0.5787 0.057 Uiso 0.50 1 d PR A 2 
C1' C 0.486(3) -0.103(3) 0.733(3) 0.034(7) Uiso 0.50 1 d PD A 2 
C2' C 0.406(3) -0.178(3) 0.655(2) 0.029(6) Uiso 0.50 1 d PD A 2 
H2' H 0.3488 -0.2143 0.6759 0.035 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.720(12) . ? 
W1 O5 1.887(12) . ? 
W1 O3 1.889(12) . ? 
W1 O6 1.901(12) . ? 
W1 O2 1.923(12) . ? 
W1 O4 2.302(11) . ? 
W2 O7 1.721(13) . ? 
W2 O9 1.777(12) . ? 
W2 O8 1.922(12) . ? 
W2 O6 1.950(12) . ? 
W2 O10 1.957(11) . ? 
W2 O4 2.354(11) . ? 
W3 O11 1.713(12) . ? 
W3 O14 1.865(11) . ? 
W3 O10 1.897(11) . ? 
W3 O3 1.949(11) . ? 
W3 O12 1.956(11) . ? 
W3 O13 2.377(11) . ? 
W4 O17 1.772(11) . ? 
W4 O16 1.785(13) . ? 
W4 O15 1.787(11) . ? 
W4 O18 2.034(11) . ? 
W4 O14 2.040(12) . ? 
W4 O13 2.279(11) . ? 
W5 O19 1.733(12) . ? 
W5 O18 1.872(11) . ? 
W5 O21 1.878(13) . ? 
W5 O12 1.923(12) . ? 
W5 O20 1.928(12) . ? 
W5 O13 2.385(10) . ? 
W6 O24 1.700(12) . ? 
W6 O23 1.807(11) . ? 
W6 O26 1.923(12) . ? 
W6 O21 1.945(12) . ? 
W6 O25 1.980(13) . ? 
W6 O22 2.351(11) . ? 
W7 O27 1.731(12) . ? 
W7 O29 1.811(11) . ? 
W7 O30 1.904(12) . ? 
W7 O26 1.924(12) . ? 
W7 O28 1.997(12) . ? 
W7 O22 2.301(11) . ? 
W8 O31 1.702(13) . ? 
W8 O32 1.838(13) . ? 
W8 O8 1.925(12) . ? 
W8 O30 1.943(12) . ? 
W8 O2 1.963(13) . ? 
W8 O4 2.364(11) . ? 
W9 O33 1.728(12) . ? 
W9 O25 1.911(14) . ? 
W9 O20 1.917(12) . ? 
W9 O5 1.918(13) . ? 
W9 O28 1.927(12) . ? 
W9 O22 2.360(12) . ? 
Tb1 O7M 2.16(4) . ? 
Tb1 O12M 2.24(16) . ? 
Tb1 O7W 2.30(4) . ? 
Tb1 O10W 2.32(5) . ? 
Tb1 O5W 2.34(3) . ? 
Tb1 O1 2.395(12) . ? 
Tb1 O6W 2.40(2) . ? 
Tb1 O10M 2.41(11) . ? 
Tb1 O9W 2.45(3) . ? 
Tb1 O8W 2.48(4) . ? 
Tb1 O12W 2.49(4) . ? 
Tb1 O11W 2.61(6) . ? 
As1 O4 1.784(11) . ? 
As1 O22 1.790(12) . ? 
As1 O13 1.805(11) . ? 
Fe1 O16 1.918(13) . ? 
Fe1 O23 1.919(11) . ? 
Fe1 O15 1.934(11) 2_667 ? 
Fe1 O9 1.971(12) 2_667 ? 
Fe1 O2W 2.108(14) . ? 
Fe1 O1W 2.116(13) . ? 
O3W Fe2 2.065(15) . ? 
O4W Fe2 2.056(16) . ? 
O7W O10M 1.71(11) . ? 
O7M O11W 1.80(7) . ? 
O10W O10M 0.67(10) . ? 
O11W O11M 1.69(15) . ? 
O11M O22W 1.41(15) 2_556 ? 
O12W O12M 1.02(16) . ? 
O16W O16M 1.48(9) . ? 
O16W O35 1.69(6) 2_656 ? 
O18W O18M 1.08(5) . ? 
O22W O11M 1.41(15) 2_556 ? 
O9 Fe1 1.971(12) 2_667 ? 
O15 Fe1 1.934(11) 2_667 ? 
O17 Fe2 1.976(11) 2_667 ? 
O29 Fe2 1.943(11) . ? 
O32 Fe2 1.903(12) . ? 
O34 C1 1.25(3) . ? 
O34 C1' 1.25(3) . ? 
O34 Fe2 2.026(12) . ? 
Fe2 O17 1.976(11) 2_667 ? 
O35 C1 1.26(5) . ? 
O35 O16W 1.69(6) 2_656 ? 
O36 C3 1.33(4) . ? 
N1 C2 1.58(4) . ? 
C1 C2 1.48(4) . ? 
C2 C3 1.47(4) . ? 
C3 O36' 1.33(4) . ? 
C3 C2' 1.47(4) . ? 
C3 C4 1.48(4) . ? 
O35' C1' 1.26(5) . ? 
N1' C2' 1.58(4) . ? 
C1' C2' 1.49(4) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O5 100.8(6) . . ? 
O1 W1 O3 104.0(6) . . ? 
O5 W1 O3 89.5(5) . . ? 
O1 W1 O6 96.9(6) . . ? 
O5 W1 O6 162.3(5) . . ? 
O3 W1 O6 86.8(5) . . ? 
O1 W1 O2 99.2(6) . . ? 
O5 W1 O2 91.5(5) . . ? 
O3 W1 O2 156.1(5) . . ? 
O6 W1 O2 85.0(5) . . ? 
O1 W1 O4 169.8(5) . . ? 
O5 W1 O4 86.8(4) . . ? 
O3 W1 O4 82.7(5) . . ? 
O6 W1 O4 75.6(4) . . ? 
O2 W1 O4 73.5(5) . . ? 
O7 W2 O9 103.8(6) . . ? 
O7 W2 O8 101.7(6) . . ? 
O9 W2 O8 93.2(5) . . ? 
O7 W2 O6 100.4(6) . . ? 
O9 W2 O6 155.6(5) . . ? 
O8 W2 O6 84.2(5) . . ? 
O7 W2 O10 99.9(6) . . ? 
O9 W2 O10 90.5(5) . . ? 
O8 W2 O10 156.6(5) . . ? 
O6 W2 O10 83.0(5) . . ? 
O7 W2 O4 173.0(6) . . ? 
O9 W2 O4 82.4(5) . . ? 
O8 W2 O4 74.5(4) . . ? 
O6 W2 O4 73.5(4) . . ? 
O10 W2 O4 83.0(4) . . ? 
O11 W3 O14 99.9(6) . . ? 
O11 W3 O10 100.6(6) . . ? 
O14 W3 O10 90.9(5) . . ? 
O11 W3 O3 103.2(6) . . ? 
O14 W3 O3 156.8(5) . . ? 
O10 W3 O3 87.0(5) . . ? 
O11 W3 O12 98.6(6) . . ? 
O14 W3 O12 90.3(5) . . ? 
O10 W3 O12 160.3(5) . . ? 
O3 W3 O12 84.2(5) . . ? 
O11 W3 O13 170.0(5) . . ? 
O14 W3 O13 72.5(4) . . ? 
O10 W3 O13 86.3(5) . . ? 
O3 W3 O13 84.3(5) . . ? 
O12 W3 O13 75.3(4) . . ? 
O17 W4 O16 103.6(5) . . ? 
O17 W4 O15 102.5(5) . . ? 
O16 W4 O15 97.8(6) . . ? 
O17 W4 O18 96.0(5) . . ? 
O16 W4 O18 87.1(5) . . ? 
O15 W4 O18 159.1(5) . . ? 
O17 W4 O14 94.6(5) . . ? 
O16 W4 O14 158.9(5) . . ? 
O15 W4 O14 88.5(5) . . ? 
O18 W4 O14 80.4(4) . . ? 
O17 W4 O13 163.2(5) . . ? 
O16 W4 O13 88.2(5) . . ? 
O15 W4 O13 87.4(5) . . ? 
O18 W4 O13 72.5(4) . . ? 
O14 W4 O13 71.9(4) . . ? 
O19 W5 O18 101.9(6) . . ? 
O19 W5 O21 103.0(6) . . ? 
O18 W5 O21 92.8(5) . . ? 
O19 W5 O12 96.6(6) . . ? 
O18 W5 O12 88.6(5) . . ? 
O21 W5 O12 159.6(5) . . ? 
O19 W5 O20 100.6(6) . . ? 
O18 W5 O20 157.1(5) . . ? 
O21 W5 O20 86.5(5) . . ? 
O12 W5 O20 84.3(5) . . ? 
O19 W5 O13 170.4(5) . . ? 
O18 W5 O13 72.7(4) . . ? 
O21 W5 O13 85.4(4) . . ? 
O12 W5 O13 75.7(4) . . ? 
O20 W5 O13 84.4(4) . . ? 
O24 W6 O23 103.1(6) . . ? 
O24 W6 O26 101.4(6) . . ? 
O23 W6 O26 95.5(5) . . ? 
O24 W6 O21 101.3(6) . . ? 
O23 W6 O21 90.7(5) . . ? 
O26 W6 O21 154.5(5) . . ? 
O24 W6 O25 97.7(6) . . ? 
O23 W6 O25 158.8(5) . . ? 
O26 W6 O25 84.4(5) . . ? 
O21 W6 O25 81.0(5) . . ? 
O24 W6 O22 171.3(5) . . ? 
O23 W6 O22 84.3(5) . . ? 
O26 W6 O22 73.0(5) . . ? 
O21 W6 O22 83.0(4) . . ? 
O25 W6 O22 75.3(5) . . ? 
O27 W7 O29 104.0(5) . . ? 
O27 W7 O30 100.7(6) . . ? 
O29 W7 O30 89.6(5) . . ? 
O27 W7 O26 98.3(6) . . ? 
O29 W7 O26 91.9(5) . . ? 
O30 W7 O26 160.0(5) . . ? 
O27 W7 O28 94.5(5) . . ? 
O29 W7 O28 161.5(5) . . ? 
O30 W7 O28 85.4(5) . . ? 
O26 W7 O28 86.8(5) . . ? 
O27 W7 O22 166.2(5) . . ? 
O29 W7 O22 88.0(5) . . ? 
O30 W7 O22 85.9(4) . . ? 
O26 W7 O22 74.2(4) . . ? 
O28 W7 O22 73.8(4) . . ? 
O31 W8 O32 103.6(6) . . ? 
O31 W8 O8 101.6(6) . . ? 
O32 W8 O8 92.0(5) . . ? 
O31 W8 O30 99.6(6) . . ? 
O32 W8 O30 88.7(5) . . ? 
O8 W8 O30 158.0(5) . . ? 
O31 W8 O2 96.9(6) . . ? 
O32 W8 O2 159.1(5) . . ? 
O8 W8 O2 87.6(5) . . ? 
O30 W8 O2 84.0(5) . . ? 
O31 W8 O4 167.6(6) . . ? 
O32 W8 O4 88.3(5) . . ? 
O8 W8 O4 74.2(4) . . ? 
O30 W8 O4 83.9(4) . . ? 
O2 W8 O4 71.4(4) . . ? 
O33 W9 O25 99.4(6) . . ? 
O33 W9 O20 103.4(6) . . ? 
O25 W9 O20 85.5(5) . . ? 
O33 W9 O5 99.9(5) . . ? 
O25 W9 O5 160.6(5) . . ? 
O20 W9 O5 88.2(5) . . ? 
O33 W9 O28 101.0(6) . . ? 
O25 W9 O28 88.0(5) . . ? 
O20 W9 O28 155.4(5) . . ? 
O5 W9 O28 90.2(5) . . ? 
O33 W9 O22 173.1(5) . . ? 
O25 W9 O22 76.3(4) . . ? 
O20 W9 O22 81.8(5) . . ? 
O5 W9 O22 84.7(4) . . ? 
O28 W9 O22 73.7(4) . . ? 
O7M Tb1 O12M 49(4) . . ? 
O7M Tb1 O7W 49.3(15) . . ? 
O12M Tb1 O7W 78(4) . . ? 
O7M Tb1 O10W 89.4(18) . . ? 
O12M Tb1 O10W 71(4) . . ? 
O7W Tb1 O10W 58.3(18) . . ? 
O7M Tb1 O5W 117.2(14) . . ? 
O12M Tb1 O5W 143(4) . . ? 
O7W Tb1 O5W 121.2(13) . . ? 
O10W Tb1 O5W 144.8(15) . . ? 
O7M Tb1 O1 76.4(11) . . ? 
O12M Tb1 O1 68(4) . . ? 
O7W Tb1 O1 125.5(11) . . ? 
O10W Tb1 O1 136.6(13) . . ? 
O5W Tb1 O1 75.3(7) . . ? 
O7M Tb1 O6W 139.1(12) . . ? 
O12M Tb1 O6W 95(4) . . ? 
O7W Tb1 O6W 155.5(12) . . ? 
O10W Tb1 O6W 97.2(16) . . ? 
O5W Tb1 O6W 78.0(10) . . ? 
O1 Tb1 O6W 71.2(6) . . ? 
O7M Tb1 O10M 76(3) . . ? 
O12M Tb1 O10M 69(5) . . ? 
O7W Tb1 O10M 42(3) . . ? 
O10W Tb1 O10M 16(2) . . ? 
O5W Tb1 O10M 147(2) . . ? 
O1 Tb1 O10M 137(2) . . ? 
O6W Tb1 O10M 113(3) . . ? 
O7M Tb1 O9W 142.4(13) . . ? 
O12M Tb1 O9W 137(4) . . ? 
O7W Tb1 O9W 93.2(13) . . ? 
O10W Tb1 O9W 68.5(16) . . ? 
O5W Tb1 O9W 76.7(12) . . ? 
O1 Tb1 O9W 140.2(9) . . ? 
O6W Tb1 O9W 75.8(10) . . ? 
O10M Tb1 O9W 76(3) . . ? 
O7M Tb1 O8W 79.5(14) . . ? 
O12M Tb1 O8W 124(4) . . ? 
O7W Tb1 O8W 48.1(14) . . ? 
O10W Tb1 O8W 89.4(17) . . ? 
O5W Tb1 O8W 74.6(11) . . ? 
O1 Tb1 O8W 126.5(10) . . ? 
O6W Tb1 O8W 140.6(11) . . ? 
O10M Tb1 O8W 79(3) . . ? 
O9W Tb1 O8W 70.6(12) . . ? 
O7M Tb1 O12W 73.2(13) . . ? 
O12M Tb1 O12W 24(4) . . ? 
O7W Tb1 O12W 94.6(14) . . ? 
O10W Tb1 O12W 65.6(15) . . ? 
O5W Tb1 O12W 141.1(11) . . ? 
O1 Tb1 O12W 71.1(9) . . ? 
O6W Tb1 O12W 73.0(11) . . ? 
O10M Tb1 O12W 70(3) . . ? 
O9W Tb1 O12W 119.4(12) . . ? 
O8W Tb1 O12W 142.6(13) . . ? 
O7M Tb1 O11W 43.1(16) . . ? 
O12M Tb1 O11W 87(4) . . ? 
O7W Tb1 O11W 67.5(17) . . ? 
O10W Tb1 O11W 124.5(19) . . ? 
O5W Tb1 O11W 74.5(15) . . ? 
O1 Tb1 O11W 69.3(13) . . ? 
O6W Tb1 O11W 136.3(14) . . ? 
O10M Tb1 O11W 108(3) . . ? 
O9W Tb1 O11W 128.1(15) . . ? 
O8W Tb1 O11W 60.6(15) . . ? 
O12W Tb1 O11W 110.1(15) . . ? 
O4 As1 O22 96.1(5) . . ? 
O4 As1 O13 98.1(5) . . ? 
O22 As1 O13 98.2(5) . . ? 
O16 Fe1 O23 92.2(5) . . ? 
O16 Fe1 O15 93.2(6) . 2_667 ? 
O23 Fe1 O15 95.7(5) . 2_667 ? 
O16 Fe1 O9 94.5(5) . 2_667 ? 
O23 Fe1 O9 168.6(5) . 2_667 ? 
O15 Fe1 O9 93.2(5) 2_667 2_667 ? 
O16 Fe1 O2W 177.2(5) . . ? 
O23 Fe1 O2W 85.1(5) . . ? 
O15 Fe1 O2W 86.6(6) 2_667 . ? 
O9 Fe1 O2W 88.3(5) 2_667 . ? 
O16 Fe1 O1W 91.6(5) . . ? 
O23 Fe1 O1W 87.5(5) . . ? 
O15 Fe1 O1W 174.1(6) 2_667 . ? 
O9 Fe1 O1W 83.1(5) 2_667 . ? 
O2W Fe1 O1W 88.8(6) . . ? 
O10M O7W Tb1 72(4) . . ? 
O11W O7M Tb1 82(2) . . ? 
O10M O10W Tb1 90(10) . . ? 
O10W O10M O7W 138(10) . . ? 
O10W O10M Tb1 74(10) . . ? 
O7W O10M Tb1 65(4) . . ? 
O11M O11W O7M 109(6) . . ? 
O11M O11W Tb1 145(6) . . ? 
O7M O11W Tb1 55.1(19) . . ? 
O22W O11M O11W 153(10) 2_556 . ? 
O12M O12W Tb1 64(9) . . ? 
O12W O12M Tb1 91(10) . . ? 
O16M O16W O35 149(5) . 2_656 ? 
W1 O1 Tb1 148.8(7) . . ? 
W1 O2 W8 121.6(6) . . ? 
W1 O3 W3 144.9(7) . . ? 
As1 O4 W1 135.8(6) . . ? 
As1 O4 W2 118.4(5) . . ? 
W1 O4 W2 91.2(4) . . ? 
As1 O4 W8 116.7(6) . . ? 
W1 O4 W8 93.3(4) . . ? 
W2 O4 W8 90.4(4) . . ? 
W1 O5 W9 155.1(6) . . ? 
W1 O6 W2 119.4(6) . . ? 
W2 O8 W8 120.9(6) . . ? 
W2 O9 Fe1 142.4(7) . 2_667 ? 
W3 O10 W2 145.6(6) . . ? 
W5 O12 W3 119.5(6) . . ? 
As1 O13 W4 114.7(5) . . ? 
As1 O13 W3 127.6(5) . . ? 
W4 O13 W3 94.1(4) . . ? 
As1 O13 W5 128.2(5) . . ? 
W4 O13 W5 93.6(4) . . ? 
W3 O13 W5 89.4(4) . . ? 
W3 O14 W4 121.5(6) . . ? 
W4 O15 Fe1 179.0(8) . 2_667 ? 
W4 O16 Fe1 169.6(7) . . ? 
W4 O17 Fe2 163.6(7) . 2_667 ? 
W5 O18 W4 121.0(5) . . ? 
W9 O20 W5 145.2(7) . . ? 
W5 O21 W6 147.5(6) . . ? 
As1 O22 W7 117.2(6) . . ? 
As1 O22 W6 118.3(6) . . ? 
W7 O22 W6 91.9(4) . . ? 
As1 O22 W9 135.6(6) . . ? 
W7 O22 W9 93.1(4) . . ? 
W6 O22 W9 90.2(4) . . ? 
W6 O23 Fe1 145.6(6) . . ? 
W9 O25 W6 118.0(6) . . ? 
W6 O26 W7 120.8(6) . . ? 
W9 O28 W7 119.2(6) . . ? 
W7 O29 Fe2 137.9(6) . . ? 
W7 O30 W8 145.9(6) . . ? 
W8 O32 Fe2 138.7(7) . . ? 
C1 O34 C1' 56(3) . . ? 
C1 O34 Fe2 134.3(19) . . ? 
C1' O34 Fe2 145(2) . . ? 
O32 Fe2 O29 87.6(5) . . ? 
O32 Fe2 O17 99.1(5) . 2_667 ? 
O29 Fe2 O17 98.2(5) . 2_667 ? 
O32 Fe2 O34 91.0(5) . . ? 
O29 Fe2 O34 90.6(5) . . ? 
O17 Fe2 O34 166.9(5) 2_667 . ? 
O32 Fe2 O4W 93.3(7) . . ? 
O29 Fe2 O4W 173.9(6) . . ? 
O17 Fe2 O4W 87.7(6) 2_667 . ? 
O34 Fe2 O4W 83.3(6) . . ? 
O32 Fe2 O3W 175.2(6) . . ? 
O29 Fe2 O3W 89.3(6) . . ? 
O17 Fe2 O3W 85.0(6) 2_667 . ? 
O34 Fe2 O3W 85.4(6) . . ? 
O4W Fe2 O3W 89.3(8) . . ? 
C1 O35 O16W 133(5) . 2_656 ? 
O34 C1 O35 125(4) . . ? 
O34 C1 C2 119(3) . . ? 
O35 C1 C2 117(4) . . ? 
C3 C2 C1 123(3) . . ? 
C3 C2 N1 109(3) . . ? 
C1 C2 N1 108(3) . . ? 
O36' C3 O36 138(4) . . ? 
O36' C3 C2' 112(3) . . ? 
O36 C3 C2' 60(3) . . ? 
O36' C3 C2 70(3) . . ? 
O36 C3 C2 93(3) . . ? 
C2' C3 C2 42(2) . . ? 
O36' C3 C4 103(3) . . ? 
O36 C3 C4 118(3) . . ? 
C2' C3 C4 112(3) . . ? 
C2 C3 C4 120(3) . . ? 
O34 C1' O35' 111(4) . . ? 
O34 C1' C2' 119(3) . . ? 
O35' C1' C2' 124(4) . . ? 
C3 C2' C1' 110(3) . . ? 
C3 C2' N1' 113(3) . . ? 
C1' C2' N1' 108(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.967 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.967 
_refine_diff_density_max    3.563 
_refine_diff_density_min   -5.720 
_refine_diff_density_rms    0.513 
  


#===END


  
data_12-Dy 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Dy2 Fe4 N2 O116 W18' 
_chemical_formula_weight          6094.49 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Dy'  'Dy'  -0.1892   4.4098 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.6307(11) 
_cell_length_b                    13.5293(11) 
_cell_length_c                    16.1950(14) 
_cell_angle_alpha                 106.8530(10) 
_cell_angle_beta                  99.7760(10) 
_cell_angle_gamma                 97.1530(10) 
_cell_volume                      2565.5(4) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8740  
_cell_measurement_theta_min       1.60 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky  
_exptl_crystal_colour             'Light yellow'  
_exptl_crystal_size_max           0.46 
_exptl_crystal_size_mid           0.23 
_exptl_crystal_size_min           0.06 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.945 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2730 
_exptl_absorpt_coefficient_mu     22.840 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0338 
_exptl_absorpt_correction_T_max   0.3411 
_exptl_absorpt_process_details    SADABS
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none 
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12802 
_diffrn_reflns_av_R_equivalents   0.0328 
_diffrn_reflns_av_sigmaI/netI     0.0623 
_diffrn_reflns_limit_h_min        -14 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -16 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -19 
_diffrn_reflns_limit_l_max        14 
_diffrn_reflns_theta_min          1.60 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8740 
_reflns_number_gt                 7837 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral.
 However, its structure is pseudo-centrosymmetric, i.e. most of the
 structure fits space group P¨C1, therefore, its structure was solved
 and refined in centrosymmetric space group P¨C1. Such phenomena are
 rather common. An attempt to refine the structure in P¨C1 shows the
 disorder around the chiral centre of L-thr (because we impose inversion
 on a chiral entity), as a result, C1, C2, N1, O35 and O36 atoms on L-thr
 are disordered over two positions. In addition, some coordination water
 molecules on Dy3+ cations are disordered over two positions. The ISOR
 instruction is used for C4, O23, O24, O18 and O14. The DELU instruction
 is used for C3 and C4. The SADI instruction is used for C2' C1' C2 C1,
 O34 C1' O34 C1, O35' C1' O35 C1, N1' C2' N1 C2, C3 C2' C3 C2, O36 C3 O36'
 C3, N1' C2' N1 C2. The EADP instruction is used for C2 and C2', N1 and N1',
 O36 and O36'. The O7M, O8W, O10W, O10M, O11W, O11M, O12W, O12M, O13W, O14W,
 O15W, O16W, O16M, O18W, O18M, O22W, O35, O35', O36, O36', C1, C1', C2, C2',
 N1 and N1' are refined isostropicallly. 654 parameters and 37 restraints
 are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0639P)²+63.4873P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00023(4) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8740 
_refine_ls_number_parameters      654 
_refine_ls_number_restraints      37 
_refine_ls_R_factor_all           0.0543 
_refine_ls_R_factor_gt            0.0489 
_refine_ls_wR_factor_ref          0.1265 
_refine_ls_wR_factor_gt           0.1233 
_refine_ls_goodness_of_fit_ref    1.042 
_refine_ls_restrained_S_all       1.040 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.21089(5) 0.31191(4) 0.59396(4) 0.01475(15) Uani 1 1 d . . . 
W2 W 0.46649(4) 0.44245(4) 0.67933(4) 0.01367(15) Uani 1 1 d . . . 
W3 W 0.24561(5) 0.57536(4) 0.75400(4) 0.01349(15) Uani 1 1 d . . . 
W4 W 0.35717(4) 0.61342(4) 0.97108(4) 0.00994(15) Uani 1 1 d . . . 
W5 W 0.09441(4) 0.48649(4) 0.87831(4) 0.01245(15) Uani 1 1 d . . . 
W6 W 0.15058(5) 0.25681(4) 0.94473(4) 0.01438(15) Uani 1 1 d . . . 
W7 W 0.24593(5) 0.08956(4) 0.79027(4) 0.01461(16) Uani 1 1 d . . . 
W8 W 0.41218(5) 0.18425(4) 0.65272(4) 0.01580(16) Uani 1 1 d . . . 
W9 W 0.04202(4) 0.21332(4) 0.73107(4) 0.01364(15) Uani 1 1 d . . . 
Dy1 Dy 0.11779(8) 0.24097(8) 0.33104(7) 0.0415(2) Uani 1 1 d . . . 
As1 As 0.33889(11) 0.35944(10) 0.83518(9) 0.0084(3) Uani 1 1 d . . . 
Fe1 Fe 0.38174(15) 0.42986(15) 1.10037(14) 0.0120(4) Uani 1 1 d . . . 
O1W O 0.2410(8) 0.4510(9) 1.1551(8) 0.027(3) Uani 1 1 d . . . 
O2W O 0.4082(10) 0.3159(9) 1.1644(8) 0.030(3) Uani 1 1 d . . . 
O3W O 0.5532(12) 0.0495(9) 0.9311(9) 0.040(3) Uani 1 1 d . . . 
O4W O 0.6867(9) 0.1198(10) 0.8229(10) 0.039(3) Uani 1 1 d . . . 
O5W O 0.247(2) 0.1466(16) 0.3791(17) 0.105(9) Uani 1 1 d . . . 
O6W O 0.2746(15) 0.3764(14) 0.4049(12) 0.069(5) Uani 1 1 d . . . 
O7W O -0.048(3) 0.177(2) 0.219(2) 0.069(8) Uiso 0.60 1 d P . . 
O7M O -0.050(3) 0.215(3) 0.344(3) 0.062(11) Uiso 0.40 1 d P . . 
O8W O 0.067(3) 0.068(3) 0.227(3) 0.167(13) Uiso 1 1 d . . . 
O9W O 0.2376(19) 0.224(2) 0.2296(15) 0.110(9) Uani 1 1 d . . . 
O10W O 0.090(4) 0.343(4) 0.236(3) 0.121(14) Uiso 0.65 1 d P . . 
O10M O 0.035(4) 0.296(4) 0.201(4) 0.062(13) Uiso 0.35 1 d P . . 
O11W O 0.019(3) 0.102(3) 0.372(3) 0.095(11) Uiso 0.60 1 d P . . 
O11M O -0.072(9) 0.012(8) 0.388(7) 0.18(4) Uiso 0.40 1 d P . . 
O12W O 0.060(3) 0.407(3) 0.376(2) 0.073(9) Uiso 0.60 1 d P . . 
O12M O -0.011(4) 0.340(4) 0.381(4) 0.078(14) Uiso 0.40 1 d P . . 
O13W O -0.117(2) 0.196(2) 0.064(2) 0.127(9) Uiso 1 1 d . . . 
O14W O 0.766(4) -0.011(4) 0.911(3) 0.098(14) Uiso 0.50 1 d P . . 
O15W O 0.146(15) 0.556(14) 0.503(14) 0.39(10) Uiso 0.50 1 d P . . 
O16W O 0.310(3) -0.051(3) 0.360(2) 0.083(10) Uiso 0.60 1 d P . . 
O16M O 0.319(4) -0.135(4) 0.416(4) 0.084(15) Uiso 0.40 1 d P . . 
O17W O 0.3793(17) 0.1337(12) 1.0406(11) 0.070(5) Uani 1 1 d . . . 
O18W O 0.368(2) -0.1209(19) 0.8939(17) 0.059(6) Uiso 0.70 1 d P . . 
O18M O 0.303(4) -0.128(4) 0.913(3) 0.045(11) Uiso 0.30 1 d P . . 
O19W O -0.1650(11) 0.2894(11) 0.8701(10) 0.043(3) Uani 1 1 d . . . 
O20W O 0.7401(14) 0.3507(14) 0.7263(14) 0.079(6) Uani 1 1 d . . . 
O21W O -0.0985(17) 0.3971(15) 0.6319(13) 0.080(6) Uani 1 1 d . . . 
O22W O 0.1162(18) 0.0012(17) 0.5080(16) 0.088(6) Uiso 1 1 d . . . 
O23W O 0.1342(16) -0.2037(16) 0.5114(12) 0.073(5) Uani 1 1 d . . . 
O1 O 0.1320(9) 0.2919(8) 0.4892(7) 0.024(3) Uani 1 1 d . . . 
O2 O 0.2856(8) 0.1971(8) 0.5670(7) 0.018(2) Uani 1 1 d . . . 
O3 O 0.1812(8) 0.4401(7) 0.6638(7) 0.017(2) Uani 1 1 d . . . 
O4 O 0.3380(8) 0.3315(7) 0.7191(6) 0.013(2) Uani 1 1 d . . . 
O5 O 0.1128(8) 0.2388(7) 0.6415(7) 0.016(2) Uani 1 1 d . . . 
O6 O 0.3379(8) 0.3952(8) 0.5817(7) 0.020(2) Uani 1 1 d . . . 
O7 O 0.5545(9) 0.5126(9) 0.6371(8) 0.027(3) Uani 1 1 d . . . 
O8 O 0.4942(8) 0.3017(7) 0.6334(7) 0.017(2) Uani 1 1 d . . . 
O9 O 0.5435(8) 0.4619(7) 0.7892(7) 0.018(2) Uani 1 1 d . . . 
O10 O 0.3828(8) 0.5489(7) 0.7281(7) 0.017(2) Uani 1 1 d . . . 
O11 O 0.2211(9) 0.6656(9) 0.6998(8) 0.025(2) Uani 1 1 d . . . 
O12 O 0.1105(8) 0.5591(7) 0.7924(7) 0.015(2) Uani 1 1 d . . . 
O13 O 0.2720(7) 0.4715(7) 0.8499(7) 0.016(2) Uani 1 1 d . . . 
O14 O 0.3143(8) 0.6671(7) 0.8672(7) 0.013(2) Uani 1 1 d U . . 
O15 O 0.4818(8) 0.5916(8) 0.9386(7) 0.019(2) Uani 1 1 d . . . 
O16 O 0.3557(8) 0.5273(7) 1.0359(7) 0.016(2) Uani 1 1 d . . . 
O17 O 0.3938(8) 0.7404(7) 1.0510(7) 0.016(2) Uani 1 1 d . . . 
O18 O 0.1925(7) 0.6004(7) 0.9641(6) 0.012(2) Uani 1 1 d U . . 
O19 O -0.0288(8) 0.5183(8) 0.8986(8) 0.025(3) Uani 1 1 d . . . 
O20 O 0.0458(8) 0.3606(8) 0.7759(7) 0.017(2) Uani 1 1 d . . . 
O21 O 0.1217(8) 0.3942(7) 0.9439(7) 0.015(2) Uani 1 1 d . . . 
O22 O 0.2213(8) 0.2613(7) 0.8211(7) 0.013(2) Uani 1 1 d . . . 
O23 O 0.2897(8) 0.3131(7) 1.0055(6) 0.014(2) Uani 1 1 d U . . 
O24 O 0.0853(9) 0.2364(8) 1.0250(7) 0.022(2) Uani 1 1 d U . . 
O25 O 0.0206(9) 0.2104(8) 0.8431(9) 0.027(3) Uani 1 1 d . . . 
O26 O 0.1803(8) 0.1184(8) 0.8929(7) 0.019(2) Uani 1 1 d . . . 
O27 O 0.2312(9) -0.0459(7) 0.7666(8) 0.023(2) Uani 1 1 d . . . 
O28 O 0.0986(8) 0.0870(8) 0.7193(7) 0.018(2) Uani 1 1 d . . . 
O29 O 0.3813(9) 0.1382(8) 0.8600(7) 0.019(2) Uani 1 1 d . . . 
O30 O 0.3010(8) 0.1084(8) 0.6931(7) 0.018(2) Uani 1 1 d . . . 
O31 O 0.4521(10) 0.0798(10) 0.5816(8) 0.033(3) Uani 1 1 d . . . 
O32 O 0.5065(8) 0.2058(8) 0.7595(8) 0.023(2) Uani 1 1 d . . . 
O33 O -0.0897(8) 0.1673(8) 0.6710(8) 0.023(2) Uani 1 1 d . . . 
O34 O 0.4817(10) -0.0062(8) 0.7482(8) 0.028(3) Uani 1 1 d D . . 
Fe2 Fe 0.53287(16) 0.13553(15) 0.84566(14) 0.0151(4) Uani 1 1 d . . . 
O35 O 0.619(2) -0.043(2) 0.680(2) 0.055(6) Uiso 0.50 1 d PD . 1 
O36 O 0.510(4) -0.270(4) 0.662(3) 0.090(9) Uiso 0.50 1 d PD A 1 
H36 H 0.5334 -0.3258 0.6491 0.135 Uiso 0.50 1 d PR A 1 
N1 N 0.332(2) -0.144(3) 0.627(3) 0.043(6) Uiso 0.50 1 d PD A 1 
H1A H 0.2954 -0.1958 0.5792 0.051 Uiso 0.50 1 d PR A 1 
H1B H 0.3237 -0.1594 0.6746 0.051 Uiso 0.50 1 d PR A 1 
H1C H 0.3063 -0.0851 0.6276 0.051 Uiso 0.50 1 d PR A 1 
C1 C 0.521(2) -0.057(3) 0.687(2) 0.032(6) Uiso 0.50 1 d PD A 1 
C2 C 0.449(3) -0.144(2) 0.609(3) 0.046(7) Uiso 0.50 1 d PD A 1 
H2 H 0.4526 -0.1273 0.5545 0.055 Uiso 0.50 1 calc PR A 1 
C3 C 0.461(3) -0.2574(19) 0.5953(19) 0.072(8) Uani 1 1 d DU . . 
C4 C 0.384(2) -0.347(2) 0.533(2) 0.073(7) Uani 1 1 d U A . 
H4A H 0.3557 -0.3305 0.4815 0.110 Uiso 1 1 d R . . 
H4B H 0.4202 -0.4059 0.5177 0.110 Uiso 1 1 d R . . 
H4C H 0.3259 -0.3627 0.5603 0.110 Uiso 1 1 d R . . 
O35' O 0.581(2) -0.121(2) 0.763(2) 0.055(6) Uiso 0.50 1 d PD A 2 
O36' O 0.523(4) -0.219(4) 0.557(3) 0.090(9) Uiso 0.50 1 d PD A 2 
H36' H 0.5079 -0.1630 0.5524 0.135 Uiso 0.50 1 d PR A 2 
N1' N 0.343(3) -0.116(3) 0.600(2) 0.043(6) Uiso 0.50 1 d PD A 2 
H1'A H 0.2927 -0.1590 0.5543 0.064 Uiso 0.50 1 d PR A 2 
H1'B H 0.3115 -0.0685 0.6331 0.064 Uiso 0.50 1 d PR A 2 
H1'C H 0.3930 -0.0829 0.5798 0.064 Uiso 0.50 1 d PR A 2 
C1' C 0.490(3) -0.099(2) 0.734(2) 0.032(6) Uiso 0.50 1 d PD A 2 
C2' C 0.411(3) -0.174(3) 0.652(2) 0.046(7) Uiso 0.50 1 d PD A 2 
H2' H 0.3581 -0.2129 0.6747 0.055 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.743(11) . ? 
W1 O5 1.889(10) . ? 
W1 O3 1.897(10) . ? 
W1 O2 1.900(10) . ? 
W1 O6 1.916(10) . ? 
W1 O4 2.288(10) . ? 
W2 O7 1.725(11) . ? 
W2 O9 1.805(10) . ? 
W2 O8 1.932(9) . ? 
W2 O10 1.954(10) . ? 
W2 O6 1.957(11) . ? 
W2 O4 2.369(10) . ? 
W3 O11 1.726(11) . ? 
W3 O14 1.878(10) . ? 
W3 O10 1.903(10) . ? 
W3 O12 1.921(10) . ? 
W3 O3 1.954(10) . ? 
W3 O13 2.389(10) . ? 
W4 O17 1.775(9) . ? 
W4 O15 1.775(10) . ? 
W4 O16 1.780(10) . ? 
W4 O14 2.037(10) . ? 
W4 O18 2.046(9) . ? 
W4 O13 2.298(10) . ? 
W5 O19 1.724(10) . ? 
W5 O18 1.881(9) . ? 
W5 O21 1.886(10) . ? 
W5 O20 1.945(10) . ? 
W5 O12 1.946(10) . ? 
W5 O13 2.386(9) . ? 
W6 O24 1.721(11) . ? 
W6 O23 1.811(10) . ? 
W6 O26 1.929(10) . ? 
W6 O21 1.942(10) . ? 
W6 O25 2.006(12) . ? 
W6 O22 2.339(10) . ? 
W7 O27 1.739(10) . ? 
W7 O29 1.807(10) . ? 
W7 O30 1.894(11) . ? 
W7 O26 1.943(11) . ? 
W7 O28 2.005(10) . ? 
W7 O22 2.303(9) . ? 
W8 O31 1.734(12) . ? 
W8 O32 1.848(11) . ? 
W8 O8 1.920(10) . ? 
W8 O30 1.948(10) . ? 
W8 O2 1.992(11) . ? 
W8 O4 2.360(9) . ? 
W9 O33 1.716(10) . ? 
W9 O25 1.890(13) . ? 
W9 O20 1.905(10) . ? 
W9 O28 1.905(10) . ? 
W9 O5 1.917(11) . ? 
W9 O22 2.374(10) . ? 
Dy1 O7M 2.16(4) . ? 
Dy1 O12M 2.34(5) . ? 
Dy1 O5W 2.35(2) . ? 
Dy1 O10W 2.36(5) . ? 
Dy1 O8W 2.38(4) . ? 
Dy1 O6W 2.394(15) . ? 
Dy1 O12W 2.40(3) . ? 
Dy1 O9W 2.40(2) . ? 
Dy1 O7W 2.40(3) . ? 
Dy1 O1 2.421(12) . ? 
Dy1 O11W 2.44(4) . ? 
Dy1 O10M 2.53(5) . ? 
As1 O22 1.800(9) . ? 
As1 O13 1.802(9) . ? 
As1 O4 1.804(10) . ? 
Fe1 O16 1.931(10) . ? 
Fe1 O23 1.933(10) . ? 
Fe1 O9 1.949(10) 2_667 ? 
Fe1 O15 1.959(10) 2_667 ? 
Fe1 O2W 2.121(12) . ? 
Fe1 O1W 2.132(11) . ? 
O3W Fe2 2.055(13) . ? 
O4W Fe2 2.064(12) . ? 
O7M O12M 1.61(7) . ? 
O10W O10M 0.86(6) . ? 
O11W O11M 1.67(11) . ? 
O11M O28 1.81(11) 2_556 ? 
O12W O12M 1.21(6) . ? 
O16W O16M 1.65(7) . ? 
O16W O35 1.79(5) 2_656 ? 
O18W O18M 0.93(5) . ? 
O9 Fe1 1.949(10) 2_667 ? 
O15 Fe1 1.959(10) 2_667 ? 
O17 Fe2 1.984(10) 2_667 ? 
O28 O11M 1.81(11) 2_556 ? 
O29 Fe2 1.971(11) . ? 
O32 Fe2 1.911(11) . ? 
O34 C1' 1.23(3) . ? 
O34 C1 1.24(3) . ? 
O34 Fe2 2.043(11) . ? 
Fe2 O17 1.984(10) 2_667 ? 
O35 C1 1.27(3) . ? 
O35 O16W 1.79(5) 2_656 ? 
O36 C3 1.22(4) . ? 
N1 C2 1.56(4) . ? 
C1 C2 1.52(4) . ? 
C2 C3 1.51(4) . ? 
C3 O36' 1.23(4) . ? 
C3 C4 1.44(4) . ? 
C3 C2' 1.51(4) . ? 
O35' C1' 1.27(3) . ? 
N1' C2' 1.55(4) . ? 
C1' C2' 1.52(4) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O5 100.9(5) . . ? 
O1 W1 O3 103.8(4) . . ? 
O5 W1 O3 88.9(4) . . ? 
O1 W1 O2 99.4(4) . . ? 
O5 W1 O2 91.4(4) . . ? 
O3 W1 O2 156.3(4) . . ? 
O1 W1 O6 97.0(5) . . ? 
O5 W1 O6 162.1(5) . . ? 
O3 W1 O6 86.2(4) . . ? 
O2 W1 O6 86.3(4) . . ? 
O1 W1 O4 170.2(4) . . ? 
O5 W1 O4 86.2(4) . . ? 
O3 W1 O4 83.0(4) . . ? 
O2 W1 O4 73.4(4) . . ? 
O6 W1 O4 76.2(4) . . ? 
O7 W2 O9 102.9(5) . . ? 
O7 W2 O8 101.7(5) . . ? 
O9 W2 O8 93.4(4) . . ? 
O7 W2 O10 100.7(5) . . ? 
O9 W2 O10 89.9(4) . . ? 
O8 W2 O10 155.9(4) . . ? 
O7 W2 O6 100.8(5) . . ? 
O9 W2 O6 156.1(5) . . ? 
O8 W2 O6 84.8(4) . . ? 
O10 W2 O6 82.6(4) . . ? 
O7 W2 O4 172.9(5) . . ? 
O9 W2 O4 83.1(4) . . ? 
O8 W2 O4 73.8(4) . . ? 
O10 W2 O4 83.0(4) . . ? 
O6 W2 O4 73.5(4) . . ? 
O11 W3 O14 99.8(5) . . ? 
O11 W3 O10 100.4(5) . . ? 
O14 W3 O10 91.2(4) . . ? 
O11 W3 O12 99.2(5) . . ? 
O14 W3 O12 89.9(4) . . ? 
O10 W3 O12 159.9(4) . . ? 
O11 W3 O3 103.6(5) . . ? 
O14 W3 O3 156.5(4) . . ? 
O10 W3 O3 86.7(4) . . ? 
O12 W3 O3 84.3(4) . . ? 
O11 W3 O13 170.2(5) . . ? 
O14 W3 O13 72.5(4) . . ? 
O10 W3 O13 86.1(4) . . ? 
O12 W3 O13 75.1(4) . . ? 
O3 W3 O13 84.0(4) . . ? 
O17 W4 O15 103.0(5) . . ? 
O17 W4 O16 103.6(5) . . ? 
O15 W4 O16 96.9(5) . . ? 
O17 W4 O14 94.6(4) . . ? 
O15 W4 O14 89.6(4) . . ? 
O16 W4 O14 158.6(4) . . ? 
O17 W4 O18 95.8(4) . . ? 
O15 W4 O18 159.3(4) . . ? 
O16 W4 O18 86.7(4) . . ? 
O14 W4 O18 80.3(4) . . ? 
O17 W4 O13 163.4(4) . . ? 
O15 W4 O13 87.1(4) . . ? 
O16 W4 O13 88.0(4) . . ? 
O14 W4 O13 72.0(4) . . ? 
O18 W4 O13 72.7(3) . . ? 
O19 W5 O18 100.6(5) . . ? 
O19 W5 O21 103.1(5) . . ? 
O18 W5 O21 92.8(4) . . ? 
O19 W5 O20 101.2(5) . . ? 
O18 W5 O20 157.8(4) . . ? 
O21 W5 O20 85.9(4) . . ? 
O19 W5 O12 98.1(5) . . ? 
O18 W5 O12 88.2(4) . . ? 
O21 W5 O12 158.3(4) . . ? 
O20 W5 O12 85.0(4) . . ? 
O19 W5 O13 170.6(4) . . ? 
O18 W5 O13 73.4(4) . . ? 
O21 W5 O13 84.7(4) . . ? 
O20 W5 O13 84.4(4) . . ? 
O12 W5 O13 74.7(4) . . ? 
O24 W6 O23 102.9(5) . . ? 
O24 W6 O26 100.9(5) . . ? 
O23 W6 O26 95.1(4) . . ? 
O24 W6 O21 101.6(5) . . ? 
O23 W6 O21 91.2(4) . . ? 
O26 W6 O21 154.6(4) . . ? 
O24 W6 O25 98.3(5) . . ? 
O23 W6 O25 158.5(5) . . ? 
O26 W6 O25 83.8(4) . . ? 
O21 W6 O25 81.4(4) . . ? 
O24 W6 O22 171.3(4) . . ? 
O23 W6 O22 84.3(4) . . ? 
O26 W6 O22 73.4(4) . . ? 
O21 W6 O22 82.8(4) . . ? 
O25 W6 O22 74.8(4) . . ? 
O27 W7 O29 103.5(5) . . ? 
O27 W7 O30 101.2(5) . . ? 
O29 W7 O30 89.8(5) . . ? 
O27 W7 O26 97.8(5) . . ? 
O29 W7 O26 91.1(5) . . ? 
O30 W7 O26 160.2(4) . . ? 
O27 W7 O28 95.7(5) . . ? 
O29 W7 O28 160.8(4) . . ? 
O30 W7 O28 85.8(4) . . ? 
O26 W7 O28 86.8(4) . . ? 
O27 W7 O22 166.2(4) . . ? 
O29 W7 O22 87.9(4) . . ? 
O30 W7 O22 86.3(4) . . ? 
O26 W7 O22 74.0(4) . . ? 
O28 W7 O22 73.1(4) . . ? 
O31 W8 O32 103.0(5) . . ? 
O31 W8 O8 101.2(5) . . ? 
O32 W8 O8 92.1(5) . . ? 
O31 W8 O30 100.2(5) . . ? 
O32 W8 O30 88.4(5) . . ? 
O8 W8 O30 157.9(4) . . ? 
O31 W8 O2 97.5(5) . . ? 
O32 W8 O2 159.2(4) . . ? 
O8 W8 O2 87.6(4) . . ? 
O30 W8 O2 84.3(4) . . ? 
O31 W8 O4 166.9(5) . . ? 
O32 W8 O4 89.6(4) . . ? 
O8 W8 O4 74.2(4) . . ? 
O30 W8 O4 83.7(4) . . ? 
O2 W8 O4 70.3(4) . . ? 
O33 W9 O25 99.5(5) . . ? 
O33 W9 O20 102.4(5) . . ? 
O25 W9 O20 85.7(5) . . ? 
O33 W9 O28 102.2(5) . . ? 
O25 W9 O28 87.7(5) . . ? 
O20 W9 O28 155.2(4) . . ? 
O33 W9 O5 100.1(5) . . ? 
O25 W9 O5 160.3(4) . . ? 
O20 W9 O5 88.1(4) . . ? 
O28 W9 O5 90.1(4) . . ? 
O33 W9 O22 173.5(4) . . ? 
O25 W9 O22 76.0(4) . . ? 
O20 W9 O22 82.1(4) . . ? 
O28 W9 O22 73.2(4) . . ? 
O5 W9 O22 84.6(4) . . ? 
O7M Dy1 O12M 41.6(17) . . ? 
O7M Dy1 O5W 122.6(14) . . ? 
O12M Dy1 O5W 140.9(15) . . ? 
O7M Dy1 O10W 95.4(17) . . ? 
O12M Dy1 O10W 75.1(18) . . ? 
O5W Dy1 O10W 140.3(14) . . ? 
O7M Dy1 O8W 83.5(15) . . ? 
O12M Dy1 O8W 122.5(16) . . ? 
O5W Dy1 O8W 75.0(11) . . ? 
O10W Dy1 O8W 100.7(16) . . ? 
O7M Dy1 O6W 134.9(13) . . ? 
O12M Dy1 O6W 96.0(14) . . ? 
O5W Dy1 O6W 77.8(7) . . ? 
O10W Dy1 O6W 83.3(13) . . ? 
O8W Dy1 O6W 141.2(11) . . ? 
O7M Dy1 O12W 70.6(14) . . ? 
O12M Dy1 O12W 29.6(14) . . ? 
O5W Dy1 O12W 141.2(10) . . ? 
O10W Dy1 O12W 57.9(14) . . ? 
O8W Dy1 O12W 143.2(12) . . ? 
O6W Dy1 O12W 70.9(9) . . ? 
O7M Dy1 O9W 145.2(13) . . ? 
O12M Dy1 O9W 141.1(16) . . ? 
O5W Dy1 O9W 75.0(11) . . ? 
O10W Dy1 O9W 66.4(14) . . ? 
O8W Dy1 O9W 72.0(12) . . ? 
O6W Dy1 O9W 74.6(8) . . ? 
O12W Dy1 O9W 116.3(11) . . ? 
O7M Dy1 O7W 49.8(14) . . ? 
O12M Dy1 O7W 72.9(15) . . ? 
O5W Dy1 O7W 129.2(9) . . ? 
O10W Dy1 O7W 65.6(15) . . ? 
O8W Dy1 O7W 54.9(12) . . ? 
O6W Dy1 O7W 148.6(9) . . ? 
O12W Dy1 O7W 88.2(11) . . ? 
O9W Dy1 O7W 95.5(10) . . ? 
O7M Dy1 O1 76.5(12) . . ? 
O12M Dy1 O1 65.6(13) . . ? 
O5W Dy1 O1 76.2(7) . . ? 
O10W Dy1 O1 128.8(12) . . ? 
O8W Dy1 O1 127.6(10) . . ? 
O6W Dy1 O1 70.1(5) . . ? 
O12W Dy1 O1 72.0(9) . . ? 
O9W Dy1 O1 138.2(6) . . ? 
O7W Dy1 O1 126.3(8) . . ? 
O7M Dy1 O11W 50.6(15) . . ? 
O12M Dy1 O11W 86.0(16) . . ? 
O5W Dy1 O11W 72.6(12) . . ? 
O10W Dy1 O11W 140.5(16) . . ? 
O8W Dy1 O11W 61.1(14) . . ? 
O6W Dy1 O11W 133.8(10) . . ? 
O12W Dy1 O11W 114.5(12) . . ? 
O9W Dy1 O11W 128.0(12) . . ? 
O7W Dy1 O11W 75.8(12) . . ? 
O1 Dy1 O11W 68.9(10) . . ? 
O7M Dy1 O10M 82.6(17) . . ? 
O12M Dy1 O10M 74.9(18) . . ? 
O5W Dy1 O10M 144.1(14) . . ? 
O10W Dy1 O10M 19.9(13) . . ? 
O8W Dy1 O10M 84.1(16) . . ? 
O6W Dy1 O10M 103.1(14) . . ? 
O12W Dy1 O10M 67.3(14) . . ? 
O9W Dy1 O10M 70.9(14) . . ? 
O7W Dy1 O10M 46.0(15) . . ? 
O1 Dy1 O10M 138.5(12) . . ? 
O11W Dy1 O10M 121.7(16) . . ? 
O22 As1 O13 98.0(4) . . ? 
O22 As1 O4 96.1(4) . . ? 
O13 As1 O4 98.3(5) . . ? 
O16 Fe1 O23 92.3(4) . . ? 
O16 Fe1 O9 94.8(4) . 2_667 ? 
O23 Fe1 O9 168.4(5) . 2_667 ? 
O16 Fe1 O15 92.5(4) . 2_667 ? 
O23 Fe1 O15 95.6(4) . 2_667 ? 
O9 Fe1 O15 93.2(4) 2_667 2_667 ? 
O16 Fe1 O2W 176.8(5) . . ? 
O23 Fe1 O2W 84.7(4) . . ? 
O9 Fe1 O2W 88.3(4) 2_667 . ? 
O15 Fe1 O2W 86.5(5) 2_667 . ? 
O16 Fe1 O1W 92.5(5) . . ? 
O23 Fe1 O1W 87.4(4) . . ? 
O9 Fe1 O1W 83.2(5) 2_667 . ? 
O15 Fe1 O1W 174.1(5) 2_667 . ? 
O2W Fe1 O1W 88.7(5) . . ? 
O12M O7M Dy1 75(2) . . ? 
O10M O10W Dy1 91(5) . . ? 
O10W O10M Dy1 69(5) . . ? 
O11M O11W Dy1 168(4) . . ? 
O11W O11M O28 99(6) . 2_556 ? 
O12M O12W Dy1 72(3) . . ? 
O12W O12M O7M 139(5) . . ? 
O12W O12M Dy1 78(3) . . ? 
O7M O12M Dy1 63(2) . . ? 
O16M O16W O35 147(3) . 2_656 ? 
W1 O1 Dy1 148.4(6) . . ? 
W1 O2 W8 121.9(5) . . ? 
W1 O3 W3 144.9(6) . . ? 
As1 O4 W1 136.0(5) . . ? 
As1 O4 W8 116.5(4) . . ? 
W1 O4 W8 94.1(3) . . ? 
As1 O4 W2 117.4(4) . . ? 
W1 O4 W2 91.3(3) . . ? 
W8 O4 W2 90.6(3) . . ? 
W1 O5 W9 156.4(6) . . ? 
W1 O6 W2 118.7(5) . . ? 
W8 O8 W2 121.4(5) . . ? 
W2 O9 Fe1 142.9(6) . 2_667 ? 
W3 O10 W2 146.1(5) . . ? 
W3 O12 W5 120.6(5) . . ? 
As1 O13 W4 114.4(5) . . ? 
As1 O13 W5 128.9(5) . . ? 
W4 O13 W5 93.3(3) . . ? 
As1 O13 W3 127.6(5) . . ? 
W4 O13 W3 93.7(3) . . ? 
W5 O13 W3 89.4(3) . . ? 
W3 O14 W4 121.7(5) . . ? 
W4 O15 Fe1 178.0(7) . 2_667 ? 
W4 O16 Fe1 168.6(6) . . ? 
W4 O17 Fe2 164.1(6) . 2_667 ? 
W5 O18 W4 120.3(5) . . ? 
W9 O20 W5 145.6(6) . . ? 
W5 O21 W6 148.1(6) . . ? 
As1 O22 W7 117.2(4) . . ? 
As1 O22 W6 118.8(5) . . ? 
W7 O22 W6 92.5(3) . . ? 
As1 O22 W9 134.7(5) . . ? 
W7 O22 W9 93.0(3) . . ? 
W6 O22 W9 90.5(3) . . ? 
W6 O23 Fe1 144.7(6) . . ? 
W9 O25 W6 118.4(5) . . ? 
W6 O26 W7 120.0(5) . . ? 
O11M O28 W9 120(4) 2_556 . ? 
O11M O28 W7 111(3) 2_556 . ? 
W9 O28 W7 120.5(5) . . ? 
W7 O29 Fe2 136.8(6) . . ? 
W7 O30 W8 147.2(6) . . ? 
W8 O32 Fe2 138.4(6) . . ? 
C1' O34 C1 56(2) . . ? 
C1' O34 Fe2 140.2(18) . . ? 
C1 O34 Fe2 134.5(17) . . ? 
O32 Fe2 O29 88.7(5) . . ? 
O32 Fe2 O17 98.4(5) . 2_667 ? 
O29 Fe2 O17 98.1(4) . 2_667 ? 
O32 Fe2 O34 89.9(5) . . ? 
O29 Fe2 O34 89.9(4) . . ? 
O17 Fe2 O34 168.5(5) 2_667 . ? 
O32 Fe2 O3W 175.4(5) . . ? 
O29 Fe2 O3W 89.8(5) . . ? 
O17 Fe2 O3W 86.0(5) 2_667 . ? 
O34 Fe2 O3W 85.8(5) . . ? 
O32 Fe2 O4W 91.7(5) . . ? 
O29 Fe2 O4W 175.0(5) . . ? 
O17 Fe2 O4W 86.8(5) 2_667 . ? 
O34 Fe2 O4W 85.1(5) . . ? 
O3W Fe2 O4W 89.4(6) . . ? 
C1 O35 O16W 129(3) . 2_656 ? 
O34 C1 O35 127(3) . . ? 
O34 C1 C2 121(3) . . ? 
O35 C1 C2 112(3) . . ? 
C3 C2 C1 120(3) . . ? 
C3 C2 N1 103(3) . . ? 
C1 C2 N1 104(3) . . ? 
O36 C3 O36' 112(4) . . ? 
O36 C3 C4 117(3) . . ? 
O36' C3 C4 110(3) . . ? 
O36 C3 C2 113(3) . . ? 
O36' C3 C2 71(3) . . ? 
C4 C3 C2 124(3) . . ? 
O36 C3 C2' 90(3) . . ? 
O36' C3 C2' 111(3) . . ? 
C4 C3 C2' 116(3) . . ? 
C2 C3 C2' 41(2) . . ? 
O34 C1' O35' 119(3) . . ? 
O34 C1' C2' 115(3) . . ? 
O35' C1' C2' 121(3) . . ? 
C3 C2' C1' 115(3) . . ? 
C3 C2' N1' 114(3) . . ? 
C1' C2' N1' 112(3) . . ? 
  
_diffrn_measured_fraction_theta_max    0.968 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.968 
_refine_diff_density_max    2.647 
_refine_diff_density_min   -4.784 
_refine_diff_density_rms    0.424 
  



#===END

  
data_13-Er 
  
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'C8 H106 As2 Er2 Fe4 N2 O116 W18' 
_chemical_formula_weight          6104.01 
  
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'C'  'C'   0.0033   0.0016 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'As'  'As'   0.0499   2.0058 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Fe'  'Fe'   0.3463   0.8444 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'N'  'N'   0.0061   0.0033 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Er'  'Er'  -0.2586   4.9576 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
  
_symmetry_cell_setting            Triclinic 
_symmetry_space_group_name_H-M    P-1 
  
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
  
_cell_length_a                    12.5799(9) 
_cell_length_b                    13.4462(10) 
_cell_length_c                    16.0508(12) 
_cell_angle_alpha                 106.5070(10) 
_cell_angle_beta                  99.8130(10) 
_cell_angle_gamma                 97.3250(10) 
_cell_volume                      2520.2(3) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     296(2) 
_cell_measurement_reflns_used     8566 
_cell_measurement_theta_min       1.75 
_cell_measurement_theta_max       25.00 
  
_exptl_crystal_description        flaky  
_exptl_crystal_colour             'Light yellow' 
_exptl_crystal_size_max           0.46 
_exptl_crystal_size_mid           0.41 
_exptl_crystal_size_min           0.17 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     4.022 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2734 
_exptl_absorpt_coefficient_mu     23.434 
_exptl_absorpt_correction_type    multi-scan 
_exptl_absorpt_correction_T_min   0.0329 
_exptl_absorpt_correction_T_max   0.1089 
_exptl_absorpt_process_details    SADABS 
  
_exptl_special_details 
; 
 ? 
; 
  
_diffrn_ambient_temperature       296(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'Bruker P4' 
_diffrn_measurement_method        'ω scans' 
_diffrn_detector_area_resol_mean  none
_diffrn_standards_number          none 
_diffrn_standards_interval_count  none 
_diffrn_standards_interval_time   none 
_diffrn_standards_decay_%         none 
_diffrn_reflns_number             12430 
_diffrn_reflns_av_R_equivalents   0.0478 
_diffrn_reflns_av_sigmaI/netI     0.0842 
_diffrn_reflns_limit_h_min        -13 
_diffrn_reflns_limit_h_max        14 
_diffrn_reflns_limit_k_min        -15 
_diffrn_reflns_limit_k_max        15 
_diffrn_reflns_limit_l_min        -18 
_diffrn_reflns_limit_l_max        19 
_diffrn_reflns_theta_min          1.75 
_diffrn_reflns_theta_max          25.00 
_reflns_number_total              8566 
_reflns_number_gt                 7566 
_reflns_threshold_expression      >2sigma(I) 
  
_computing_data_collection        'Bruker XSCANS' 
_computing_cell_refinement        'Bruker XSCANS' 
_computing_data_reduction         'Bruker SHELXTL' 
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL' 
_computing_publication_material   'Bruker SHELXTL' 
  
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. Its structure contains 
 a chiral L-thr ligand, theoretically its structure should be chiral. 
 However, its structure is pseudo-centrosymmetric, i.e. most of the 
 structure fits space group P¨C1, therefore, its structure was solved 
 and refined in centrosymmetric space group P¨C1. Such phenomena are
 rather common. An attempt to refine the structure in P¨C1 shows
 the disorder around the chiral centre of L-thr (because we impose
 inversion on a chiral entity), as a result, C1, C2, N1, O35 and O36 
 atoms on L-thr are disordered over two positions. In addition, some
 coordination water molecules on Er3+ cations are disordered over two
 positions. The ISOR instruction is used for O15W, O8, O9, O13, O16, 
 O7, O1W, O27, O21, O22, O23, O32, O33, O34, C4, O18W, O13, O29, W1, 
 W4, As1, O2, O3, O4, O14, O18, O28, O6, W9, O12, O17, O20 and O26.
 The SADI instruction is used for C2' C1' C2 C1, O34 C1' O34 C1, O35'
 C1' O35 C1, N1' C2' N1 C2, C3 C2' C3 C2, O36 C3 O36' C3, N1' C2' N1
 C2. The EADP instruction is used for C2 and C2', N1 and N1', O36 
 and O36'. The O7W, O7M, O8W, O10W, O10M, O11W, O11M, O12W, O12M,
 O13W, O14W, O15W, O16W, O16M, O18W, O18M, O22W, O35, O35', O36, 
 O36', C1, C1', C2, C2', N1 and N1' are refined isostropicallly.
 654 parameters and 192 restraints are used in the refinement.
; 
  
_refine_ls_structure_factor_coef  Fsqd 
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc 
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.1270P)²+68.5397P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    geom 
_refine_ls_hydrogen_treatment     noref 
_refine_ls_extinction_method      SHELXL 
_refine_ls_extinction_coef        0.00041(7) 
_refine_ls_extinction_expression 
 'Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^' 
_refine_ls_number_reflns          8566 
_refine_ls_number_parameters      654 
_refine_ls_number_restraints      192 
_refine_ls_R_factor_all           0.0778 
_refine_ls_R_factor_gt            0.0709 
_refine_ls_wR_factor_ref          0.1932 
_refine_ls_wR_factor_gt           0.1867 
_refine_ls_goodness_of_fit_ref    1.038 
_refine_ls_restrained_S_all       1.048 
_refine_ls_shift/su_max           0.002 
_refine_ls_shift/su_mean          0.000 
  
loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.20849(7) 0.31123(6) 0.59306(5) 0.0127(2) Uani 1 1 d U . . 
W2 W 0.46463(6) 0.44241(6) 0.67773(5) 0.0112(2) Uani 1 1 d . . . 
W3 W 0.24410(7) 0.57493(6) 0.75307(5) 0.0114(2) Uani 1 1 d . . . 
W4 W 0.35702(6) 0.61313(6) 0.97077(5) 0.0078(2) Uani 1 1 d U . . 
W5 W 0.09403(6) 0.48520(6) 0.87901(5) 0.0104(2) Uani 1 1 d . . . 
W6 W 0.15092(6) 0.25534(6) 0.94635(5) 0.0120(2) Uani 1 1 d . . . 
W7 W 0.24537(6) 0.08819(6) 0.79099(5) 0.0124(2) Uani 1 1 d . . . 
W8 W 0.41047(7) 0.18386(6) 0.65155(5) 0.0132(2) Uani 1 1 d . . . 
W9 W 0.04098(6) 0.21164(6) 0.73210(5) 0.0118(2) Uani 1 1 d U . . 
Er1 Er 0.11856(11) 0.24593(11) 0.33260(8) 0.0389(3) Uani 1 1 d . . . 
As1 As 0.33818(15) 0.35862(14) 0.83505(12) 0.0065(4) Uani 1 1 d U . . 
Fe1 Fe 0.3822(2) 0.4295(2) 1.10176(18) 0.0099(6) Uani 1 1 d . . . 
O1W O 0.2406(13) 0.4537(13) 1.1579(11) 0.025(4) Uani 1 1 d U . . 
O2W O 0.4076(14) 0.3162(13) 1.1671(12) 0.031(4) Uani 1 1 d . . . 
O3W O 0.5535(16) 0.0502(14) 0.9332(14) 0.042(5) Uani 1 1 d . . . 
O4W O 0.6873(15) 0.1216(16) 0.8267(17) 0.052(6) Uani 1 1 d . . . 
O5W O 0.240(3) 0.147(2) 0.3816(18) 0.087(10) Uani 1 1 d . . . 
O6W O 0.277(2) 0.3787(19) 0.4046(15) 0.059(6) Uani 1 1 d . . . 
O7W O -0.045(6) 0.160(6) 0.215(5) 0.13(2) Uiso 0.60 1 d P . . 
O7M O -0.050(5) 0.206(5) 0.349(5) 0.067(17) Uiso 0.40 1 d P . . 
O8W O 0.073(4) 0.075(4) 0.229(3) 0.143(16) Uiso 1 1 d . . . 
O9W O 0.233(3) 0.219(4) 0.228(2) 0.109(13) Uani 1 1 d . . . 
O10W O 0.039(4) 0.300(4) 0.212(3) 0.080(12) Uiso 0.65 1 d P . . 
O10M O 0.005(13) 0.219(12) 0.167(11) 0.15(5) Uiso 0.35 1 d P . . 
O11W O 0.052(5) 0.088(4) 0.368(4) 0.095(16) Uiso 0.60 1 d P . . 
O11M O -0.067(10) 0.014(10) 0.394(8) 0.15(4) Uiso 0.40 1 d P . . 
O12W O 0.057(4) 0.413(4) 0.382(3) 0.060(10) Uiso 0.60 1 d P . . 
O12M O 0.009(8) 0.362(7) 0.381(6) 0.10(3) Uiso 0.40 1 d P . . 
O13W O -0.084(6) 0.197(5) 0.074(5) 0.20(2) Uiso 1 1 d . . . 
O14W O 0.770(6) -0.019(6) 0.903(5) 0.11(2) Uiso 0.50 1 d P . . 
O15W O 0.157(8) 0.531(7) 0.508(7) 0.14(3) Uiso 0.50 1 d P . . 
O16W O 0.305(4) -0.054(4) 0.356(3) 0.070(12) Uiso 0.60 1 d P . . 
O16M O 0.310(7) -0.140(6) 0.414(6) 0.09(2) Uiso 0.40 1 d P . . 
O17W O 0.385(2) 0.1351(18) 1.0415(15) 0.063(7) Uani 1 1 d . . . 
O18W O 0.370(4) -0.122(3) 0.895(3) 0.081(12) Uiso 0.70 1 d P . . 
O18M O 0.282(6) -0.133(5) 0.917(5) 0.042(15) Uiso 0.30 1 d P . . 
O19W O -0.1658(16) 0.2880(15) 0.8723(11) 0.040(5) Uani 1 1 d . . . 
O20W O 0.737(2) 0.351(2) 0.7310(16) 0.080(10) Uani 1 1 d . . . 
O21W O -0.100(2) 0.398(2) 0.6315(16) 0.069(7) Uani 1 1 d . . . 
O22W O 0.115(3) 0.003(2) 0.509(2) 0.079(8) Uiso 1 1 d . . . 
O23W O 0.128(2) -0.211(2) 0.5073(17) 0.065(7) Uani 1 1 d . . . 
O1 O 0.1298(12) 0.2901(12) 0.4871(11) 0.022(3) Uani 1 1 d . . . 
O2 O 0.2858(12) 0.1957(11) 0.5666(10) 0.016(3) Uani 1 1 d U . . 
O3 O 0.1802(11) 0.4409(11) 0.6648(10) 0.015(3) Uani 1 1 d U . . 
O4 O 0.3380(10) 0.3313(10) 0.7184(9) 0.008(3) Uani 1 1 d U . . 
O5 O 0.1103(11) 0.2374(11) 0.6408(9) 0.013(3) Uani 1 1 d . . . 
O6 O 0.3369(12) 0.3971(11) 0.5793(10) 0.018(3) Uani 1 1 d U . . 
O7 O 0.5546(13) 0.5160(12) 0.6378(11) 0.024(3) Uani 1 1 d U . . 
O8 O 0.4912(12) 0.3012(11) 0.6304(9) 0.016(3) Uani 1 1 d U . . 
O9 O 0.5415(11) 0.4631(10) 0.7882(10) 0.015(3) Uani 1 1 d U . . 
O10 O 0.3807(13) 0.5497(11) 0.7265(11) 0.020(3) Uani 1 1 d . . . 
O11 O 0.2178(13) 0.6644(14) 0.6970(12) 0.030(4) Uani 1 1 d . . . 
O12 O 0.1096(12) 0.5574(11) 0.7934(10) 0.017(3) Uani 1 1 d U . . 
O13 O 0.2727(11) 0.4734(11) 0.8524(9) 0.012(3) Uani 1 1 d U . . 
O14 O 0.3137(10) 0.6681(9) 0.8667(9) 0.007(2) Uani 1 1 d U . . 
O15 O 0.4823(13) 0.5942(12) 0.9364(10) 0.021(3) Uani 1 1 d . . . 
O16 O 0.3577(12) 0.5264(11) 1.0372(9) 0.015(3) Uani 1 1 d U . . 
O17 O 0.3942(12) 0.7410(11) 1.0522(10) 0.016(3) Uani 1 1 d U . . 
O18 O 0.1938(10) 0.6005(10) 0.9654(9) 0.008(3) Uani 1 1 d U . . 
O19 O -0.0291(12) 0.5157(13) 0.8994(11) 0.025(4) Uani 1 1 d . . . 
O20 O 0.0427(11) 0.3582(10) 0.7756(9) 0.012(3) Uani 1 1 d U . . 
O21 O 0.1212(12) 0.3942(10) 0.9461(9) 0.015(3) Uani 1 1 d U . . 
O22 O 0.2201(11) 0.2594(10) 0.8208(9) 0.011(3) Uani 1 1 d U . . 
O23 O 0.2905(11) 0.3105(11) 1.0042(9) 0.014(3) Uani 1 1 d U . . 
O24 O 0.0880(14) 0.2347(12) 1.0291(10) 0.025(4) Uani 1 1 d . . . 
O25 O 0.0200(12) 0.2116(13) 0.8468(10) 0.023(3) Uani 1 1 d . . . 
O26 O 0.1814(11) 0.1178(11) 0.8942(10) 0.016(3) Uani 1 1 d U . . 
O27 O 0.2320(12) -0.0476(11) 0.7685(10) 0.019(3) Uani 1 1 d U . . 
O28 O 0.1001(12) 0.0863(11) 0.7203(10) 0.017(3) Uani 1 1 d U . . 
O29 O 0.3811(12) 0.1373(11) 0.8599(10) 0.020(3) Uani 1 1 d U . . 
O30 O 0.2998(12) 0.1064(12) 0.6901(10) 0.021(3) Uani 1 1 d . . . 
O31 O 0.4477(14) 0.0795(13) 0.5799(12) 0.031(4) Uani 1 1 d . . . 
O32 O 0.5033(12) 0.2057(10) 0.7558(11) 0.019(3) Uani 1 1 d U . . 
O33 O -0.0918(13) 0.1663(13) 0.6739(12) 0.029(4) Uani 1 1 d U . . 
O34 O 0.4847(13) -0.0055(11) 0.7494(11) 0.025(3) Uani 1 1 d DU . . 
Fe2 Fe 0.5328(2) 0.1361(2) 0.84566(19) 0.0132(6) Uani 1 1 d . . . 
O35 O 0.619(4) -0.044(4) 0.683(4) 0.064(9) Uiso 0.50 1 d PD A 1 
O36 O 0.486(4) -0.277(4) 0.677(3) 0.071(10) Uiso 0.50 1 d PD B 1 
H36 H 0.5094 -0.3326 0.6644 0.106 Uiso 0.50 1 d PR B 1 
N1 N 0.334(4) -0.130(4) 0.624(4) 0.044(9) Uiso 0.50 1 d PD A 1 
H1A H 0.2980 -0.1825 0.5764 0.053 Uiso 0.50 1 d PR A 1 
H1B H 0.3263 -0.1460 0.6717 0.053 Uiso 0.50 1 d PR A 1 
H1C H 0.3088 -0.0717 0.6247 0.053 Uiso 0.50 1 d PR A 1 
C1 C 0.527(3) -0.058(3) 0.692(3) 0.024(7) Uiso 0.50 1 d PD A 1 
C2 C 0.458(4) -0.141(3) 0.618(3) 0.034(8) Uiso 0.50 1 d PD A 1 
H2 H 0.4700 -0.1250 0.5641 0.041 Uiso 0.50 1 calc PR A 1 
C3 C 0.466(4) -0.259(3) 0.603(3) 0.068(11) Uani 1 1 d D . . 
C4 C 0.376(3) -0.345(3) 0.529(2) 0.051(8) Uani 1 1 d U B . 
H4A H 0.3475 -0.3286 0.4775 0.077 Uiso 1 1 d R . . 
H4B H 0.4120 -0.4040 0.5137 0.077 Uiso 1 1 d R . . 
H4C H 0.3177 -0.3608 0.5563 0.077 Uiso 1 1 d R . . 
O35' O 0.558(4) -0.129(4) 0.766(3) 0.064(9) Uiso 0.50 1 d PD A 2 
O36' O 0.524(4) -0.221(4) 0.557(4) 0.071(10) Uiso 0.50 1 d PD B 2 
H36' H 0.5093 -0.1654 0.5530 0.106 Uiso 0.50 1 d PR B 2 
N1' N 0.346(4) -0.120(4) 0.589(3) 0.044(9) Uiso 0.50 1 d PD A 2 
H1'A H 0.2954 -0.1635 0.5434 0.066 Uiso 0.50 1 d PR A 2 
H1'B H 0.3142 -0.0730 0.6222 0.066 Uiso 0.50 1 d PR A 2 
H1'C H 0.3957 -0.0874 0.5689 0.066 Uiso 0.50 1 d PR A 2 
C1' C 0.480(3) -0.101(3) 0.733(3) 0.024(7) Uiso 0.50 1 d PD A 2 
C2' C 0.407(4) -0.174(4) 0.654(3) 0.034(8) Uiso 0.50 1 d PD A 2 
H2' H 0.3499 -0.2119 0.6744 0.041 Uiso 0.50 1 calc PR A 2 
  
  
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
  
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O1 1.741(15) . ? 
W1 O5 1.882(14) . ? 
W1 O3 1.910(14) . ? 
W1 O2 1.921(13) . ? 
W1 O6 1.945(15) . ? 
W1 O4 2.288(13) . ? 
W2 O7 1.730(14) . ? 
W2 O9 1.796(14) . ? 
W2 O8 1.930(13) . ? 
W2 O6 1.946(15) . ? 
W2 O10 1.959(14) . ? 
W2 O4 2.345(12) . ? 
W3 O11 1.727(14) . ? 
W3 O14 1.882(13) . ? 
W3 O10 1.889(14) . ? 
W3 O3 1.922(14) . ? 
W3 O12 1.923(14) . ? 
W3 O13 2.388(13) . ? 
W4 O15 1.781(14) . ? 
W4 O17 1.786(14) . ? 
W4 O16 1.790(13) . ? 
W4 O18 2.024(12) . ? 
W4 O14 2.032(12) . ? 
W4 O13 2.245(14) . ? 
W5 O19 1.713(13) . ? 
W5 O21 1.872(14) . ? 
W5 O18 1.895(13) . ? 
W5 O12 1.915(14) . ? 
W5 O20 1.957(14) . ? 
W5 O13 2.375(12) . ? 
W6 O24 1.726(15) . ? 
W6 O23 1.794(14) . ? 
W6 O26 1.918(13) . ? 
W6 O21 1.951(13) . ? 
W6 O25 1.984(15) . ? 
W6 O22 2.338(13) . ? 
W7 O27 1.737(14) . ? 
W7 O29 1.797(15) . ? 
W7 O26 1.927(14) . ? 
W7 O30 1.927(15) . ? 
W7 O28 1.973(14) . ? 
W7 O22 2.290(13) . ? 
W8 O31 1.717(15) . ? 
W8 O32 1.794(16) . ? 
W8 O8 1.910(14) . ? 
W8 O30 1.922(16) . ? 
W8 O2 1.950(14) . ? 
W8 O4 2.345(12) . ? 
W9 O33 1.708(16) . ? 
W9 O20 1.890(13) . ? 
W9 O28 1.902(13) . ? 
W9 O25 1.904(15) . ? 
W9 O5 1.917(14) . ? 
W9 O22 2.353(13) . ? 
Er1 O7M 2.20(7) . ? 
Er1 O12M 2.28(9) . ? 
Er1 O5W 2.33(3) . ? 
Er1 O8W 2.35(5) . ? 
Er1 O1 2.354(16) . ? 
Er1 O10W 2.37(5) . ? 
Er1 O6W 2.37(2) . ? 
Er1 O9W 2.38(3) . ? 
Er1 O12W 2.43(4) . ? 
Er1 O11W 2.43(6) . ? 
Er1 O7W 2.44(8) . ? 
Er1 O10M 2.70(16) . ? 
As1 O22 1.801(14) . ? 
As1 O4 1.803(13) . ? 
As1 O13 1.815(13) . ? 
Fe1 O16 1.905(13) . ? 
Fe1 O9 1.935(15) 2_667 ? 
Fe1 O15 1.941(15) 2_667 ? 
Fe1 O23 1.958(15) . ? 
Fe1 O2W 2.107(15) . ? 
Fe1 O1W 2.150(15) . ? 
O3W Fe2 2.062(17) . ? 
O4W Fe2 2.042(18) . ? 
O7W O10M 1.42(15) . ? 
O10W O10M 1.11(15) . ? 
O10M O13W 1.62(16) . ? 
O12W O12M 0.85(9) . ? 
O16W O16M 1.67(9) . ? 
O18W O18M 1.22(7) . ? 
O9 Fe1 1.935(15) 2_667 ? 
O15 Fe1 1.941(15) 2_667 ? 
O17 Fe2 1.955(15) 2_667 ? 
O29 Fe2 1.962(15) . ? 
O32 Fe2 1.941(15) . ? 
O34 C1' 1.23(4) . ? 
O34 C1 1.23(4) . ? 
O34 Fe2 2.024(16) . ? 
Fe2 O17 1.955(15) 2_667 ? 
O35 C1 1.19(5) . ? 
O36 C3 1.27(4) . ? 
N1 C2 1.59(5) . ? 
C1 C2 1.44(5) . ? 
C2 C3 1.56(5) . ? 
C3 O36' 1.27(4) . ? 
C3 C2' 1.56(5) . ? 
C3 C4 1.56(5) . ? 
O35' C1' 1.19(5) . ? 
N1' C2' 1.59(5) . ? 
C1' C2' 1.44(5) . ? 
  
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O1 W1 O5 100.9(7) . . ? 
O1 W1 O3 105.1(6) . . ? 
O5 W1 O3 89.1(6) . . ? 
O1 W1 O2 99.2(7) . . ? 
O5 W1 O2 91.6(6) . . ? 
O3 W1 O2 155.1(6) . . ? 
O1 W1 O6 96.4(7) . . ? 
O5 W1 O6 162.8(6) . . ? 
O3 W1 O6 85.7(6) . . ? 
O2 W1 O6 86.2(6) . . ? 
O1 W1 O4 169.1(6) . . ? 
O5 W1 O4 86.9(5) . . ? 
O3 W1 O4 82.4(5) . . ? 
O2 W1 O4 72.7(5) . . ? 
O6 W1 O4 76.1(5) . . ? 
O7 W2 O9 101.4(7) . . ? 
O7 W2 O8 102.7(7) . . ? 
O9 W2 O8 94.8(6) . . ? 
O7 W2 O6 101.2(7) . . ? 
O9 W2 O6 156.9(6) . . ? 
O8 W2 O6 84.6(6) . . ? 
O7 W2 O10 99.6(7) . . ? 
O9 W2 O10 89.5(7) . . ? 
O8 W2 O10 156.0(6) . . ? 
O6 W2 O10 82.4(6) . . ? 
O7 W2 O4 174.7(6) . . ? 
O9 W2 O4 83.0(5) . . ? 
O8 W2 O4 73.7(5) . . ? 
O6 W2 O4 74.7(5) . . ? 
O10 W2 O4 83.4(5) . . ? 
O11 W3 O14 100.1(7) . . ? 
O11 W3 O10 100.1(7) . . ? 
O14 W3 O10 91.3(6) . . ? 
O11 W3 O3 103.2(8) . . ? 
O14 W3 O3 156.5(5) . . ? 
O10 W3 O3 86.9(6) . . ? 
O11 W3 O12 99.8(7) . . ? 
O14 W3 O12 89.6(6) . . ? 
O10 W3 O12 159.6(6) . . ? 
O3 W3 O12 84.2(6) . . ? 
O11 W3 O13 169.8(7) . . ? 
O14 W3 O13 71.9(5) . . ? 
O10 W3 O13 86.6(5) . . ? 
O3 W3 O13 84.7(5) . . ? 
O12 W3 O13 74.3(5) . . ? 
O15 W4 O17 102.6(7) . . ? 
O15 W4 O16 97.8(7) . . ? 
O17 W4 O16 102.9(6) . . ? 
O15 W4 O18 159.8(6) . . ? 
O17 W4 O18 95.3(6) . . ? 
O16 W4 O18 87.2(6) . . ? 
O15 W4 O14 88.4(6) . . ? 
O17 W4 O14 94.7(6) . . ? 
O16 W4 O14 159.5(6) . . ? 
O18 W4 O14 80.7(5) . . ? 
O15 W4 O13 87.5(6) . . ? 
O17 W4 O13 163.7(6) . . ? 
O16 W4 O13 88.1(6) . . ? 
O18 W4 O13 73.0(5) . . ? 
O14 W4 O13 72.6(5) . . ? 
O19 W5 O21 102.3(7) . . ? 
O19 W5 O18 101.0(7) . . ? 
O21 W5 O18 92.4(6) . . ? 
O19 W5 O12 98.4(7) . . ? 
O21 W5 O12 158.8(6) . . ? 
O18 W5 O12 88.1(6) . . ? 
O19 W5 O20 100.3(7) . . ? 
O21 W5 O20 86.6(6) . . ? 
O18 W5 O20 158.4(5) . . ? 
O12 W5 O20 85.2(6) . . ? 
O19 W5 O13 170.3(7) . . ? 
O21 W5 O13 85.2(6) . . ? 
O18 W5 O13 72.2(5) . . ? 
O12 W5 O13 74.8(5) . . ? 
O20 W5 O13 86.2(5) . . ? 
O24 W6 O23 103.2(7) . . ? 
O24 W6 O26 101.2(7) . . ? 
O23 W6 O26 94.1(6) . . ? 
O24 W6 O21 101.6(7) . . ? 
O23 W6 O21 91.5(6) . . ? 
O26 W6 O21 154.7(6) . . ? 
O24 W6 O25 98.7(7) . . ? 
O23 W6 O25 157.8(6) . . ? 
O26 W6 O25 85.1(7) . . ? 
O21 W6 O25 80.6(6) . . ? 
O24 W6 O22 171.5(6) . . ? 
O23 W6 O22 83.4(5) . . ? 
O26 W6 O22 72.7(5) . . ? 
O21 W6 O22 83.4(5) . . ? 
O25 W6 O22 75.1(5) . . ? 
O27 W7 O29 103.0(7) . . ? 
O27 W7 O26 98.1(7) . . ? 
O29 W7 O26 91.1(6) . . ? 
O27 W7 O30 100.9(7) . . ? 
O29 W7 O30 90.0(7) . . ? 
O26 W7 O30 160.2(6) . . ? 
O27 W7 O28 96.7(6) . . ? 
O29 W7 O28 160.3(6) . . ? 
O26 W7 O28 87.4(6) . . ? 
O30 W7 O28 84.9(6) . . ? 
O27 W7 O22 166.5(6) . . ? 
O29 W7 O22 88.1(6) . . ? 
O26 W7 O22 73.7(5) . . ? 
O30 W7 O22 86.6(5) . . ? 
O28 W7 O22 72.7(5) . . ? 
O31 W8 O32 103.9(8) . . ? 
O31 W8 O8 101.5(7) . . ? 
O32 W8 O8 92.2(6) . . ? 
O31 W8 O30 98.8(7) . . ? 
O32 W8 O30 89.5(6) . . ? 
O8 W8 O30 158.5(6) . . ? 
O31 W8 O2 96.4(8) . . ? 
O32 W8 O2 159.4(6) . . ? 
O8 W8 O2 87.1(6) . . ? 
O30 W8 O2 83.8(6) . . ? 
O31 W8 O4 166.5(7) . . ? 
O32 W8 O4 89.1(5) . . ? 
O8 W8 O4 74.0(5) . . ? 
O30 W8 O4 84.7(5) . . ? 
O2 W8 O4 70.9(5) . . ? 
O33 W9 O20 101.1(7) . . ? 
O33 W9 O28 103.4(7) . . ? 
O20 W9 O28 155.4(6) . . ? 
O33 W9 O25 98.8(8) . . ? 
O20 W9 O25 84.6(6) . . ? 
O28 W9 O25 89.4(7) . . ? 
O33 W9 O5 100.5(7) . . ? 
O20 W9 O5 88.3(6) . . ? 
O28 W9 O5 89.5(6) . . ? 
O25 W9 O5 160.4(6) . . ? 
O33 W9 O22 173.3(7) . . ? 
O20 W9 O22 83.0(5) . . ? 
O28 W9 O22 72.4(6) . . ? 
O25 W9 O22 76.2(6) . . ? 
O5 W9 O22 84.8(5) . . ? 
O7M Er1 O12M 54(3) . . ? 
O7M Er1 O5W 114.7(19) . . ? 
O12M Er1 O5W 142(3) . . ? 
O7M Er1 O8W 82(2) . . ? 
O12M Er1 O8W 130(3) . . ? 
O5W Er1 O8W 72.9(13) . . ? 
O7M Er1 O1 74.1(18) . . ? 
O12M Er1 O1 67(2) . . ? 
O5W Er1 O1 74.9(8) . . ? 
O8W Er1 O1 126.6(12) . . ? 
O7M Er1 O10W 86(2) . . ? 
O12M Er1 O10W 71(3) . . ? 
O5W Er1 O10W 146.5(14) . . ? 
O8W Er1 O10W 84.9(17) . . ? 
O1 Er1 O10W 138.2(12) . . ? 
O7M Er1 O6W 138.2(19) . . ? 
O12M Er1 O6W 90(3) . . ? 
O5W Er1 O6W 79.3(10) . . ? 
O8W Er1 O6W 138.5(13) . . ? 
O1 Er1 O6W 72.2(7) . . ? 
O10W Er1 O6W 103.3(13) . . ? 
O7M Er1 O9W 144(2) . . ? 
O12M Er1 O9W 137(3) . . ? 
O5W Er1 O9W 75.7(12) . . ? 
O8W Er1 O9W 67.2(16) . . ? 
O1 Er1 O9W 140.4(9) . . ? 
O10W Er1 O9W 72.5(14) . . ? 
O6W Er1 O9W 76.6(12) . . ? 
O7M Er1 O12W 74(2) . . ? 
O12M Er1 O12W 20(2) . . ? 
O5W Er1 O12W 141.5(12) . . ? 
O8W Er1 O12W 144.3(16) . . ? 
O1 Er1 O12W 71.8(11) . . ? 
O10W Er1 O12W 67.4(16) . . ? 
O6W Er1 O12W 72.5(13) . . ? 
O9W Er1 O12W 120.9(15) . . ? 
O7M Er1 O11W 57(2) . . ? 
O12M Er1 O11W 105(3) . . ? 
O5W Er1 O11W 59.0(16) . . ? 
O8W Er1 O11W 56.0(18) . . ? 
O1 Er1 O11W 71.0(14) . . ? 
O10W Er1 O11W 126.9(19) . . ? 
O6W Er1 O11W 129.8(15) . . ? 
O9W Er1 O11W 114.2(18) . . ? 
O12W Er1 O11W 124.4(17) . . ? 
O7M Er1 O7W 53(3) . . ? 
O12M Er1 O7W 83(3) . . ? 
O5W Er1 O7W 120.8(18) . . ? 
O8W Er1 O7W 49(2) . . ? 
O1 Er1 O7W 126.5(18) . . ? 
O10W Er1 O7W 51(2) . . ? 
O6W Er1 O7W 153.9(18) . . ? 
O9W Er1 O7W 92(2) . . ? 
O12W Er1 O7W 95(2) . . ? 
O11W Er1 O7W 76(2) . . ? 
O7M Er1 O10M 80(4) . . ? 
O12M Er1 O10M 86(4) . . ? 
O5W Er1 O10M 130(3) . . ? 
O8W Er1 O10M 61(3) . . ? 
O1 Er1 O10M 151(3) . . ? 
O10W Er1 O10M 24(3) . . ? 
O6W Er1 O10M 123(3) . . ? 
O9W Er1 O10M 69(3) . . ? 
O12W Er1 O10M 88(3) . . ? 
O11W Er1 O10M 105(4) . . ? 
O7W Er1 O10M 32(3) . . ? 
O22 As1 O4 96.3(6) . . ? 
O22 As1 O13 98.8(6) . . ? 
O4 As1 O13 99.4(6) . . ? 
O16 Fe1 O9 94.9(6) . 2_667 ? 
O16 Fe1 O15 93.1(6) . 2_667 ? 
O9 Fe1 O15 92.8(7) 2_667 2_667 ? 
O16 Fe1 O23 92.4(6) . . ? 
O9 Fe1 O23 169.6(6) 2_667 . ? 
O15 Fe1 O23 94.2(6) 2_667 . ? 
O16 Fe1 O2W 177.2(7) . . ? 
O9 Fe1 O2W 87.8(6) 2_667 . ? 
O15 Fe1 O2W 85.9(7) 2_667 . ? 
O23 Fe1 O2W 85.0(6) . . ? 
O16 Fe1 O1W 92.2(6) . . ? 
O9 Fe1 O1W 83.2(6) 2_667 . ? 
O15 Fe1 O1W 173.6(7) 2_667 . ? 
O23 Fe1 O1W 89.1(6) . . ? 
O2W Fe1 O1W 88.9(7) . . ? 
O10M O7W Er1 84(8) . . ? 
O10M O10W Er1 95(9) . . ? 
O10W O10M O7W 108(10) . . ? 
O10W O10M O13W 121(10) . . ? 
O7W O10M O13W 106(10) . . ? 
O10W O10M Er1 61(8) . . ? 
O7W O10M Er1 64(7) . . ? 
O13W O10M Er1 169(9) . . ? 
O12M O12W Er1 69(7) . . ? 
O12W O12M Er1 90(8) . . ? 
W1 O1 Er1 148.6(8) . . ? 
W1 O2 W8 122.2(8) . . ? 
W1 O3 W3 145.6(8) . . ? 
As1 O4 W1 135.1(6) . . ? 
As1 O4 W2 117.9(6) . . ? 
W1 O4 W2 91.6(4) . . ? 
As1 O4 W8 116.7(6) . . ? 
W1 O4 W8 94.0(5) . . ? 
W2 O4 W8 91.0(4) . . ? 
W1 O5 W9 155.8(8) . . ? 
W1 O6 W2 117.3(7) . . ? 
W8 O8 W2 121.2(7) . . ? 
W2 O9 Fe1 143.7(7) . 2_667 ? 
W3 O10 W2 145.7(8) . . ? 
W5 O12 W3 121.5(7) . . ? 
As1 O13 W4 115.9(7) . . ? 
As1 O13 W5 127.8(7) . . ? 
W4 O13 W5 94.5(5) . . ? 
As1 O13 W3 126.2(6) . . ? 
W4 O13 W3 94.6(5) . . ? 
W5 O13 W3 89.3(4) . . ? 
W3 O14 W4 120.9(6) . . ? 
W4 O15 Fe1 178.8(9) . 2_667 ? 
W4 O16 Fe1 169.8(9) . . ? 
W4 O17 Fe2 164.4(8) . 2_667 ? 
W5 O18 W4 120.0(6) . . ? 
W9 O20 W5 144.7(8) . . ? 
W5 O21 W6 146.9(8) . . ? 
As1 O22 W7 117.2(6) . . ? 
As1 O22 W6 118.1(7) . . ? 
W7 O22 W6 92.5(5) . . ? 
As1 O22 W9 135.0(7) . . ? 
W7 O22 W9 93.4(5) . . ? 
W6 O22 W9 90.5(4) . . ? 
W6 O23 Fe1 142.7(7) . . ? 
W9 O25 W6 118.0(7) . . ? 
W6 O26 W7 120.9(7) . . ? 
W9 O28 W7 121.3(8) . . ? 
W7 O29 Fe2 137.4(8) . . ? 
W8 O30 W7 145.5(9) . . ? 
W8 O32 Fe2 139.0(8) . . ? 
C1' O34 C1 57(3) . . ? 
C1' O34 Fe2 145(2) . . ? 
C1 O34 Fe2 134(2) . . ? 
O32 Fe2 O17 99.4(6) . 2_667 ? 
O32 Fe2 O29 88.3(6) . . ? 
O17 Fe2 O29 98.5(6) 2_667 . ? 
O32 Fe2 O34 89.5(7) . . ? 
O17 Fe2 O34 167.5(6) 2_667 . ? 
O29 Fe2 O34 90.6(6) . . ? 
O32 Fe2 O4W 93.6(8) . . ? 
O17 Fe2 O4W 85.5(8) 2_667 . ? 
O29 Fe2 O4W 175.3(7) . . ? 
O34 Fe2 O4W 85.1(8) . . ? 
O32 Fe2 O3W 174.7(7) . . ? 
O17 Fe2 O3W 85.8(7) 2_667 . ? 
O29 Fe2 O3W 89.4(7) . . ? 
O34 Fe2 O3W 85.7(8) . . ? 
O4W Fe2 O3W 88.3(9) . . ? 
O35 C1 O34 129(4) . . ? 
O35 C1 C2 111(4) . . ? 
O34 C1 C2 119(4) . . ? 
C1 C2 C3 122(4) . . ? 
C1 C2 N1 107(4) . . ? 
C3 C2 N1 107(3) . . ? 
O36' C3 O36 135(5) . . ? 
O36' C3 C2' 111(4) . . ? 
O36 C3 C2' 83(3) . . ? 
O36' C3 C2 70(3) . . ? 
O36 C3 C2 110(4) . . ? 
C2' C3 C2 40(3) . . ? 
O36' C3 C4 103(4) . . ? 
O36 C3 C4 114(3) . . ? 
C2' C3 C4 108(3) . . ? 
C2 C3 C4 118(4) . . ? 
O35' C1' O34 117(4) . . ? 
O35' C1' C2' 118(4) . . ? 
O34 C1' C2' 121(3) . . ? 
C1' C2' C3 112(3) . . ? 
C1' C2' N1' 114(4) . . ? 
C3 C2' N1' 110(4) . . ? 
  
_diffrn_measured_fraction_theta_max    0.966 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.966 
_refine_diff_density_max    4.397 
_refine_diff_density_min   -5.990 
_refine_diff_density_rms    0.706 
  


#===END